PrefaceThe market for edible films and coatings has experienced remarkable growthover the last 5 years according to the U.S. Department of Agriculture. Thisgrowth is expected to continue. Accompanying this growth is a vast amount ofknowledge on edible films and coatings acquired through research and productdevelopment work as well as advances in material science and processing tech-nology. For the past 15 years, there were numerous research articles publishedand research projects undertaken by the academic and research communitiesas well as the food and pharmaceutical industry. The impact of sustainabilityprograms, carbon foot printing and heightened interest on the use of renewableresources further propelled and will continue to propel the growth and interestson edible films and coatings. In addition, edible film and coating are addingvalue to agricultural and food industries by-products. With this backdrop, thisbook on Edible Films and Coatings for Food Applications was organized andcreated. This book brings together edible film and coating experts from variousscientific disciplines from the academic and research institutions and the foodindustry (protein, carbohydrate/polysaccharide and lipid chemistry, engineering,and manufacturing). The book starts with a valuable edible films and coatings historical and generaloverview, followed by four chapters on structure–function relationship of biomate-rials used in the preparation of edible films and coatings (proteins, polysaccharidegums, starches and waxes and lipids). These four chapters also include discussion onpreparation and properties of edible films and coatings made from these biomateri-als. The next six chapters discuss specific applications of edible films and coatingssuch as protection of fruits and vegetables, meat and poultry and for the deliveryof food additives, flavors and active ingredients. The next two chapters deal withmechanical and permeability properties and new advances in analytical techniquesfor edible films and coatings. Quite unique in this book is the discussion ofcommercial manufacture of edible films and coatings authored by one of the pioneersin the field. Each author developed his or her chapter in a comprehensive mannersuch that each chapter can stand on its own. This book was created to help thenovice in edible films and coatings as well as those already immersed in the fieldwith the hope that the topics discussed in the book will trigger future novel ideasand processes. Due to the nature of and scope of each chapter, overlapping topics v
vi Prefacecannot be completely avoided. On the other hand, these overlaps are necessary foreach chapter to be able to stand on its own. A sincere and great appreciation goes to the book chapter authors for their con-tributions and to all the researchers/scientists/authors who have toiled hard to keepthe interest and continued advancement of edible films and coatings alive. A specialthanks also goes to Springer Science for their encouragement, patience and theirwhole-hearted support of this book project. Special thanks to Sauld Embuscado forworking on selected figures.Hunt Valley, MD Milda E. EmbuscadoMoscow, ID Kerry C. Huber
Contents1 Edible Films and Coatings: Why, What, and How? ............................. 1 Attila E. Pavlath and William Orts2 Structure and Function of Protein-Based Edible Films and Coatings ...................................................................... 25 Kirsten Dangaran, Peggy M. Tomasula, and Phoebe Qi3 Structure and Function of Polysaccharide Gum-Based Edible Films and Coatings ................................................. 57 Marceliano B. Nieto4 Structure and Function of Starch-Based Edible Films and Coatings .................................................................................. 113 Michael E. Kramer5 Lipid-Based Edible Films and Coatings ................................................ 135 Frédéric Debeaufort and Andrée Voilley6 Characterization of Starch and Composite Edible Films and Coatings ...................................................................... 169 María A. García, Adriana Pinotti, Miriam N. Martino, and Noemí E. Zaritzky7 Edible Films and Coatings for Fruits and Vegetables .......................... 211 Guadalupe I. Olivas and Gustavo Barbosa-Cánovas8 Edible Films and Coatings for Meat and Poultry ................................. 245 Zey Ustunol9 Edible Films and Coatings for Flavor Encapsulation........................... 269 Gary A. Reineccius vii
viii Contents10 Delivery of Flavor and Active Ingredients Using Edible Films and Coatings.......................................................... 295 Olga Martín-Belloso, M. Alejandra Rojas-Graü, and Robert Soliva-Fortuny11 Delivery of Food Additives and Antimicrobials Using Edible Films and Coatings.......................................................... 315 Jesus-Alberto Quezada-Gallo12 Application of Infrared Analysis to Edible Films ............................... 335 Charles M. Zapf13 Mechanical and Permeability Properties of Edible Films and Coatings for Food and Pharmaceutical Applications.................. 347 Monique Lacroix14 Commercial Manufacture of Edible Films .......................................... 367 James M. RossmanIndex ................................................................................................................ 391
ContributorsGustavo Barbosa-Cánovas, Ph.D.Center for Nonthermal Processing of Food, Washington State University,Pullman, WA 99164-6120, USABarbosa@wsu.eduKirsten Dangaran, Ph.D.Dairy Processing and Product Research, Eastern Regional Research Center, ARS,USDA, 600 East Mermaid Lane, Wyndmoor, PA 19038, USAdangaran.email@example.comFrederic Debeaufort, Ph.D., Eng.Universitary Institute of Technology, Department of Bioengineering,Université de Bourgogne, 7 bd Dr Petitjean, BP 17867, F-21078, Dijon, France,firstname.lastname@example.orgMilda E. Embuscado, Ph.D.Materials and Process Technology, McCormick and Co. Inc., Hunt Valley,MD, USAMilda_Embuscado@mccormick.comMaría Alejandra GarcíaCentro de Investigación y Desarrollo en Criotecnología de Alimentos (CIDCA),CONICET, Universidad Nacional de La Plata (UNLP), 47 y 116 La Plata (1900),Argentinamagarcia@quimica.unlp.edu.arKerry C. Huber, Ph.D.School of Food Science & Toxicology, College of Agricultural andLife Sciences, University of Idaho, Moscow, ID, USAhuberk@uidaho.eduMichael E. KramerTechnical Services, Grain Processing Corporation, 1600 Oregon Street,Muscatine, IA 52761, USAMike_kramer@grainprocessing.com ix
x ContributorsMonique LacroixINRS – Institut Armand-Frappier, Research Laboratory in Science Applied toFood, Canadian Irradiation Centre, 531 des Prairies, Laval, QC, Canada H7V 1B7,Monique.email@example.comOlga Martín-BellosoDepartment of Food Technology, University of Lleida, Alcalde Rovira Roure, 191,Lleida 25198, Spain, firstname.lastname@example.orgMiriam MartinoCentro de Investigación y Desarrollo en Criotecnología de Alimentos (CIDCA),CONICET, Universidad Nacional de La Plata (UNLP), 47 y 116 La Plata (1900),Argentina, email@example.comMarceliano B. Nieto, Ph.D.TIC Gums, 4609 Richlynn Drive, Belcamp, MD 21017, USAmnieto@ticgums.comGuadalupe Isela Olivas, Ph.D.Centro de Investigación en Alimentación y Desarrollo (CIAD), Av. Río ConchosS/N, Cuauhtémoc, Chihuahua 31570, Mexicogolivas@ciad.mxWilliam Orts, Ph.D.Western Regional Research Center, ARS, USDA, Albany, CA, USAorts@pw.usda.govAttila Pavlath, Ph.D.Western Regional Research Center, ARS, USDA, Albany, CA, USAapavlath@pw.usda.govAdriana PinottiCentro de Investigación y Desarrollo en Criotecnología de Alimentos (CIDCA),CONICET, Universidad Nacional de La Plata (UNLP), 47 y 116 La Plata (1900),Argentinaimpronta@arnet.com.arPhoebe Qi, Ph.D.Dairy Processing and Product Research, Eastern Regional Research Center,ARS, USDA, 600 East Mermaid Lane, Wyndmoor, PA 19038, USAphoebe.firstname.lastname@example.orgJesus-Alberto Quezada-Gallo, Ph.D.Departamento de Ingeniera y Ciencias Qumicas, Universidad IberoamericanaCiudad de Mexico, Ediﬁcio F segundo piso, Prol. Paseo de la Reforma 880Lomas de Santa Fe, 01210 Mexico, D.F., Mexicojesus.email@example.com
Contributors xiGary A. Reineccius, Ph.D.Department of Food Science and Nutrition, 1334 Eckles Avenue, St. Paul,MN 55108-1038, USAgreinecc@umn.eduM. Alejandra Rojas-GraüDepartment of Food Technology, University of Lleida, Alcalde Rovira Roure, 191,Lleida 25198, Spainmargrau@tecal.udl.esJames M. RossmanRossman Consulting, LLC, 1706 W. Morrison Avenue, Tampa, FL 33606, USArossmanj@prodigy.netRobert Soliva-FortunyDepartment of Food Technology, University of Lleida, Alcalde Rovira Roure,191, Lleida 25198, Spainrsoliva@tecal.udl.esPeggy Tomasula, Ph.D.Dairy Processing and Product Research, Eastern Regional Research Center,ARS, USDA, 600 East Mermaid Lane, Wyndmoor, PA 19038, USAPeggy.Tomasula@ars.usda.govZey Ustunol, Ph.D.Department of Food Science & Human Nutrition, Michigan State University,2105 South Anthony Hall, Lansing, MI 48824-1225, USAUstunol@anr.msu.eduAndree Voilley, Ph.D., Eng.EMMA Department, Université de Bourgogne – ENSBANA,1 esplanade Erasme, F-21000, Dijon, Francevoilley@u-bourgogne.frMichael ZapfTechnical Innovation Center, McCormick & Company, Inc., 204 Wight Avenue,Hunt Valley, MD 21031-1501, USAMike_Zapf@mccormick.comNoemí ZaritzkyCentro de Investigación y Desarrollo en Criotecnología de Alimentos (CIDCA),CONICET, Universidad Nacional de La Plata (UNLP), 47 y 116 La Plata (1900),Argentinazaritzky@ing.unlp.edu.ar
2 A.E. Pavlath and W. Ortsconsumer. During time-consuming steps involved in handling, storage andtransportation, products start to dehydrate, deteriorate, and lose appearance, flavorand nutritional value. If no special protection is provided, damage can occurwithin hours or days, even if this damage is not immediately visible. As early as twelfth century, citrus fruits from Southern China were preserved forthe Emperor’s table by placing them in boxes, pouring molten wax over them, andsending them by caravan to the North (Hardenburg 1967). While their quality wouldnot have been acceptable to our modern selective society, the method was quite effectivefor its time, and was used for centuries for lack of more efficient ones . In Europe, theprocess was known as “larding” – storing various fruits in wax or fats for laterconsumption (Contreras-Medellin and Labuza 1981). While such protection preventedwater losses, the tight, thick layer interfered with natural gas exchange, and resulted inlower quality products. Larding was a compromise between maintaining moisturecontent and losing various qualities, including optimal taste and texture. Later in thefifteenth century, an edible film, Yuba, made from skin of boiled soy milk was used inJapan for maintaining food quality and improving appearance (Biquet and Guilbert1986; Gennadios et al. 1993). In the nineteenth century, a US patent was issued forpreservation of various meat products by gelatin (Havard and Harmony 1869). Otherearly preservation methods included smoking and/or keeping products cool in iceboxesor in underground cellars. Today various modern methods, including combinationsof these, such as refrigeration, controlled atmosphere storage, and sterilization byboth UV and gamma radiation are used to keep our food safe. Nevertheless, formany kinds of food, coating with edible film continues to be one of the most cost-effective ways to maintain their quality and safety.1.2 Definition1.2.1 Edible Films and CoatingsAny type of material used for enrobing (i.e., coating or wrapping) various food toextend shelf life of the product that may be eaten together with food with or withoutfurther removal is considered an edible film or coating. Edible films providereplacement and/or fortification of natural layers to prevent moisture losses, whileselectively allowing for controlled exchange of important gases, such as oxygen,carbon dioxide, and ethylene, which are involved in respiration processes. A filmor coating can also provide surface sterility and prevent loss of other importantcomponents. Generally, its thickness is less than 0.3 mm.1.2.2 Generally Recommended as Safe (GRAS)Items which are edible or are in contact with food should be generally recognized byqualified experts as being safe under conditions of its intended use, with amount applied
1 Edible Films and Coatings 3in accordance with good manufacturing practices. These food-safe materials musttypically have approval of the Food and Drug Administration (FDA). Since it isimpractical for FDA to have an all-inclusive list of every potential food ingredient, thereare also other opportunities to acquire GRAS status – i.e., manufacturers can petition forapproval of an ingredient or food composite provided that this petition is supported byconsiderable studies. There are three types of GRAS designations (1) Self-affirmed,where the manufacturer has carried out necessary work and is ready to defend GRASstatus if challenged, (2) FDA pending, where results of research have been submitted toFDA for approval, and (3) No comment- which is the response of FDA if after review, ithas no challenges. More detailed information on procedures to acquire such designationsfor industrial purposes can be found at the FDA website.2 However, GRAS status doesnot guarantee complete product safety, especially for consumers who have food allergiesor sensitivities, such as lactose intolerance (milk) and Celiac disease (wheat gluten).1.2.3 Shelf LifeThe time period, whereby a product is not only safe to eat, but still has acceptabletaste, texture and appearance after being removed from its natural environment, isdefined as shelf life. For practical purposes, a period of at least 2 weeks is requiredfor processed food to remain wholesome, allowing for packaging, transportation,distribution, and display prior to consumption.1.2.4 Light Processing‘Light Processing’ includes a wide variety of processes used to prepare an originalproduct or commodity for consumption, without affecting the original, “fresh-like”quality of the product (Shewfelt 1987). Light processing includes cleaning, washing,paring, coring, and dicing, for fruits and vegetables specifically, and may alsoinclude removing waste and undesirable parts from a wide variety of food products(such as de-boning of meat, etc). Although these steps are relatively unobtrusive,nature and rate of respiration changes immediately after most light processing, withthe product becoming immediately more perishable. In most cases, these processescause disruption of cell tissues and breakdown of cell membranes, creating manymembrane-related problems (Davies 1987).1.2.5 RespirationAny type of food, whether in its natural environment or otherwise, continuouslyundergoes various biochemical/biological/physiological processes, which use up2 http://www.cfsan.fda.gov/~dms/grasguid.html
4 A.E. Pavlath and W. Ortsand/or release oxygen and carbon dioxide (colloquially labeled “breathing”).Depending on oxygen level, respiration can be aerobic or anaerobic. Respirationactivity of a product is influenced by storage temperature, type of processing, oxygento carbon dioxide ratio, and absolute value of oxygen concentration itself. If a waxlayer is applied, oxygen content of the internal atmosphere will decrease as a functionof thickness of the layer, while carbon dioxide content and anaerobic respirationwill rise (Eaks and Ludi 1960). As a rule of thumb, when oxygen level drops below3%, anaerobic respiration will start replacing the Krebs cycle, with the resultingglycolytic pathway releasing unacceptable flavors and causing other problems,such as changes in color and texture. High oxygen levels (>8%) and low carbondioxide levels (<5%) can prevent or delay senescence in horticultural products, thusmaintaining food quality (Kader 1986).1.2.6 TranspirationIn addition to gases, food products may contain various liquid or solid components;water is most prevalent, but oils, various flavor components, and nutrients are alsopresent. Depending on environment, these components will migrate out of orthroughout the product if there is concentration difference acting as a driving force.1.2.7 Controlled and Modified Atmosphere StorageIn order to control respiration (i.e., transfer of various gases in and out of the prod-uct), food can be stored in an environment filled with various gases at appropriate,optimal temperatures. The right gas combination can slow respiratory metabolism,and delay compositional changes in color, flavor and texture. It can also inhibit ordelay microbial growth. However, this method can be quite expensive in other thanlarge-scale stationary storage, i.e. controlled atmosphere situations. Modifiedatmosphere packaging (MAP) is where product is enclosed in a sealed box or bagfilled with required atmosphere. Temperature, however, is critical and must bemaintained at constant level to avoid in-pack condensation leading to spoilage.1.3 Effect of Edible Films and Coatings or the Lack ThereofToday, the most widely used commercial method for long-range protection isinterim storage at low temperature (4–8°C), especially for lightly-processed food.Lowering temperature generally decreases undesirable enzyme activities, althoughtemperature decreases down to 0–5°C may actually lead to increases in respirationrate and ethylene production (Eaks 1980). Below 0°C, growth of mold is inhibited,
1 Edible Films and Coatings 5but even this low temperature does not fully eliminate undesirable chemical andphysicochemical reactions (Fennema 1993). For example, fruits and vegetablesnative to tropical climates experience harmful chilling effects such as damage tocell membranes at temperatures of 10–12°C. In addition, some cold-tolerant patho-genic microorganisms are able to grow even under refrigeration. Accordingly, an increasing amount of research has been conducted over the past50 years to encase a food product, such that rates of migration of molecules involvedin degradative processes are maintained at natural levels and/or minimized. Edible films are being used for a variety of purposes within a multitude of foodsystems, even though this fact might not be fully realized by consumers. The shinysurface of an apple in a supermarket is not provided by nature. Some candies (e.g.,M&Ms) are coated with shellac to increase product shelf life and provide desiredglaze. Medicine pills are often coated to prevent crumbling, to hide any bitter orundesirable taste before swallowing, and to provide controllable timed-release ofmedications. Even French fries are frequently coated to provide protection duringcold storage before frying, control of water losses during frying, and stabilityagainst wilting and/or loss of crispness under infrared lamps between frying andserving. Edible films may also be used to limit uptake of oil and fat during fryingprocesses (Feeney et al., 1992; Polanski, 1993). Table 1.1. provides an informative,and non-comprehensive list of examples of commercial edible coatings. Most fresh fruits and vegetables contain considerable percentage of water, theamount of which is maintained during production in their natural environment.Respiration is maintained naturally at an appropriate equilibrium between oxygen,carbon dioxide and water by skin, which controls transmission to and from sur-rounding environment. However, as soon as fruits and vegetables are separatedfrom their native production environment (i.e., harvested), the delicate balance isupset. Water activity (aw) will change, and various physiological reactions, whichwere previously kept under control in developing fruit or vegetable, will accelerateTable 1.1 List of commercially used coatingsName Main component UsesFreshseel™ Sucrose esters Extending shelf life of melonFry Shield™ Calcium pectinate Reduces fat uptake during frying fish, pota- toes, and other vegetablesNature Seal™ Calcium ascorbate Apples, avocado, carrot, and other vegetablesNutrasave™ N,O-Carboxymethyl chitosan Reduces loss of water in avocado, retains firmnessOpta Glaze™ Wheat gluten Replaces raw egg based coating to prevent microbial growthSeal gum, Spray Calcium acetate Prevents darkening of potato during frying gum™Semperfresh™ Sucrose esters Protect pome fruits from losing water and discolorationZ*Coat™ Corn protein Extends shelf-life of nut meats, pecan, and chocolate covered peanut
6 A.E. Pavlath and W. Ortspost-harvest. Respiration will be affected, resulting in altered ratios of oxygen andcarbon dioxide. Increased ethylene formation will accelerate ripening, thus chang-ing color, flavor, texture and nutritional characteristics of the fruit or vegetable(Wong et al. 1994a). Some protection against undesired changes can be obtained using controlledatmospheres and low temperatures during transportation and storage. Controlledatmosphere with high relative humidity can prevent loss of water and, with mainte-nance of appropriate carbon dioxide and oxygen concentrations, slow down senes-cence. However, with all attempts to optimize storage through controlledenvironments, they are still no match for Mother Nature’s quality control in thefield. Various undesirable changes can still occur once food has been picked andprocessed, and aging begins. More importantly, cost of maintaining controlled-storage environments can be very prohibitive. These problems are not limited to just fruits and vegetables. Quality of variousother food products, such as meat, pies and confectionery can also suffer beforereaching the consumer. Major difficulties are deterioration of vital food compo-nents including flavor chemicals, lipids, and vitamins through oxidation. The patentissued in the nineteenth century to coat meat with gelatin to delay microbe forma-tion and loss of water was just the beginning (Havard and Harmony 1869).Numerous research studies were carried out with reasonable success, paving theway for possible commercial applications. Loss of water which affects juiciness ofmeat products, was reduced by coating meat surfaces with polysaccharides to main-tain desired moisture levels (Allen et al. 1963; Shaw et al. 1980). Microbes thatcontaminate meat can cause serious health safety problems, which can be mediatedto some extent by edible films and coatings. Alginate coatings have been shown toprevent microbial growth on beef, pork, lamb and poultry (Lazarus et al. 1976;Williams et al. 1978). When frying battered or breaded meat products, too much oilmay be adsorbed if batter does not adhere adequately to meat surface. By coatingmeat first with cellulose derivatives, oil uptake is considerably lessened (Feeneyet al. 1992; Polanski 1993). Infusion of oil into chocolate presents quality problemsin confectionaries, i.e., stickiness, moisture absorption, and oxidation (Paulinka1986; Nelson and Fennema 1991). Similarly, some foods have to be protectedagainst moisture uptake that can otherwise result in loss of crispness. Hydration ofcertain snack foods can be prevented by coating with sucrose fatty acid esters(Kester et al. 1990), and dried fruit can have longer shelf life when coated with zein(Cosler 1957). In case of chewing gums, an edible film is needed to prevent loss ofmoisture (Meyers 1994). Uncontrolled migration of water is generally recognized as the biggest food storage/transportation challenge. Both loss and gain of water are almost always consideredundesirable. Even if water loss does not cause immediate visible shrinkage to afood product, it results in economic loss via weight loss. Figure 1.1 shows that evena whole unwaxed apple will show 0.5% of weight loss after 1 day, a loss that willincrease more than ten-fold when the fruit is cut in half. On the other hand, storage in high relative humidity environments may result inwater infusion causing variations in the food product between point of preparation
1 Edible Films and Coatings 7Fig. 1.1 Comparative loss of weight for whole and half apple samplesand sale. This occurrence can be a problem when regulations mandate a minimumsolids content. In heterogeneous foods, if various components have different wateractivities, water transmission during storage can also occur internally betweencomponents of the food, causing changes to sensory characteristics. For example,moisture content between the dough and toppings of a pizza are different. If thepizza is not baked immediately after assembly, internal water migration may occur,and the original optimal moisture content of the dough will change. This changewill result in different a texture of the baked product. Refrigerated storage is appliedto prevent quality and safety changes in toppings (cheese, meat etc.). While refrig-eration slows down water migration, water can still migrate even within the frozenproduct, especially if stored for a long time. Application of a film in some form onsurface of the dough, before placing on the toppings, can prevent water migrationand retain optimum dough structure. Similar problems exist with pies, where thereis need to separate moist filling from crust to prevent sogginess (Labuza 1984), orin chocolate covered nuts, where migration of oil from nuts may retard softening ofchocolate covering upon consumption (Murray and Luft 1973; Paulinka 1986;Nelson et al. 1991). Discoloration or enzymatic browning, caused by polyphenol oxidase, is anotherfrequent food issue. This phenomenon does not affect weight or nutrition, andsometimes not even taste, of food, but it is unsightly and results in loss due to con-sumer rejection. In addition, changes in gas transition result in various other equallyimportant detrimental characteristics. These include:• Loss and/or change of flavor and aroma• Aesthetically unacceptable appearance• Changes in textureOne obvious solution is to protect food from these changes until they are ready forconsumption via application of edible films, which can prevent contamination,microbial growth, and pest infestation. In addition edible films can help alleviate
8 A.E. Pavlath and W. Ortsquality issues during quarantines that are frequently invoked on fruits due topossible infection with insect eggs. For example, many exports are held back atports until costly fumigation is carried out. Fruits need to be stored at 1–2°C for14–24 days before shipping from Florida to Japan (Ismail 1989). Coatings can reduceoxygen levels within the fruit and kill larva, though this method is not always optimaland may also reduce fruit quality (Hallman et al. 1994). Since potential eggs are laidon natural skin, a better way is to remove skin and enrobe fruit with edible film.1.4 Application and Preparation of Edible FilmsEdible films can provide either clear or milky (opaque) coatings, but consumersgenerally prefer invisible, clear coatings. Coatings can be obtained in various ways(1) by dipping the product into, or by brushing or spraying it with solution containingfilm ingredients, so as to deposit the film directly on food surface (Gontard andGuilbert 1994), or (2) by creating stand alone film from solution or throughthermoformation for subsequent covering of food surface. The simplest way to apply a film is directly from solution. Depending onconcentration of coating solution, the product will absorb an appropriate amount ofcoating material necessary to form the desired layer, which when dried, forms aprotective layer at the food surface. In most cases, some plasticizer needs to beadded to coating solution to keep the developing film from becoming brittle.Possible food grade plasticizers are glycerol, mannitol, sorbitol, and sucrose. Ifcoating cracks, movement of various components will increase by orders of magnitude,resulting in mass flow instead of diffusion. Coatings should have good adhesion torough surfaces (Hershko et al. 1996). Application of a uniform film or coating layerto cut fruit and vegetable surfaces is generally difficult. Better uniformity can bepromoted by adding surfactants to solution to reduce surface tension. This strategywill also reduce the superficial aw, and in turn reduce water loss (Roth and Loncin1984, 1985). In one standard process, carboxymethylcellulose (CMC) powder wasapplied to cut fruit surfaces. The CMC adsorbed moisture within pores of the sur-face, causing the CMC to swell, which not only prevented loss of moisture, but alsoprovided a barrier against oxygen to prevent enzymatic discoloration (DeLong andShepherd 1972). Coatings derived from non-aqueous media, such as applying analcohol solution of shellac to candy, result in another level of complexity. For safetyreasons the finished coating layer should not contain any solvent residue. Thus,during large scale operation, disposal of exhaust gases may present environmentalchallenges. Should a free-standing film be required, it can be prepared from solution byevaporation. It should be pointed out that characteristics of stand-alone films mightdiffer from those of films created on food surfaces (i.e., those produced by dippingin or spraying). Films obtained through evaporation were found to have lower watervapor permeability than those prepared by spraying (Pickard et al. 1972). Varyingrate and temperature of evaporation may result in creation of films with differing
1 Edible Films and Coatings 9characteristics. For example, polymer chains may be prematurely immobilizedbefore reaching their optimal structure (by accelerated drying) to affect permeabil-ity (Reading and Spring 1984; Greener 1992). When zein films were obtained fromsolution after drying at 51°C for 10 min, plasticizer was needed to obtain a non-brittle material (Kanig and Goodman 1962). In contrast, drying at 35°C for 24 hyielded flexible zein films without addition of plasticizer (Guilbert 1986, 1988).Films can also be formed by cooling concentrated solutions. However rate of cool-ing can again result in amorphous, crystalline, or polymorphic films with differingpermeabilities. The characteristics of a polymorphic film may be further modifiedby tempering (Landman et al. 1960; Kester and Fennema 1989a, b). Formation offlexible and stretchable films was also reported from molten acetylated monoglyc-eride (Feuge et al. 1953). Other possibilities are through precipitation, either byaddition of selective miscible solvents that are not a solvent for the film component,or by desalting. In addition, some protein films can form upon heating, causingunfolding of polymeric chains and replacement of intramolecular with intermolecu-lar bonds. This transition affects permeability. In case of proteins, improved filmscan be obtained by adjusting coating solution pH in relation to the protein isoelec-tric point, where proteins become least soluble. However, this process does notnecessarily improve resistance of films to water transmission (Krochta et al. 1988).The pH can be also adjusted by high pressure liquefied carbon dioxide treatmentwhich although costly, does not leave any salt residue (Tomasul et al. 1997). When films, comprised of pectin or alginate, are prepared by evaporation fromwater-soluble components, they are subject to re-dissolution in water or destructionin high humidity conditions. This problem can be avoided by cross-linking polymersat the film surface. Various reactions can be employed to achieve enhanced covalentbonding (e.g., treatment with formaldehyde); however such reactions can create newchemical structures that might necessitate approval by FDA. The most acceptablecross-linking method involves ionic interaction between polymer chains via multi-valent ions to form ionomers. While most synthetic films have higher tensile strengththan typical edible films, ionomers are exceptions (Pavlath et al. 1999a; Pavlathet al. 1999b). For ionomers, tensile strength of their films is dependent on numberof available bonding locations. Ionomer cross-linked films can be used as wrappingmaterials or, in case of water solubility, as bags that dissolve when immersed inwater during food preparation (e.g., soup). In such cases, films do not have to bethin, because they will disappear before tasting and can further act as thickeningagents within the food product. This aspect is especially important from an environ-mental perspective, where disposal is not necessary (becomes consumed as part ofthe food). Commercial synthetic materials are not generally biodegradable, whileedible films typically are. Thus, edible films provide an ideal solution for minimizingpackaging waste onboard ships during long voyages, during which maritime regulationsforbid throwing of any refuse overboard. While most synthetic commercial pack-ages possess average life times of 200 years in a marine environment, edible filmsdecompose readily providing an environmentally-friendly solution. Thermoformation is rarely used to create edible films, because most ediblecomponents cannot be molded at elevated temperatures without causing irreversible
10 A.E. Pavlath and W. Ortsstructural changes to the material. Hydroxypropylmethylcellulose and polylacticacid, two biodegradable thermoplastics, are rare exceptions. Any protein-contain-ing cysteine, such as gluten, hair or chicken feather, represents interesting thermo-plastic biomaterials, depending on level of cysteine content. When these materialsare treated with reducing agents, such as sodium sulfite, disulfide bonds can becleaved at 90–100°C. This bond cleavage lowers protein molecular weight allowingthe material to flow under slight pressure without decomposition. The reduceddisulfide bonds can then easily reform resulting in a strong, pliable material (Palloset al. 2006). Disulfide bonds in some of these proteins are also susceptible to reduc-tion in appropriate solvents with disulfide bridges reformed during solvent evapora-tion (Beckwith and Wall 1966; Okamoto 1978; Gennadios et al. 1993). As proteinmolecules undergo unfolding upon heating, new or non-native disulfide bonds mayalso form to enhance intermolecular cross-linking (Schofield et al. 1983). It wasreported that preparation of such films under acidic conditions provided better qual-ity films than under alkaline conditions (Gontard et al. 1992). Packaging issues are further complicated by strong demand for conveniencefoods. With fast moving lifestyles of today, consumers desire to spend less time inthe kitchen preparing meals. True, an apple can be eaten as a whole fruit but to useit in an apple pie or fruit cocktail, non-edible and/or unappetizing parts of the fruitneed to be removed. Consumers do not generally want to waste time with so-calledlight processing of foods (i.e., skinning and pitting fruits, slicing vegetables, skin-ning chickens, or just cleaning food surfaces). At the same time, consumers expectappetizing appearance and mouthwatering flavor. Preparation processes can be tedious and time-consuming. In small-scale com-mercial operations, such as cafeterias, automatic processing machines can now domuch of the light processing work, but cost of such machinery is still too high fortypical home kitchens. On the other hand, large-scale commercial processing in acentrally-located factory provides both economical and environmental benefits. Inthis setting, energy costs are minimized by scale of operation, disposal and/or uti-lization of waste is carried out efficiently at centralized locations, and volume (cost)benefits are achieved. However, removal of a food from its natural state and envi-ronment also accelerates undesirable changes that can lead to deterioration ofappearance, texture, and taste. We have all likely had the experience of biting intoan apple, setting it down for a few minutes, and then observing how quickly theexposed surface has turned brown. Extensive browning is apparent on apple sliceswithin 30 min, though surface discoloration begins to occur even after just a fewminutes (Bolin et al. 1964). What is the cause of these changes? Natural skin does not hermetically seal fruitfrom its surroundings. Rather it maintains optimal gas exchange equilibrium toprotect against weight loss, discoloration, loss of flavor and texture, among otherattributes. While such products are still subject to various aerobic and anaerobicrespiratory processes, these processes are maintained in proper balance by naturalskin. However, when fruit or vegetable is cut or even just mechanically damaged,cell wall membranes are disrupted, initiating a cascade of various enzymatic proc-esses. Even minimal mechanical damage incurred during handling and transport
1 Edible Films and Coatings 11can stimulate increased formation of ethylene causing physiological disordersand deterioration (i.e., increased cell permeability, loss of compartmentalization,and increased enzyme activities) (Hyodo et al. 1978). Change in the rate of migra-tion of oxygen, carbon dioxide, and ethylene can result in anaerobic fermentationand increased ripening. Even the way in which fruits are cut can make a difference.For example, formation of a white, unappetizing layer on carrot surfaces can beprevented by peeling them with a sharp blade (Bolin and Huxsoll 1991). Waterknife cutting can also decrease slicing-related issues (Becker and Gray 1992). Cutsurfaces increase chances for growth of microorganisms, causing multiple-foldincrease in respiration (Maxcy 1982). Increased respiration rates open up possibili-ties for cascading biochemical changes, such as degradation of carbohydrates,activation of dormant biological pathways, and facilitation of new, additional enzy-matic activities (Uritani and Asahi, 1980) which may induce production of unusualmetabolites (Haard and Cody 1978; Griesbach 1987). This circumstance occurswith polyphenol oxidase, an enzyme associated with catalysis of browning in freshfruits and vegetables, via rapid oxidation of o-quinones and polymerization of oxi-dized products to melanin (reddish-brown in color). Nature generally maintains optimum level of water activity (aw) in most fruit andvegetable products. Conversely, if addition of a protective edible film undulyrestricts water migration, resulting increase in water activity may cause undesirablechanges. The most frequent problem is growth of microorganisms, such as moldand yeast. Biochemical and enzymatic reactions may also be induced by increasingwater activity affecting taste, appearance and crispness. On the other hand, increas-ing water content can plasticize cellular structure, leading to loss of crispness insome products, as well as increased permeability. Table 1.2, summarizes effect of wateractivity (aw) levels as they relates to various undesirable changes associated withfresh fruits and vegetables. For non-enzymatic browning the rate increases untilwater activity reaches 0.6 and then declines (Rockland and Nishi 1980). Many food storage issues can be minimized by dehydration or lowering of moisturecontent of a food product. Unfortunately normal food dehydration procedures mayalso remove many of the volatile flavor components, which are not restored uponsimple rehydration. Interestingly if a food product is coated and then dehydratedosmotically at room temperature (the OSMEM process), only water is removedfrom the product. This process uses thicker films (1.5–2.0 mm thickness) which,if water soluble will dissolve during rehydration process (Camirand et al.1968, 1992). Table 1.2 Quality problems associated with changes in water activity Water activity Quality problem Reference 0.2 Non-enzymatic browning Labuza (1980) 0.4 Loss of crispness Katz and Labuza (1981) 0.6 Mold formation Troller (1980) 0.7 Yeast formation Troller (1980) 0.8 Bacterial growth Troller (1980)
12 A.E. Pavlath and W. Orts1.5 Migration ProcessesSeveral important parameters need to be defined to describe diffusion processes inrelation to films. Migration between two adjacent volumes separated by a layer ormembrane, occurs in three basic steps. In the first step, the diffusing moleculecomes in contact with surface of the layer or membrane, and is adsorbed onto it.In the second step, the molecule then diffuses through the thickness of the layer ormembrane. Lastly, once the diffusing molecule reaches the other side of the layeror membrane, it will desorb. Rate of adsorption and desorption is dependent on theaffinity between the diffusing molecule and membrance (film) components, espe-cially for water migration. Hydrophilic materials rapidly adsorb water but rate ofdesorption on the opposite side of the membrane will be controlled by partial pres-sure of water in that volume. Despite surface effects noted previously, the most dominant factor in molecularmigration is bulk effect – rate of diffusion of molecules while in the membrane orfilm. In an ideal case, amount of given material (Q) passing through a film can bedetermined by Fick’s law of diffusion (1.1): Q = PA∆pt / d, (1.1)where Q increases in direct proportion to film surface area (A), and decreases withits increasing thickness (d). Increasing partial pressure difference (∆p) of migratingmolecule between two sides of the membrane and time (t) also linearly affects totalamount of permeate. Permeability coefficient (P) is defined as the product of diffu-sion coefficient (D) and solubility (S) coefficients (P = DS). In an ideal case, P is aconstant determined by characteristics and structure of the film. When a given product is encased in protective film, the outer surface conditionsare already given. Ability to maintain low partial pressure difference (for a givencomponent) between the inside of the food product and surrounding externalenvironment is generally limited by economic factors (requires a controlled atmos-phere). When a coated product is stored openly in a relatively large area, amount ofgas in the surrounding external environment is orders of magnitude higher thanamount that is diffused out from the product. If the coated product is placed withinan enclosed system (e.g., in a bag or box), equilibrium can be created between theproduct and surrounding external environment, depending on head-space volumerelative to product weight. Film thickness is another important factor in the rate ofwater and gas transmission, changing not only appearance, but also taste of a foodproduct. While an increasing film thickness will slow down rate of diffusion, thereis also a practical limit to consider. If protective coating is edible and is to beingested together with the product, it must be applied in minimal fashion so that itwill not adversely modify original product taste. An exception can be made if aflavor change is considered to be acceptable or product is baked after coating (gen-erally nullifies most additive flavors) or dissolved before being consumed.Therefore, diffusion is mostly dependent on size of the permeate molecule andabundance of “holes” or “channels” in the film molecular structure, through which
1 Edible Films and Coatings 13the permeate can move. Solubility coefficient is influenced by the permeate’s easeof condensation and its affinity to components of the film. In the earlier form of Fick’s law (1.1), it was assumed that temperature is constant.Effect of temperature on permeability constant follows Arrhenius law (1.2): P = DS = D0S0 / Exp((EaD + ∆HS) / RT), (1.2)where Do and So are reference values for diffusivity and solubility, EaD is activationenergy of diffusion, and ∆Hs is enthalpy of sorption. Since EaD is positive, diffusionincreases with increasing temperature. However, since ∆Hs is negative for water,solubility decreases at the same time (Rogers 1985). In hydrophobic films, it wasfound that water vapor permeability increased with increasing temperature indicatingthat the controlling factor is diffusion (Hagenmaier and Shaw 1991). Some anomalywas observed with the water vapor transfer rate, which decreased with decreasingtemperature over range of 40–20°C, indicating greater absorption. However, watervapor transfer rate remained constant between 20 and 10°C, and permeabilityincreased at 4°C (Kester and Fennema 1989c). A film or coating must be fairly uniform and free of pinholes, microscopiccracks, and rough surfaces. Therefore preparation conditions (e.g., rate of evaporationand temperature) are important factors in film preparation. Even a small degree ofirregularity in a film can exponentially increase rate of diffusion, which is notaccounted for by Fick’s law. However, rate of diffusion is indirectly proportional tosquare root of molecular weight of the diffusing molecule; therefore it is a relativelysmaller problem for oil, flavor, and other similarly large molecules (relative towater, oxygen, carbon dioxide and ethylene). In the molecular weight range of themost important gases (oxygen, carbon dioxide, water and ethylene), diffusion ratedue to film irregularity is by orders of magnitudes faster than that which occursthrough the film structure itself. When one pinhole, representing only 0.008% offilm surface, was intentionally made, water vapor transmission increased 2.7 times(Kamper and Fennema 1984). It is evident that Fick’s law has additional limitations, especially for cases inwhich the film includes hydrophilic polymer components. Relative humidity andtemperature may alter considerably the diffusion and solubility coefficients of filmcomponents (Gontard et al. 1996). At high relative humidity, water uptake cansoften film structure through plasticization, making it easier for diffusing moleculesto pass through the film. Solubility coefficient of film components also increases(Cairns et al. 1974). Another anomaly, shown by various authors (Landman et al.1960; Biquet and Labuza 1988; Martin-Polo et al. 1992), concerns influence ofthickness of film on water vapor transfer. In very thin films of less than 60 mm,water vapor transfer decreases according to Fick’s Law; however, above this thicknesslevel, water vapor transfer rate remains almost constant. Value for permeability (P = DS) is essentially dictated by structure of the film.At the molecular level, diffusing molecules migrate through polymer chains andside chains, which are held in place by hydrogen bonds and van der Waals forces. Sidechains can have either beneficial or detrimental influence on permeation coefficient
14 A.E. Pavlath and W. Ortsof film. In one sense, a side chain can decrease available intramolecular spacingwithin the film, which allows migration of permeates, thus making diffusion moredifficult. On the other hand, a side chain may decrease degree of crystallinity withina film by introducing more structural irregularities. Crystallinity rigidifies polymerchains, which hinders molecular migration through a film by limiting molecularmobility of film components. Thus, crystalline packing arrangement of polymersand their orientation within a film relative to flow direction especially influencemigration of molecules through a film (Fox 1958). These elements regulate “freespace” within the film available for migration, and limit molecular movement fromcavity to cavity. In certain cases, protection against migration can be created at surface of a foodproduct without addition of polymeric material. If the surface already has a polymericstructure, these surface polymers can be cross-linked, whereby the product itselfprovides a new protective layer. For example, this strategy was employed quitesuccessfully for apple slices through creation of an ionomer surface using calciumascorbate dips. In this scenario, calcium ions interacted with surface pectin molecules,closing the surface, while also incorporating ascorbic acid as an antioxidant (Pavlathet al. 1996; Chen et al. 1999). Calcium formed salt bridges between the carboxylategroups of pectin polymer chains creating cross-links that promoted a more rigidstructure (the so-called egg-box model) and decreased permeability at food surface(Grant et al. 1973; Wong et al. 1996). Such treated samples did not brown or losewater over a 2 week period (Chen et al. 1999). Similar protective layers can be formedon potato strips through treatment with calcium acetate and an oxidation inhibitor.Cross-linking at surface of potato strips prevented both oxidation and discoloration,and provided for higher quality French fries upon frying (Mazza and Qi 1991). There are various synthetic films and packaging materials available for minimizingmigration, but with few exceptions, these materials are not edible and cannot beconsumed together with food. Thus, they must be removed before consumption.Economics is a primary driver in the choice between use of synthetic and ediblefilms. Edible films are relatively more expensive, with their commercial utilizationbeing limited to convenience food items (e.g., snack foods), where consumers arewilling to may pay more. Synthetic, non-edible materials are generally better suitedfor creating modified packaging environments, creating sealed, box-like enclosuresthat may be supplemented with special atmosphere. Edible film materials generallydecompose more rapidly or lose their quality and integrity faster (oxidation,dissolution, etc.) than those of synthetic origin. On the other hand, synthetic packagingmaterials have to be removed before eating, leading to challenges in relation todisposal and environment. Many packaging materials end up as litter. Edible encasing materials must meet standards first, by ensuring that they arelabeled GRAS for consumption by the Food and Drug Administration. Secondly,consumers are very selective and finicky in relation to what they choose to eat.Unless different a flavor or texture is intended to enhance consumer acceptance, thefilm or encasing should not adversely change taste and flavor of the food product,and should also be invisible and undetectable to taste. What materials can then beused to fulfill these difficult requirements?
1 Edible Films and Coatings 151.6 Possible Components of Edible FilmsThe main components of our everyday foods (e.g., proteins, carbohydrates andlipids) can fulfill requirements for preparation of edible films. As a general rule,fats are used to reduce water transmission; polysaccharides are used to controloxygen and other gas transmission, while protein films provide mechanical stability.These materials can be utilized individually or as mixed composite blends to formfilms provided that they do not adversely alter food flavor. A major objective inpreparing films for many foods (e.g., fresh fruit and vegetables) is to ensure that thegenerated films afford physical and chemical properties necessary to maintaintransmission of various gases and liquids at the same rates as they occur within theirnative systems. Chemical structures of the three major components used to preparefilms differ widely, and therefore attributes that each component contributes tooverall film properties are different too. The following is a short informativesummary of these concepts. Films from various sources of protein, such as corn, milk, soy, wheat and whey,have been used for years, their major advantage being their physical stability. Itshould be mentioned, however, that most of these protein sources are in factmixtures of various proteins comprising a range of molecular weights. If they areused in solution rather than in emulsion, the solution will contain different proteinfractions than the emulsion (unless all protein fractions are equally dissolved).Lower molecular weight components are generally more easily solubilized, thoughthey exhibit higher permeabilities than higher molecular weight entities withinfilms. While this limitation can be counteracted with cross-linking, edibility andmouthfeel of a film can be jeopardized by such treatment. When selecting proteinfor use in an edible film, consideration should extend beyond just protein functiona-lity and GRAS status. It is important to recognize that a given segment of population isallergic to certain proteins, specifically to those of wheat. Consequently, collagencan be extruded to desired shapes such as a casing for sausage links. Collagenreplaced traditional casing material (derived from animal intestines) because of itsease of manufacture and scale-up. In general, value of proteins as moisture barriersis low, and they also do not adequately control transfer of oxygen, carbon dioxideand other gases that are important to stability of various foods. Their major advantageis their structural stability, which makes it possible to hold a required form (e.g.,sausage casing). Cross-linking can also occur in proteins where the isoelectric pointis dependent on interaction of the amino and carboxylic groups of the protein. Thusdepending on protein composition, permeability can also be altered. It was reportedthat depending on the pH of solution from which the film was cast, properties (e.g.,color, texture, tensile strength) were markedly different (Gennadios et al. 1993;Gontard et al. 1992.) Water adsorption occurs readily at surface of polysaccharide films (e.g., those ofalginate, carrageenan, cellulose and its derivatives, dextrin, pectin and starch),because of the hydrophilic nature of most polysaccharides. Some polysaccharidessuch as cellulose derivatives, have lower water transmission than average polysac-charides, though they are still less effective than wax. The primary advantages of
16 A.E. Pavlath and W. Ortspolysaccharide films are their structural stability and ability to slow down oxygentransmission. As a general rule films which do not provide protection against watertransmission often have desirable properties in preventing oxygen transmission andvice versa (Banker 1966). Resistance to gas transmission can be so effective forpolysaccharide films that it can be a challenge to manipulate. For example, perme-ability for oxygen in high amylose starch films was found to be virtually zerodespite addition of plasticizers that were known to increase gas permeability (Market al. 1966). Therefore, in spite of their shortcomings with regard to water permeability,polysaccharides can be used to protect food from oxidation. Alginate coating canprevent lipid oxidation and stop rancidity (Mate et al. 1996). Another interestingrole of polysaccharide films is to act as “a sacrificing agent” instead of as a barrier.Since most polysaccharides and other hydrophilic materials provide low protectionagainst water transmission (i.e., they are highly hygroscopic), they may be appliedas relatively thick films at food surfaces to intentionally absorb water and providetemporary protection against further moisture loss (similar to how a surfer’s wetsuit takes in water, but provides protection). Carrageenan, a sulfated polysaccharideof d-galactopyranosyl units was found to form a structured gel, which acted assacrificing agent (Glicksman 1982, 1983). Alginate gels were also reported topossess this function (Shaw et al. 1980). Thus the coated product itself does notlose significant moisture until the sacrificing agent or film itself is dehydrated. If asurfactant is added to the coating, surface water activity can be altered withoutaltering water content inside. Waxes and fats are the oldest known edible film components. While most waxesare of natural origin, synthetic acetylated monoglycerides have similar characteris-tics and have been used with the blessing of the FDA in edible films for meat, fishand poultry. Originally, lipid coatings were applied by simply pouring molten par-affin or wax over citrus fruits. This process slowly gave way to adding a thin shinylayer by applying small amount of various wax through dipping or spraying. The hydro-phobic fruit surface, which also protects against abrasion during transportation,adds an aesthetic appearance. At the same time, thin wax coatings still allow somebreathing to occur. They are excellent barriers to water transmission, while stillslowing or altogether preventing other gas migration. Wax will affect oxygen andcarbon dioxide transmission, and thus, can result in unwanted physiological proc-esses, such as anaerobic respiration. This process in turn, will diminish quality ofthe product, resulting in softening of tissue structure, alteration of flavor, delay ofripening, and promotion of microbiological reactions (Eaks et al. 1960). In case ofhorticultural products with minimal respiration such as root vegetables, thick layersof wax are less harmful and can be used (Hardenburg 1967). It was reported thatwater vapor transmission through fatty acid monolayers decreased logarithmicallyas length of the fatty acid hydrocarbon chain increased, though this effect was notindefinite (LaMer et al. 1964). However, there is disagreement about the most effi-cient chain length. According to one group, the most efficient chain length isC12–C14 (Wong et al. 1992; Pavlath et al. 1993; Talbot 1994), while another groupfound that chain lengths of C16–C18 (Hagenmaier and Shaw 1990; Koelsch andLabuza 1992; McHugh and Krochta 1994; Park et al. 1994) gave best results.
1 Edible Films and Coatings 17However, introduction of double bonds into the chain increases water vapor trans-mission 80-fold (Roth and Loncin 1985; Hagenmaier and Baker 1997), which is attrib-uted to loss of crystallinity. Application of edible films is especially difficult when applying lipophilic materialto wet surfaces, such as cut fruits and vegetables. Direct application of any lipid toa hydrophilic or wet surface results in weak adhesion at the film-food interface.Dual-coating is one possible solution to this problem, as it provides protectionagainst more than one permeate through use of different laminate layers. For example,the wet cut surface of an apple was first coated with alginate cross-linked viacalcium ions. This initial coating provided a more appropriate foundation for sub-sequent hydrophobic coating with acetylated monoglyceride (Wong et al. 1994a).Unfortunately, two coating processes increase product cost and may also reducecommercial viability. Emulsions represent another approach to apply film, althoughit is still not clear whether emulsion-cast films are better than dual-coatings. Twoconflicting reports, each claiming multiple-fold advantages cite that emulsions aremuch better than dual coatings (Kamper and Fennema 1984) and vice versa(Martin-Polo et al. 1992, Debeaufort et al. 1993). A more recent study forwards thegeneral belief that multilayer films provide better protection than single layer filmsfrom emulsions (Debeaufort et al. 1998). From an economic point of view, emulsion-cast films have commercial appealfor several reasons.Use of a mixture of fat and carbohydrate components emulsifiedby protein, allows for direct adhesion of hydrophilic carbohydrate material at foodsurface and formation of a hydrophobic layer or coating at the external food surface.An aqueous emulsion containing 10% casein, 1% alginic acid and 15% of acetylatedmonoglyceride by weight resulted in a coating that reduced moisture losses forapple slices by 75% over a 3-day period – relative to uncoated slices. Effectivenessof this coating was unexpected, because alginic acid is hydrophilic and moisturelosses should have been less if it were left out from the mixture. However, whenthe coating mixture did not contain either alginic acid or casein, there was onlyminimal decrease in water loss. It can be implied that casein provided a bridgebetween hydrophilic alginic acid and hydrophobic lipid, allowing adhesion to thehydrophilic cut surface (Pavlath et al. 1993; Wong et al. 1994b). Characteristics of emulsion-derived films however, are sensitive to quality ofemulsion – generally requiring droplet sizes of <0.5 mm (Platenius 1939). In fact,droplet size should be in the 10–100 nm range to obtain an optimal thermodynamicallystable microemulsion (Das and Kinsellar 1990). However, there are several drawbacksto emulsion-type coatings. These coatings can be wet and difficult to handle andmay function more as a sacrificial layer as opposed to a true moisture barrier.Emulsion stability is also sensitive to temperature and its efficiency can be affectedby quality of emulsifier used. Such variations represent a handicap to commercialapplication. One particularly interesting breakthrough that eliminates the need toemulsify polysaccharide-fat coating mixtures is use of amphiphilic compounds,molecules containing both hydrophilic and lipophilic moieties. One such exampleis sucrose fatty acid ester, which was efficient for retaining crispiness of a snackfood (Kester et al. 1990). Casein treated with acyl esters of N-Hydroxysuccinimide
18 A.E. Pavlath and W. Ortsyielded fatty acid acylated casein with hydrophobic characteristics (Nippon 1984).Another possibility is chitosan fatty acid salts, where length of the fatty acid chainplays an important role in rate of water vapor transmission. Microstructure of thesesalts changes dramatically though, when lauric acid is incorporated into the chi-tosan film instead of shorter or longer fatty acids. Chitosan laureate had the bestmoisture barrier properties in comparison to both shorter and longer fatty acid chaincomplexes (Wong et al. 1992). The product is a composite film in which fatty acidmolecules are distributed within the chitosan matrix, suggesting the importance of themorphological arrangement of the lipid within the chitosan matrix (Pavlath et al.1993). This arrangement would have an added advantage, since both chitosan andlauric acid alone are antimicrobial agents (Kabara and Ecklund 1991; Darmadji andIzomimoto 1994). Unfortunately, chitosan is still not fully accepted in the UnitedStates for food applications, even though it is approved for use in Canada and Japan.1.7 ConclusionsVarious reviews have been written about properties and potential uses of ediblefilms (Kester and Fennema 1986; Guilbert 1986; Krochta 1992; Krochta et al.1994; Morillon et al. 2002). An extensive review on antimicrobial films was alsopublished (Cagri et al. 2004), and a special review is available for applications onvarious types of meat products (Gennadios et al. 1997). Much more research isneeded as there is no universal edible film that is applicable for every problem.Obviously, specific barrier requirements and food product specifications will determinethe type of layer that is best for a given situation. Products with high moisture con-tents need fatty layers to prevent loss of water. To prevent possible discoloration,an oxygen barrier component is needed. Unsaturated fats which are easily oxidizedrequire similar protective layers. As stated above, water and oxygen permeabilitygenerally are inversely related; thus, many films will need to be composite materialswith multiple properties (not unlike Mother Nature’s own protection). Ideal ediblefilm should have the following characteristics:• Contain no toxic, allergic and non-digestible components• Provide structural stability and prevent mechanical damage during transportation, handling, and display• Have good adhesion to surface of food to be protected providing uniform coverage• Control water migration both in and out of protected food to maintain desired moisture content• Provide semi-permeability to maintain internal equilibrium of gases involved in aerobic and anaerobic respiration, thus retarding senescence• Prevent loss or uptake of components that stabilize aroma, flavor, nutritional and organoleptic characteristics necessary for consumer acceptance while not adversely altering the taste or appearance• Provide biochemical and microbial surface stability while protecting against contamination, pest infestation, microbe proliferation, and other types of decay
1 Edible Films and Coatings 19• Maintain or enhance aesthetics and sensory attributes (appearance, taste etc.) of product• Serve as carrier for desirable additives such as flavor, fragrance, coloring, nutrients, and vitamins. Incorporation of antioxidants and antimicrobial agents can be limited to the surface through use of edible films, thus minimizing cost and intrusive taste.• Last but not least – be easily manufactured and economically viableReferencesAllen L, Nelson AI, Steinberg MP, McGill JN (1963) Edible carbohydrate food coatings II. Evaluation of fresh meat products. Food Technol. 17: 1442–1448Banker GS (1966) Film coating theory and practice. J. Pharm. Sci. 55: 81–89Becker R, Gray GM (1992) Evaluation of a water jet cutting system for slicing potatoes. J. Food Sci. 57(1): 132–137Beckwith AC, Wall JS (1966) Reduction and reoxidation of wheat glutenin. Biochim. Biophys. Acta 130: 155–162Biquet B, Guilbert S (1986) Relative diffusivitives of water in model intermediate moisture foods. Lebensm. Wis. Technol. Food Sci. Technol. 19: 208–214Biquet B, Labuza TP (1988) Evaluation of moisture permeability characteristics of chocolate films as an edible moisture barrier. J. Food Sci. 53: 989–998Bolin HR, Huxsoll CC (1991) Control of minimally processed carrot (Daucus carota) Surface discoloration caused by abrasion peeling. J. Food Sci. 56: 416–418Bolin HR, Nury FS, Finkle BJ (1964) An improved process for preservation of fresh peeled apples. Bakers Dig. 38(3): 46–48Cagri A, Ustonol Z Ryser ET (2004) Review: Antimicrobial edible films and coatings. J. Food Prot. 67(4): 833–848Cairns JA, Owing CR, Paine FA (1974) Packaging for climate protection. The Institute of Packaging, Newnes-Butterworth, London, EnglandCamirand WM, Forrey RR, Popper K, Boyle FP, Stanley WL (1968) Dehydration of membrane coated foods by osmosis. J. Sci. Food Agric. 19: 472–474Camirand WM, Krochta JM, Pavlath AE, Cole ME (1992) Properties of some edible carbohydrate polymer coatings for potential use in osmotic dehydration. Carbohydr polym. 13: 39–49Chen C, Trezza TA, Wong DWS, Camirand WM, Pavlath AE (1999) Methods of preserving fresh fruits and produce thereof. U.S. Patent. 5, 939, 117Contreras-Medellin R, Labuza TP (1981) Prediction of moisture protection requirements for foods. Cereal Food World. 26(7): 335–340Cosler HB (1957) Methods of producing zein coated confectionery. U.S. Patent, 2, 791, 509Darmadji P, Izumimoto (1994) Effect of chitosan in meat preservation. Meat Sci. 38: 243–254Das KP, Kinsella JE (1990) Stability of food emulsions: Physicochemical role of protein and non- protein emulsifiers. Adv. Food Nutr. Res. 34: 81–201Davies E (1987) Plant responses to wounding. In the Biochemistry of Plants Vol. 12, D. D. Davies (ed.), P.K. Stumpf. and E.E. Conn (eds-in-chief) Academic, New York, NY, Chapter 7, pp 243–264Debeaufort F, Martin-Polo M, Voilley A (1993) Polarity, homogeneity and structure affect water vapor permeability of model edible films. J. Food Sci. 58: 426–429, 434Debeaufort F, Quezada-Gallo JA, Voilley A (1998) Edible films and coatings: tomorrow’s packag- ing: A review. Crit. Rev. Food Sci. Nutr. 38: 299–313Delong CF, Shepherd TH (1972) Produce coating. U.S. Patent 3, 669, 691
20 A.E. Pavlath and W. OrtsEaks IL (1980) Effect of chilling on respirations and volatiles of California lemon fruit. J. Amer. Soc. Hort. Sci. 105: 865–869Eaks IL, Ludi WA (1960) Effects of temperature, washing and waxing on the composition of internal atmosphere of orange fruits. Proc. Am. Soc. Hortic. Sci. 76: 220–228Feeney RD, Hararalampu SG, Gross A (1992) Method of collating food with edible oil barrier film and product thereof. U.S. Patent 5, 126, 152Fennema OR (1993) Frozen foods: challenges of the future. Food Aust. 45(8): 374–380Feuge RO, Vicknair EJ, Lovegren NV (1953) Modification of vegetable oils XIII. Some additional properties of acetostearin products. JAOCS. 30: 283–290Fox RC (1958) The relationship of wax crystal structure to water vapor transmission rate of wax films. TAPPI. 41(6): 283–289Gennadios A Weller CL, Testin RF (1993) Modification of physical and barrier properties of edible wheat gluten-based films. Cereal Chem. 70(4): 426–429Gennadios A, Hanna MA, Kurth LB (1997) Application of edible coatings on meats, poultry and seafoods: A review. Lebensm. Wiss. Technol. 30: 337–350Glicksman M (1982) Functional properties. In Food Hydrocolloids, M. Glicksman, (ed.) CRC, Boca Raton, FL Vol. 1 p. 47Glicksman M (1983) Red seaweed extracts. In Food Hydrocolloids, M. Glicksman, (ed.) CRC, Boca Raton, FL Vol. 2 p. 73Gontard N, Guilbert S (1994) Biopackaging technology and properties of edible and/or biodegrad- able material of agricultural origin. In Food packaging and preservations. M. Mathlouthi, (ed.) Blackie Academic and Professional, Glasgow, pp 159–181Gontard N, Guilbert S, Cuq JL (1992) Edible wheat gluten films: Influence of the main process variables on film properties using response surface methodology, J. Food Sci. 57: 190–199Gontard N, Thibault R, Cuq B, Guilbert S (1996) Influence of relative humidity and film composi- tion on oxygen and carbon dioxide permeabilities of edible films. J. Agric. Food Chem. 44(4): 1064–1068Grant GT, Morris ER, Rees DA, Smith PJC, Thom D (1973) Biological interactions between polysaccharides and divalent cations. The eggbox model. FEBS Lett. 32: 195–198Greener I (1992) Physical Properties of Edible Films and Their Components. Ph.D. dissertation, University of WisconsinGriesbach H (1987) New insights into ecological role of secondary plant metabolites. Comments Agric. Food Chem. 1: 27–45Guilbert S (1986) Technology and application of edible protective films, In Food Packaging and Preservation: Theory and Practice, M. Mathlouthi, (ed.) Elsevier Applied Science Publishing Co., London, UK, pp 371–399Guilbert S (1988) Use of superficial edible layer to protect intermediate moisture foods: Application to the protection of tropical fruits dehydrated by osmosis. In Food Preservation by Moisture Control, C.C. Seaow, (ed.) Elsevier Applied Science Publishers Ltd. Essex, England, pp 199–219Haard NF, Cody M (1978) Stress metabolites in postharvest fruits and vegetables role of ethylene. In Postharvest Biology and Biotechnology, H.O. Huttin and M. Milner (eds.) Food and Nutrition Press Inc, Westport, CT.Hagenmaier RD, Baker RA (1997) Edible coatings from morpholine-free wax microemulsions. J. Agric. Food Chem. 45: 349–352Hagenmaier RD, Shaw PE (1990) Moisture permeability of edible films made with fatty acid and (hydroxypropyl) methylcellulose. J. Agric. Food Chem. 38: 1799–1803Hagenmaier RD, Shaw PE (1991) Permeability of coatings made with emulsified polyethylene wax. J. Agric. Food Chem. 39: 1705–1708Hallman GJ, Nisperos-Carriedo MO, Baldwin EA, Campbell CA (1994) Mortality of Carribean fruit fly (Diptera: Tephritidae) immatures in coated fruits. J. Econ. Entomol. 87: 752–757Hardenburg RE (1967) Wax related coatings for horticultural products. A bibliography. Agricultural Research Service Bulletin 51–15, United States Department of Agriculture, Washington, DCHavard C, Harmony MX (1869) Improved process for preserving meat, fowls, fish etc. U.S. Patent 90, 944
1 Edible Films and Coatings 21Hershko V, Klein E, Nuvissovitch A (1996) Relationships between edible coating and garlic skin J. Food Sci. 61: 769–777Hyodo H, Kuroda H, Yang SF (1978) Induction of phenylalanine ammonia-lyase and increase in phenolics in lettuce leaves in relation to the development of russet spotting caused by ethylene. Plant Physiol. 62: 31–35Ismail M (1989) Cold treatment: a successful quarantine method for Florida grapefruit shipped to Japan. Packinghouse Newsletter No. 158: 1–2Kabara JJ, Ecklund T (1991) Organic acids and esters. In Food Preservatives, N.J. Russell and G.W. Gould (eds.) Blackie and Son, Glasgow, pp 21Kader AA (1986) Biochemical and physiological basis for effects of controlled and modified atmospheres on fruits and vegetable. Food Technol. 40: 99–104Kamper SL, Fennema OR (1984) Water vapor permeability of an edible, fatty acid, bilayer film. J. Food Sci. 49: 1482–1485Kanig JL, Goodman H (1962) Evaluative procedures for film-forming materials used in pharma- ceutical applications. J. Pharm. Sci. 51(1): 77–83Katz EE, Labuza TP (1981) Effect of water activity on the sensory crispness and mechanical deformation of snack food products. J. Food Sci. 46: 403Kester JJ, Fennema OR (1986) Edible films and coatings: A review. Food Technol. 39: 47Kester JJ, Fennema OR (1989a) The influence of polymorphic form on oxygen and water vapor transmission through lipid films. JAOCS. 66(8): 1147–1153Kester JJ, Fennema OR (1989b) Tempering influence on oxygen nd water vapor transmission through a stearyl alcohol film. JAOCS. 66(8): 1154–1157Kester JJ, Fenema OR (1989c) An edible film of lipids and cellulose ether: barrier properties to moisture transmission and structural evaluation. J Food Sci. 54: 1383–1389Kester JJ, Bernhardy JJ, Elsen J, Letton J, Fox M (1990) Polyol polyesters as protective moisture barrier for foods. U.S. Patent 4, 960, 600Koelsch CM, Labuza TP (1992) Functional, physiological and morphological properties of methyl cellulose and fatty acid-based edible barriers. Lebensm Wiss Technol. 25: 404–411Krochta JM (1992) Control of mass transfer in foods with edible coatings and films. In Advances in Food Engineering, W.E. Speiss and H. Schubert (eds.) Elsevier, Essex, EnglandKrochta JM, Hudson JS, Camirand WM, Pavlath AE (1988) Edible films for light processed fruits and vegetables, Paper Presented at International Winter Meeting of the American Society of Agricultural Engineers, Chicago, ILKrochta JM, Baldwin EA, Nisperos-Carriedo MO (1994) Edible Coatings and Films to Improve Food Quality, Technomic Publ. Co., Lancaster, PA, pp 1–379Labuza TP (1980) The effect of water activity on reaction kinetics of food deterioration. Food Technol. 34(4): 36–40Labuza TP (1984) Moisture Sorption: Practical Aspects of Isotherm Measurement and Use American Association of Cereal Chemists, St. Paul, MNLaMer VK, Healy TW, Aylmore LAG (1964) The transport of water through monolayers of long- chain n-paraffinic alcohols. J. Coll. Sci. 19: 673Landman W, Lovegren NV, Feuge RD (1960) Permeability of some fat products moisture. JAOCS. 37: 1–4Lazarus CR, West RL, Oblinger JJ, Palmer AZ (1976) Evaluation of calcium alginate coating and protective plastic wrapping for the control of lamb carcass shrinkage. J. Food Sci. 41: 639–642Mark AM, Roth WB, Mehltretter CL, Rist CE (1966) Oxygen permeability of amylomaize starch films. Food Technol. 20: 75Mate JI, Saltweil ME, Krochta JM (1996) Peanut and walnut rancidity: effects of oxygen concen- tration and relative humidity J. Food Sci. 61: 465–472Martin-Polo M, Mauguin C, Voilley A (1992) Hydrophobic films and their efficiency against moisture transfer. I. Influence of the film preparation technique. J. Agric. Food Chem. 40: 407–412Maxcy RB (1982) Fate of microbial contaminants in lettuce juice. J. Food Protection. 45: 335–339
22 A.E. Pavlath and W. OrtsMazza G, Qi H (1991) Control after-cooking darkening in potatoes with edible film-forming products and calcium chloride. J. Agric. Food Chem. 39(10): 2163–2166McHugh TH, Krochta J (1994) Milk-protein-based edible films and coatings. Food Technol. 48(1): 97–103Meyers MA (1994) Use of edible films to prolong chewing gum shelf-life. U.S. Patent 5, 286, 502Morillon V, Debeaufort F, Blond G, Capelle M, Voilley A (2002) Factors affecting the moisture permeability of lipid-based edible films: A review. Critical Reviews in Food Science and Nutrition. 42(1): 67–89Murray DG, Luft L (1973) Low D.E. Corn starch hydrolysates. Food Technol. 27(3): 32–39Nelson K, Fennema OR (1991) Methylcellulose films to prevent lipid migration in confectionery products. J. Food Sci. 56(2): 504–508Nippon Shinyuku Co. Ltd. (1984) Fatty acid acylated casein. Japan Kokai Tokyo Koho, Japan Patent 59, 155, 396Okamoto S (1978) Factors affecting protein film formation. Cereal Foods World. 23: 256–262Pallos FM, Robertson GH, Pavlath AE, Orts WJ (2006) Thermoformed wheat gluten biopolymers. J. Agric. Food Chem. 54: 349–352Park JW, Testin RF, Park HJ, Vergano PJ, Weller CI (1994) Fatty acid concentration effect on tensile strength, elongation and water vapor permeability of laminated edible films. J. Food Sci. 59: 916–919Paulinka F (1986) Quality consideration in the selection of confectionery fats. The Manufacturing Confectionerie (May) 75–81Pavlath AE, Wong DSW, Kumosinski TF (1993) New Coatings for cut fruits and vegetables. CHEMTECH. 23(2): 36–40Pavlath AE, Wong DSW, Hudson JS, Robertson GH (1996) Edible films for the extension of shelf life of lightly processed agricultural products. ACS Symposium, Series No. 647. G. Fuller, T.A. McKeon and D.D. Bills (eds.) Chapter 8, pp 107–110Pavlath AE, Gossett C, Camirand W, Robertson GH (1999a) Ionomeric films of alginic acid, J. Food Sci. 64(1): 61–63Pavlath AE, Voisin A, Robertson GH (1999b) Pectin-based biodegradable water insoluble films. Macromol. Symp. 140: 106–113Pickard JF, Rees JE, Elworthy PH (1972) Water vapour permeability of pored and sprayed polymer films. J. Pharm. Pharmac. 24(Suppl): 39PPlatenius H (1939) Wax emulsions for vegetables. Cornell Univ. Agric. Exp. Sta. Bull. 723: 43Polanski S (1993) Frying food with reduced frying medium uptake – by cooking food to remove water applying coating of swollen dispersion containing natural edible polymer, drying and frying. U.S. Patent 5, 232, 721Reading S, Spring M (1984) The effects of binder film characteristics on granule and tablet prop- erties. J. Pharm. Pharmacol. 36: 421–426Rockland LB, Nishi SK (1980) Influence of water activity on food product quality and stability. Food Technol. 34(4): 42Rogers CE (1985) Permeation of gases and vapors in polymers. In Polymer Permeability, J. Comyn (ed.) Elsevier Applied Science Publisher, New York, NY, pp 11–73Roth T, Loncin M (1984) Superficial activity of water. In Engineering and Food. Vol. 1. B.M. McKenna (ed.) Elsevier Applied sciences Publishers, London, England, pp 433Roth T, Loncin M (1985) Fundamentals of diffusion of water and rate of approach of equilibrium Aw. In Properties of Water in Foods in Relation to Quality and Stability, D. Simatos, JL. Multon (eds.) Martinus Nijhoff Publishing, Dordrecht, The Netherlands, pp. 331Schofield JD, Bottomley RC, Timms MF, Booth MR (1983) The effect of heat on wheat gluten and the involvement of sulphhydryl-disulphide interchange reactions, J. Cereal Sci. 1: 241–253Shaw CP, Secrist JL, Tuomy JM (1980) Method of extending the storage life in the frozen state of precooked foods and products thereof. U.S. Patent 4, 196, 219
1 Edible Films and Coatings 23Shewfelt RL (1987) Quality of minimally processed fruits and vegetables. J. Food Quality. 10: 143–156Talbot G (1994) Minimisation of moisture migration in food systems, Reprint from F.I.E. ParisTomasul PM, Craig JC Jr., Boswell T (1997) A continuous process for casein production using high-pressure carbon dioxide. J. Food Eng. 33(3): 405–419Troller JA (1980) Influences of water activity on microorganisms in foods. Food Technol. 34 (5): 7Uritani I, Asahi T (1980) Respiration and related metabolic activity in wounded and infected tis- sues. In Biochemistry of Plants, Vol. 2. PK Stumpf and EE Conn (eds.) Academic, Orlando, FL, Chapter 11, pp 463–485Williams SK, Oblinger JL, West RL (1978) Evaluation of calcium alginate film for use on beef cuts. J. Food Sci. 43: 292–301Wong DWS, Gastineau FA,Gregorski KS, Tillin SJ, Pavlath AE (1992) Chitosan-lipid films: Microstructure and surface energy. J. Agric. Food Chem. 40(4): 540–544Wong DWS, Camirand WM, Pavlath AE (1994a) Development of edible coatings for minimally processed fruits and vegetables. In Edible Coatings and films to improve Food Quality, Lancaster, PA., Technomic Publ. Co. Chapter 3, 65–88Wong DWS, Tillin SJ, Hudson JS, Pavlath AE (1994b) Gas exchange in cut apples with bilayer coatings. J. Agric. Food Chem. 42(10): 2278–2285Wong DWS, Gregorski KS, Hudson JS, Pavlath AE (1996) Calcium alginate films: thermal prop- erties and permeability to sorbate and ascorbate. J. Food Sci. 61(2): 337–341
26 K. Dangaran et al. The large demand for resources created by WWI and WWII was a catalyst forscientific and technological improvements to protein-based polymers. Additionally,the idea of developing new, non-food uses from agricultural crops received widesupport and distinction in the form of the Chemurgy Movement (Finlay 2004). In the1920s and 1930s, the National Farm Chemurgic Council was formed, promotingthe move to generate new products from agricultural commodities that were usefulto industry. For a time, this original “green” movement had a growing influencethroughout the country. Supporters included important figures like William Hale, aprominent figure within Dow Chemical, and Henry Ford, a leader in the automotiveindustry, who promoted and used biobased plastics, textiles and fuels in his auto-mobiles. In response to the demand, the USDA established four regional researchcenters, devoted to creating value-added products, developing renewable biobasedmaterials, and discovering new routes for industrial utilization of agricultural materials(Kelley 1993). However, production and use of agricultural-based polymeric materialsdeclined after WWII due to the development of petroleum-based products, which werecheaper, easier to produce, and generally superior to their agricultural counterparts. Still today, the four USDA research centers remain mainstays of the AgriculturalResearch Service (ARS), the research arm of the USDA. While the mission ofARS has expanded to address additional challenges currently facing agriculture, asignificant portion of the mission is dedicated to research on value-added foodsand bio-based products. Today, there is renewed interest in biobased materials;consumers demand environmentally-friendly products that lower dependence on oiland other non-renewable resources (Comstock et al. 2004). As evidenced byPresidential Initiatives 13101 and 13134, which call for increased use and developmentof agricultural-based products, biobased product research has become a priority forgovernment, academic, and industrial research institutions. With their proven track record for function and commercialization, packagingapplications are well suited to be made from biobased materials and to incorporateprotein-based materials. Food packaging innovation, including films and coatings,is driven by (1) distribution needs, especially as globalization increases the distance,products are shipped; (2) consumer demands for convenient packaging, includingeasily recyclable packaging; and (3) environmental legislation. During the last 5–10years, especially in the UK and Japan, government legislation has accelerated thedevelopment of environmentally-friendly packaging (Sonneveld 2000; Comstocket al. 2004). Moreover, increasing energy costs also raise the prices of conventionalpackaging materials. In 2005–2006, food packagers in Europe experienced a30–80% increase in the cost of packaging materials, mostly due to the escalatingcost of petroleum (Anonymous 2006). The inherent properties of proteins make them excellent starting materials forfilms and coatings. The distribution of charged, polar and non-polar amino acids(Fig. 2.1a–c) along the protein chain creates chemical potential. Figure 2.2 showsa representation of beta-lactoglobulin, the major protein found in whey. The shadingillustrates the domains of polar and non-polar areas along the protein chain.The resulting interactive forces produce a cohesive protein film matrix. Films formand are stabilized through electrostatic interactions, hydrogen bonding, van derWaals forces, covalent bonding, and disulfide bridges (Krochta et al. 1994). Protein
2 Structure and Function of Protein-Based Edible Films and Coatings 27Fig. 2.1 (a) Non-polar amino acids. (b) Polar amino acids. (c) Charged amino acidsfilm-forming capabilities are best demonstrated in emulsified systems in whichamphipathic proteins form films at air–water or water–oil interfaces. There are alsosecondary benefits for using proteins to form films and coatings. Proteins have multiplesites for chemical interaction as a function of their diverse amino acid functionalgroups, which can allow for property improvement and tailoring. Chemical changes canimprove the stability of films and coatings. Cross-linked protein films are often morestable than their polysaccharide-based counterparts and have a longer lifetime (Baroneand Schmidt 2006). Figure 2.3 depicts the enzymatic cross-linking of proteins.
Fig. 2.1 (continued)
2 Structure and Function of Protein-Based Edible Films and Coatings 29Fig. 2.2 Examples of polar (light gray) and non-polar (dark gray) domains in proteins asdepicted by the beta-lactoglobulin moleculeFig. 2.3 Cross-linking reaction of protein chains catalyzed by the enzyme transglutaminase
30 K. Dangaran et al. Protein-based films and coatings are also biodegradable and compostable. As theydegrade, they provide a source of nitrogen, which contributes a fertilizer benefit notavailable with other non-protein-based films and coatings. Finally, there is emergingevidence that the bioactive peptides produced upon digestion of proteins (dairy sourcesin particular) have antihypertensive and radical scavenging health benefits (Aimutis2004; FitzGerald et al. 2004). This chapter will cover the most commonly studied proteins used for research infilms and coatings. Film formation, properties, and future trends will be discussed.2.2 CompositionFilms and coatings may be made from proteins of both animal and plant origin.Protein-based films and coatings are prepared from solutions comprised of threemain components: protein, plasticizer and solvent. The properties of the final filmare affected by the intrinsic properties of the film or coating components and extrinsicprocessing factors (Panyam and Kilara 1996). Intrinsic properties of proteins includeamino acid composition, crystallinity (of the protein and/or plasticizer), hydropho-bicity/hydrophilicity, surface charge, pI, molecular size, and three-dimensional shape.Table 2.1 provides the amino acid composition for several proteins used to makeTable 2.1 Amino acid composition (mol %) of some proteins used to make edible ﬁlms andcoatings b-lactoglobulina (whey) aS1-caseina k-caseina a-zeinb (corn)Alanine 5.4 2.7 5.6 11.0Arginine 2.5 4.0 4.1 2.8Asparagine 3.1 3.8 4.2 6.7Aspartic acid 6.9 3.4 2.4 –Cysteine 2.8 – 1.0 0.5Glutamic acid 6.2 8.1 9.4 18.0Glutamine 11.2 13.1 8.2 0.6Glycine 0.9 2.2 0.6 0.5Histidine 1.5 2.9 2.2 1.9Isoleucine 6.2 5.3 7.7 5.7Leucine 13.6 8.1 4.8 21.6Lysine 10.5 7.6 6.1 –Methionine 2.8 2.8 1.4 3.0Phenylalanine 3.2 5.0 3.1 5.3Proline 4.2 7.0 10.2 9.7Serine 3.3 3.0 5.5 7.1Threonine 4.4 2.1 7.4 3.2Tryptophan 2.0 1.6 1.0 –Tyrosine 3.6 6.9 8.0 4.4Valine 5.4 4.6 5.7 7.7a Kinsella and others (1989)b Adapted from Larkins and others (1993)
2 Structure and Function of Protein-Based Edible Films and Coatings 31edible films and coatings. The presence of cysteine allows for potential disulfidebridge formation, as noted for beta-lactoglobulin. High concentrations of leucine,alanine and other nonpolar amino acids can create hydrophobic proteins, as seen ina-zein. Extrinsic factors include processing temperature, drying conditions, pH,ionic strength, salt-type, relative humidity during processing and storage, shear andpressure (Damodaran 1996). A brief summary of the properties for some proteinscommonly used for making films and coatings is given below.2.2.1 Animal Proteins126.96.36.199 CaseinCasein is the major dairy protein group occurring at 24–29 g/l in bovine or goat milk(Audic et al. 2003). There are four main subunits – alpha s1-casein, alpha s2-casein,beta-casein and kappa-casein that make up 38%, 10%, 36% and 13% of caseincomposition, respectively (Audic et al. 2003). Each of the four protein fractions hasunique properties that affect casein’s ability to form films. Alpha s1 is a 23.6 kDaprotein with a net charge of −21.9 at a pH of 6.6 and a pI of 4.94. It has eightphosphorylated serine residues, 17 proline residues, 25 glutamine residues and nocysteine residues. Alpha s1 has the majority of its charge isolated between the hydro-phobic N- and C-terminals, making the protein amphipathic. The phosphorylatedserine residues are clustered with glutamine residues, forming calcium-binding sites.Consequently, alpha s1 is Ca2+ sensitive, which means that the protein will aggregateand precipitate in low concentrations of the ion. Because it does not contain freecysteine, it cannot participate in disulfide bond formation and cross-linking. Alpha s2-casein is also Ca2+ sensitive. It has a net charge of −13.8, a pI of 5.37,and two regions of high-charge density, making it more hydrophilic than othercasein proteins. Beta-casein is an amphipathic protein with a polar N-terminal, but a largehydrophobic domain. It is also Ca2+ sensitive. The solubility of beta-casein increaseswhen the temperature is dropped to 4°C. Kappa-casein is the other major casein protein; however, it is different from theother three casein fractions, because it is not calcium ion sensitive. Kappa-casein islocated at the outer layer of a casein micelle, and is very amphipathic with a polardomain that interacts with polar solvents. It is often described as the “hairy layer”of the casein micelle (Swaisgood 1993, 1996).188.8.131.52 Whey ProteinWhey is a byproduct of the cheese-making process, and whey proteins aretechnically defined as those that remain in the milk serum after coagulation of thecaseins at a pH of 4.6 and a temperature of 20°C (Morr and Ha 1993). Whey protein is
32 K. Dangaran et al.comprised of several individual proteins, with beta-lactoglobulin, alpha-lactalbumin,bovine serum albumin, and immunoglobins being the main proteins (deWit andKlarenbeek 1983; Kinsella 1984). Whey proteins differ from caseins in that theirnet negative charge is evenly distributed over the protein chain. The hydrophobic,polar and charged amino acids are also uniformly distributed. Consequently, theproteins fold so that most of the hydrophobic groups are buried within the wheyprotein molecule. Extensive self-association does not occur under neutral conditions,as seen among casein proteins (Swaisgood 1996). The protein interactions thatoccur between chains determine film network formation and properties. Beta-lactoglobulin is an 18.3 kDa protein that consists of about 160 amino acids,depending on the genetic variant, and comprises 48–58% of the total whey protein.It does not denature as pH changes, but is thermolabile. Its secondary structureis dominated by an eight-stranded beta-barrel, and also possesses a three-turnalpha-helix. For film formation, there is an important free sulfhydryl group, cysteine121 (CYS121), and two disulfide bonds between cysteine 66-cysteine 160 andcysteine 106-cysteine 119. In the native form, CYS121 is hidden by the alpha-helix(Sawyer et al. 1999). After thermal denaturation, the thiol group is exposed andavailable for intermolecular disulfide bond formation. Consequently, edible filmsmade from denatured whey protein are stronger and more cohesive than those madefrom native protein (Perez-Gago et al. 1999). The denaturation temperature ofbeta-lactoglobulin is 78°C in a 0.7 M phosphate buffer (pH 6) (deWit and Klarenbeek1983). The most abundant amino acids in bovine beta-lactoglobulin are leucine,glutamic acid, and lysine. Notably, beta-lactoglobulin is low in tyrosine residues(Etzel 2004), which limits its ability to cross-link through the bi-tyrosine radicalsthat form when proteins are exposed to irradiation treatment. Alpha-lactalbumin is the second most abundant whey protein, comprising 13–19%of the total whey protein, with a molecular weight of 14.2 kDa. It contains fourinternal disulfide bridges. Bovine serum albumin (BSA) is the longest single-chainwhey protein, with a molecular weight of 66 kDa. It is prone to precipitation around60–65°C, due to increased hydrophobic binding between the chains (deWit andKlarenbeek 1983). The immunoglobulins are a mixture of proteins, and are verythermolabile.184.108.40.206 Meat ProteinsThere are three types of meat proteins: sarcoplasmic, stromal and myofibrillar.Enzymes, myoglobulin, and cytoplasmic proteins are examples of sarcoplasmicproteins. Stromal proteins include collagen and elastin, while myofibrillar proteinsinclude myosin, actin, tropomysin, and troponins. Stromal and myofibrillar proteinsare used for making edible films and coatings. Collagen is a fibrous, stromal protein extracted from connective tissue, tendons,skin, bones and vascular system, which are waste products of meat processing.Collagen is made from three parallel alpha-chains, which combine to make a triple-stranded superhelical structure. The amino acid sequence of collagen is dominated
2 Structure and Function of Protein-Based Edible Films and Coatings 33by a repeating trio of Gly-X-Y residues (where X and Y are often proline andhydroxyproline, respectively) (Haug et al. 2004). Gelatin is formed when collagenis exposed to a mild heat treatment under acidic or alkaline conditions (Badii andHowell 2006). In this process, collagen is partially denatured, but upon cooling,partially reforms the triple helix structure, though unstructured domains also exist.The resulting protein material is referred to as gelatin. Gelatin contains a largeamount of proline, hydroxyproline, lysine, and hydroxylysine, which can react inan aldol-condensation reaction to form intra- and intermolecular cross-links amongthe protein chains. Gelatin is used in the food industry to thicken and texturize foods, because of itsgood gelling properties. It also has excellent foaming properties that translate to itbeing a good edible film former. Gelatin has been used as a coating by the food andpharmaceutical industry for years. Recently, marine gelatins have attracted increasedinterest due to the perceived risk and stigma associated with bovine spongiformencephalopathy (BSE), which is a potential risk associated with gelatin obtainedfrom cows. Fish gelatin is also getting more attention as the fish industry tries to findnew outlets for their skin and bone by-products. In Alaska alone, over one millionpounds of by-product are generated annually (Avena-Bustillos et al. 2006). Fish gelatinfrom those species that live in cold water environments has amino acid compositionsthat differ from those of mammalian gelatin. Cold water fish gelatins contain alower percentage of proline and hydroxyproline; consequently, fish gelatins have alower melting and gelation temperature (Balian and Bowes 1977). Myosin and actin make up the major fractions of myofibrillar proteins. Likecollagen and gelatin, the secondary structure of myofibrillar proteins possesses thealpha-helix as the dominant secondary structure. The proteins are soluble in saltsolutions. There is interest in using myofibrillar proteins for edible films and coatings,because of the need to find economic uses for this by-product-stream originatingfrom the Alaskan fish industry.220.127.116.11 Egg AlbumenEgg albumen is the second major component of liquid egg white, water being thefirst, and makes up approximately 10% of the total liquid egg white weight. Withinegg albumen, there are five main protein fractions: ovalbumin, ovotransferrin,ovomucoid, ovomucin and lysozyme. Differential scanning calorimetry analysis showsthree main endotherms that occur during heating of egg white protein that correspondto the denaturation of ovotransferrin, lysozyme, and ovalbumin. Ovalbumin is thepredominant egg white protein fraction, comprising nearly 50% of the overall proteincontent. Ovalbumin is a 44.5 kDa protein that contains free sulfhydryl groups availablefor cross-linking (Mine 1995). Ovotransferrin is an iron-binding protein with a weightof 77.7 kDa and a pI of ~6.1. Lysozyme, one of the most studied proteins due to itsantimicrobial activity, has been found to be active against gram-negative bacteria. Egg albumen proteins are thermolabile, and form strong heat-set gels. During heatdenaturation, egg white proteins form stable intermolecular beta-sheet structures
34 K. Dangaran et al.between ovalbumin, ovotransferrin, and lysozyme. Above 60°C, egg white proteinsunfold, exposing their internal sulfhydryl groups that can effect disulfide bondformation, and surface hydrophobicity increases (Mine et al. 1990). Denaturationof egg white proteins can be affected by pH, salt concentration, sucrose, or pre-heattreatment. Over time, as a result of thiol cross-linking, ovalbumin forms s-ovalbumin,which is a more stable form of the protein with a higher denaturation temperature(Ternes 2001).18.104.22.168 Feather KeratinAnnually, approximately 2.3 billion pounds of feathers are generated as a byproduct-stream of the poultry processing industry. Feather keratin, a fibrous protein, hasunique film-forming properties due in part to its disulfide bonds that can be reducedto facilitate intermolecular cross-linking of protein chains. Feather keratin is alsosemi-crystalline, which adds to its high strength and stiffness (Barone et al. 2005).Chicken feathers are 91% protein, 1% lipid and 8% water (Kock 2006). The mostabundant amino acids are cysteine, glycine, proline and serine; there are very fewhistidine, lysine, or methionine residues (Schmidt 1998).2.2.2 Plant ProteinsFruits and vegetables are generally low in protein content, with polysaccharidesbeing the predominant biopolymers obtained from these sources for making ediblefilms and coatings. However, cereal grains, tubers, legumes, and pulses possess higherprotein contents than fruits and vegetables. These proteins have been isolated andstudied for film formation.22.214.171.124 Wheat ProteinsDue to the importance of bread products in both food and culture, the breadmakingprocess has been extensively studied. More specifically, the properties of wheatgluten, which is a major contributor to bread properties, have been investigated indetail. Wheat gluten, which contains a small proportion of charged amino acids(lysine, histidine, arginine) and a high proportion of non-polar amino acids, aggregateseasily due to hydrophobic interactions (Haard and Chism 1996). There are four primarywheat protein fractions, classified by their solubility: albumins (water soluble),globulins (soluble in dilute salt solutions), gliadins (soluble in 70–90% ethanol),and glutenin (insoluble under all of the previously mentioned conditions) (Haardand Chism 1996). Glutenin and gliadin are the major proteins within wheat flour, making up 47%and 34% of the total protein content, respectively (Kinsella 1982). Gliadin is a
2 Structure and Function of Protein-Based Edible Films and Coatings 35single chained peptide of approximately 40 kDa, consisting of four distinct fractions:w5, w1,2, a/b, g, with a/b and g gliadins containing intramolecular disulfide bonds(Kinsella 1982). These play a role in film formation, strength and elasticity. Gluteninis a mixture of proteins and has a molecular weight distribution between 100 and1,000 kDa, depending on the number of intermolecular disulfide linkages. Someglutenin molecules are branched. The disulfide bonds present in glutenin and gliadinplay an important role in determining the strength of the protein matrix. Oxidizingagents, such as potassium bromate, potassium iodate and ascorbic acid, can be addedto affect the strength and elasticity of the matrix. Low molecular weight thiol-containing compounds, like glutathione, also can be present in wheat protein. Thesesmall thiol compounds react with the disulfide bonds within and between glutenmolecules and cleave them, weakening the wheat protein matrix. Oxidizing agents canselectively react with the small thiol groups, making it easier for protein–proteinSS/SH exchange to take place and subsequently, increasing the strength and elasticityof gluten (Kinsella 1982). The gluten protein matrix is also affected by shear, which causes proteins to unfold,hydrogen bonds to weaken, and a general rearrangement of the proteins to formparallel fibers. These changes increase the elasticity and stretchiness of the resultingmatrix. During exposure to shear stress, hydrophobic areas are pulled apart andbecome exposed to water within the dough matrix, leading to a hydrophobic effectand a re-ordering of water molecules. When the stress is removed, the proteinsrelax, the hydrophobic areas refold, and the water becomes less structured. Gluten,therefore, can be considered both plastic and elastic.126.96.36.199 Soy ProteinSoy protein is comprised of a mixture of globular proteins. Approximately 90% ofsoy proteins separate into either a 2S, 7S, 11S or 15S fraction, based on molecularweight and sedimentation coefficient (Cho and Rhee 2004). The two main globularproteins are beta-conglycinin (7S globulin) and glycinin (11S globulin), whichmake up 37% and 31% of the soy proteins, respectively. Conglycinin (140–170 kDa)consists of various combinations of three subunits, which are heavily glycosylated(Kunte et al. 1997). Glycinin (340–375 kDa) is made of six AB subunits, whichare each comprised of an acidic (A) and a basic (B) polypeptide, linked together viadisulfide bonds. As with other film-forming proteins, glycinin is known to be a gelling agent,emulsifier and foaming agent (Subirade et al. 1998). Heat and alkaline conditionscan denature soy proteins, affecting film formation. Similar to beta-lactoglobulin(whey protein), glycinin (11S protein) forms intermolecular disulfide bonds whendenatured, which bonds affect the tensile properties of a formed film. Soy proteinassociation and stability is dependent on the pH and ionic strength (Petruccelliand Anon 1994). Beta-conglycinin is less heat stable than glycinin; the proteinshave denaturation temperatures of approximately 70°C and 80°C, respectively(Renkema and Vliet 2002).
36 K. Dangaran et al.188.8.131.52 Corn ZeinZein protein from corn has some unique characteristics compared to most otheragricultural proteins used for edible films and coatings. Zein possesses a highpercentages of nonpolar amino acids and low proportions of basic and acidic aminoacids. The three primary amino acids in corn zein protein are glutamine (21–26%),leucine (20%) and proline (10%) (Shukla and Cheryan 2001). Consequently, corn zeinprotein is insoluble in water, a characteristic that affects the barrier properties of itsfilms. The two major fractions of zein are alpha-zein and beta-zein. Alpha-zein is solublein 95% ethanol, and makes up approximately 80% of the total prolamines present incorn, while beta-zein is soluble in 60% ethanol. A helical secondary structuredominates zein proteins (Shukla and Cheryan 2001). When formed into films, zeinis glossy, tough and greaseproof, with a low water vapor permeability compared to mostother agriculturally-based protein films. Zein has been commercially used as a coatingfor medical tablets, and has the potential to be used in biodegradable packaging.2.3 SolventsWater and ethanol are the solvents of choice for making edible films and coatings,because they are safe for consumption. However, if the application of the film orcoating from an agricultural protein is not intended for a food application, otherorganic solvents may be used. In a study by Yoshino et al. (2002), zein films weremade using either aqueous ethanol or aqueous acetone as the solvent system. Whenethanol was used as the solvent, resulting films initially had higher tensile strengthas compared to those made with acetone; however, they were also more susceptibleto moisture and high humidity environments. As the relative humidity of the storageenvironment increased from 5 to 90%, the tensile strength of the ethanol-solventzein films dropped over 75% (from 29 to 7 MPa), while the acetone-solvent zeinfilms lost only 15% of their initial strength (from 25 to 21 MPa). Thus, choice ofsolvent can affect the properties of a formed film.2.4 PlasticizersPlasticizers are small molecular-weight compounds that can be added to an ediblefilm or coating solution to improve the flexibility and mechanical properties ofthe film matrix. Most protein-based films and coatings are very strong, but verybrittle when not plasticized (Gennadios et al. 1994); thus, a plasticizer is necessaryto improve the application potential of protein-based films. While plasticizers canimprove the flexibility and elongation of protein films, they also affect the permeabilityof the films and coatings (McHugh and Krochta 1994). As a general rule, the additionof a plasticizer increases the permeability of a film or coating. There are two types of plasticization: internal and external. Internal plasticizerschemically modify a protein chain through addition of substituent groups attached
2 Structure and Function of Protein-Based Edible Films and Coatings 37Fig. 2.4 Examples of chemical modification of protein chainsvia covalent bonds. Common chemical derivatization schemes are acetylation,succinylation and Maillard reactions with monosaccharides (Fig. 2.4). Internalplasticizers create steric hindrance between the protein chains, leading to increasedfree volume and improved flexibility. External plasticizers solvate and lubricate theprotein chains, lowering the glass transition temperature of the proteins and alsoincreasing the free volume. Common plasticizers used in edible films and coatings are typically polyols,including glycerol, propylene glycol, polypropylene glycol, sorbitol and sucrose.Fatty acids have also been used as plasticizers in edible films and coatings, thoughthey are not as common. The most effective plasticizer is, of course, water. The effec-tiveness of a plasticizer is dependent upon three things: size, shape and compatibilitywith the protein matrix (Sothornvit and Krochta 2001). The state of the plasticizerunder normal storage conditions may also affect its permeability and flexibility. Solidplasticizers may have an “antiplasticizing” effect, and decrease matrix flexibility,while improving permeability (Dangaran and Krochta 2007). In traditional polymer-plasticizer systems, antiplasticization occurs when a plasticized system is harderand less flexible than the pure polymer at a temperature below the glass transitionor Tg (Chang et al. 2000; Morara et al. 2002). Several researchers have conducted studies to evaluate the efficiency of differentplasticizers in protein-based films, and have developed empirical models to describethe observed phenomena (Sothornvit and Krochta 2000, 2001; Dangaran and Tomasula2006). Dangaran and Tomasula (2006) used a modified version of the Gordon–Taylor
38 K. Dangaran et al.Fig. 2.5 Gordon–Taylor equationequation (Fig. 2.5), and applied it to determine the effect of glycerol, propylene glycol,and sorbitol on three types of caseins, each differing in structure and chemical func-tionality (water solubility). They determined that the effectiveness of a plasticizer wasaffected by the microstructure and chemical nature of the plasticizer, with glycerolbeing the most efficient. Sothornvit and Krochta (2001) also found glycerol to bethe most efficient plasticizer in a whey protein film matrix. Their empirical modelfit the changes in the observed tensile properties and oxygen permeabilities forfilms with up to 30% plasticizer. They reported an exponential relationship betweenfilm properties and plasticizer content. The properties of the protein (crystallinity,hydrophobicity/hydrophilicity) also affect the plasticizer–protein interaction.2.5 Film and Coating PreparationThere are several ways to form edible films and coatings from agricultural proteins,all of which affect the properties of the final film or coating. Films can be formedvia several processes, depending on the starting material. Lipid and wax films canbe formed through solidification of the melted material (Fennema and Kester1991). Biopolymers in solution can form films by changing the conditions of thesolution. Applying heat, adding salt or changing the pH may alter conditions in thesolution, such that the biopolymers aggregate in a separate film phase. This processis called coacervation (Krochta et al. 1994; Debeaufort et al. 1998).2.5.1 Solvent CastingSolvent casting is the preferred method used to form edible protein films for research.Various types of equipment are available for solvent casting of films, from simplecasting-plates to more advanced batch and continuous lab coaters (Fig. 2.6a, b).Because it is effective and cost-efficient, the most commonly used method forforming protein film samples for research is by manually spreading dilute filmsolutions (usually 5–10% solids) of protein and plasticizer into level Petri dishes or
Fig. 2.6 (a) Casting plate andcasein films. (b) Continuous labcoater and rolls of edible films
40 K. Dangaran et al.plates, and then drying them under ambient conditions or controlled relative humidity.More sophisticated equipment can produce larger protein films by mechanicallyspreading the solution to a fixed thickness. Kozempel and Tomasula (2004) developed a continuous process for solventcasting of protein films. This process was demonstrated using casein-based films.Parameters that need to be determined for continuous film production are air tempera-ture, surface properties of the substrate upon which the films are formed, flow rate,and drying time. Films can be dried under ambient conditions, with hot air, infraredenergy, or microwave energy. The method of drying can significantly affect thephysical properties of the final film, including film morphology, appearance, andbarrier and mechanical properties (Perez-Gago and Krochta 2000).2.5.2 Extrusion of Edible FilmsAn alternative to solvent casting is extrusion, which uses elevated temperatureand shear to soften and melt the polymer, thus allowing a cohesive film matrix toform. Extrusion of proteins into films has certain advantages over solvent casting.Comparatively, extrusion is faster and requires less energy, due to the fact that moreconcentrated film solutions can be fed into the extruder. For solvent casting, evapo-rating ethanol or especially water, is both energy intensive and time consuming,adding to the production costs of edible films. The use of extrusion reduces timeand energy inputs to bring the cost of biopolymer film formation into a competitiverange with synthetic film production. Results from recent studies (Hernandez et al. 2005, 2006) investigated theprocessing parameters to extrude transparent, flexible whey protein sheets using atwin-screw extruder. Feed composition, temperature and screw speed were varied.These extruder dimensions and operating conditions allowed for sufficient heat-denaturing and cross-linking of the whey protein to produce sheets that hadimproved tensile properties, as compared to solvent-cast heat-denatured wheyprotein films (Hernandez 2007). Extrusion can be applied to other protein materials as well. In a study by Zhanget al. (2001), sheets were extruded from soy protein, and the effects of plasticizertype, plasticizer amount, and cross-linking agent were measured. The tensilestrength and elastic modulus of soy protein sheets were comparable to LDPE,depending on the processing agents (plasticizer, cross-linker) used. Gluten-basedfilms have also been extruded. In a study by Hochstetter et al. (2006), extrudedsheets of wheat gluten and glycerol were successfully made. They determined thatunder the shear and temperature conditions used to make the films, there was anorientation of the protein film matrix. Films tested either parallel or perpendicularto the direction of extruder flow, gave different tensile properties. Films cut in thecross direction of the extruder flow were stronger (25 MPa tensile strength) withshorter elongation (120%), compared to those tested in the direction of the machineflow (17 MPa and 170% for tensile strength and elongation, respectively). However,films were brown in color due to Maillard reactions that occurred during high
2 Structure and Function of Protein-Based Edible Films and Coatings 41temperature extrusion (130°C). In a study by Obuz et al. (2001), wheat gluten wasextruded with varying proportions of LDPE or metallocene-catalyzed ethylene-butene copolymer (MCEBC). In tests containing up to 25% of the wheat glutenbiopolymer, the tensile properties of films were similar to the pure synthetic materials.However, if higher amounts of the biopolymer were incorporated, there was asignificant detrimental effect on both elongation and tensile strength. Given theprocessing advantages of extrusion for producing stand-alone films, more researchon extrusion of protein films is warranted.2.5.3 SpinningWet-spinning is a processing technique most commonly used by the textile industryto form fibers (Rampon et al. 1999). During fiber formation, a solution of polymeris passed through a pin hold spinneret under pressure. Frinnault et al. (1997) modifiedthe spinning process to form films from casein, replacing the spinneret with a platedie to form flat films. Protein solutions were extruded into a coagulating bath, andthen collected onto a roller. The modified wet-spinning process has also been usedto make films from soy protein. Rampon et al. (1999) hypothesized that soy proteinchains could be oriented similar to textile fibers using the spinning method. Theyfurther theorized that an increased orientation of protein chains within the ediblefilm might facilitate an increase in the elongation values of the films. Though theywere successful in forming films, no increase in the orientation of the protein chainswas observed. As the modified film formation process used a pressure lower thanthat commonly used textile processing, the authors suggested that shear couldpossibly play a role in orientation.2.5.4 Edible Coating FormationEdible coatings are formed using the same processes and according to the samemechanisms associated with solvent casting of films. A dilute protein solution isapplied to the surface of the food product, and the coating forms upon evaporationof solvent. Typical methods for forming a coating include panning, fluidized-bedprocessing, spray-coating, and dipping. Panning is a method used by both pharmaceutical and confectionery industries,and entails putting the product to be coated into a large, rotating bowl, referred toas the pan (Minifie 1989). The coating solution is ladled or sprayed into the rotatingpan, and the product is tumbled within the pan to evenly distribute the coating solutionover the surface of the food or pharmaceutical material. Forced air, either ambientor of elevated temperature, is used to dry the coating. In a study by Lee et al. (2002a,b),whey protein coatings were applied to chocolate candies to provide a clear, glossyfinish to a confectionery product. Edible shellac is currently used to finish choco-lates and other candies, such as jelly beans, with a gloss surface. However, shellac
42 K. Dangaran et al.is an ethanol-based coating that emits volatile compounds into the air. Whey proteincoatings plasticized with sucrose were found to be highly glossy (Dangaran andKrochta 2003), and were preferred to shellac-coated chocolate products in a consumerstudy (Lee et al. 2002a–c). Fluidized-bed coating, a method used commonly by the pharmaceutical industryto coat tablets, has been studied for formation of whey protein edible coatings toprotect nuts and peanuts. Lin and Krochta (2006) found that alternating the spray-ing of coating solutions with periods of drying allowed for the gradual formation ofthe coating. The action of the fluidized-bed during drying of the coating appearedto reduce the formation of clusters of coated product, a problem commonly encoun-tered with formation of coatings via panning. Spray-coating is used to apply a uniform coating over a food surface, and is apotentially a more controllable method of coating application than pan- or fluidized-bed-coating. However, spray-coating requires that the bottom surface of the product becoated in a separate operation after application of the initial coating and drying. In thisscenario, the product must then be turned to expose the bottom for subsequent coatingapplication. Spray-coating is preferred for items possessing a large surface area. Dipping, the other possible method of forming edible coatings on the surfacesof food, is best-suited for irregularly-shaped food objects. Final formed coatingsmay be less uniform than coatings applied by other methods, and multiple dipping(with draining and drying steps between dipping operations) may be necessary toensure full coverage (Krochta et al. 1994).2.6 Effects of Processing on Properties of Protein-Based Films and CoatingsWhile there are several methods for forming protein-based films and coatings, sol-vent casting still predominates. Most of the literature reports have investigated theproperties of solvent-casted films. The main properties of interest for films and coat-ings are tensile properties (tensile strength, elongation at break and elastic modulus),gas permeability, water vapor permeability and appearance. All of these propertiescan be affected by the extrinsic conditions used to process and produce the films.2.6.1 Drying ConditionsThe effect of drying conditions (e.g., temperature, relative humidity, type of energysource, etc.) on the properties of protein-based films have been investigated forwhey protein and casein as well as other protein sources. In all reported studiesinvestigating the films made from either of the dairy proteins, drying effects on filmproperties were minor, but still measurable. Kozempel et al. (2003) investigated theeffects of air temperature, air flow, relative humidity, and initial total solids content
2 Structure and Function of Protein-Based Edible Films and Coatings 43on the drying rate and tensile properties of calcium caseinate films. Using convec-tion drying, they found that an air temperature of 34°C and a low relative humiditydrastically reduced the period of constant drying from approximately 1,300 to 400min compared to ambient air temperature, flow and high relative humidity. Also,increasing the initial total solids of solutions from 6 to 15% dropped the constantdrying period from 1,300 to 300 min. While drying time was significantly reduced,differences in film tensile properties were not observed. However, tensile strengthand elastic modulus did trend upward as the initial total solids were increased.Alcantara et al. (1998) reported similar results for whey protein films dried underdifferent conditions; tensile strength and elastic modulus were marginally increasedby an elevated drying air temperature. In a study by Kaya and Kaya (2000), theeffect of microwave energy drying was investigated in relation to the properties ofwhey protein films. They observed no statistically significant increase in film watervapor permeability or tensile properties, compared to films dried under ambientconditions. However, film gloss was significantly increased as a result of micro-wave drying, and drying time was shortened to 5 min.2.6.2 Cross-Linking184.108.40.206 Heat DenaturationSolvent-cast protein films, for which the solvent is water, are typically formed atroom temperature and stabilized through electrostatic interactions, hydrogen bonding,and van der Waals forces among the protein chains. The protein film network maybe improved through heat-denaturation, which improves the tensile and barrierproperties of solvent casted films by induction of cross-linking between the proteinchains. Disulfide bond formation, which occurs with heat-denaturation in protein-based films, is often used to modify film properties (Perez-Gago et al. 1999).Heat-denaturation, and the subsequent polymerization of protein chains, hasbeen studied for two proteins commonly used to make edible films: whey proteinand soy protein. For whey protein, temperature increases exposure of a free thiol group, CYS121of beta-lactoglobulin, due to alpha-helix shifts. Polymerization occurs throughintermolecular disulfide bond exchange, provided that the temperature is held at >60–65°C (Galani and Apenten 1999). However, polymerization is not the onlychemical reaction involved in whey protein film network formation. Noncovalentaggregation also occurs through new hydrophobic, ionic and van der Waals interac-tions that occur between newly-exposed groups of the heat-denatured whey proteins.These interactions increase as pH is decreased toward the whey protein isoelectricpoint (Kinsella 1984; Kinsella and Whitehead 1989). For soy protein films, thermal treatment is also important for the formation of afilm matrix. As reported by Renkema and Vliet (2002), soy proteins (with theexception of beta-conglycinin) and purified glycinin participate in heat-induced gel
44 K. Dangaran et al.formation, which aggregation is facilitated through formation of disulfide bonds toprovide matrix cohesion. In a study by Okamoto (1978), films made from 11S soyprotein were stronger than those made from the 7S fraction because of the intermo-lecular disulfide bonds formed between 11S protein chains.220.127.116.11 IrradiationThere are other methods for inducing cross-linking of protein chains besides heatdenaturation. Irradiation has been successfully used to cross-link casein proteins, aswell as soy proteins (Lacroix et al. 2002). Water forms hydroxyl radicals whenexposed to gamma-irradiation. Aromatic amino acids, such as phenylalanine andtyrosine, are more likely to react with the hydroxyl radicals than aliphatic aminoacids (Sabato et al. 2001). A mechanism hypothesized to explain the radical polym-erization process involves the formation of bi-tyrosine linkages between proteinchains (Brault et al. 1997). When exposed to 32 kGy of energy, soy protein and soyprotein-whey protein blends form stronger films than their non-treated counterparts.Brault et al. (1997) did find that caseinate films cross-linked through irradiationbecame very brittle and required a plasticizer to improve their properties.18.104.22.168 Enzymatic and Chemical Cross-linkingCross-linking of proteins has been induced by both chemical and enzymatic means.Formaldehyde, glutaraldehyde, and lactic acid have been used to cross-link wheyproteins through lysine residues (Fig. 2.7). However, the cross-linked products areno longer edible, due to the toxicity of the cross-linking agents (Galietta et al.1998). More recently, genipin, a small molecule with no cytotoxicity issues, hasbeen investigated as a protein cross-linking agent. In a study by Bigi et al. (2002),gelatin films were cross-linked using genipin. Film elongation decreased drasticallyand stiffness increased as a result of genipin cross-linking. For 0%, 1%, and 2%genipin addition levels, elongation was 211%, 16% and 13%, respectively, whileelastic modulus values were 1 MPa, 5.6 MPa and 6.8 MPa, respectively. Also,genipin cross-linked films did not swell as much as untreated films when exposedto aqueous solutions. Transglutaminase is a food grade enzyme that uses the acyl-transferase mechanismto link the gamma-carboxyamide (acyl donor) of a glutamine residue to the gamma-amine (acyl acceptor) of lysine residues along protein chains (Mahmoud and Savello1992). This enzyme is known to improve elasticity in foods. Originally, transglutam-inase was extracted from Guinea pig liver, making it expensive and cost-prohibitivefor large-scale production (Zhu et al. 1995). Transglutaminase is now posible to beobtained at a lower cost from microbial sources (Chambi and Grosso 2006), and hasbeen used in both homogenous protein systems and mixtures of proteins to affecttensile and permeability properties. Whey protein, casein, soy, egg albumin andwheat gluten have all been investigated for treatment with this enzyme. The molecular
2 Structure and Function of Protein-Based Edible Films and Coatings 45Fig. 2.7 Chemical agents for protein chain cross-linkingweight of alpha-lactalbumin, beta-lactoglobulin and alpha-lactalbumin/beta-lactoglobulin mixtures was shown to increase after transglutaminase treatment,indicative of cross-linking. Moreover, transglutaminase-treated proteins were alsomore heat stable relative to untreated ones (Truong et al. 2004). The cross-linkedprotein networks were less soluble, which may improve the water vapor permeabilityproperties of films formed from the cross-linked proteins. Egg white proteins wereeffectively cross-linked using transglutaminase (Lim et al. 1998), as marked by anincrease in protein molecular weight determined by SDS-PAGE. Cross-linking wasenhanced as the incubation temperature increased, as more of the proteins wereunfolded, exposing more amino acids to the transglutaminase enzyme. Elongationof the transglutaminase-treated egg white films was 50–100%, depending on theglycerol content. Tensile strength reached a maximum of nearly 10 MPa, dependingalso on the plasticizer content and relative humidity conditions. Blends of proteins treated with transglutaminase have also been investigated.Chambi and Grosso (2006) made mixtures of gelatin and casein in an attempt toleverage the functionality of both proteins to create an improved film system.According to Howell (1995), three main phenomena can happen when proteins areblended (1) synergistic interaction, (2) precipitation, and (3) phase separation.When treated with transglutaminase, gelatin and casein, in a 1:3 ratio by mass, theyhad a synergistic effect on film elongation. Elongation increased to nearly 55% inthe enzyme-treated mixture, compared to 14–17% elongation for pure individualcasein and gelatin enzyme-treated film systems.
46 K. Dangaran et al. Cross-linking can improve elongation in that the protein chains of the filmmatrix are associated through covalent bonds instead of relatively weaker van derWaals interactions (Chambi and Grosso 2006). In a study by Yildirim andHettiarachchy (1998), whey protein and the 11S fraction of soy protein were cross-linked using transglutaminase and formed into a film. The untreated protein in thecontrol films had a water-solubility ranging between 325%, depending on pH. Aftertreatment with transglutaminase, solubility dropped to 0.5–6% under the sameexperimental conditions. Lower water solubility was expected to lead to lowerwater vapor permeability; however, WVP actually increased for transglutaminasefilms. The authors did not investigate changes to surface hydrophobicity or micro-structure for a possible explanation for the increased diffusion of moisture throughthe treated-films. Nevertheless, a positive effect was observed in tensile strengthvalues of the transglutaminase films. The treated films were over two times strongerthan control films which had an average value of 6.26 MPa. The tensile strength oftransglutaminase-treated films (made from 50:50 mixture of 11S and whey protein)increased to 17.86 MPa.2.6.3 Ionic StrengthThe properties of the protein-based films can be affected by the solubility of theprotein in a given solvent system. For example, increasing the water solubilityof a protein can improve the appearance and increase the elongation of proteinfilms. Similarly, the moisture barrier properties of a film can be improved bydecreasing the solubility of the protein in water. Changing the ionic strength ofthe solution from which a film is cast represents one of the many ways to affectthe solubility of the final film product. In a study by Qi et al. (2006), the solubilityof various caseins was analyzed as a function of salt (NaCl) concentration.CO2-precipitated casein (CO2CN) and calcium caseinate were both studied(Tomasula et al. 1995). The results showed that the solubility of CO2CNincreased significantly as a function of salt concentration; however, the solubilityof calcium caseinate remained essentially unchanged. Based on transmissionelectron microscope (TEM) investigations, CO2CN protein aggregates wereobserved to disintegrate and became much smaller and of uniform size at ele-vated salt conditions, suggesting that electrostatic interactions among caseinsbrought about by pressurized CO2 processing might be a dominating force in theformation of these aggregates.2.6.4 Particle SizeChanges in particle size in relation to either the protein matrix or additives to thefilm system can affect the properties of the film. Non-soluble particles embedded
2 Structure and Function of Protein-Based Edible Films and Coatings 47within a film matrix can affect the permeability of gas through a film. Permeabilityis affected by the solubility of the diffusing compound in the film and by the diffu-sion coefficient (Rogers 1985). Changing the path of travel for a molecule of gasdiffusing through the film can change the rate of diffusion. Thus, in a film matrix,insoluble particles create a hindrance to diffusing molecules migrating through thefilm. For a given mass of an insoluble additive, such as fat, a more tortuous diffu-sion path can be created by making the particles smaller, thereby lengthening themigration time and improving the barrier properties of the film (Pérez-Gago andKrochta 2001). In a study by Dangaran et al. (2006), the tensile and water vapor properties ofcasein-based films were affected by decreasing the particle size of insolubleCO2CN particles. Films made from CO2CN, which are only partially soluble inwater, are opaque and hazy. Dangaran et al. (2006) found that the use of high shearcould reduce the particle size of the insoluble portion of CO2CN. The effect ofprotein particle size reduction on tensile properties, water vapor permeability, andgloss was studied using the ASTM methodology. As the particle size of the CO2CNwas reduced from 126 to 111 mm, the tensile strength and elastic modulus of thefilms increased, while water vapor permeability decreased. Comparing films madefrom proteins of the same particle size reduction, gloss increased, on an average,from 55.3 to 73.0 gloss units, but all films were still hazy. With a particle size lessthan 86 mm, CO2CN films were glossy and transparent; however, tensile strengthdecreased and WVP increased.2.7 Analytical Tools for Determining Protein StructureChanges in protein structure, due to processing conditions, can be measured and charac-terized with appropriate instrumentation. Understanding the fundamental changes in themolecular structures of the proteins can be advantageous to improving the functionalproperties of the protein-based films for various applications. Modern chromatographic,spectroscopic, and microscopic techniques can be used for analyzing the protein film-making process, from the solutions (often concentrated) used to make the films to theactual films themselves. Some commonly used spectroscopic techniques, such as circu-lar dichroism (CD) and Fourier Transform Infrared (FTIR) spectroscopy (Curley et al.1998; Farrell et al. 2002), used to study changes at the secondary structure level, can alsobe applied to study protein conformational changes within films. However, one technicalrequirement of CD is that the film samples must be transparent. After processing treat-ments, it is possible for protein films to darken in color, due to Maillard browning, orto become hazy, making CD analysis problematic. FTIR, on the other hand, is highlyversatile and can be used for samples of various states, including solutions, powdersand films. Changes in the hydrophobicity of protein films can be investigated usingfluorescence spectroscopy and water-solubility analysis. The Bradford ProteinAssay is a commonly-used specrophotometric method that quantitatively determines
48 K. Dangaran et al.the concentration of protein in a solution. Tryptophan residues in protein molecules arefrequently used as indicators of their environment (polar or non-polar) by yielding char-acteristic fluorescence spectra. By following changes in their fluorescence behavior,changes in the local environment of these tryptophan residues can be determined (Liu etal. 2005). Changes in complex protein–protein interactions, which may be attributedto denaturation and aggregation, can be studied using high-resolution microscopicimaging techniques, including atomic force microscopy (AFM), scanning electronmicroscopy (SEM), TEM, and confocal laser scanning microscopy. These changeswill presumably cause differences in the observed film properties.2.8 Function and Applications of Protein-Based FilmsBased on the required tensile, barrier and appearance characteristics and properties,protein-based edible films for specific applications can be designed. Table 2.2provides an extensive list of various protein-based films, including gas barrier,water vapor barrier and tensile properties, as well as potential applications. At thecurrent state of edible film technology, the best application potential lies in protectivecoatings for foods. When applied to the surfaces of foods as a coating, protein-basededible films can protect food from chemical or microbial damage, thus lengtheningproduct shelf life and maintaining high product quality. As evident in Table 2.1, most protein-based films provide excellent barriers tooxygen. This characteristic has been utilized to effectively protect high-fat foods,which are known to form rancid off-flavors, due to oxidation. In two studies, per-formed on peanuts (Lee and Krochta 2002; Lee et al. 2002a–c), the shelf life ofpeanuts could be extended to 273 days by coating them with whey protein, com-pared to only 136 days for uncoated samples. The development of hexanal, anindicator of lipid oxidation, was prolonged for 330 days when the peanuts werecoated with a whey protein film that contained vitamin E, an antioxidant. As barriers to mass transfer of carbon dioxide, protein-based coatings have beenfound to increase the shelf life of eggs and fresh-cut fruits. Egg quality drops overtime as carbon dioxide migrates out of the shell, causing changes to the internal pH.These pH changes can deleteriously affect color and yolk quality. A study by Caner(2005) showed that the shelf life of whey protein-coated Grade A eggs could beextended one week longer than uncoated eggs, when stored under ambient laboratoryconditions. In the case of fresh-cut produce, browning and ripening times are majorfactors determining product shelf life. Protein-based edible coatings that have moder-ate oxygen, carbon dioxide and water vapor permeability can be applied to the sur-faces of fresh-cut produce to extend product shelf life by delaying ripening, inhibitingenzymatic browning, reducing water loss, and minimizing aroma loss (Olivas andBarbosa-Canovas 2005). In a study by Le Tien et al. (2001), whey protein coatingssignificantly delayed browning in fresh-cut Macintosh apples and Russet potatoes. Edible films used to protect fresh-cut produce have advantages over modifiedatmosphere packaging or treating the cut surfaces with ascorbic acid (which inhibits
2Table 2.2 Barrier and tensile properties of solvent-casted protein ﬁlms Tensile Elastic modu- PercentProtein Plasticizer OP WVP strength (MPa) lus (MPa) elongation (%) Comments ReferencesNative WPI Glycerol – 5.06 3.1 100 7 By crosslinking WPI films through Perez-Gago and (30%) heat denaturation, mechani- Krochta (1999) cal properties were improved. Improvements in mechanical properties expand the application potential of edible filmsDenatured Glycerol – 4.96 6.9 199 41 Application Possibility: Pouches for Perez-Gago and WPI (30%) dry ingredients or coatings that Krochta (1999) add mechanical strength to brittle products such as corn flakesDenatured Glycerol 18.5 2.37 29 1,100 4 Increasing plasticizer content McHugh and WPI (15%) increased elongation but increased Krochta (1994)Denatured Glycerol 76.1 4.96 18 625 5 permeability. Permeability can be McHugh and WPI (30%) improved by incorporating a solid Krochta (1994)Denatured Sorbitol 4.3 – 14 1,040 3 plasticizer sorbitol. Application McHugh and WPI (30%) Possibility: The oxygen perme- Krochta (1994)Calcium Sorbitol 1.3 – 12.8 356 56 ability is 1–2 orders of magnitude Dangaran and Structure and Function of Protein-Based Edible Films and Coatings Caseinate (30%) better than PE and rivals Nylon. Tomasula (CaCN) Protein-based edible films with (2007)Sodium Sorbitol 6.1 – 7.6 246 27 the correct plasticizer can be used Dangaran and Caseinate (30%) to coat high fat foods such as nuts Tomasula and coffee beans to protect them (2007) from oxidative rancidity 49
50 K. Dangaran et al.browning). Modified atmosphere packaging can slow oxidation; but if oxygen lev-els are reduced to a very low level, anaerobic conditions could be created, creatingthe risk of anaerobic bacterial growth. Effective levels of ascorbic acid may be sohigh that flavor is negatively affected (Perez-Gago et al. 2003). While edible coatings that hinder mass transfer of oxygen, carbon dioxide, watervapor, or aroma compounds represent the majority of applications investigated forprotein-based edible coatings, they also have the potential to improve appearanceby adding gloss (Lee et al. 2002a–c) or by protecting food from microbial spoilageif the film contains an active antimicrobial. Such applications have been investi-gated for protecting meat products, as well as fruits (Vachon et al. 2003; Cagri et al.2004; Min et al. 2006a, b).2.9 Future TrendsMuch progress has been accomplished in the research and development of ediblefilms and coatings based on agricultural proteins. Table 2.3 provides a brief listof suppliers of agricultural proteins for edible films research, as well as equip-ment sources. Based on what is currently known about their properties, protein-based films and coatings are on the brink of broad application in both the foodand non-food sectors. Concerning commercialization, the best potential for suc-cess is for food coatings that protect against chemical and biological damage,thus lengthening product shelf life. Protein-based solutions intended for film-making can also be used in commercial equipment used for coating. Protein-based coatings are good gas barriers (especially to oxygen) and can act asvehicles for active compounds like antimicrobials or nutrients. Moreover, theycould be combined with thermal or non-thermal processing to further increaseproduct shelf life. These concepts have been successfully proven in the laboratorysetting (Ouattara et al. 2002). Both edible and non-edible protein-based films have the potential to function in“green” packaging applications. The oxygen permeability (OP) properties of caseinfilms are superior to those of LDPE. Tests in our laboratory have demonstrated thatcoating an LDPE with a casein film reduces its oxygen permeability from 1,560 to86 cc mm/m2 d kPa. With the growing trend for increased convenience and indi-vidualized portion size, packaging per unit has also increased (Marsh and Bugusu2007). As companies like Wal-Mart and McDonald’s begin to seek biobased mate-rials to fulfill their packaging needs, more biobased products with the functionalityof petroleum-based packaging are likely to be produced. Protein-based films can be replacements for synthetic gas barriers, but theirmechanical properties still need improvement. Nanotechnology is a viable route toimprove both tensile and barrier properties. Nanoparticles and variations at thenanometer scale affect electronic and atomic interactions without changing thechemistry (Lagaron et al. 2005). The water vapor permeability (WVP) of wheat gluten
2 Structure and Function of Protein-Based Edible Films and Coatings 51Table 2.3 Ingredient suppliers and equipment sourcesIngredient/Equipment Supplier AddressWhey protein Davisco 11000 West 78th St Suite 210 Eden Prairie, MN 55344 phone 800-757-7611Whey protein Proliant, Inc. 2425 SE Oak Tree Court Ankeny, IA 50021 USA (USA) Phone: 800-369-2672 Fax: 515-289-5110Whey protein, Fonterra (USA) Sales Office 100 Corporate Center Drive Suite 101 casein/caseinates Camp Hill PA 17011-1758 Ph + 1 717 920 4000Casein American Casein 109 Elbow Lane Burlington, New Jersey 08016- Company 4123 USA Incorporated: 1956 Telephone: 609- 387-3130 FAX: 609-387-7204 Sales Email: Sales@109elbow.comWheat protein Tate & Lyle 2200 East Eldorado Street Decatur, IL 62525 United StatesSoy protein The Solae PO Box 88940 St. Louis, MO 63188 Local: Company (314)659-3000 Phone: (800)325-7108 Tel: 1 717 920 4000Soy protein Cargill Cargill Health & Food Technologies P.O. Box 9300 MS 110 Minneapolis, MN 55440-9300 E-mail us at firstname.lastname@example.org (866) 456-8872Soy protein ADM Soy Proteins 217-451-5141 866-545-8200 4666 Faries Parkway Decatur, IL 62526 Email: Sales@109elbow.comLaboratory film Werner Mathis 2260 HWY 49 N.E. P.O.Box 1626 CONCORD N.C. equipment USA Inc 28026 Tel: + 1 7047 866 157 Fax: + 1 7047 866 159 E-Mail: email@example.comPermeability testing Mocon, Inc. 7500 Boone Ave. N. Minneapolis. MN 55428 USA equipment Phone: (763) 493-6370 Fax: (763) 493-6358This is just a partial list and does not indicate endorsement of these companies by the USDAfilms was improved by including montmorillonite clay nanoparticles, while tensilestrength and elastic modulus were also increased (Olabarrieta et al. 2006). Edible films and coatings from proteins (as well as other biobased materials) fitwell into the Environmental Protection Agency’s (EPA) suggested plan for improvedmunicipal waste management and reduction. As stated in its summary on municipalsolid waste in the US (2006), recycling has increased from 10% in 1980 to 32% in2005. For further and continued improvements of U.S. waste management practices,the EPA suggests reducing the initial amount of packaging, and promotes compost-ing. For reduction, the EPA suggests designing packaging systems that reduce theamount of environmentally toxic materials used in packaging to make it easier toreuse or compost them. They also suggest packaging that reduces the amount ofdamage or spoilage to food products. Protein-based edible films and coatings fit bothcriteria. They can reduce the complexity of packaging systems, making them eithereasier to recycle or compostable. Edible coatings can also protect food from chemi-cal or biological damage, thereby lengthening product shelf life.
52 K. Dangaran et al.ReferencesAimutis WR (2004) Bioactive properties of milk proteins with particular focus on anticariogenesis. J Nutr 134: 989S–995SAlcantara CR, Rumsey TR, Krochta JM (1998) Drying rate effect on the properties of whey protein films. J Food Proc Eng 21: 387–405Anonymous (2006) Bioplastics demand experiencing boom in Europe. Food Navigator.comAudic JL, Chaufer B, Daufin G (2003) Non-food applications of milk components and dairy co-products: A review. Lair 83: 417–438Avena-Bustillos RJ, Olsen CW, Olson DA, Chiou B, Yee E, Bechtel PJ, McHugh TH (2006) Water vapor permeability of mammalian and fish gelatin films. J Food Sci 71(4): E202–E207Badii F, Howell NK (2006) Fish gelatin: structure, gelling properties and interaction with egg albumen proteins. Food Hydrocolloids 20: 630–640Balian G, Bowes J (1977) The structure and properties of collagen. In: Ward AG, Courts A (eds) The Science and Technology of Gelatin, London, Academic Press, pp 1–31Barone JR, Schmidt WF (2006) Nonfood applications of proteinaceous renewable materials. J Chem Education 83(7): 1003–1009Barone JR, Schmidt WF, Liebner CFE (2005) Thermally process keratin films. J Applied Polymer Sci 97: 1644–1651.Bigi A, Cojazzi G, Panzavolta S, Roveri N, Rubini K (2002) Stabilization of gelatin films by crosslinking with genipin. Biomaterials 23: 4827–4832Brault D, D’’Aprano G, Lacroix M (1997) Formation of free-standing sterilized edible films from irradiated caseinates. J Agric Food Chem 45: 2964–2969Brooks M (2006) Forgotten fibres: issues in the collecting and conservation of regenerated protein fibres. In: Rogerson C, Garside P (eds) The Future of the Twentieth Century: Collecting, Interpreting and Conserving Modern Materials, London, Archetype, pp 33–40Brother GH (1940) Casein plastics. Ind Eng Chem January 32(1): 31–34Cagri A, Ustunol Z, Ryser ET (2004) Antimicrobial edible films and coatings. J Food Protection 67(4): 833–848Caner C (2005) Whey protein isolate coating and concentration effects on egg shelf life. J Sci Food and Agric 85: 2143–2148Chambi H, Grosso C (2006) Edible films produced with gelatin and casein cross-linked with transglutaminase. Food Research International 39: 458–466Chang YP, Cheah PB, Seow CC (2000) Plasticizing-antiplasticizing effects of water on physical properties of tapioca starch films in the glassy state. J Food Sci 65(3): 445–451Cho SY, Rhee C (2004) Mechanical properties and water vapor permeability of edible films made from fractionated soy proteins with ultrafiltration. Lebenem Wiss u Technol 37: 833–839Comstock KD, Farrell D, Godwin C, Xi Y (2004) From hydrocarbons to carbohydrates: Food packaging for the future. Journal name volume pages ?Retrieved on January 30, 2006, from the University of Washington Environmental Management Certificate Program website: http:// depts.washington.edu/poeweb/gradprograms/envmgt/index.htmlCurley DM, Unruh JJ, Farrell HM (1998) Changes in secondary structure of bovine casein by FTIR spectroscopy. J Dairy Sci 81: 3154–3162Damodaran S (1996) Amino acids, peptides and proteins. In: Fennema O (ed) Food Chemistry. New York, NY, Marcel Dekker, pp 321–430Dangaran KL, Krochta JM (2003) Aqueous whey protein coatings for panned products. Manufacturing Confectioner 83(1): 61–65Dangaran KL, Krochta JM (2007) Preventing the loss of tensile, barrier and appearance properties caused by plasticizer crystallization in whey protein films. Internation J Food Sci Technol 42(9): 1094–1100Dangaran KL , Tomasula PM (2006) Empirical modeling (in preparation)Dangaran KL, Cooke P, Tomasula PM (2006) The effect of protein particle size reduction on the physical properties of CO2-precipitated casein films. J Food Sci 71(4): E196–E201
2 Structure and Function of Protein-Based Edible Films and Coatings 53Debeaufort F, Quezada-Gallo JA, Voilley A (1998) Edible films and coatings: Tomorrow’s packagings: A review. Crit Reviews Food Sci and Nutr 38(4): 299–313deWit JN, Klarenbeek G (1983) Effects of various heat treatments on structure and solubility of whey proteins. Journal of Dairy Science 67: 2701–2710EPA (2006) Municipal Solid Waste in the United States: 2005 Facts and Figures (Executive Summary)Etzel MR (2004) Manufacture and use of dairy protein fractions. J Nutrition 134: 996S–1002SFarrell HM, Qi PX, Wickham ED, Unruh JJ (2002) Secondary structural studies of bovine caseins: structure and temperature dependence of beta-casein phosophopeptide (1-25). J Protein Chem 21: 307–321Fennema O, Kester JJ (1991) Resistance of lipid films to transmission of water vapor and oxygen. In: Levine H, Slade L (eds) Water Relationships in Food., New York, NY, Springer, pp 703–719Finlay MR (2004) Old efforts at news uses: a brief history of the chemurgy movement and the American search for biobased materials. J Industrial Ecol.ogy 7: 33–46FitzGerald RJ, Murray BA, Walsh DJ (2004). Hypotensive peptides from milk proteins. The Journal of Nutrition 134: 980S–988SFrinnault A, Gallant DJ, Bouchet B, Dumont JP (1997) Preparation of casein films by a modified wet spinning process. J Food Sci 62(4): 744–747Galani D, Apenten RKO (1999) Heat-induced denaturation and aggregation of beta-lactoglobulin: kinetics of formation of hydrophobic and disulphide-linked aggregates. International J Food Sci Technol 34: 467–476.Galietta G, Gioia LD, Guilbert S, BCuq B (1998) Mechanical and thermomechanical properties of films based on whey proteins as affected by plasticizer and crosslinking agents. J Dairy Sci 81: 3123–3130Gennadios A, McHugh TH, Weller CL, Krochta JM (1994) Edible coatings and films based on proteins. In: Krochta JM, Baldwin EA, Nisperos-Carriedo MO (eds) Edible Coatings and Films to Improve Food Quality., Lancaster, PA, Technomic, pp 201–278Gettens RJ, Stout GL (1984) Painting Materials: A Short Encyclopedia. Courier Dover Publications, New York, NYHaard NF, Chism GW (1996) Characteristics of edible plant tissue. In: Fennema O (ed) Food Chemistry. Marcel Dekker, New York, NY, p 1067Haug IJ, Draget KI, Smidsrod O (2004) Physical and rheological properties of fish gelatin compared to mamalian gelatin. Food Hydrocolloids 18: 203–213Hernandez VM (2007) Thermal properties, extrusion and heat-sealing of whey protein edible films. Ph.D. thesisUniversity of California, DavisHernandez VM, Reid DS, McHugh TH, Berrios J, Olson D, Krochta JM (2005) Thermal transi- tions and extrusion of glycerol-plasticized whey protein mixtures. IFT Annual Meeting and Food Expo, New Orleans, LAHernandez VM, McHugh TH, Berrios J, Olson D, Pan J, Krochta JM (2006) Glycerol content effect on the tensile properties of whey protein sheets formed by twin-screw extrusion. IFT Annual Meeting and Food Expo, Orlando, FLHochstetter A, Talja RA, Helen HJ, Hyvonen L, Jouppila K (2006) Properties of gluten-based sheet produced by twin-screw extruder. Lebenam Wiss u Technol 39: 893–901Howell NK (1995) Synergism and interactions in mixed protein systems. In: Harding E, Hill SE, Mitchell JR (eds) Biopolymer Mixtures. Nottingham University Press, Nottingham pp 329–347Kaya S, Kaya A (2000) Microwave drying effects on properties of whey protein isolate edible films. J Food Eng 43: 91–96Kelley HW (1993) Always something new. USDA Miscellaneous Publication Number 1507Kinsella JE (1982) Relationships between structure and functional properties of food proteins. In: Fon and Codon ed. Food Proteins, Springer 51–104Kinsella JE (1984) Milk proteins: Physicochemical and functional properties. Crit Reviews Food Sci and Nutr 21(3): 197–262
54 K. Dangaran et al.Kinsella JE, Whitehead DM (1989) Proteins in whey: chemical, physical, and functional properties. Advances in Food and Nutrition Research 33: 343–427Kinsella JE, Whitehead DM, Brady J, Bringe NA (1989) Milk Proteins: Possible relationships of structure and funtion. In PF Fon ed. Developments in Dairy Chemistry, New York, Elsevier 55–96 .Kiplinger J (2003) Meet the Azlons from A to Z: Regenerated & rejuvenated. Fabrics.net January/ FebruaryKock J (2006) Physical and Mechanical Properties of Chicken Feather Materials. M.S. thesis, Georgia Tech p 114Kozempel M, Tomasula PM (2004) Development of a continuous process to make casein films. J Agric Food Chem 52(5): 1190–1195Kozempel M, McAloon AJ, Tomasula PM (2003) Drying kinetics of calcium caseinate. Journal of Agricultural and Food Chemistry 51(3): 773–776Krochta JM, Baldwin EA, Nisperos-Carriedo MO (1994) Edible Coatings and Films to Improve Food Quality. CRC Press LLC, Boca Raton, FLKunte LA, Gennadios A, Cuppett SL, Hanna MA, Weller CL (1997) Cast films from soy protein isolates and fractions. Cereal Chem 74(2): 115–118Lacroix M, Le TC, Ouattara B, Yu H, Letendre M, Sabato SF, Mateescu MA, Patterson G (2002) Use of gamma-irradiation to produce films from whey, casein, and soya proteins: structure and functionals characteristics. Radiation Physics and Chemistry 63: 827–832Lagaron JM, Cabedo L, Cava D, Feijoo JL, Gavara R, and Gimenez E (2005) Improving packaged food quality and safety Part 2: Nanocomposites. Food Additives and Contaminants 22(10): 994–998.Larkins BA, Lending CR, Wallace JC (1993) Modification of maize-seed-protein quality. American Journal of Clinical Nutrition. 58: 264S–269S.Le Tien C, Vachon C, Mateescu MA, Lacroix M (2001) Milk protein coatings prevent oxidative browning of apples and potatoes. J Food Sci 66(4): 512–516.Lee SY, Dangaran KL, Krochta JM (2002a) Gloss stability of whey-protein/plasticizer coating formulations on chocolate surface. J Food Sci 67(3): 1121–1125Lee SY, Dangaran KL, Guinard JX, Krochta JM (2002b) Consumer acceptance of whey-protein-coated as compared with shellac-coated chocolate. J Food Sci 67(7): 2764–2769Lee SY, Krochta JM (2002) Accelerated shelf-life testing of whey-protein-coated peanuts analyzed by static headspace gas chromatography. J Agric Food Chem 50(7): 2022–2028Lee SY, Trezza TA, Guinard JX, Krochta JM (2002c) Whey-protein-coated peanuts assessed by sensory evaluation and static headspace gas chromatography. J Food Sci 67(3): 1212Lin SY, Krochta JM (2006) Whey protein coating efficiency on mechanically roughened hydrophobic peanut surfaces. J Food Science 71(6): E270–E275Lim LT, Mine Y, Tung MA (1998) Transglutaminase cross-linked egg white protein films: tensile properties and oxygen permeability. J Agric Food Chem 46: 4022–4029.Liu X, Powers JR, Swanson BG, Hill H, Clark S (2005) Modification of whey protein concentration hydrophobicity by high hydrostatic pressure. Innovative Food Science and Emerging Technology 6: 310–317Mahmoud R, Savello P (1992) Mechanical properties of and water vapor transferability through whey protein films. J Dairy Science 75: 942–946Marsh K, Bugusu B (2007) Food packaging – roles, materials, and environmental issues. J Food Science 72(3): R39–R55McHugh TH, Krochta JM (1994) Plasticized whey protein edible films: water vapor permeability properties. J Agric Food Chem 59(2): 416–419Min S, Harris LJ, Krochta JM (2006a) Inhibition of Salmonella enterica and Escherichia coli O157:H7 on roasted turkey by edible whey protein coatings incorporating lactoperoxidase system. J of Food Protection 69(4): 784–793Min S, Rumsey TR, Krochta JM (2006b) Lysozyme diffusion in smoked salmon coated with whey protein films incorporating lysozyme. IFT Annual Meeting and Food Expo, Orlando, FL
2 Structure and Function of Protein-Based Edible Films and Coatings 55Mine Y (1995) Recent advances in the understanding of egg white protein functionality. Trends in Food Sci Technol 6: 225–232Mine Y, Noutomi T, Haga N (1990) Thermal induced changes in egg white proteins. J Agric Food Chem 38: 2122–2125Minifie B (1989) Chocolate, Cocoa and Confectionery: Science and Technology. Springer Publishing, New York, NYMorara CI, Lee TC, Karwe MV, Kokini JL (2002) Plasticizing and antiplasticizing effects of water and polyols on a meat-starch extruded matrix. J Food Science 67(9): 3396–3401Morr CV, Ha EYW (1993) Whey protein concentrates and isolates: processing and functional properties. Crit Reviews Food Sci and Nutr 33(6): 431–476Obuz E, Herald TJ, Rausch K (2001) Characterization of extruded plant protein and petroleum-based packaging sheets. Cereal Chemistry 78(1): 97–100Okamoto S (1978) Factors affecting protein film formation. Cereal Foods World 23: 256–262Olabarrieta I, Gallstedt M, Ispizua I, Sarasua JR, Hedenqvist MS (2006) Properties of aged montmorrillonite-wheat gluten composite films. J Agric Food Chem 54: 1283–1288Olivas GI, Barbosa-Canovas GV (2005) Edible coatings for fresh-cut fruits. Crit Reviews Food Sci and Nutr 45: 657–670Ouattara BS, Sabato SF, Lacroix M (2002) Use of gamma-irradiation technology in combination with edible coating to produce shelf-stable foods. Radiation Physics and Chemistry 63: 305–310Panyam D, Kilara A (1996) Enhancing the functionality of food proteins by enzymatic modification. Trends in Food Sci Tech 7: 120–125Perez-Gago MB, Krochta JM (2000) Drying temperature effect on water vapor permeability and mechanical properties of whey protein–lipid emulsion films. J Agric Food Chem 48(7): 2687–2692Perez-Gago MB, Krochta JM (2001) Lipid particle size effect on water vapor permeability and mechanical properties of whey protein/beeswax emulsion films. J of Agric Food Chem 49(2): 996Perez-Gago MB, Nadaud P, Krochta JM (1999) Water vapor permeability, solubility, and tensile properties of heat-denatured versus native whey protein films. J Food Sci 64(6): 1034–1037Perez-Gago MB, Serra M, Alonso M, Mateos M, Del Rio MA (2003) Effect of solid content and lipid content of whey protein isolate-beeswax edible coatings on color change of fresh-cup apples. J Food Sci 68(7): 2186–2191Petruccelli S, Anon MC (1994) Relationship between the method of obtention and the structural and functional properties of soy protein isolates 1. Structural and hydration properties J Agric Food Chem 42: 2161–2169Qi PX, Cooke P, Dangaran KL, Tomasula PM (2006) Characterization of casein films made by pressurized carbon dioxide: salt effect on water solubility. 97th AOCS Ann Meeting & ExpoRampon V, Robert P, Nicolas N, Dufour E (1999) Protein structure and network orientation in edible films prepared by spinning process. J Food Sci 64(2): 313–316Renkema JM, Vliet TV (2002) Heat-induced gel formation of soy proteins at neutral pH. J Agric Food Chem 50: 1569–1573Rogers CE (1985) Permeation of gases and vapours in polymers. In: Comyn J (ed) Polymer Permeability. J. Comyn. Kluwer Academic Publishers, London, 11–74Sabato SF, Ouattara FB, Yu H, D’’Aprano G, Le Tien C, Manteescu MA, Lacroix M (2001) Mechanical and barrier properties of cross-linked soy and whey protein based films. J Agric Food Chem 49: 1397–1403Sawyer L, Kontopidis G, Wu SY (1999) Beta-lactoglobulin – a three-dimensional perspective. Internation J Food Sci Tech 34: 409–418Schmidt WF (1998) Innovative feather utilization strategies. 1998 National Poultry Waster Management Symposium, Springdale, ARShukla R, CHheryan M (2001) Zein: the industrial protein from corn. Industrial Crops and Products 13: 171–192
56 K. Dangaran et al.Sonneveld K (2000) What drives (food) packaging innovation. Packaging Technol Sci 13: 29–35Sothornvit R, Krochta JM (2000) Plasticizer effect on oxygen permeability of beta-lactoglobulin films. J Agric Food Chem 48: 6298–6302Sothornvit R, Krochta JM (2001) Plasticizer effect on mechanical properties of beta-lactoglobulin films. J Food Eng 50(3): 149–155Subirade M, Kelly I, Gueguen J, Pezolet M (1998) Molecular basis of film formation from a soybean protein: Comparison between the conformation of glycinin in aqueous solution and in films. International J Biol Macro 23: 241–249Swaisgood HE (1993) Review and update of casein chemistry. J Dairy Sci 76: 3054–3061Swaisgood HE (1996) Characteristics of milk. In: Fennema O (ed) Food chemistry. Marcel Dekker, New York, NY, p 1067Ternes W (2001) Egg proteins. In: Sikorski Z (ed) Chemical and functional properties of food proteins. CRC Press, Boca Raton, FL, CRC Press, p 415Tomasula PM, Craig JC, Boswell RT, Cook RD, Kurantz MJ, Maxwell M (1995) Preparation of casein using carbon dioxide. J Dairy Sci 78: 506–514Truong VD, Clare DA, Catignani GL, Swaisgood HE (2004) Cross-linking and rheological changes of whey proteins treated with microbial transglutaminase. J Agric Food Chem 52: 1170–1176Vachon C, D’’Aprano G, Lacroix M, Letendre M (2003) Effect of edible coating process and irradiation treatment of strawberry fragaria spp. on storage-keeping quality. J Food Sci 68(2): 608–611Yildirim M, Hettiarachchy NS (1998) Properties of films produced by cross-linking whey proteins and 11S globulin using transglutaminase. J Food Sci 63(2): 248–252Yoshino T, Isobe S, Maekawa T (2002) Influence of preparation conditions on the physical properties of zein films. J Am Oil Chem Soc 79(4): 345–349Zhang J, Mugara P, Jane J (2001) Mechanical and thermal properties of extruded soy protein sheets. Polymer 42: 2569–2578Zhu Y, Rinzema A, Tramper J, Bol J (1995) Microbial transglutaminase–a review of its production and application in food processing. Applied Micro Biotech 44: 277—282
58 M.B. NietoFig. 3.1 Intermolecular hydrogen bonding formed during hydration of gums in waterFig. 3.2 A simple lab process for making gum films
3 Structure and Function of Polysaccharide Gum-Based Edible Films and Coatings 59 Figure 3.2 shows a simple process of making films from polysaccahide gums.The gum is first dissolved in water at a suitable concentration to make it thickenough to cast, typically between 6,000 and 10,000 cP. Then, using a casting knife,a thin, uniform layer of slurry is drawn on a smooth surface such as a glass plate, apiece of stainless steel, or even a plastic sheet. The film is then dried to the propermoisture or humidity level, and peeled. Whether or not the film peels away from thecasting plate depends largely on the type of gum polymer used and also on the thick-ness of the cast. Interestingly, the solubility of gum-based films takes after the solu-bility of the original gum polymer from which it is made. Gums that dissolve in coldwater like methylcellulose, alginate, carboxymethylcellulose (CMC) and others willproduce films that are likewise cold water-soluble. Gums that require heat for dis-solution, like agar, will form films that are cold water insoluble. Those gums that areonly partially soluble in cold water such as kappa- and iota-carrageenan, gellan andlocust bean gum, will produce films with the same similar solubility. Why and how these polysaccharides produce different types of film structures willbe discussed in detail in this chapter. Hydration properties, solubilities and intermo-lecular chain associations of polysaccahide gums will be discussed in relation to theirrespective chemical structures to explain variations in film-forming properties.3.2 Structure and Film Forming Properties of PolysaccharidesThe unique means by which gums interact with water is the basis for their moretechnical name, hydrocolloids. Hydrocolloids are polymers of high average molec-ular weight, ranging from ~2,000 (e.g., inulin) to >2 million (e.g., xanthan, konjac,guar, b-glucan). Gum polymers are either linear consisting of one sugar monomeror linear consisting of a repeating dimer; linear a sugar side chain on the linearbackbone; or branched consisting of a mixture of different sugars. In addition,polysaccharides can exhibit either a neutral charge (e.g., acetate esters, methylethers, other neutral sugars), negative charge (e.g., carboxylate, sulfate groups), orpositive charge (e.g., amino groups) due to the presence various chemical groupsattached to individual monosaccharide units. All of these structural features ofpolysaccharides contribute to their differences in solubility; synergy or incompatibi-lity with each other or with other ingredients (e.g., proteins, minerals, acids andlipids); thickening, gelling, and emulsifying properties; and, more importantly,their film-forming properties. Table 3.1 summarizes several of these characteristicsand properties for some polysaccharide gums.3.2.1 Linear, Neutral PolysaccharidesAmong the various gums, linear and neutral polysaccharides generally exhibit thebest film-forming properties, and provide the greatest film strength. Because of
60Table 3.1 Chemical and physical properties of gums polysaccharides for use in edible films and coatings Viscosity, cP Other structuralGum 1% at 25°C Sugar composition features Ionic charge Class Film forming/other propertiesGum Arabic 2–5 Galactose, arabinose, rhamnose, Highly branched Anionic Natural Cold water soluble, dissolves up to 55%, glucuronic acid, Arabino-galactan- weak non-cohesive film, form flakes protein complex (AGP)Karaya 400–1,200 Glacturonic aicd, galactose, rhamnose, Branched Anionic Natural Cold water soluble, dissolves up to glucuronic acid 5–8%, weak film non-cohesive film, form flakesGhatti 30–100 Galactose, arabinose, mannose, xylose, Branched Anionic Natural Cold water soluble, dissolves up to glucuronic acid ~5–8%, weak non-cohesive film, form flakesLarch 2–4 Arabinose, galactose Highly branched Anionic Natural Cold water soluble, dissolves up to 60%, weak non-cohesive film, form flakesi-Carrageenan 1,000–2,000 l-galactose, 3,6-anhydrogalactose Linear, sulfate Anionic Natural Thickens cold but requires ~65°C or substitution higher to fully hydrate, dissolves up to 8%, moderately strong film M.B. Nieto
3 Structure and Function of Polysaccharide Gum-Based Edible Films and Coatings 61their linear and non-ionic natures, polymer chains can associate more intimately(through intermolecular hydrogen bonding) to produce stronger films. However, nomatter the gum, the first requirement is to ensure that the gum is fully hydrated ordissolved in water, with or without heating. Once hydrated, polymer chains mayarrange themselves in an ordered fashion to form intermolecular networks neededfor film formation. Several examples of linear, neutral gums possessing appropriatestructural features for film formation include agar, curdlan and cereal b-glucan.Other examples include methylcellulose, hydroxypropyl methylcellulose (HPMC),gellan, and konjac glucomannan, all of which have methyl, hydroxypropyl, acyl oracetyl substituents covalently attached to their individual sugar molecules. Thoughalso linear and nonionic, cellulose and microcrystalline cellulose are insoluble inwater, and require sodium hydroxide and sodium sulfide treatments at high tem-peratures and pressures to separate the cellulose fibers and partially hydrate themolecules for film structures to form. Cellulose and microcrystalline cellulose,however, can be used in conjunction with soluble gum polymers to alter thestrength, melting characteristics, and solubility of the finished film.22.214.171.124 Agar [E406; CAS#64-19-7; 21CFR 182.101; FEMA# 2006]Agar is extracted from two major commercial sources of red seaweed: Gelidium sp.and Gracilaria sp. It consists of a mixture of agarose (gelling fraction) and agaro-pectin (non-gelling fraction), which is slightly branched and sulfated. In the com-mercial manufacture of food grade agar, most of the agaropectin is removed duringprocessing; hence, commercial agars are mainly composed of the agarose fraction.Agarose is a linear polymer with a molecular weight of about 120,000, and is com-posed of a repeating dimer of d-galactosyl and 3,6-anhydro-l-galactosyl units con-nected via alternating a-(1→3) and b-(1→4) glycosidic linkages (Labropouloset al. 2002). Its structural formula is depicted in Fig. 3.3. Most applications for agar are based on its gelling ability and the fact that it ismore stable to low pH and high temperature conditions compared to other gellingsystems. Gelation results from formation of a network of agarose double helices,forming junction zones. These double helices are stabilized by the presence of watermolecules bound inside the double helical cavity (Labropoulos et al. 2002). Exteriorhydroxyl groups allow for aggregation of these double helices via intermolecularhydrogen bonds, upon cooling of agar solution. In this aggregation process suprafib-ers (consisting of up to 10,000 double helices) are formed, and contribute to thestrength of agar films. Agar solution gels at a temperature range of 90–103°C; so,when making an agar film, the solution and casting surface need to be maintainedabove the agarose gel-setting temperature to avoid premature gelation. Agar film is clear and strong, but is insoluble in water under ambient conditions,just like the parent agar. The linear, nonionic nature of agar allows hydrated mole-cules to associate more intimately, forming a network that is stabilized by intensiveintermolecular hydrogen bonding during drying of the film. The dried film is strongenough to peel off the belt or casting surface in one piece when a 4% solution of agar
62 M.B. NietoFig. 3.3 Molecular structure of agarose and picture of its film, cast from a 4% solution and thick-ness of 20 mils (0.02 in. or 508 mm)is cast at a thickness of 20 mils (0.02 in.). Tensile strength, across a 2.5 cm widestrip, and puncture strength values for this film were 2,540 g and 2,150 g of force,respectively. In comparison, films of many other gums would be too weak to peeloff in one piece at this concentration and casting thickness, and would be requiredto be cast at twice the thickness possible for agarose films, or greater. However, itwas not possible to produce a solid film with agar by casting its 4% solution at athickness of 10 mils (0.01 in.), although its film at 20 mils was stronger than that ofmethylcellulose. In general, agar films are brittle and lack elasticity or stretch.126.96.36.199 Methylcellulose [E461; CAS#99638-59-2; 21 CFR§182.1480; FEMA 2696]Cellulose is the most abundant biomass resource on earth. It is the insoluble mate-rial found in plant cell walls of all fruits and vegetables, and is present in the leaves,trunks, and barks of higher plants as a structural component. Cellulose is the sourceof cotton used as clothing material, and also contributes significantly to the insolu-ble dietary fiber intake of the human diet. Cellulose derived from pine trees and cotton linters is used as the base materialfor a number of highly functional water-soluble cellulose derivatives. These deriva-tives possess wide-ranging properties, which are dependent on the type and degreeof derivatization. Chemical modification of cellulose introduces various chemicalgroups onto the hydroxyl groups of glucose units, posing steric hindrance to nativeintermolecular interactions of cellulose. Methyl, carboxymethyl, and hydroxypropylcellulose ethers provide both nonionic and anionic modified derivatives that possessunique functional properties, such as thermal gelation and superior clarity.
3 Structure and Function of Polysaccharide Gum-Based Edible Films and Coatings 63Fig. 3.4 Molecular structure of methylcellulose and picture of its film, cast from a 3% solutionand thickness of 10 mils (0.01 in. or 254 mm) and 20 mils (0.02 in. or 508 mm) Methylcellulose is a chemically-derived cellulose ether with a methyl degree ofsubstitution of 1.6–1.9 on O-6, O-2 or O-3 positions of glucose units (Fig. 3.4). It isboth linear and nonionic. The addition of methyl ether groups to the cellulose back-bone opens up its structure, and because of steric hindrance, methylcellulose doesnot re-associate into microfibrils when dried, unlike its insoluble parent cellulose.This chemical substitution is what gives methylcellulose its solubility in cold water,by opening it up for hydration and hydrogen bonding with water. Although substitu-tion reduces the number of free hydroxyl groups on cellulose molecules, methylether groups still provide sites for hydrogen bonding with water and intermolecularhydrogen bonding. Because of its linear structure, nonionic nature and high degreeof solubility, methylcellulose films are strong and clear. Methylcellulose is unique in the sense that, although it completely dissolves incold water and forms a clear solution, it gels upon heating between 48° and 64°C,depending on grade. The gelling phenomenon is a stage in the flocculation process,where methylcellulose molecules are losing their water or hydration, causing mol-ecules to pack or associate more intimately. Depending on the concentration, how-ever, the heated methylcellulose solution can either hold the gel or can completelyfall out and settle. For a 2% solution of high viscosity methylcellulose in water(~6,000–8,000 cP), the heated solution will hold an intact gel, but will show somedegree of syneresis or weeping. At lower concentrations, or in the presence of com-peting solutes or interfering insoluble solids, the methylcellulose can completely fallout of solution. As the solution cools, methylcellulose re-dissolves and will thickenagain. Methylcellulose is stable over the pH range of 3–11 (Murray 2000). When a 3% solution of high viscosity methylcellulose is cast at a thickness of 10mils (0.01 in.), its dried film has enough strength to peel off in one piece, likeagar. Pictures of methylcellulose films cast at 10 and 20 mils are shown in Fig. 3.4.
64 M.B. NietoThese films had tensile strengths of 760 g and 1,400 g and puncture strengths of350 g and 830 g, respectively. In contrast to agar and the other films discussed here,methylcellulose films provide some stretch when pulled, which property is also truefor films of other derivatized forms of cellulose, such as HPMC and the non-foodgrade ethylhydroxyethylcellulose (EHEC).188.8.131.52 Hydroxypropylmethylcellulose [E464; CAS#9004-65-3; 21 CFR 172.874]HPMC is also included in the group of compounds known as cellulose ethers. It ismanufactured by first reacting purified cellulose with alkylating reagent (methylchloride) in the presence of base, typically sodium hydroxide, and an inert diluentto form methylcellulose. The addition of base, in combination with water, activatesthe cellulose matrix by disrupting its crystalline structure and increasing the accessof polymer hydroxyl groups to the alkylating agent to promote the etherificationreaction. This activated matrix is called alkali cellulose (Kirk-Othmer 1993). Onceactivated, the methylcellulose is then further reacted with the staged addition of analkylene oxide, which in the case of HPMC, is propylene oxide (Kirk-Othmer1993; Dow Chemical 2002). Hydroxypropylmethylcellulose (HPMC) is essentially the same as methylcellu-lose in structure, except that in addition to methyl substitution, some of the remainingfree hydroxyl groups of glucose are substituted with hydroxypropyl groups(Fig. 3.5), which further opens up the cellulose molecule. HPMC is soluble in coldFig. 3.5 Molecular structure of HPMC and picture of its film, cast from a 3% solution and thick-ness of 20 mils (0.02 in. or 508 mm)
3 Structure and Function of Polysaccharide Gum-Based Edible Films and Coatings 65water like methylcellulose, but its flocculation temperature is higher (~82°C). Incontrast to methylcellulose, a 2% HPMC solution in water, when heated to 82°C orhigher will cause the hydrated gum to completely fall out of solution. Similar tomethylcellulose, however, it re-dissolves when the water cools down to room tem-perature or lower. HPMC produces a strong film, but not as strong as that of methylcellulose. Likemethylcellulose, its linear structure and nonionic nature are ideal for micelle formationor for film structure development, except that the larger hydroxypropyl groups keeppolymer chains farther apart due to steric hindrance. When a 3% solution of HPMC iscast at a thickness of 20 mils (0.02 in.), a clear film is produced. This film is strongenough to peel off the casting surface in one piece (Fig. 3.5), with a tensile strength of~1,100 g and a puncture strength of ~590 g. These values are relatively low in compari-son with those obtained for methycellulose films tested under the same conditions.184.108.40.206 Konjac Gum [E425; CAS# 37220-17-0]Konjac gum is a hydrocolloid derived from the root of the plant Amorphophallusspp., and is synonymous with konjac mannan and konjac glucomannan. Konjac iscommon to traditional Chinese foods that have a history spanning over 2,000 years,and are also popular health foods in Asian markets. Konjac is a heteropolysaccha-ride consisting of glucose and mannose monosaccharide units in the ratio of 5:8(Shimahara 1975a), connected by b-(1→4) glycosidic bonds (Fig. 3.6). Physicalimages, obtained by atomic force spectroscopy and transmission electronFig. 3.6 Plausible structure of konjac mannan linear chain showing the repeating units (adaptedfrom Maeda et al. 1980). Other proposed repeating structural units are G-G-M-M-M-G-M or G-G-M-G-M-M-M-M (Kato and Matsuda 1969) and G-G-M-M-G-M-M-M-M-M-G-G—M (Maedaet al. 1980; Takahashi et al. 1984). Also shown is a konjac film, cast from a 1.5% solution andthickness of 20 mils (0.02 in. or 508 mm)
66 M.B. Nietomicroscopy, revealed that the konjac glucomannan molecule is an extended, semi-flexible linear chain without branches. This report is in agreement with konjacglucomannan molecular chain parameters determined using the Mark–Houwinkequation by Li et al. (2006). This conclusion, however, is contrary to the molecularstructure proposed for konjac mannan in earlier studies by Shimahara (1975b) andKato (1973), which proposed slight branching, every 50–60 backbone sugar units.In addition, konjac mannan also contains approximately one acetyl ester group per19 sugar residues (Maekaji 1974). The molecular weight of konjac mannan dependson the species, or even variety, of Amorphophallus from which it is extracted and onthe extraction method employed. Sugiyama (1972) reported average molecularweight values of 0.67–1.9 million, depending on the Amorphophallus variety used,while Li et al. (2006) reported an average molecular weight of 1.04 million Daltons.The proposed molecular structure of konjac is shown in Fig. 3.6. Konjac solution gels if it is heated after treatment or exposure to alkali. This gela-tion occurs as a result of the hydrolysis of acetyl groups, which no longer hinderintermolecular hydrogen bonding of chains (Maekaji 1978). A further interestingcharacteristic of konjac gum lies in its synergy with other hydrocolloids. Takigami(2000) reported synergy between konjac mannan and xanthan, forming an elasticgel, and a significant increase in the gel strength of konjac mannan–carrageenan andkonjac mannan-agar mixtures. Furthermore, konjac mannan is unique in that it pro-duces a viscosity as high as 25,000 cP for a 1% solution (Table 3.1), the highestviscosity ever reported for any gum. Solutions of konjac gum are also pH and heatstable, and unlike those of xanthan gum and have smoother texture and flow. Konjac, like other gums with a linear structure, produces strong films. The acetylester groups impart konjac with a slight negative charge and a greater steric hindrancethan hydroxyl group, and to a certain degree, this affects film structure. In fact, theremoval of acetyl ester groups strengthens the intermolecular association of konjacmolecules, such that they form stronger gels and films. This, combined with its highmolecular weight and its nonionic nature, makes konjac a good polymer material foredible films. However, a potential disadvantage of konjac mannan is that it is too vis-cous. A gum needs to be used at the highest possible concentration for processingefficiency. Konjac, however, can only be dissolved in water at relatively lower concen-trations compared to other gums, (e.g., 1.5%), before the solution becomes too vis-cous. Konjac gum is by far the most viscous natural gum, giving a viscosity of up to25,000 cP at 1% concentration in water. Konjac film, made by casting a 1.5% solutionat a casting thickness of 20 mils, has a tensile strength of ~805 g and a puncturestrength of ~630 g. These values are remarkable considering how low the konjac man-nan gum concentration is compared to films prepared from other gums.220.127.116.11 Pullulan [E1204; CAS#9257-02-7; GRAS]Pullulan is a water-soluble, extracellular polysaccharide produced by certain strainsof the polymorphic fungus Aureobasidium pullulans, formerly known as Pullulariapullulans, an organism first described by De Bary in 1866. The basic structure ofpullulan was elucidated from the works of several researchers (Bernier 1958; Bender
3 Structure and Function of Polysaccharide Gum-Based Edible Films and Coatings 67and Wallenfels 1961; Wallenfels et al. 1961, 1965; Bouveng et al. 1962, 1963; Sowaet al. 1963; and Ueda et al. 1963). From the results of these studies, pullulan wascharacterized as a linear polymer of maltotriose subunits (glucose joined by a-(1→4)linkages) connected via a-(1→6) glycosidic linkages. Catley and coworkers subse-quently established the occurrence of a minor percentage of randomly-distributedmaltotetraose subunits in pullulan (Catley et al. 1966; Catley 1970; Catley andWhelan 1971; Carolan et al. 1983), and reported that these subunits were also joinedby a-(1→6) linkages. Commercial production of pullulan began in 1976 byHayashibara Company, Ltd., in Okayama, Japan (Tsujisaka and Mitsuhashi 1993),which remains the principal commercial source of pullulan today. This is the samecompany that petitioned the U.S. FDA for its GRAS status in 2002. The regular occurrence of a-(1→6) linkages kinks the structure of pullulan andinterrupts what would otherwise be a linear starch amylose chain. The unique patternof a-(1→6) linkages between maltotriose subunits gives the pullulan polymer distinc-tive physical properties, such as structural flexibility and high water solubility, resultingin distinct film- and fiber-forming characteristics. Leathers (2003) reported that pullulanfilms and fibers resemble certain synthetic polymers, such as plastics derived frompetroleum, and possess the following unique functional characteristics: (1) oxygenimpermeability in contrast to other polysaccharide films; (2) being edible and biode-gradable, although more expensive than plastics; and (3) highly soluble in water. Pullulan solutions are of relatively low viscosity compared to most gums.Depending on grade, a 25% solution of pullulan could be ~22,000 cP, which ismore viscous than a solution of gum Arabic at the same concentration (~80–120cP), but is significantly less viscous compared to other gums. Comparing the struc-tures of pullulan and gum Arabic, there is no branching in the structure of pullulan;hence, polymer chains are still able to associate and form a much stronger film thangum Arabic, even if almost every third glycosidic linkage in pullulan is a (1→6)linkage that resembles a substitution. Pullulan films are formed by drying a pullulan solution (from 5 to 25%, depend-ing on viscosity grade) cast onto an appropriate smooth surface. As shown in Fig. 3.7,a 25% solution of this grade of pullulan and a casting thickness of 20 mils wasrequired to produce a film that peeled off in one piece. The casting solution had aviscosity of ~22,000 cP, and the resulting film exhibited a tensile strength of ~9,000 gand a puncture strength of ~1,800 g. Pullulan films are clear, highly oxygen-imper-meable, and have excellent mechanical properties (Yuen 1974). Specialty films mayinclude colors or flavors, and decorative pullulan chips are produced for food uses.Alternatively, pullulan may be applied directly to foods as a protective glaze.18.104.22.168 Microcrystalline Cellulose (MCC) [E460(i); CAS#99331-82-5; GRAS]Microcrystalline cellulose (MCC) is produced from cellulose powder, which issubjected to acid hydrolysis to reduce the molecular length of the polymer chainswithin the cellulose microfibers from 1,000–1,500 DP to 200–300 DP (Iijima andTakeo 2000). The chemical structure of MCC is, therefore, the same as that of
68 M.B. NietoFig. 3.7 Molecular structure of pullulan and picture of its film, cast from a 25% solution andthickness of 20 mils (0.02 in. or 508 mm)cellulose, except that MCC chains are a little shorter due to hydrolysis. Anyglucose oligosaccharides that are generated during acid hydrolysis are removed bywashing. Refined MCC wet cake, which contains only pure crystalline regions ofnatural cellulose, is mixed with water, neutralized, and dried to produce powderedMCC grades. This grade is insoluble in water and difficult to swell (requires extensiveshear to break apart crystalline microfibrils due to intermolecular associationsformed on drying). Colloidal grades are also produced by co-processing the wetcake with another hydrocolloid, such as CMC, to coat the crystalline cellulose andminimize re-aggregation of the fibrils during subsequent drying. Hence, this gradecan be dispersed uniformly when mixed in water with adequate shear, a propertythat is used by formulators to mimic the mouthfeel of fat in fat-free and reduced-fat products. Pure MCC does not form a film (Fig. 3.8). When cast and dried, it leaves a pow-dery material similar to the starting MCC. This is because the polymer does notdissolve in water, even with heating. Although linear and non-ionic, MCC needs toopen first and hydrate to form the structure; however, without a chemical treatmentand the harsh pulping process, separation of the individual fibers (or even partialhydration) does not happen. Nevertheless, MCC and cellulose powder can be usedin conjunction with other film formers to alter the resulting film’s properties.22.214.171.124 Inulin [CAS#9005-80-5; GRAS]Inulin is naturally present in many regularly-consumed vegetables and fruits, suchas leek, onion, garlic, chicory, artichoke and banana, but is commercially producedfrom chicory root and Jerusalem artichoke. It consists predominantly of a linearchain of b-(1→2)-linked d-fructofuranose units, attached to a terminal glucose unitin a linkage involving both reducing ends, as in sucrose (Fig. 3.9). Until recently,
3 Structure and Function of Polysaccharide Gum-Based Edible Films and Coatings 69Fig. 3.8 Molecular structure of microcrystalline cellulose and picture showing its lack of film-forming propertiesFig. 3.9 Molecular structure of inulin and picture of its film (scraped and unscraped), cast froma 35% solution and thickness of 20 mils (0.02 in. or 508 mm)native inulin was considered to be a linear molecule; however, using permethylationanalysis, it was shown that native chicory inulin (DP 12) has a very small degree ofbranching (1–2%). This is also true for inulin from Dahlia (DeLeenheer andHoebregs 1994). For chicory inulin, the number of fructose units linked to a
70 M.B. Nietoterminal glucose unit can vary from 2 to 70 (De Leenheer and Hoebregs 1994);Thus, commercial inulin is a mixture of oligomers and polymers. Inulin is a polymer with a relatively much lower molecular weight compared toother partially-hydrolyzed linear gums, such as low viscosity grades of guar, meth-ylcellulose and CMC. Although it is linear and nonionic, inulin does not form agood film. Its solubility at room temperature is only 20–25% (w/w) in water,depending on grade or DP. In hot water, inulin will dissolve at 50% concentrationor higher; but as soon as the solution cools, it starts to crystallize, thicken, and forma consistency of a white sugar icing. When a hot solution of inulin (35%) is cast ona surface, it forms a very uniform, white layer that is harder and stronger than thatof sugar; but it also flakes (Fig. 3.9). In confectionery coatings, the traditional sugarshell over chocolate candy, gum balls, or even the softer sugar shell of jelly beanscan be strengthened by partial replacement of sugar with inulin. Inulin can also beused in combination with sugar alcohols in the panning process to replace sugar insugar-free recipes.3.2.2 Linear, Anionic PolysaccharidesAnionic gums exist as a polymers of: sugar acids (e.g., alginate); sugar unitsbiosynthesized with anionic substituents (e.g., carrageenans); or sugars that arechemically substituted (such as the CMC). The presence of these anionic groupsincreases the polarity and water-solubility of gum polymers, though the inherentcharge weakens intermolecular associations between polymer chains due torepulsion. However, when cast and dried the structure is preserved; hence, allthese gum polymers form good films. The negative charge on molecules preventsgums from forming an excessively tight fiber structure in the dried state, whichcharacteristic allows the polymers to imbibe water readily during the hydrationprocess. Depending on the extent and distribution of charge on polymer mole-cules, the gum is either completely soluble in cold water, as in the case of algi-nate, lambda-carrageenan and the highly-substituted CMC; or only partiallysoluble in water, such as kappa-carrageenan, iota-carrageenan and pectin. Thelatter are all less anionic and, therefore, require heat activation to fully hydratethe polymer molecules. The film-forming properties of these gums are good, despite the presence ofnegative charge, although they may be required to be cast thicker compared tomost nonionic gums. In general, anionic gums do form a structure that is strongenough to hold the film together during peeling from the casting surface. Itappears that the distribution of charge over the length of a linear gum moleculehas less of an effect on film structure and strength than the presence of single ormultiple neutral sugar side chains substituted along a linear backbone chain. Asa general rule, the larger the substitution or the side chain, the greater the sterichindrance and interference to intermolecular association, resulting in a weakerfilm structure.
3 Structure and Function of Polysaccharide Gum-Based Edible Films and Coatings 7126.96.36.199 Sodium Alginate [E401; CAS#9005-38-3; 21CFR184.1724; FEMA 2015]Alginate is extracted from brown seaweed of the family Phaeophyceae. Commercialsources include Laminaria sp., Macroscystis pyrifera, Ascophyllum nodosum,Eclonia sp., Lessonia nigrescens, Durvillae antarctica and Sargassum spp. (Draget2000). Alginate is present in seaweed as a salt of sodium, calcium, magnesium,strontium and barium in gelled form; hence, the first step in the extraction processis to apply an acid treatment to convert alginate into alginic acid, followed by analkali treatment (Na2CO3 or NaOH) to produce water-soluble sodium alginate. Alginates are linear, unbranched polymers containing b-(1→4)-linked d-mannuronicacid (M) and a-(1→4)-linked l-guluronic acid (G) units, and are therefore highly ani-onic polymers. Alginates are not strictly random copolymers, but are instead blockcopolymers. They consist of blocks of both similar and alternating sugar units (i.e.,MMMMMM, GGGGGG and GMGMGMGM) (Fig. 3.10), with each of these blockshaving different conformational structures . For example, the M/G ratio of alginate fromMacrocystis pyrifera is about 1.6:1, whereas that from Laminaria hyperborea is about0.45:1. Alginates may also be prepared with a wide range of average chain lengths(50–100,000 DP) to suit the application. Commercial grades that are high in guluronicacid are usually labeled HG. Gelation of alginate, with calcium or a bivalent ion, is instantaneous. TheG-block responds to calcium cross-linking faster than the M-blocks, because of itsthree-dimensional “egg box” molecular conformation, which structure accommo-dates Ca2+ ions to form salt bridges, corresponding to junction zones betweenadjacent polymer chains (i.e., zipping together of guluronate chains). Nevertheless,mannuronate segments (M-blocks) may also associate through Ca2+ salt bridges,Fig. 3.10 Structure of alginate showing polyguluronic, polymannuronic and alternating guluronic-mannuronic fractions, and picture of its film, cast from a 4% solution and thickness of 20 mils(0.02 in. or 508 mm)
72 M.B. Nietoforming more rigid gels with good heat stability (Donati et al. 2005). When gelationis required, a high guluronic alginate is used, whereas a high mannuronic alginateis used when thickening is the desired attribute. Different viscosity grades of eitherhigh G or high M alginates are commercially produced, and some alginate gradesincorporate a sequestering agent to reduce calcium sensitivity. Sodium alginate forms a decent strong film, despite the negative charge on themolecule (Fig. 3.10). The carboxylate groups make alginate very soluble in water, butthese negative charges do not have as much impact on alginate’s film-forming propertyas the steric hindrance of a substitution. Comparison of negatively-charged gums withdifferent sized substituent groups seems to indicate that charge repulsion has less effecton film structure than steric hindrance as exemplified by sodium alginate and sodium-CMC, the latter forming a weaker film. When cast at 4% concentration and thicknessof 20 mils, the alginate film produced a tensile strength of ~1,500 g and a puncturestrength of ~830 g. However, removing the negative charge by cross-linking thealginate with calcium increased the tensile strength of the resulting film, indicating thatfilm structure forms better without the charge repulsion.188.8.131.52 Carrageenan [E407; CAS# 9000-07-1; 21CFR 172.620; FEMA #2596]Carrageenan is a collective term for polysaccharides extracted from certain speciesof red seaweed of the family, Rhodophycae. Commercial sources are Eucheumaspinosum, Eucheuma cottonii, Gigartina spp. and Chondrus crispus. In terms ofchemical make-up and structure, there are 4 types of carrageenan extracts: kappa I,kappa II, iota and lambda types. Different seaweeds produce different carrageen-ans, with one type being more predominant in any species of seaweed. A purerkappa and iota-carrageenan can be produced following potassium chloride precipi-tation, where kappa and iota fractions are made insoluble, and lambda is removedin the soluble phase. Physical separation of different species of seaweed, or pickingof seaweed contaminants, is also a good way to obtain high-quality fractions. Carrageenans are made up of alternating galactopyranosyl units dimer linked byalternating b-(1→4) and a-(1→3) glycosidic bonds. The sugar units are sulfatedeither at C-2, C-3 or C-6 of the galactose or C-2 of the anhydrogalactose unit (Fig. 3.11).They are similar in structure to agar, except for the presence of 3,6-anhydro-d-ga-lactose rather than 3,6-anhydro-l-galactose units found in agar and the presence ofsulfate groups in carraggeenan. Carrageenans are linear polymers of about 25,000DP with regular but imprecise structures, depending on the source and extractionconditions (Falshaw et al. 2001). The difference between the four types of carra-geenan comes in the degree of sulfation – kappa I being the least sulfated, with 25%sulfate ester content, and the lambda being the most, with 35%. These differencesin sulfation levels give carrageenans varying degrees of negative charge and solu-bility in water. Lambda carrageenan is completely cold-water soluble, while kappa-carrageenan is only partially cold-water soluble and requires heating to 82°C forfull activation. The iota-carrageenan has solubility in between that of lambda- andkappa-types.
3 Structure and Function of Polysaccharide Gum-Based Edible Films and Coatings 73Fig. 3.11 Structural formulas of various carrageenan fractions and pictures of kappa-iota- andlambda-carrageenan films, cast from 4% solutions and thicknesses of 20 mils (0.02 in. or 508 mm)and 40 mils (0.04 in. or 1,016 mm) Refined carrageenans produce clear solutions and, therefore, clear films. Kappa 1,being the least negatively-charged and least soluble in cold water, requires heating to~80–82°C to fully hydrate; but hydrated molecules are more free to associate becauseless repulsion allows for more intermolecular hydrogen bonding, better gelling andslightly stronger film formation upon drying. The dried film is also only partiallysoluble in cold water, similar to the parent carrageenan, which requires heating to~50°C to dissolve. Lambda, on the other hand, being the most soluble in cold waterand most negatively-charged, produces a slightly weaker film than both kappa andiota carrageenan. As might be expected, lambda film dissolves in cold water. Carrageenan films of the kappa-, iota-, and lambda-types are shown in Fig. 3.11.When cast at 4% concentration and a thickness of 40 mils (0.04 in.), the tensilestrength of the kappa-carrageenan film was the highest at 1,940 g, compared to 944g for the iota and 659 g for the lambda films. Thus, kappa, due in part to its lowestrelative degree of sulfate substitution and negative charge, produced the strongest
74 M.B. Nietofilms. However, the puncture strengths of the three carrageenan types were unex-pectedly not significantly different from each other, ranging from 955 to 1,040 g.As expected, solubilities of the resulting films differed markedly, especially betweenlambda-carrageenan and kappa-carrageenan films, the latter being only sparinglysoluble in the mouth.184.108.40.206 Pectin [E440; CAS#7664-38-2; 21CFR184-69-5]Pectin is commercially produced from citrus peel as a by-product from extractionof lime, lemon and orange juices; or from apple pomace, the dried residue remainingafter extraction of apple juice. Pectin is a heteropolysaccharide in its native state,but extraction with hot mineral acid removes most of the neutral sugars such asrhamnose, galactose, arabinose, etc., that comprise the branched or “hairy” regionsof the polymer. Thus, commercial pectin consists of a homopolymeric linear chainof a-(1→4)-d-galacturonic acid units, where the uronic acid group may be eitherfree or esterified with methanol (Fig. 3.12) (Pérez et al. 2000, 2003). By definition,for use in food and pharmaceuticals, pectin contains at least 65% galacturonic acidand methyl galacturonate. By convention, if the degree of methyl esterification (DE) is greater than 50%,the pectin is called high methoxyl (HM) grade or high ester, while if it is less than50%, it is called low methoxyl (LM) or low ester pectin. Depending on how theextraction process is controlled and how much de-esterification occurs, pectin canFig. 3.12 Plausible structure of pectin and picture of its film, cast from an 8% solution and thick-ness of 20 mils (0.02 in. or 508. mm)
3 Structure and Function of Polysaccharide Gum-Based Edible Films and Coatings 75have a degree of esterification as high as 77% or as low as 20%. Low ester pectinwith amidation is also produced commercially. Pectin is used in food mainly for its gelling property, which is influenced byits degree of esterification (DE). Gelation properties also translate into betterinterpolymer chain associations and film formation; therefore, pectins will gener-ally form stronger films when gelation conditions (pH and/or presence of cal-cium) are met. With regard to DE, HM pectin that has a DE greater than 69% isa rapid-set pectin, whereas pectin with a DE of 60–61% is a slow-set pectin.When conditions for gelling are met, rapid-set pectin will gel at a higher tempera-ture and, depending on the cooling rate, will set the product faster than a slow-setpectin. In other words, gelation depends not only on pectin DE, but also on bothtime and temperature. May (2000) reported that HM rapid-set pectin sets at atemperature as high as ~85°C at pH 3.0 or at ~70°C at pH 3.2; while HM slow-setpectin sets at ~58°C at a pH of 2.8 and at ~50°C at pH 3.0. Special grades of HMpectin, with DE between 50 and 60%, are also commercially produced and arereferred to as extra slow-set. To form a gel, HM pectins require a pH below 3.5, with optimum levels around2.8–3.0, and the presence of sugar solids in the range of 60–65%; heating is alsorequired to fully hydrate and activate pectin molecules. Some adjustment of pH isnecessary to cause protonation of unesterified galacturonic acid units to reduce thenegative charge and intermolecular repulsion of pectin molecules. The combinationof a high sugar concentration and the protonation or neutralization of negativecharges on galacturonic acid groups promotes intermolecular associations of poly-mer chains through intermolecular hydrogen bonding, resulting in gel formation. Gelation of conventional LM pectins requires addition of calcium, sugar rangingfrom 20 to 55% and pH levels of 3.0–5.0. Low methoxylpectins (<50% esterified)gel by calcium divalention bridging between adjacent two-fold helical chains,forming the so-called ‘egg-box’ junction zone structures; a minimum of 14–20galacturonic acid residues is required at junction zones (Ralet et al. 2001). Gelstrength increases with increasing Ca2+ concentration, but decreases with increasingtemperature and acidity, or reduction of pH lower than 3.0 (Lootens et al. 2003).Gelation of amidated LM pectin, on the other hand, only requires a calcium sourceand pH adjustment. It works in both sugar-free formulations without sugar solidsand in high Brix jelly recipes containing as high as 80% sugar. Gels produced usingLM pectin are thermoreversible, meaning that they can be re-melted and reformedon cooling. Pectin films are generally not as strong as alginate films. Methyl substitution(a larger group than –COOH) and the presence of some remaining “hairy regions”or branching on pectin molecules seem to pose more steric hindrance to film forma-tion than the smaller uronic acid groups of alginate. Pectin films cast at 8% concen-tration and a thickness of 20 mils (0.02 in.) had a tensile strength of 3,850 g and apuncture strength of 1,120 g. However, compared to alginate at 4% concentrationand a thickness of 20 mils, pectin casted at 8% and 10 mils, gave tensile strengthof 965 g and puncture strength of 28 g demonstrating a significantly weaker film.
76 M.B. Nieto220.127.116.11 Gellan Gum [E418; CAS#7101052-1; 21 CFR 172.665]Gellan gum is a bacterial exopolysaccharide, like xanthan gum, that is produced fromaerobic fermentation of a carbohydrate substrate by the bacterium, Sphyngomonaselodea, previously called Pseudomonas elodea. It is a linear, anionic polymer ofabout 50,000 DP, consisting of a tetrasaccharide repeat of →4)-a-l-rhamnopyranosyl-(1→3)-b-d-glucopyranosyl-(1→4)-d-glucuronopyranosyl-(1→4)-b-d-glucopyrano-syl-(1→. The (1→3)-linked glucose unit possesses a l-glyceryl attached through C-2and acetyl at C-6 (Chandrasekaran and Radha 1995) (Fig. 3.13). Gellan gum may ormay not be de-esterified by alkali treatment to produce the low acyl and high acylgrades, respectively. The functionality of gellan gum depends on its degree of acylation. High acylgellan forms soft, very elastic, transparent, flexible gels, while low acyl gellanforms hard, non-elastic, brittle gels (Sworn 2000). High acyl gellan gel is moreflexible than xanthan–LBG gel and firmer and more brittle than agar gel. Bothgrades produce thermoreversible gels. Though insoluble in cold water, gellan, like carrageenan, swells and thickens asthe solution is heated, but loses viscosity as it fully dissolves. Sworn (2000) sum-marizes other differences between low acyl and high acyl gellans. These include(1) low acyl gellan is fully hydrated between 80°–95°C; high acyl gellan is fullyhydrated at 70°C or higher; (2) low acyl gellan sets between 10 and 60°C, depend-ing on the concentration and presence of ions; high acyl gellan sets at 70°–80°C,both grades showing no hysteresis; (3) low acyl gellan shows improved gellingwhen acids and mono- and divalent ions are added; high acyl gellan is not affectedFig. 3.13 Molecular structure of gellan gum and picture of its film, cast from a 4% solution andthickness of 50 mils (0.05 in. or 1,270 mm)
3 Structure and Function of Polysaccharide Gum-Based Edible Films and Coatings 77by these ions; (4) low acyl gellan experiences reduced firmness and modifiedtexture when sugar is added; high acyl gellan experiences increased gel strengthunder the same conditions. Gellan gum films (Fig. 3.13) are not as strong as those of agar. At 4% concentra-tion and a casting thickness of 20 mils, gellan gives a tensile strength of ~700 g anda puncture strength of ~250 g, values that are significantly less than those observedfor agar film (see Sect. 18.104.22.168). Like agar film, however, gellan film is clear and,like the parent material, is insoluble in cold water. Intuitively, a low acyl gellan gumthat produces stronger gel will also produce a stronger film. If gellan is de-esteri-fied, or all of its acyl groups are removed, the linear gellan polymer could becomecompletely insoluble in cold water like agar, and would require higher temperatureor boiling to dissolve; but de-esterification will result in stronger films.22.214.171.124 Carboxymethylcellulose or Cellulose Gum (CMC) [E466; CAS#:9004-32-4; 21CFR 182.1745]Carboxymethylcellulose (CMC) is a cellulose derivative that is mainly used inmany food applications for its viscosity, water binding properties, and solution clar-ity. There are several available viscosity grades of CMC, ranging from ~50 (2%concentration) to 13,000 cP (1% concentration) in water. For general thickeningapplications, high viscosity grades are chosen for economic reasons, as the price ofCMC is dictated more by the uniformity of esterification rather than the viscosityeach grade provides. However, in other applications like flavored syrups, the rheol-ogy of CMC and absence of graininess in solution, due to unsubstituted and insolu-ble regions in the molecule, are sufficient reasons to use the lower viscosity grades,which are less prone to this problem. In film applications, low viscosity CMC ispreferred over viscous grades, because higher gum concentrations can be achievedin casting solutions. The CMC structure involves carboxymethyl substitution of the native cellulosepolymer at C-2, C-3 or C-6 positions of anhydroglucose units (Fig. 3.14). Thedegree of substitution (DS) is generally in the range of 0.6–0.95, but the legal limitis a DS of 1.0. The higher the DS, the more soluble and stable the CMC solution.However, the uniformity of substitution along the cellulose backbone also influ-ences the solubility and smoothness of CMC solutions. CMC is anionic due to the terminal carboxylate group that ionizes to COO−when CMC is dissolved in water at neutral pH. It is commercially produced as thesodium salt. At acidic pH levels of 3.0 or less, CMC becomes insoluble and loseswater binding properties. Different viscosity grades for CMC vary in degree ofpolymerization (DP) and molecular weight. Smaller molecules, or low DP pro-ducts, produce lower viscosity solutions than larger molecules, or high DP mole-cules, due to effects of chain length. To a certain extent, molecular weight affectsfilm strength; but, as long as there is sufficient length in the polymer chain, filmstructure will form. For CMC, a DP of 50 is capable of forming a cohesive film at8% concentration.
78 M.B. NietoFig. 3.14 Structure of carboxymethylcellulose and picture of its film, cast from a 3% solutionwith thicknesses of 60 mils (0.06 in. or 1,524 mm) and 80 mils (0.08 in. or 2,032 mm) Figure 3.14 shows CMC films based on a 3% solution and casting thicknesses of60 (0.06 in.) and 80 mils (0.08 in.). The 60-mil film had a tensile strength of 1,920 gand a puncture strength of 1,170 g. In addition to steric hindrance due to carboxymethylsubstitution, negative repulsion between chains further weakens intermolecularassociations and the structure of CMC films. This scenario explains why a 3% CMCsolution had to be cast at 80 mils to form a cohesive film – compared to alginate andmethylcellulose (nonionic), which form cohesive films at 27 and 10 mil film thick-nesses, respectively, using identical concentrations of gum.126.96.36.199 Propylene Glycol Alginate [E405; CAS#9005-38-3; 21CFR172.858; FEMA#2941]Sodium alginate has poor acid stability and is highly sensitive to calcium ions.These properties are drawbacks to many applications because of issues regardingprocessing and timing with premature gelation. These limitations are removedthrough chemical modification of alginate to propylene glycol alginate (PGA). Infact, this chemical modification gives entirely new properties to the native gum. Propylene glycol alginate is chemically derived by treatment of alginate withpropylene oxide under acidic conditions. This treatment introduces a propyleneglycol ester group bonded to the carboxyl groups of guluronic and mannuronicunits (Fig. 3.15). Conversion of alginate, or alginic acid, to PGA reduces themolecule charge to a minimum, and changes the behavior of the polymer in manyways compared to standard alginate. Commercial PGAs are esterified at ~90% orhigher. Esterification makes PGA less calcium sensitive; it thickens to someextent in the presence of calcium ions, but does not gel. PGA also tolerates low
3 Structure and Function of Polysaccharide Gum-Based Edible Films and Coatings 79Fig. 3.15 Molecular structure of propylene glycol alginate and picture of its film, cast from a 4%solution and thickness of 20 mils (0.02 in. or 0,508 mm)pH conditions, and has superior emulsifying and foaming properties relative tonative alginate. Reduction of negative charge, however, does not confer additional tensilestrength to the film, because the propylene glycol ester group is bulkier (relative tothe carboxyl group of native alginate) and impedes inter-polymer chain association.Film formed with PGA is quite strong and peels off in one piece when cast at a 4%concentration and thickness of 20 mils (0.02 in.) (Fig. 3.15). Tensile strength of thisfilm was 990 g and puncture strength was 445 g, which values are lower or weakercompared to those of the film made with sodium alginate using the same experi-mental parameters.3.2.3 Linear, Cationic Polysaccharides188.8.131.52 Chitosan [CAS#9012-76-4]Chitosan is the principal derivative of chitin, the material comprising the exoskel-etons of crustaceans and mollusks, and is produced by alkaline deacetylation ofchitin. Chitosan is poly-b-(1→4)-2-amino-deoxy-d-glucopyranose; its idealizedstructure is shown in Fig. 3.16. Typical commercial chitosan is about 85%deacetylated. In solution, chitosan forms micelle-like aggregates from fullyacetylated segments of polysaccharide chains, interconnected by blocks of almostfully deacetylated polysaccharide, stretched by electrostatic repulsion (Pedroni etal. 2003). Chitosan in the free amine form is insoluble in water at neutral pH.However, it is soluble in glacial acetic acid and dilute HCl, but insoluble in dilutesulfuric acid at room temperature. Chitosan carries a large number of amino groupsalong its chain and is, thus, capable of forming multiple complexes. At acid pH, the
80 M.B. NietoFig. 3.16 Structure of chitosan and picture of its film, cast from a 4% solution and thicknesses of20 mils (0.02 in. or 508 mm) and 40 mils (0.04 in. or 1,016 mm)protonation of –NH2 groups converts them to –NH3+, which can associate withpolyanions to form complexes and bind anionic sites at bacterial and fungal cellwall surfaces. At higher pH levels (>4), chitosan can form complexes with color-ants and heavy metals. These appealing features make chitosan widely applicablein wound healing, production of artificial skin, food preservation, cosmetics, andwastewater treatment (Risbud et al. 2000; Juang and Shao 2002). Chitosan forms strong films. Figure 3.16 shows films made with chitosan at aconcentration of 4% and casting thicknesses of 20 (0.02 in.) and 40 mils (0.04 in.).Film tensile strengths were 1,780 g and 2,970 g, and puncture strengths were 1,500g and 2,035 g, respectively. When a plastic wrap made from chitosan was used forstorage of fresh mangoes, the shelf life of the produce was extended up to 18 days,without any microbial growth and off-flavor (Srinivasa et al. 2002).3.2.4 Linear, Substituted, Neutral PolysaccharidesLinear, substituted gums are polysaccharides with linear backbones and sugarsubstituents that occur mainly on C-6, as in the case of seed gums like fenugreek,guar, tara, locust bean and cassia gum, or C-3 as in the case of xanthan. The sugarsubstituent in seed gums is galactose, a monosaccharide, which is present on16–50% of backbone sugar units, and in xanthan, the substituent is a trisacharride,a larger side chain. Presence of these sugar substituent groups, their frequency ornumber, and size ultimately impact these gums’ solubility, viscosity, and film-forming properties.
3 Structure and Function of Polysaccharide Gum-Based Edible Films and Coatings 8184.108.40.206 Fenugreek [CAS#977155-29-5; FEMA 2484; GRAS as Botanical Substance to Supplement Diet]Fenugreek,1 Trigonella foenum-graecum, is a legume that used to be grown only inthe Mediterranean region, but today it is grown all over the world. It grows up to60 cm in height, branching off with trefoil leaves and little white flowers. It pro-duces sickle-shaped pods, containing 10–20 brownish diamond-shaped seeds witha diameter of 3–4 mm and a deep groove in the middle. Traditionally, fenugreek hasbeen used in folk medicine for tonic, nutrition, as an appetizer and an antifebrile. Ithas also been shown to lower cholesterol better than other seed gums, such as guarand locust bean (Evans et al. 1992). Fenugreek gum is simply the milled endosperm of fenugreek seeds, andpossesses a similar sugar composition as guar, tara, locust bean, and cassia gums.Fenugreek is a galactomannan, consisting of a linear chain of mannose linked byb-(1→4) glycosidic bonds, with galactose substitution at the C-6 position (Fig. 3.17).The ratio of mannose to galactose is ~1:1. A linear mannan polymer is completelyinsoluble in water, just like native cellulose. However, galactose substitution infenugreek prevents polymer chains from associating intimately during drying,making it completely soluble in cold water. In fact, fenugreek is the most solubleof the seed gums. However, galactose substitution on every mannose unit in the linear backboneweakens intermolecular hydrogen bonding between polymer chains; thus, it doesnot form a cohesive film at the same concentration and thickness as methycelluloseFig. 3.17 Structure of fenugreek and picture of its film, cast from a 3% solution and thickness of40 mils (0.04 in. or 1,016 mm)1 http://www.airgreen.co.jp/fenugreek/index_e.html
82 M.B. Nietoor any of the other gums described earlier (Fig. 3.17). Furthermore, the absence ofelectrostatic charge on the fenugreek molecule makes this polymer hydrate slower;nevertheless, fenugreek, like guar gum, achieves full hydration in cold water withtime. The finer the mesh, the faster the fenugreek gum hydrates. The fenugreek film shown in Fig. 3.17 was prepared using a 3% solution and acasting thickness of 40 mils (0.4 in.). This film had a tensile strength of 2,330 g anda puncture of strength of 230 g. Fenugreek possesses the weakest film structure ofall seed gums, due to its relatively denser galactose substitution, that poses moresteric hindrance to inter-polymer chain association.220.127.116.11 Guar Gum [E412, CAS#9000-30-0; 21CFR184.1339; FEMA#2537]Guar gum is the ground endosperm of guar seed from the leguminous shrubCyamopsis tetragonoloba, and is a galactomannan similar to fenugreek, tara andlocust bean gum. It consists of a linear mannose chain linked by ß-(1→4) glyco-sidic bonds, with galactose substitution at the C-6 position of approximately everyother mannose unit (Fig. 3.18). Guar gum is a nonionic polymer, consists of longerchain molecules (DP 10,000) than those found in locust bean gum. Higher galac-tose substitution of guar gum compared to locust bean gum (Petkowicz et al. 1998)increases the solubility of this galactomannan; hence, like fenugreek, guar alsoachieves full hydration in cold water; however, guar dissolves slower. Standard grade of guar gum has a viscosity of ~4,500 cP at 1% in water, makingit by far the most economical thickener for stabilizing foods. It hydrates slowerthan fenugreek, but yields a higher viscosity due to its higher molecular weight. Ithas the same type of short texture as the heated locust bean gum solution. Becauseof its solubility in cold water, guar gum, like fenugreek, will show better stabilityFig. 3.18 Structure of guar gum and a guar gum film, cast from a 3% solution and thickness of40 mils (0.04 in. or 1,016 mm)
3 Structure and Function of Polysaccharide Gum-Based Edible Films and Coatings 83to freeze-thaw cycles than locust bean gum. On thawing, guar gum will regain itswater binding property, whereas locust bean gum will sparingly rehydrate. As ageneral rule, gums that are cold water soluble are also freeze-thaw stable. Galactose substitution in guar also poses steric hindrance, reducing intermolecularhydrogen bonding, but not to the same extent as in fenugreek. Figure 3.18 shows guarfilm, cast at 3% concentration and with a casting thickness of 40 mils (0.04 in.). It gavea tensile strength of 4,580 g and a puncture strength of 655 g, values that are signifi-cantly higher than those of fenugreek film produced under the same conditions.18.104.22.168 Tara Gum [E417; CAS#39300-88-4; GRAS]Tara gum is the ground endosperm of seeds from the tara tree (Cesalpinia spinosaLin). The plant is native to South America, where it grows as a tree or a bush.Today, tara is also cultivated in Morocco and East Africa. Like fenugreek, guar gumand locust bean gum, tara gum is a galactomannan, comprised of approximately25% of galactose and 75% mannose. Galactose substitution in tara gum occurs onapproximately every third mannose unit (Fig. 3.19). Tara gum is partially soluble in cold water, and its solution is more viscous thanthose of either guar gum or carob bean gum at the same concentration. Like carobbean gum, tara gum forms a composite gel, together with xanthan. It also exhibitsgelling synergy with both agar and carrageenan.Fig. 3.19 Structure of tara gum and picture of its film, cast from a 3% solution and thickness of20 mils (0.02 in. and 508 mm)
84 M.B. Nieto Based on steric hindrance, tara gum, which possesses less galactose substitutionthan fenugreek and guar, will, therefore, produce a stronger film. A film preparedusing a 3% tara gum and a casting thickness of 20 mils (0.02 in.) as shown in Fig.3.19 peeled off the surface in one cohesive piece, which was not possible with theother two seed gums prepared at the same casting thickness. The tensile strength ofthis film was 1,365 g, and the puncture strength was 390 g.22.214.171.124 Locust Bean Gum (LBG) [E410; CAS#9000-40-2; 21CFR184.1343; FEMA#2648]Locust bean gum, or carob bean gum, is derived from the endosperm of carob seedsfrom the tree Ceratonia siliqua. Chemically, it is a nonionic polysaccharide thatconsists of a linear backbone of mannose linked by b-(1→4)-glycosidic bonds, withthe galactose substitution occurring at the C-6 position of every fourth mannoseunit on average (Fig. 3.20). There are regions of the molecule that are densely sub-stituted and regions where galactose substitution occurs on only every 10–11 man-nose units (Wielinga 2000). The galactose content of locust bean gum is reportedto be between 17 and 26% (Wielinga 2000). The linear mannose chain is quitesimilar to cellulose; hence, without galactose substitution, this gum would beinsoluble in water. The degree and sporadic nature of galactose substitution makeit sparingly soluble in cold water. Heating to 82°C is required to fully activatelocust bean gum; thus, when it is frozen or the solution is re-dried, locust bean gumreverses to being almost insoluble in cold water, like the original material. Therefore,locust bean gum is one gum polymer that can be used to make film that will onlypartially melt in the mouth. Fully hydrated locust bean gum has a viscosity of2,500–3,300 cP at 1% concentration in water and, like all other gums, its viscosityincreases exponentially with concentration.Fig. 3.20 Structure of locust bean gum and picture of its film, cast from a 3% solution and thick-ness of 20 mils (0.02 in. and 508 mm)
3 Structure and Function of Polysaccharide Gum-Based Edible Films and Coatings 85 Locust bean gum exhibits strong synergy with xanthan gum. Neither gum formsa gel when used alone, but together, their water binding properties are dramaticallyimproved. A 60/40 to 50/50 blend of LBG/xanthan yields the most synergistic ratio(Sworn 2000). At concentrations of up to 0.4% of the total gum blend, its heatedsolution shows a pseudoplastic, gel-like behavior. Between 0.4 and 1.0% total gumconcentrations, it is a soft gel; at 1% total gum concentration or higher, it forms anelastic gel that is not prone to syneresis. Locust bean gum is also synergistic with kappa-carrageenan, with the optimumratio being around 20/80 LBG/carrageenan. LBG makes the carrageenan gel moreelastic, as demonstrated by the shift in the fracture point of the gel during compres-sion testing. This synergy also gives stability to the carrageenan gel, allowing itsuse in acidic applications, between pH 3.0 and 5.0. Similar synergy is exhibited byLBG and agar. There is yet another seed gum with the same sugar components that deserves tobe mentioned in this section – cassia gum. It has a lower degree of galactose sub-stitution than locust bean gum. It is obtained from Cassia tora (also known asCassia obtusifolia), and has a mannose to galactose ratio between five and seven.It has a fairly regular substitution pattern (Daas et al. 2000) and even lower solubil-ity in cold water than locust bean gum. It is not currently allowed for general fooduse in the U.S., but it is allowed in pet foods. Periodically, supply of locust bean suffers a cycle of shortage, dramaticallyincreasing its cost. Attempts to engineer guar gum, a low-cost seed gum in the samechemical family, as locust bean gum, by specifically removing some of the pendantgalactose groups using certain a-galactosidases, is a promising approach for creat-ing a viable locust bean gum substitute in times of shortage. Expectedly, locust bean gum film, like tara gum, film peeled off easily whencast at a 3% concentration and thickness of 20 mils (Fig. 3.20). With galactosesubstitution that occurs at about every fourth mannose, vs. every third in tara gum,inter-polymer chain association is less restricted with locust bean gum, resultingin a stronger film structure. Tensile strength of its film was 2,000 g and puncturestrength was 460 g, values that are higher than other seed gum films preparedunder the same conditions.3.2.5 Linear, Substituted, Anionic Polysaccharides126.96.36.199 Xanthan Gum [E415; CAS#11138-66-2; 21CFR172.695;]Xanthan gum is a polysaccharide that is produced by the bacterium, Xanthomonascampestris, during a fermentation process involving a carbohydrate substrate andother growth-supporting nutrients. This gum is actually an excretion to protectbacterial cells when the pH of the fermentation medium becomes too low andunfavorable for growth. It is likely because of this native protective function thatxanthan gum demonstrates superior stability to acid over other gums. It is stable over
86 M.B. NietoFig. 3.21 Structure of xanthan gum as adapted from (Jansson et al. 1975 and Melton et al. 1976)and a picture of its film, cast from a 3% solution and thicknesses of 40 mils (0.04 in. or 1,016 mm)and 80 mils (0.08 in. or 2,032 mm)a wide range of pH, from 1 to 13; very resistant to enzyme hydrolysis; tolerant ofhigh salt, high sugar and high alcohol systems; stable at boiling temperatures; andtolerates retort processing better than most other gums. Xanthan gum is an anionic polymer with a molecular structure that consists of alinear glucose chain linked by b-(1→4) glycosidic bonds; it also possesses a trisac-charide side chain attached through O-3 of alternate glucose units of the main chain(Jansson et al. 1975; Melton et al. 1976). The trisaccharide side chain is composedof an inner mannose unit, partially acetylated at the C-6 position; a glucuronic acidunit; and a terminal mannose unit, partially substituted with pyruvic acid in theform of a 4, 6-cyclic acetal (Fig. 3.21). Glucuronic acid and pyruvate groups confera negative charge to the xanthan molecule. The repeating unit of xanthan, therefore,is a pentamer. Each molecule consists of about 7,000 pentamers. Xanthan gum is soluble in cold water and, like most powders that thicken, itforms lumps if mixed in water with insufficient agitation. It forms a moderatelyviscous solution with water and, at 1% concentration, gives a viscosity between1,200 and 1,600 cP. Xanthan solution is highly pseudoplastic and shows a drasticdecrease in viscosity with increasing shear rate. It can have a soft, gel-like consist-ency, depending on concentration and shear applied, typical of a pseudoplastic fluid.The superior suspending property of xanthan gum is attributed to its weak-gel,shear-thinning properties. It hydrates rapidly in cold water, even in the presence ofhigh levels of sugar, salt or alcohol. The consistent water-holding ability of xanthanmay be used for control of syneresis and to retard ice recrystallization in freeze-thaw
3 Structure and Function of Polysaccharide Gum-Based Edible Films and Coatings 87situations. Xanthan gum shows superior freeze-thaw stability (Giannouli and Morris2000). Its viscosity is relatively unaffected by ionic strength, pH level (1–13), shearor temperature. Xanthan gum is capable of synergistic interactions with glucomannan likekonjac gum, and with galactomannans such as guar, tara and locust bean gums(previously discussed in Sect. 188.8.131.52). With guar, a boost in water binding capacityand viscosity is achieved at all ratios, with the optimum ratio being between 75:25and 80:20 – guar to xanthan. With locust bean gum, optimal synergy and gelationis achieved at 50:50 LBG to xanthan (Goycoolea et al. 2001). Tara gum exhibitssynergy with xanthan intermediate of that achieved with guar and locust beangums. An extreme synergy between xanthan and konjac mannan takes place at anoptimal ratio of 80:20 konjac to xanthan, respectively, with viscosity build-up as highas 161,000 cP at a 1% total gum concentration (Takigami 2000). This noted synergyallows for very low usage levels of this gum combination in food applications. Figure 3.21 illustrates a cohesive xanthan film formed at 3% concentration andcasting thickness of 80 mils (0.08 in.); no film was formed at 40 mils (0.04 in.). Bycomparison, guar gum, with its smaller galactose side chain compared to the trisac-charide side chain of xanthan, produced a cohesive film at 40 mils thickness undersimilar parameters (0.04 in.).3.2.6 Branched PolysaccharidesFilm-forming properties of gum polymers are greatly affected by branching.Although most branched gums have very large molecular weights, their moleculesassume a globular conformation. This shape does not allow the formation of micellesconsisting of polymer chains intimately associated with each other. Although someintermolecular bonding does still take place, it occurs only on a limited basis.Consequently, their films do not have the structural strength, except if cast at exceed-ingly high gum concentrations and film thicknesses. All branched gums – such asthose from gum Arabic, ghatti, karaya and larch gum – will not peel off in one piecewhen cast and dried, but will flake off instead when cast at the same or a signifi-cantly higher concentrations and thickness than the linear polysaccharides.184.108.40.206 Gum Arabic [E414; CAS#9000-01-5; 21 CFR 184.1330; FEMA 2001]Gum Arabic is an exudate from the stems and branches of sub-Saharan Acaciasenegal and Acacia seyal trees that either naturally exude sap or are tapped to formlarge nodules of gum to seal wounds in the bark of the tree. The chemical structureof gum Arabic has been reviewed by Verbeken et al. (2003). Gum Arabic is acomplex and variable mixture of arabinogalactan oligosaccharides, polysaccha-rides, and glycoproteins. Depending on the source, the glycan components contain
88 M.B. Nietoa greater proportion of l-arabinose relative to d-galactose (A. seyal) or d-galactoserelative to l-arabinose (A. senegal). The gum extracted from A. seyal also containssignificantly more 4-O-methyl-d-glucuronic acid, but less l-rhamnose and unsub-stituted d-glucuronic acid, than that from A. senegal (Williams and Phillips2000). Goodrum et al. (2000), as cited by Chaplin (2008), reported that gum Arabic isa highly-branched polymer with a main chain of (1→3)-linked b-d-galactopyrano-syl units, with side chains of (1→3) b-d-galactopyranosyl units joined to it by(1→6) links and with a molecular weight of ~250,000. The side chains are 2–5units in length. Both the main chain and the side chains have attached units of a-l-arabinofuranosyl, a-l-rhamnopyranosyl, b-d-glucuronopyranosyl and 4-O-methyl-b-d-glucuronopyranosyl units. In addition, gum Arabic has a minor fraction of anarabinogalactan-protein (AGP) complex with an MW of ~2.5 × 106 Da. The cova-lently-linked protein, ~2% of the total gum, is rich in hydroxyproline, containing arepetitive and almost symmetrical 19-residue consensus motif – ser-hypa-hypa-hypa-thr-leu-ser-hypb-ser-hypb-thr-hyp-thr-hypa-hypa-hypa-gly-pro-his – with con-tiguous hydroxyprolines (a) attached to oligo-a-1→3-l-arabinofurans andnon-contiguous hydroxyprolines (b) attached to galactose residues of oligo-arabi-nogalactans combining a b-1→3-galactopyran core with rhamnoglucuronoarabi-nogalactose pentasaccharide side chains. Figure 3.22 shows the plausible structure of gum Arabic. The high degree ofbranching makes gum Arabic assume a more globular shape despite its high molec-ular weight, a configuration that prevents the formation of micelles. In solution,gum Arabic molecules have limited sites for intermolecular hydrogen bonding, dueto the extensive branching that deters such interactions from developing. Althoughthe gum dissolves and forms hydrogen bonds with water, it does not effectivelyimmobilize water. The result is a poor thickening property, compared to most lineargums and the lack of film strength when its solution is cast and dried. Comparing A. Senegal and A. seyal gum sources, Naouli (2006) determinedthat the latter is more branched using a Mark–Houwink plot of log intrinsic viscosityvs. log molecular weight. Corollary to this finding, when cast at the same thicknessand concentration, the film of A. seyal is weak and cracks on drying, whereas thefilm obtained from A. senegal, though it also does not peel from the casting surfacein one piece, does not crack on drying. Rather, it remains uniform, coating thesurface like a laminate. The greater branching of the A. seyal is likely to be respon-sible for its weaker, non-cohesive film. Solubility of both films is very good. Thelow viscosity of gum Arabic and the lack of film strength increases its dissolutionin the mouth because it disintegrates faster in the saliva.220.127.116.11 Gum Ghatti [E419; CAS#9000-28-6; 21 CFR 184.1333; FEMA#2519]Gum ghatti, also called Indian gum, is an exudate gum from the tree Anoggeissus latifolia,found in India and Sri Lanka. Its applications are similar to those of gum Arabic in
3 Structure and Function of Polysaccharide Gum-Based Edible Films and Coatings 89Fig. 3.22 Plausible structure of the gum Arabic molecule, showing the main polysaccharidecomponent (AGP complex not shown) and picture of A. seyal and A. senegal films, cast from a35% solution and thickness of 20 mils (0.02 in. or 508 mm)the food and pharmaceutical industries, where it is used as an emulsifier except thatthis gum is much more viscous than gum Arabic and is difficult to spray dry for com-mercial production. Commercial ghatti, therefore, is mainly milled. The structure of gum ghatti has been extensively studied (Aspinall et al. 1955,1958a; Aspinall et al. 1958b, 1965; Aspinall and Christensen 1965). It was foundthat ghatti consists of l-arabinose, d-galactose, d-mannose, d-xylose and d-glu-curonic acid, in a molar ratio of 48:29:10:5:10, respectively; it also has traces ofrhamnose. Tischer et al. (2002) showed that gum ghatti is made up of arabinose,galactose, manose, glucuronic acid and rhamnose, in a molar ratio of 61:39:6:10:6,but xylose was not detected. The polysaccharide has a backbone chain of (1→6)-linked ß-d-galactopyranosyl units, with some (1→4)-d-glucopyranosyluronic acidunits, some joining (1→2)-d-mannopyranosyl units and some l-arabinofuranoseunits (Fig. 3.23). Hanna and Shaw (1941) reported a mean molecular weight of thesoluble portion of gum ghatti to be ~12,000 Da, as determined by osmotic pressuremeasurements. The gum ghatti film does not crack when dried, and provides a uniform laminateon the casting surface prior to scraping. However, like gum Arabic and other branchedgum films, it is not strong enough to peel off in one piece when cast at a concentrationof 5.5% and casting thickness of 20 mils (Fig. 3.23). Because it provides much higherviscosity than gum Arabic, dissolution of ghatti film is not as fast.
90 M.B. NietoFig. 3.23 Plausible structure of gum ghatti (adapted from Tischer et al. 2002) and a gum ghattifilm, cast from a 5.5% solution and thickness of 20 mils (0.02 in. or 508 mm)18.104.22.168 Karaya [E416; CAS#9000-36-6; 21 CFR 184.1349; FEMA#2605]Gum karaya is exuded from Sterculia urens, a bushy tree found in dry regions ofNorth India. Native gum karaya is a branched, acetylated polysaccharide with areported molecular weight of 9–16 million (Le Cerf et al. 1990). Structurally,karaya is heavily acetylated, containing a-d-galacturonic acid and a-l-rhamnoseunits as the main chains, with O-4 of the acid and O-2 of rhamnose linkages, andthe acid is linked by 1, 2 linkage of b-d-galactose or by 1, 3 linkage of b-d-glucuronicacid on side chains, where one half of the rhamnose units carry at O-4 by 1,4 link-age of b-d-galactose units (Stephen and Churms 1995) as shown in Fig. 3.24.Because of its lesser degree of branching and much larger molecular weight com-pared to gum Arabic, karaya solutions exhibit high viscosity, between 400 and1,200 cP for a 1% solution by weight. Karaya film possesses the same limitation as the ghatti film; it lacks adequatetensile strength to peel off from the casting surface in one piece. However, it doescoat surfaces uniformly without cracking when the film dries. It is also tacky andadheres well to the casting surface, a characteristic of most tree exudates. Karayafilm is soluble in cold water, but will dissolve slower in the mouth, due to its highviscosity, much like ghatti film.
3 Structure and Function of Polysaccharide Gum-Based Edible Films and Coatings 91Fig. 3.24 Plausible structure of karaya gum and picture of its film, cast from a 5.5% solution andthickness of 40 mils (0.04 in. or 1,016 mm)22.214.171.124 Larch Arabinogalactan [CAS#9036-66-2; 21 CFR 172.610; FEMA#3254]Larch gum, also known as arabinogalactan, is the polysaccharide derived fromwood of the Western Larch, or Larix occidentalis. Arabinogalactans occur in othertypes of larch, but the grade that is marketed for supplement use comes fromWestern Larch. Larch gum, like other tree exudates, exists as a polydisperse,densely-branched polysaccharide with a molecular weight ranging from 10,000 to120,000 Da. Using compositional and methylation analyses in conjunction with NMR spec-troscopy, Ebringerova et al. (2005) reported that larch gum has the following struc-tural features: (a) most main-chain Galp residues carry a side chain on O-6; (b) abouthalf of the side chains are b-(1→6)-linked Galp dimers; (c) about a quarter of theside chains are single Galp residues; (d) the rest of the side chains contain three ormore Galp residues and include most of the arabinose present; and (e) arabinoseoccurs as single a-Araf units and dimeric side chains of b-l-Arap-(1→3)-a-l-Araf-(1→6). The presumed structure of larch gum is shown in Fig. 3.25. Larch gum, like gum Arabic, has very high solubility in water, due to its highdegree of branching. A high concentration of larch gum, e.g. as high as 55–60%,can be dissolved in water with ease. It is tacky, like gum Arabic and the other treeexudates, and shows good adhesion and casting properties. The resulting film,however, is very weak as expected and cannot support its own structure, shown asflakes in Fig. 3.25. It is very soluble in cold water; and, therefore, its rate of dissolu-tion in the mouth is also fast, producing a rapid melting sensation contributed partlyby its low viscosity.3.3 Composite Films and FlakesGum polymers can hold insoluble particulates, soluble solutes, drugs, flavors andother active ingredients in the film matrix. Other polymers, such as proteins andlipids, can be used in conjunction with the gums to alter solubility and water vapor
92 M.B. NietoFig. 3.25 Plausible molecular structure of larch gum and a larch gum film, cast from a 40%solution and thickness of 40 mils (0.04 in. or 1,016 mm)and oxygen permeabilities of a film. Plasticizers – such as glycerol, propyleneglycol and sugar alcohols – can also be used to increase plasticity of a film. Thereis a wide choice of gum polymers, including their various combinations that can beused in film applications – such as breath film; sore throat and cold-flu film strips;fresh produce coatings; and confection coatings and glazes. Whether one gum poly-mer or a combination of gums is used, the property of the final film is dictated byboth the gum polymers used and by composite effects of all ingredients used tomake the film. Below is a guideline for using polysaccharide gums in film applications:1. Choose the gum or gum combination that will achieve the desired film prop- erty. Many film applications – such as breath film, sore throat film, and cold and flu films – require that the film dissolve rapidly in the mouth and that the gum polymer is strong enough to provide adequate structural support to the film, so that it can be peeled off in one piece from the production belt. In other applications, such as cake glitters, films do not have to be as strong, just strong enough that, when scraped at the end of the production belt after drying, they come off as flakes of desired size. Another requirement might be that a film needs to be shiny; while most gums give sheen in the cast state, some are shinier than others. For instance, gum Arabic gives a shiny film that readily flakes off the belt.2. Know the viscosity of the gum polymer being used. Depending on the gum or gum combination, the formulator needs to vary gum concentration, based on the available water in the recipe, to provide proper casting viscosity. It is important to control viscosity of the film slurry for uniform casting and final film thickness. There is a period of about 5–10 s before the cast slurry enters the drying tunnel; during this period, the cast slurry could spread if it is too thin, resulting in uneven film thickness. Viscosity is especially critical for drug delivery films that have strict specifications on the dose of active per sheet. For machinability, a casting
3 Structure and Function of Polysaccharide Gum-Based Edible Films and Coatings 93 viscosity between 6,000 and 10,000 cP is ideal and practical for ease of batch preparation and casting uniformity. However, a much thicker slurry – as high as 83,000 cP for a 3% guar and 118,000 cP for 1.5% konjac – can be successfully cast, dried and peeled. In these situations, adjustment of casting speed is needed, i.e., slowing it to allow the slurry to coat the belt or the surface evenly.3. Know how to hydrate or dissolve the gum polymer. A film slurry requires a much higher concentration of gums than most other food applications, typically 4–8%, or even higher for non-viscous gums. From an economic standpoint, film recipes also require the highest dose or concentration of the other ingredients, so that the slurry has the minimum amount of water needed during casting. Drying water off the slurry is the most expensive part of the process; the less water that is present, the cheaper the process becomes.All gums that hydrate in cold water – such as CMC, xanthan, guar, alginate – tendto form lumps if added to the batch without sufficient mixing. It is desirable to dryblend gums with other ingredients for ease of dispersion and dissolution, or gumscould be slurried in glycerol, alcohol, oil or any suitable solvent that is called for inthe film recipe, to minimize lumping. Alternatively, readily-dispersible or agglom-erated versions of traditional gum powders may also be used. It is also important to know whether the gum polymer requires heating or boilingto fully activate the molecule and to know the best way to put the particular gum insolution. If the gum is not hydrated, film structure will not form. For example,traditional agar requires boiling for about 3–5 min to fully dissolve; however, there isa grade of quick-soluble agar that will dissolve between 65 and 82°C that can beused instead. Kappa-carrageenan and locust bean gum require heating to 82°C to fullyactivate; iota-carrageenan and tara gum require heating to ~65°C to achievefull activation. Methylcellulose and HPMC, which are cold water-soluble gums, arebest hydrated by dispersing the gum powder in half of the water that is between55–60°C for methylcellulose and 82°C for HPMC, and then adding the other halfof the water ice-cold. These gums will hydrate with minimal lumping and foamingif dissolved this way. Table 3.2 summarizes results of a study done by Nieto and Grazaitis (2006),comparing the dissolution times of various film composites (without flavor, coloror active ingredients). The films were prepared using sodium alginate and CMCin combination with other gums and a plasticizer. Twelve composite film recipeswith different tensile strengths and solubilities are shown. Solubility of the alginate-CMC film is greatly improved by addition of gums that do not form cohesive films(weak gums), such as gum Arabic, inulin, resistant maltodextrin, and polydex-trose, as well as insoluble MCC. This phenomenon is mainly due to the weakeningof the film matrix structure, leading to faster disintegration of the film. To thecontrary, glycerol, a plasticizer, strengthens and increases dissolution time of theresulting film. Active ingredients can be incorporated directly into these recipes before the filmis cast. These active ingredients, which can comprise up to 30% of a film by weight,become locked into the film matrix, and must remain stable until product consumption.
Table 3.2 Tensile and puncture strengths and dissolution times of edible film composites basedon the work of Nieto and Grazaitis (2006)Composite film recipe Tensile strength (g) Puncture strength (g) Dissolution time (s)Water 91.1% 1,168.7 468.9 40.25 Na Alginate 4.0% LV CMC 4.0% Glycerin 0.9%Water 89.1% 1,360.4 192.9 24.5 Na Alginate 4.0% LV CMC 15F 4.0% MCC 2.0% Glycerin 0.9%Water 89.1% 1,701.7 356.9 34.75 Na Alginate 4.0% LV CMC 4.0% Maltodextrin 2.0% Glycerin 0.9%Water 95.0% 735.9 189.5 28 Na Alginate 2.5% LV CMC 1.25% K-Carrageenan 1.25%Water 87.6% 1,255.1 244.9 83 LV CMC 8.0% K-Carrageenan 3.5% Glycerin 0.9%Water 91.1% 1,171.3 1,175.5 48.5 Pectin 4.0% Na Alginate 4.0% Glycerin 0.9%Water 95.0% 834.1 341.2 31 Na Alginate 2.5% LV CMC 2.5%Water 95.0% 713.7 290.2 20 Na Alginate 2.5% LV CMC 1.25% Gum Arabic 1.25%Water 95.0% 456.1 102.0 16 Na Alginate 2.5% LV CMC 1.25% Insulin 1.25%Water 95.0% 804.3 107.5 12.6 Na Alginate 2.5% LV CMC 1.25% Polydextrose 1.25%Water 95.0% 761.9 122.1 14.2 Na Alginate 2.5% LV CMC 1.25% Maltodextrin 1.25%Water 95.0% 355.7 86.88 15.4 Na Alginate 2.5% LV CMC 1.25% MCC 1.25%Tensile strength across a 2.5-cm wide film strip and puncture strength measured using the TA XTPlus Texture Analyzer probes TA-96B and TA-1085-5, respectively. Dissolution times measuredusing a sensory panel on two ~0.05-mm thick by, 1 cm film samples.
3 Structure and Function of Polysaccharide Gum-Based Edible Films and Coatings 95Examples of actives used in film strips include ingredients for oral hygiene, suchas mint; alertness, such as caffeine; nutrients and botanicals. Color and flavor mayalso be added.3.3.1 Rapid Melt Film CompositeIn general, a weak film dissolves and undergoes rapid disintegration in the mouth.With a combination of the right gum and other ingredients, a rapid-melt film canbe produced. In applications such as breath film, this fast dissolution attribute isdesirable. However, gum polymer or polymers need to provide adequate tensilestrength to the film so that adequate machinability is maintained during processingand drying. Any of the recipes from H to L in Table 3.2 can be used or furthermanipulated to produce films that dissolve faster in the mouth. Addition of gumArabic, inulin, polydextrose, or resistant maltodextrin can improve the rapid-meltcharacteristic of films, with only minimal reductions in tensile strength, leavingroom for further adjustment to achieve desired solubility in the mouth. There are many options for making rapid-melt films using various polymers asmatrix materials. For instance, pectin, lambda-carrageenan, and methylcellulosecan be used together to provide the primary film structure, while other ingredientscan be added to weaken the film for rapid melting.3.3.2 Slow Melt Film CompositeSlow-melt films are easily produced by increasing the solids with gums thatenhance film structure, as well as by casting films thicker to improve their strength.In the study by Nieto and Grazaitis (2006), doubling of casting thickness for recipesH to L (Table 3.2) increased dissolution time from 1.4 to 3.3 times. Use of gums that produce strong, but cold water-soluble films – such as methyl-cellulose, HPMC and konjac – will also increase the tensile strength of the resultingfilms, allowing them to dissolve more slowly. There is also a viscosity effect thatcontributes to the slow-melting sensation; for films comprised of gums that formviscous solutions, film melting is significantly hindered, especially with the limitedliquid available in the mouth during ingestion.3.3.3 Insoluble FilmsAs a general rule, the initial water-solubility of a particular gum determines thesolubility of its resulting film. Therefore, agar and gellan are the best choices for
96 M.B. Nietomaking insoluble films, because they require high heat – 100°C and 95°C, respec-tively – to fully hydrate and solubilize. Though both are relatively expensive,kappa-carrageenan and locust bean gum represent less expensive alternatives forproducing films with acceptable insolubility in cold water or in the mouth. Kappa-carrageenan and glycerol produce a film that is only sparingly soluble in cold water.Locust bean gum, because it is practically insoluble in cold water, will also yield afilm that is sparingly soluble in the saliva when placed on the tongue. Cross-linkingalginate with calcium also yields a strong, clear film that is insoluble in water; thiscombination has been used to microencapsulate probiotics, such as Lactobacillusacidophilus, to increase its survival under gastric conditions. Based on a study byChandramouli et al. (2004), the viability of bacterial cells within calcium-alginatemicrocapsules increased as both capsule size and alginate concentration increased.Agar and gellan may also be used in this same application.3.3.4 Method of ManufactureIn a commercial setting, production of composite films and flakes requires anelaborate setup of machines for automated processing on an industrial scale (seeChap. 14). This section focuses on the required handling and processing of polysac-cahide gums to maximize their functionality in film applications.1. Preparation of the film slurry. For proper hydration of gums, a mixing tank with allowance for heating, such as a steam jacket, and high speed mixing are needed since gums and other solid components are normally used at high concentrations to reduce the amount of water to be later removed during drying. Casting viscosi- ties of 6,000–10,000 cP are commonly used, and gum usage is typically as high as 8%, or even higher. Entrainment of air is a problem when mixing a thick slurry; consequently, the mixing kettle is either fitted with a vacuum system, or an anti- foaming agent may be used. Flavors, colors, and active ingredients are generally used at very low levels that do not increase solids in the slurry appreciably. However, composite films may include sweeteners and bulking agents, such as maltodextrin, that can boost solids to make the process energy efficient. In making gum Arabic flakes, a higher concentration (40–50% gum in water) is needed, because its solution at these higher concentrations is just viscous enough to cast.2. Casting. After mixing the gum and other ingredients, slurry is pumped into a reservoir to be fed onto a belt through a casting knife. The casting knife sits on top of the stainless steel belt, which is moved by two drum rollers on each end of the line. The casting knife adjusts the clearance between the knife and the belt and, therefore, thickness of the cast. It is important that the gum is fully hydrated and lump-free at this time. Any lumping will cause uneven cast or slitting and tearing of the film when peeled at the other end of the belt.3. Drying. The cast slurry goes through a temperature- and humidity-controlled tunnel dryer. There is an ideal moisture content or humidity level for the gum
3 Structure and Function of Polysaccharide Gum-Based Edible Films and Coatings 97 films to peel away from the casting belt (~24–29%). If too dry, gum films become brittle and can easily tear, a shortcoming that is overcome by addition of a plasticizer – glycerol, propylene glycol or sorbitol – if needed. When mak- ing flakes, the product is dried on the belt to its final moisture, scraped off and collected for packing. Otherwise, the peeled film is rolled and stored under con- trolled humidity until further processed.4. Slitting and Packing. The last step in the process involves cutting the film into desired shapes and dimensions for packing, which is often the most elaborate step in the process. It is critical for the film to have the appropriate moisture content at this point. Uniformity of the film structure affects the yield of edible filmstrips; the more uniform the filmstrips, the lower the amount of waste.3.4 Edible Coatings3.4.1 Fruits and Vegetable CoatingsThe demand to increase product shelf life and enhance microbial safety of freshfruits and vegetables has prompted the development of edible coating technologybased on polysaccharides, lipids and/or proteins. These materials can function asbarriers to water vapor, gases, and other solutes, and also as carriers of functionalingredients, including antimicrobial agents and antioxidants. Fruits and vegetablesare living tissue up until the time they are consumed or cooked/processed for con-sumption. Controlling respiration within these living tissues improves storabilityand extends the shelf life of fresh produce. Lin and Zhao (2007) published a verycomprehensive review of innovations in edible coatings for fresh and minimally-processed fruits and vegetables. Many polysaccharides have been evaluated or used for forming films and coat-ings, including starch, dextrins, cellulose derivatives, alginates, carrageenan, xan-than, chitosan, pectin and others. The variety and versatility of gum polymersprovide a broad choice of materials for producing films for fresh fruits and vegeta-bles that have unique functions, including adhesion and cling, oxygen permeability,plasticity, oil barrier properties, etc. Cellulose derivatives – such as methylcellulose, CMC, HPC, and HPMC – havebeen studied as edible coating materials for fruits and vegetables to provide barriersto oxygen, oil, and/or moisture (Sanderson 1981; Morgan 1971; Sacharow 1972;Krumel and Lindsay 1976; Maftoonazad and Ramaswamy 2005). They retain thefirmness and crispness of apples, berries, peaches, celery, lettuce, and carrots whenused in a dry-coating process (Mason 1969), and are also used to preserve impor-tant flavor components of fresh fruits and vegetables (Nisperos-Carriedo andBaldwin 1990). In addition, they reduce oxygen uptake without increasing internalcarbon dioxide levels within coated apples and pears by simulating a controlledatmosphere and environment (Lowings and Cutts 1982; Banks 1985; Meheriuk andLau 1988; Santerre et al. 1989).
98 M.B. Nieto Very promising results have been reported regarding oil barrier properties ofalginate-based films providing cling, reducing weight loss by acting as a sacrificingmoisture coat and sealing volatiles (Fisher and Wong 1972; Cottrell and Kovacks1980; King 1983; Kester and Fennema 1986; Conca and Yang 1993; Amanatidouet al. 2000; Hershko and Nussinovitch 1998). In addition, other gums, includingexudate gums like gum Arabic, are used to coat pecan nuts, to seal in the oil(Arnold 1968), and potatoes, to prevent darkening (Mazza and Qi 1991). Xanthangum provides a uniform coating with good cling and improved adhesion in wetcoating batters (Chen and Nussinovitch 2000). Carrageenan-based coatings havebeen applied to fresh fruits and vegetables, such as apples, to reduce moisture loss,oxidation, and/or disintegration (Bryan 1972; Lee et al. 2003). Chitosan has beenextensively studied as an edible coating for fresh produce, because of its excellentfilm-forming behavior, oxygen and CO2 barrier properties, broad antimicrobialactivity and compatibility with other substances, such as vitamins, minerals, andantimicrobial agents (Krochta 1997; Shahidi et al. 1999; Park and Zhao 2004; Hanet al. 2004a, b; Durango et al. 2006; Vargas et al. 2006; Chien et al. 2007; Ribeiroet al. 2007). A chitosan coating on sliced mango fruit slowed down the rate of waterloss and drop in sensory quality; increased the soluble solids content, titratableacidity and ascorbic acid content; and inhibited growth of microorganisms (Chienet al. 2007). In addition to providing barrier properties, films made from gums have alsobeen studied as carriers of actives, such as antimicrobial agents and nutrients.Kappa-carrageenan films can effectively carry food-grade antimicrobials – such aslysozyme, nisin, grape seed extract, and EDTA – for a wide range of applicationsin food packaging materials (Choi et al. 2001). These films can also deliver anti-browning agents, such as ascorbic acid, producing positive sensory results and areduction of microbial levels in minimally-processed apple slices (Lee et al. 2003).Xanthan gum coating was used to carry 5% Gluconal Cal, a mixture of calciumlactate and gluconate, and 0.2% a-tocopherol acetate (vitamin E) (Mei et al.2002). On its own, chitosan coating has been used for its antifungal properties(Zhang and Quantick 1998; Park et al. 2005). Iverson and Ager (2003) invented achitosan-based antifungal coating, mixed with an edible wax emulsion and/or apreservative such as sodium benzoate and/or an adhesion additive, such as zincacetate, and/or a wetting agent to form a composition having a solid content of15% or higher.3.4.2 Confection CoatingsConfection coating is applied to candy centers or discreet product pieces in a proc-ess called panning. This process is done in a coating pan, a bowl that is motordriven to provide a tumbling action. The product moves continuously during thecoating process, and coating material is applied to the product as the pan rotates.Coating material, such as sugar syrup, needs to adhere to the product surface and
3 Structure and Function of Polysaccharide Gum-Based Edible Films and Coatings 99dry quickly, so that repeated charges of coating material, up to ~60 times, can beapplied within a reasonable period of time. There are three types of panning: soft panning, hard panning and chocolatepanning. With soft panning, a sugar shell is built around surfaces of candy centersby wetting them with a sugar syrup, and dusting it with confectioner’s sugar orsome type of dusting powder. This process produces a soft sugar shell, like thatused for jellybeans. Hard panning, on the other hand, produces a harder sugar shellthrough application of repeated charges of the engrossing and smoothing syrupswithout dusting. Each individual coat of syrup is dried prior to adding the next,and the result is a denser, more compact sugar shell encasing the candy center(e.g., the sugar shell of gumballs, coated peanuts and chocolate candies). The thirdtype, chocolate panning, consists of building a layer of chocolate around candycenters – such as nuts, maltballs and raisins – by melting the chocolate and spray-ing it on the centers while tumbling. Coated product is either polished, glazed andpacked for sale with a chocolate finish, or hard-panned to add a layer of sugar shellfor strength. This shell could also be food-colored and polished for added appeal(Fig. 3.26). When candy centers contain oil, they must be pre-sealed, or oil will migratethrough the chocolate layer to the product surface and will spoil the appearance ofthe finished confection. Pre-sealing is achieved by coating candy centers withseveral charges of a 40% concentration of gum Arabic syrup to wet and form aFig. 3.26 Confections with hard sugar shell and chocolate finish
100 M.B. Nietofilm around the centers. Other low-viscosity polysaccharides can also be used,such as larch gum and inulin, separately or in combination with the gum Arabic.High viscosity gums are not suitable for this application, even though they formstronger films or seals, because most of them are already too viscous at 1–2%concentration. Further, wetted centers take too long to dry or can become soggy.In addition, gum Arabic syrup is used for polishing coated product to impart sheento the surface. Other than for functions discussed above, gums have limited use in standardconfection coatings due to cost. However, for sugar-free recipes, polysaccha-rides are inevitable replacements for sugar or augmenting ingredients, and areused in combination with sugar alcohols, like maltitol, erythritol, and sorbitol.Again, gum Arabic, larch gum, inulin, and resistant maltodextrin are the mostsuitable choices due to their low solution viscosities. A gum Arabic and maltitolcombination is used for applying a sugar-free shell layer around chewing gumsand candies with soft centers. Below is a recipe for sugar-free coated peanuts.Sugar-free, Chocolate-coated PeanutsProcedureIngredients lb.Peanut centers [Batch Size] 100.0Sealing syrup-40% Gum Arabic ~3.0Sealing powder (Cocoa/Inulin 50/50 blend) ~5.0Unsweetened bakers Chocolate for Engrossing 100.0Sugar-free hard panning:Engrossing syrup and smoothing syrup 100.0Polishing syrup (40% gum Arabic) ~2.0Shellac glaze ~0.51. Pre-sealing. Count 50 pieces of candy centers; weigh and record their weight. Place 100 lb. of candy centers in a coating pan, and start rotation of the pan at 25 rpm. Scoop ~500 mL of 40% gum Arabic syrup into the coating pan, and allow the batch to run until all candy center surfaces are wet (about 1 min). Using a scoop, add enough sealing powder to dry the surface. Run until all pow- der adheres to the candy center surfaces. Repeat the process for the second and third applications. Spread batches onto trays to harden overnight.2. Engrossing. Take 50 pieces of sealed candy centers; weigh and record their weight. Melt the chocolate and keep melted (between 43 and 49°C). If using a clean pan, smear some chocolate inside the pan before engrossing. Start the pan and begin coating with chocolate (by spraying or using a ladle). Use cold air as required to set chocolate and dry product surfaces. Continue coating chocolate to twice the weight of the center. Separate doubles and clusters of candy centers by hand. If needed, run warm air to partially melt chocolate and smooth the surface. Weigh batch and record weights. Spread onto trays to harden in a cool, dry room.3. Sugar-Free Hard Panning (This step is not required for chocolate finish). a) Prepare the gum solution, diluting the 40% gum Arabic solution to make a 20% syrup. Prepare the sugar-free dusting powder by mixing maltitol
3 Structure and Function of Polysaccharide Gum-Based Edible Films and Coatings 101 and inulin at 80:20 ratio. Start the pan and add a charge of gum Arabic syrup to candy centers. Mix for about one minute. Record the amount of syrup added. Add a small amount of dusting powder to the pan in front of the candy centers to get the centers rolling. As candy centers become sticky, add more dusting powder to prevent them from sticking together (begin with just a small amount, and add only enough to keep the centers separate). Dry centers thoroughly with air while centers are tumbling. Add two more charges of gum Arabic syrup, increasing the amount of syrup as needed, and dust in the same way as previously described. Record the volume of syrup used in each charge. b) Prepare 70% engrossing syrup by dissolving 60 parts maltitol, 3 parts gum Arabic powder, and 7 parts inulin in 30 parts water (by weight). Bring syrup to a boil, and cool it to ~29°C before use. Weigh 50 pieces, and record their weight. If manually ladling syrup, add enough of a charge of engrossing syrup to completely wet the surfaces of the candy centers, distributing syrup throughout the bed while mixing. Record charge size and time on batch sheet. Mix for about 1 min. Apply air to dry the centers thoroughly. If using an automatic spray system dry until humidity in the pan is about 12–16%. Repeat process until half of the desired coating weight has been applied. This is determined by weighing 50 pieces of centers periodically. c) Prepare 65% smoothing syrup by diluting the 70% engrossing syrup to ~65°Brix. Add a charge of smoothing syrup (1/3 less than the engrossing syrup), and distribute it throughout the bed by mixing. Record the volume added. When candy centers begin to roll freely, apply air to dry them thor- oughly as in step 3b. Repeat the process until desired coating weight is achieved. Weigh 50 centers periodically to aid this determination. d) Add coloring by mixing 20% of color lake dispersion with 80% of smoothing syrup. Apply four charges to candy centers; for each charge, mix until candy centers begin to roll freely, and dry with air thoroughly as in step 3b. Add a fifth charge as follows: divide into two half-charges, apply the first half- charge, and dry without air. When dry, add the second half-charge, but allow candy centers to tumble only until drying starts. Stop the pan and dry centers by jogging the pan every 10 min. Do not leave pan running to prevent scuffing of the coat.4. Polishing with gum Arabic. Use this step only if the candy has a chocolate finish. Place the coated batch in a clean, ribbed pan. Ensure the product is cold and hard. Start the pan and add one wetting of polishing solution of 40% gum Arabic. Stop the pan as soon as the product surface is no longer sticky. Use as little air as needed. Repeat the polishing step one or two more times. Dry thor- oughly after the last application. (For sugar-coated product, skip polishing and proceed directly to step 5).5. Glazing with Shellac. Use a clean ribbed pan. Without air, start the pan, and wet batches with a shellac glaze. After wetting, use air to dry. Stop the pan and jog it every minute to prevent pieces from sticking together.
102 M.B. Nieto3.4.3 Bakery Coatings-Icings and GlazesMany bakery products owe their appeal to icings and glazes applied to their sur-faces. Toppings on these products are usually what consumers notice first (Fig.3.27). They not only enhance overall appearance, but also add sweetness and flavorto the finished products, as well as improve texture and shelf life. While consumersenjoy these topical applications, there are many challenges that need to be over-come in ensuring that a commercial icing or glaze, when applied, will remainappealing until the product is consumed. Will glaze melt and disappear in thedoughnut on a hot summer day? Will glaze stick to packaging during transport ofthe product? Will sugar crystallize out of the icing and harden before the product isconsumed? Sugar, the main ingredient in icings and glazes, can be a very problematic ingre-dient, because it absorbs water from the environment and melts with high humidityand temperature. Therefore, a glaze can easily disappear and sip into a donut as aresult of moisture uptake; or even without humidity, it can just melt. A gum likeagar is used to minimize melting of the sugar coating, and to give the glaze a set.Either traditional agar or quick-soluble agar can be used in a glaze. However,because agar is quite expensive, kappa-carrageenan can be used as a cheaper alter-native in some cases. A gum blend consisting of sodium alginate and gum Arabic,where calcium from gum Arabic forms cross-links between alginate polymers toform a gel and set the glaze. Agar and alginate-gum Arabic systems are also used in icing to prevent sugarfrom crystallizing and icing from hardening prematurely. Agar is used in icings atFig. 3.27 Gum application in bakery icing and glaze
3 Structure and Function of Polysaccharide Gum-Based Edible Films and Coatings 103~0.2% and in doughnut glazes typically at 0.4% or higher to prevent sugar crystal-lization and reduce tendency of the glaze to chip, crack or “weep”. The alginate-gum Arabic system, on the other hand, is used in icing at 1.0%, and may also beused in glazes at 1.0–1.5%. See recipes below.A. Bakery glazeIngredients %Water 38.90Glucose syrup 5.00Sucrose 55.00Agar 0.40Citric acid 0.20Potassium sorbate 0.10Flavor/color q.s. (as much as enough) 100.00Procedure1. Add water and glucose syrup to the mixing tank and start heating.2. Turn on the mixer, and add potassium sorbate and agar. Bring mixture to a boil, and mix ~3 min until agar is fully dissolved.3. Add all of the sugar.4. Continue cooking until Brix is ~60.5. Lower the temperature to 74°C and add citric acid.6. Apply glaze warm. (Note: Quick-soluble agar that dissolves at 65–82°C may also be used.)B. Icing recipeIngredients %Confectioners sugar (10×) 69.00Water 28.60Shortening 2.00Alginate-gum Arabic blend 1.00Citric Acid 0.20Potassium sorbate 0.10Vanilla 0.10 100.00Procedure1. Add water to batch tank.2. Add potassium sorbate.3. Dry blend gums with 10 parts of sugar and add blend to water in the batch tank while mixing.4. Add vanilla and the rest of the sugar.5. Add shortening to the mix, and cream.6. Mix well, and heat to 120°F.In addition to icings and glazes, another coating applied to bakery products thatdeserves to be mentioned under this heading is the egg wash. Breads and pastrieswill look much more appealing with an egg wash applied on the surface before they
104 M.B. Nietoare baked. A polysaccharide, such as gum Arabic, can actually replace egg wash inthis application. Gum Arabic provides sheen that adds shelf appeal; in addition, itis much less prone to burning.3.5 Regulatory StatusMost gum polymers discussed in this chapter are approved for use in foods and/orare GRAS, except for chitosan and cassia gum, which are only allowed in supple-ments and pet food applications, respectively. This is good news because regulationof edible films will take an easier route if using food approved or GRAS ingredi-ents. Druchta and Johnston (1997) published a scientific status summary on ediblefilms that includes their safety and health issues. They reported that the process ofdetermining acceptability of materials for edible polymer films follows proceduresidentical to those used in determining appropriateness of such materials for foodformulation. The process is outlined as follows:1. An edible polymer will be generally recognized as safe (GRAS) for use in edible films if the material has previously been determined as GRAS, and its use in an edible film is in accordance with current good manufacturing practices (food grade, prepared and handled as a food ingredient, and used in amounts no greater than necessary to perform its function), and within any limitations speci- fied by the Food and Drug Administration (FDA).2. If the edible polymer film uses a protein – such as wheat, soy, corn or any ingre- dient that could potentially contain an allergen – each such ingredient must be declared appropriately to the consumer, no matter how small the amount used, with the appropriate warning about the allergenic ingredient.3. If the edible polymer film material used is not currently GRAS, but the manu- facturer can demonstrate its safety, the manufacturer may either file a GRAS Affirmation Petition to the FDA or proceed to market the material without FDA concurrence (self-determination).4. The manufacturer may not need to establish that use of an edible polymer in edible films is GRAS if the material had received pre-1958 FDA clearance and thus has “prior sanction.”5. Finally, if the material cannot be demonstrated to be GRAS or does not have “prior sanction,” the manufacturer must submit a food additive petition to the FDA prior to its use in films and coatings.If the intent is to make biodegradable polymer packaging film, the FDA regulatesall materials proposed for food packaging to ensure they are safe for food contactunder conditions of the intended use. As summarized by Druchta and Johnston(1997), there are several categories of biodegradable polymers acceptable for useas food packaging:1. If a biodegradable polymer developed for use in food packaging is found to be GRAS by the developer (self-determination) or affirmed as GRAS by the FDA,
3 Structure and Function of Polysaccharide Gum-Based Edible Films and Coatings 105 the polymer may be used in food packaging; if a GRAS polymer is combined with a food-grade synthetic polymer to enhance biodegradable character, the developer should supply the FDA with information that addresses whether the proposed use of the product can be considered a “good manufacturing practice.” FDA requires information on the migration profile and identity of migrants from biodegradable packaging to food during typical storage conditions and times; the agency also requires information on environmental aspects of the biodegrad- able package use.2. If a biodegradable polymer developed for use in food packaging is not GRAS, it may be used only after a food additive petition and environmental assessment are approved.Most of polysaccharides are natural polymers; these offer the greatest opportuni-ties as materials for biodegradable films and packages, since their safety, biode-gradability and environmental compatibility are already assured. Even thechemically derived gum polymers – such as CMC, HPMC and PGA – that arefood approved, are potential polymeric materials for use in biodegradable pack-aging. However, if these gum polymers require complexing or cross-linking withother chemicals to achieve rigidity, elasticity or water impermeability of theirplastic packages, then their regulation changes and could follow the fate of non-edible, polymeric materials. Examples of these materials include cellophane,microbial polyesters (e.g., polyhydroxybutyrate/valerate co-polymers), polylacticacid, and combinations of starch with polyvinyl alcohol, where migration of toxiccomponents to food could be a possibility. Hence, in this case, safety of thesepackaging films needs to be established first with the FDA. Any questionablesubstance that can reasonably be expected to migrate from the package into foodsis classified as an indirect food additive, subject to FDA regulations per 21CFR 126.96.36.199 Future Trends3.6.1 Novelty FilmsWith the versatility and established safety of most gum polymers, novel applica-tions for gum films seem almost limitless. The concept of drug, vitamin and min-eral delivery films is likely to expand and, while there are more and more noveltyfilm products appearing in stores, other creative concepts are likely to evolve,including cheese, ketchup, or sour cream films, or various spice films that foodscientists, product formulators or chefs could create. Convenience and microbialstability of dried forms of food films is the biggest selling point for developingthese products. The market for edible films has already experienced noteworthygrowth, from ~$1 million in 1999 to more than $100 million per year today.According to Tara McHugh of the U.S. Department of Agriculture, as quoted by
106 M.B. NietoKlapthor, 2 breath mint and cold medication markets have been responsible formuch of that growth. James Rossman, former maker of edible films and a currentconsultant, projects that retail sales of edible film, about $100 million a year today,are expected to hit at least $350 million by 2008 and $2 billion by 2012 (http://www.foodnavigator.com/Financial-Industry/Tate-Lyle-invests-in-edible-films-market).33.6.2 Biodegradable Films and PackagesDeveloping cost-effective biodegradable films and rigid/semi-rigid packages thatmatch properties of synthetic plastics is still a task to be accomplished in the future.In 2005, a total of 28.9 tons of synthetic plastic materials were generated and 16.3tons discarded as municipal solid waste (EPA 2006). Likewise, there have alwaysbeen health concerns regarding residual monomers and components in plastics –including stabilizers, plasticizers and condensation components, such as bisphenol– that can migrate into food (Marsh and Bugusu 2007). However, bioplastics arecurrently much more expensive than most petroleum-based polymers, so substitu-tion is likely to result in increased packaging costs. Cellophane, a biodegradable,cellulose-derived film, was invented a long time ago (in 1908), but has not reallycompeted with plastics. Natureworks, LLC, owned by Cargill Inc., manufacturespolylactide from corn sugar; and now Wal-Mart uses biopolymers by employingpolylactide to package fresh-cut produce (Bastioli 2005). Research should focus onimproving heat sealability and the printability of biodegradable films, in additionto making them cost-competitive with plastics.3.6.3 Edible Films and CoatingsAccording to Lin and Zhao (2007), despite significant benefits from using ediblecoatings for extending product shelf life and enhancing the quality and microbialsafety of fresh and minimally-processed fruits and vegetables, commercial applicationson a broad range of edible coating of fruits and vegetables are still very limited. Ofmany improvements that needed for polysaccharides to be used more extensively asedible film and coating materials, most important is improving the water-resistanceof gum films. Creation of nanocomposites, incorporation of lipid to the gum polymermatrix, or formation of nanolaminates can provide solutions to this challenge. Weisset al. (2006), in their scientific status summary on materials in food nanotechnology,describe how a polysaccharide-clay nanocomposite can be formed. A carbohydrate ispumped together with clay layers, through a high shear cell, to produce a film thatcontains exfoliated clay layers.4 The nanocomposite carbohydrate film has substantially2 http://www.am-fe.ift.org/cms/?pid=1000355]3 http://www.businessweek.com/magazine/content/06_31/ b3995059.htm4 http:www.pre.wur.nl/ UK/Research/Food+Structuring/ Microstructured/
3 Structure and Function of Polysaccharide Gum-Based Edible Films and Coatings 107reduced water vapor permeability. Similarly, chitosan containing exfoliated hydroxya-patite layers maintains functionality in humid environments, with good mechanicalproperties. Incorporation of hydrophobic ingredients – such as lipids for improving themoisture barrier, while maintaining the desirable resistance to vapor, gas, or soluteis another research area that can be pursued. Decher and Schlenoff (2003) createda nanolaminate based on deposition technique in which charged surfaces are coatedwith interfacial films that consist of multiple nanolayers of different materials.Nanolaminates can give food scientists advantages for the preparation of ediblecoatings and films over conventional technologies, because they can be moreefficient moisture, lipid and gas barriers.3.6.4 Gum SuppliersAqualon Products: Cellulose Derivatives, Guar http://aqualon.comColloides Naturels International Products: Gum arabic http://www.cniworld.comCP Kelco Products: Carrageenan, cellulosics, gellan, pectin, xanthan http://www.cpkelco.comDanisco Products: Pectin, LBG, guar gum, alginate, carrageenan, xanthan gum,cellulose gum http://danisco.comDegussa Products: General Hydrocolloids and blends (alginates, agar, pectin, xanthan, carrageenans, galactomannan) http://www.texturantsystems.comFMC biopolymer Products: Carrageenan, alginate, microcrystalline cellulose and konjac http://www.fmcbiopolymer.com/Gum technology Products: General hydrocolloids and blends (Acacia, Agar, Alginates, Carrageenans, Cellulose Gum, Fenugreek, Gelatin, Guar Gum, Gum Blends, Inulin, Karaya, Konjac, Locust Bean Gum, Oat Fiber, Pectin, PGA, Pullulan, Tara Gum, Tragacanth, Xanthan Gum) http://www.gumtech.com/products/index.phpISC [Importers Service Corporation] Products: Gum Arabic, Karaya, Ghatti, Tragacanth http://www.iscgums.com/product.htm
108 M.B. NietoPL Thomas Products: General hydrocolloids and blends http://www.plthomas.com/gums_overview.htmRoko Products: agar http://www.rokoagar.comTate and Lyle Products: Xanthan http://www.tateandlyle.co.ukTIC Gums, Inc. Products: General Hydrocolloids and specialty blends (Gum Acacia, Agar, Alginates, Carrageenans, Cellulose Gum, Guar Gum, HPMC, Tara gum, Gum Ghatti, Inulin, Karaya, Konjac, Locust Bean Gum, Methylcellulose, Modified Gum Acacia, Pectin, PGA, Tara Gum, Tragacanth, Xanthan Gum, and specialty blends of gums, starches and emulsifiers) http://www.ticgums.comAcknowledgements I would like to recognize the assistance of the following TIC Gums employ-ees in preparing and testing the gum films and in editing the photos and figures shown in thischapter for print quality: Nick Pippen, Dan Grazaitis, Renrick Atkins, Frances Bowman andMaureen Akins.ReferencesAmanatidou A, Slump RA, Gorris LGM, Smid EJ (2000) High oxygen and high carbon dioxide modified atmospheres for shelf life extension of minimally processed carrots. J Food Sci 65:61–6Arnold FW (1968) Infrared roasting of coated nutmeats. U.S. patent 3, 383, 220Aspinall GO, Christensen JB (1965) Gum ghatti (Indian gum) Part IV. Acidic oligosaccharides from the gum. J Chem Soc 2673–2676 DOI: 10.1039/JR9650002673Aspinall GO, Hirst EL, Wickstrom A (1955) Gum ghatti (Indian gum) Part I. The composition of the gum and the structure of two aldobiuronic acids derived from it. J Chem Soc 1160–1165 DOI: 10.1039/JR9550001160Aspinall GO, Auret BJ, Hirst EL (1958a) Gum ghatti (Indian gum) Part II. The hydrolysis prod- ucts obtained from the methylated degraded gum and the methylated gum. J Chem Soc 221– 230 DOI: 10.1039/JR9580000221. 47Aspinall GO, Auret BJ, Hirst EL (1958b) Gum ghatti (Indian gum) Part III. Neutral oligosaccha- rides formed on partial acid hydrolysis of the gum. J Chem Soc 4408–4414 DOI: 10.1039/ JR9580004408Aspinall GO, Bhavanadan VP, Christensen JB (1965) Gum ghatti (Indian gum) Part V. Degradation of the periodate-oxidized gum. J Chem Soc 2677–2684 DOI: 10.1039/JR9650002677Banks NH (1985) Internal atmosphere modification in pro-long coated apples. Acta Hort 157:105Bastioli C (2005) Handbook of biodegradable polymers. Toronto-Scarborough, Ontario, Canada, Chem Tec Publishing, 553 pBender H, Wallenfels K (1961) Investigations on pullulan II. Specific degradation by means of a bacterial enzyme. Biochem Z 334:79–95Bernier B (1958) The production of polysaccharides by fungi active in the decomposition of wood and forest litter. Can J Microbiol 4:195–204
3 Structure and Function of Polysaccharide Gum-Based Edible Films and Coatings 109Bouveng HO, Kiessling H, Lindberg B, McKay J (1962) Polysaccharides elaborated by Pullularia pullulans. I. The neutral glucan synthesized from sucrose solutions. Acta Chem Scand 16:615–622Bouveng HO, Kiessling H, Lindberg B, McKay J (1963) Polysaccharides elaborated by Pullularia pullulans. II. The partial acid hydrolysis of the neutral glucan synthesised from sucrose solu- tions. Acta Chem Scand 17:797–800Bryan DS (1972) Prepared citrus fruit halves and method of making the same. U.S. patent 3, 707, 383Carolan G, Catley BJ, McDougal FJ (1983) The location of tetrasaccharide units in pullulan. Carbohydr Res 114:237–243Catley BJ (1970) Pullulan, a relationship between molecular weight and fine structure. FEBS Lett 10:190–193Catley BJ, Whelan WJ (1971) Observations on the structure of pullulan. Arch Biochem Biophys 143:138–142Catley BJ, Robyt JF, Whelan WJ (1966) A minor structural feature of pullulan. Biochem J 100:5P–8PChandramouli V, Kailasapathy K, Peiris P, Jones M (2004) An improved method of microencap- sulation and its evaluation to protect Lactobacillus spp. in simulated gastric conditions. J Microbiol Methods 57:27–35Chandrasekaran R, Radha A (1995) Molecular architectures and functional properties of gellan gum and related polysaccharides. Trends Food Sci 6:143–148Chaplin M (2008) Water Structure and Science – Gum Arabic http://www.lsbu.ac.uk/water/hyara- bic.htmlChen S, Nussinovitch A (2000) The role of xanthan gum in traditional coatings of easy peelers. Food Hydrocolloids 14(4):319–326(8)Chien PJ, Sheu F, Yang FH (2007) Effects of edible chitosan coating on quality and shelf life of sliced mango fruit. J Food Eng 78:225–9Choi JH, Cha DS, Park HJ (2001) The antimicrobial films based on Na-alginate and k-carra- geenan. In: IFT Annual Meeting, Food Packaging Division (74D). New Orleans, LAConca KR, Yang TCS (1993) Edible food barrier coatings. In: Ching C, Kaplan D, Thomas D (eds) Biodegradable Polymers and Packaging. Technomic Publishing Co. Inc, Lancaster, PA, pp 357–69Cottrell IW, Kovacks P (1980) Alginates. In: Davidson RL (ed) Handbook of Water-Soluble Gums and Resins. McGraw-Hill, New York, NY, p 143Daas PJH, Schols HA, de Jongh HHJ (2000) On the galactosyl distribution of commercial galac- tomannans. Carbohydr Res 329:609–619Decher G, Schlenoff JB (2003) Multilayer thin films: sequential assembly of nanocomposite materials. Wiley VCH, Weinheim, Germany, p 543DeLeenheer L, Hoebregs H (1994). Progress in the elucidation of the composition of chicory inulin. Starch 46:193Donati I, Holtan S, Mørch YA, Borgogna M, Dentini M, Skjåk-Bræk (2005) New hypothesis on the role of alternating sequences in calcium-alginate gels. Biomacromolecules 6:1031–1040Dow Chemical (2002) METHOCEL Cellulose Ethers Technical Handbook. http://www. dowchemical.com/methocel/ pharm/ resource/lit_gnl.htmDraget KI (2000) Alginates. In: Phillips GO, Williams PA (eds) Handbook of Hydrocolloids. CRC , Boca Raton, FL pp 379–395Druchta JM, Jonhston CD (1997) An Update on Edible Films-Scientific Status Summary. Food Technol 51(2):60, 62–63Durango AM, Soares NF, Andrade NJ (2006) Microbiological evaluation of an edible antimicro- bial coating on minimally processed carrots. Food Control 17:336–41Ebringerova A, Hromadkova Z, Heinze T (2005) Hemicellulose. In: Heinze T (ed) Advances in Polymer Science  Polysaccharides-Structure Characterization and Use. Springer, Berlin, pp 1–68Environmental Protection Agency, US (2006) Municipal solid waste in the United States: 2005 facts and figures. EPA530-R-06-011, Washington D.C., p 153
110 M.B. NietoEvans AJ, Hood RL, Oakenfull DG, Sidhu GS (1992) Relationship between structure and function of dietary fibre: A comparative study of the effects of three galactomannans on cholesterol metabolism in the rat. Br J Nutr 68(1):217–229Falshaw R, Bixler HJ, Johndro K (2001) Structure and performance of commercial kappa-2 carrageenan extracts I. Structure analysis. Food Hydrocolloids 15:441–452Fisher LG, Wong P (1972) Method of forming an adherent coating on foods. U.S. patent 3, 676, 158Giannouli P, Morris ER (2000) Cryogelation of xanthan. Food Hydrocolloids 17:495–501Goodrum LJ, Patel A, Leykam JF, Kieliszewski MJ (2000) Gum arabic glycoprotein contains glycomodules of both extensin and arabinogalactan-glycoproteins. Phytochemistry 54:99–106Goycoolea FM, Milas M, Rinaudo M (2001) Associative phenomena in galactomannan- deacetylated xanthan systems. Int J Biol Macromol 29:181–192Han C, Lederer C, McDaniel M, Zhao Y (2004a) Sensory evaluation of fresh strawberries (Fragaria ananassa) coated with chitosan-based edible coatings. J Food Sci 70:S172–8Han C, Zhao Y, Leonard SW, Traber MG (2004b) Edible coatings to improve storability and enhance nutritional value of fresh and frozen strawberries (Fragaria ananassa) and raspberries (Rubus ideaus). Postharvest Biol Technol 33:67–78Hanna D, Shaw EHJ (1941) Chemical constitution of gum ghatti. Proc S Dakota Acad Sci 21:78Hershko V, Nussinovitch A (1998) Relationships between hydrocolloid coating and mushroom structure. J Agric Food Chem 46:2988–97Iijima H, Takeo K (2000) Microcrystalline cellulose: an overview. In: Handbook of Hydrocolloids, Phillips GO, Williams PA (eds) CRC/Woodhead Publishing, Boca Raton, p 664Iverson CE, Ager SP (inventors) CH.sub.2O Incorporated (assignee)(2003) Method of coating food products and a coating composition. U.S. patent 6, 586, 029Jansson PE, Keene L, Lindberg B (1975) Structure of the exocellular polysaccharide from Xanthomonas campestris, Carbohydr Res 45:275–82Juang RS, Shao HJ (2002) A simplified equilibrium model for sorption of heavy metal ions from aqueous solutions on chitosan. Water Res 36(12):2999–3008Kato K (1973) Isolation of oligosaccharides corresponding to the branching-point of Konjac Mannan. Agr Biol Chem 37(9):2045–2051Kato K, Matsuda K (1969) Studies on the chemical stucture of konjac mannan. Part I. Isolation and characterization of oligosaccharides from the partial acid hydrolyzate of mannan. Agric Biol Chem 33, 1446–1453.Kester JJ, Fennema OR (1986) Edible films and coatings: a review. Food Technol 40(12):47–59King AH (1983) Brown seaweed extracts (alginates). In: Food Hydrocolloids. vol II Glicksman M (ed) CRC, Boca Raton FL, pp 115–88Kirk-Othmer (1993) Cellulose ethers. In: Encyclopedia of Chemical Technology, 4th edn. vol 5, Kroschwitz J (ed). Wiley, New York, NY, pp 541–561Krochta JM (1997) Edible protein films and coatings. In: Food Proteins and Their Applications. Damodaran S, Paraf A (eds) Marcel Dekker, New York, NYKrumel KL, Lindsay TA (1976) Nonionic cellulose ethers. Food Technol 30(4):36–8, 40, 43Labropoulos KC, Niesz DE, Danforth SC, Kevrekidis PG (2002) Dynamic rheology of agar gels: theory and experiment. Part I. Development of a rheological model. Carbohydr Polym 50:393–406Le Cerf D, Irinei F, Muller G (1990) Solution properties of gum exudates from Steculia urens [karaya gum]. Carbohydr Polym 13(4):375–386Leathers TD (2003) Biotechnological production and applications of pullulan. Appl Microbiol Biotechnol. 62:468–473Lee JY, Park HJ, Lee CY, Choi WY (2003) Extending shelf-life of minimally processed apples with edible coatings and antibrowning agents. Lebens Wissen Technol 36:323–9Li B, Xie B, Kennedy JF (2006) Studies on the molecular chain morphology of konjac glucoman- nan. Carbohydr Polym 64(4):510–515Lin D, Zhao Y (2007) Innovations in the Development and Application of Edible Coatings for Fresh and Minimally Processed Fruits and Vegetables. Compr Rev Food Sci Food Safety 6(3):60–75
3 Structure and Function of Polysaccharide Gum-Based Edible Films and Coatings 111Lootens D, Capel F, Durand D, Nicolai T, Boulenguer P, Langendorff V (2003) Influence of pH, Ca concentration, temperature and amidation on the gelation of low methoxyl pectin. Food Hydrocolloids 17:237–244Lowings PH, Cutts DF (1982) The preservation of fresh fruits and vegetables. In Proceedings of the Institute of Food Science and Technology Annual Symposium, Nottingham, UK, p 52Maeda M, Shimahara H, Sugiyama N (1980) Detailed examination of the branched structure of konjac glucomannan. Agric Biol Chem 44:245–252Maekaji K (1974) The mechanism of gelation of konjacmannan. Agric. Biol. Chem., 38, 315–321Maekaji K (1978) Nippon Nogeikagakukaishi. 52:251, 485, 513Maftoonazad N, Ramaswamy HS (2005) Postharvest shelf-life extension of avocados using methyl cellulose-based coating. Lebens Wissen Technol 38:617–24Mason DF (1969) Oct 14. Fruit preservation process. U.S. patent 3, 472, 662Mazza G, Qi H (1991) Control of after cooking darkening in potatoes with edible film-forming products and calcium chloride. J Agric Food Chem 39:2163–6Marsh K, Bugusu B (2007). Food packaging-roles, materials and environmental issues. J Food Sci 72(3):39–55May CD (2000) Pectins. In: Handbook of Hydrocolloids. Phillips GO and Williams, PA (eds) Woodhead Publishing Ltd, Cambridge, UK, pp. 219–229Meheriuk M, Lau OL (1988) Effect of two polymeric coatings on fresh quality of ‘Bartlett’ and ‘d’Anjou’ pears. J Am Soc Hort Sci 113:222–6Mei Y, Zhao Y, Yang J, Furr HC (2002) Using edible coating to enhance nutritional and sensory qualities of baby carrots. J Food Sci 67(5):1964–1968Melton LD, Mindt L, Rees DA, Sanderson GR (1976) Covalent structure of the polysaccharide from Xanthomonas campestris: Evidence from partial hydrolysis studies. Carbohydr Res 46:245–57Morgan BH (1971) Edible packaging update. Food Prod Devel 5:75–7, 108Murray JCF (2000) Cellulosics. In: Handbook of Hydrocolloids. Phillips GO, Williams PA (eds) Woodhead Publishing Ltd, Cambridge, UK, pp 219–229Naouli N (2006) Molecular weight analysis of linear and branched gums using triple detection technique. Application Report Number 0076-06 by Polymer Laboratories. (Unpublished)Nieto M, Grazaitis D (2006) Edible Films with Unique Properties Using Gums. (Unpublished) Presented at IFT in Orlando, FLNisperos-Carriedo MO, Baldwin EA (1990) Edible coatings for fresh fruits and vegetables. In: Subtropical Technology Conference Proceedings. Lake Alfred, FLPark SI, Zhao Y (2004) Incorporation of a high concentration of mineral or vitamin into-chitosan- based films. J Agric Food Chem 52:1933–9Park S, Stan SD, Daeschel MA, Zhao Y (2005) Antifungal coatings on fresh strawberries (Fragaria ananassa) to control mold growth during cold storage. J Food Sci 70: M202–7Pedroni VI, Schulz PC, Gschaider ME, Andreucetti N (2003) Chitosan structure in aqueous solu- tion. Colloid Polym Sci 282(1):100–102Petkowicz CLO, Reicher F, Mazeau K (1998) Conformational analysis of galactomannans: from oligomeric segments to polymeric chains. Carbohydr Polym 37:25–39Pérez S, Mazeau K, Hervé du Penhoat C (2000) The three-dimensional structures of the pectic polysaccharides. Plant Physiol Biochem 38:37–55Pérez S, Rodríguez-Carvajal MA, Doco T (2003) A complex plant cell wall polysaccharide: rham- nogalacturonan II. A structure in quest of a function, Biochimie 85:109–121Ralet MC, Dronnet V, Buchholt HC, Thibault JF (2001) Enzymatically and chemically de-esteri- fied lime pectins: characterisation, polyelectrolyte behaviour and calcium binding properties. Carbohydr Res 336:117–125Ribeiro C, Vicente AA, Teixeira JA Miranda C (2007) Optimization of edible coating composition to retard strawberry fruit senescence. Postharvest Bio Technol 44:63–70Risbud M, Hardikar A, Bhonde R (2000) Growth modulation of fibroblast by chitosan-polyvinyl pyrrolidone hydrogel: implications for wound management. J Biosci 25(1):147–159Sacharow S (1972) Edible films. Packaging 43:6, 9
112 M.B. NietoSanderson GR (1981) Polysaccharides in foods. Food Technol 35:50–7, 83Santerre CR, Leach TF, Cash JN (1989) The influence of the sucrose polyester, Sempfresh, on the storage of Michigan grown ‘McIntosh’ and ‘Golden Delicious’ apples. J Food Proc Preserv 13:293–305Shahidi F, Arachchi JKV, Jeon Y (1999) Food applications of chitin and chitosans. Trends Food Sci Technol 10:37–51Shimahara H, Suzuki H, Sugiyama N, Nishizawa K (1975a) Isolation and Characterization of Oligosaccharides from an Enzymic Hydrolysate of Konjac Glucomannan. Agri Biol Chem 39(2):293–299Shimahara H, Suzuki H, Sugiyama N, Nishizawa K (1975b) Partial Purification of ß-Mannanases from the Konjac tubers and Their Substrate Specificity in Relation to the Structure of Konjac Glucomannan. Agri Biol Chem 39(2):301–312Sowa W, Blackwood AC, Adams GA (1963) Neutral extracellular glucan of Pullularia pullulans (de Bary) Berkhout. Can J Chem 41:2314–2319Srinivasa P, Baskaran R, Ramesh M, Harish Prashanth K, Tharanathan R (2002) Storage studies of mango packed using biodegradable chitosan film. Eur Food Res Technol 215(6):504–508Stephen AM, Churms SC (1995) Gums and mucilages. In: Food Polysaccharides and Their Applications. Stephen AM (ed) Marcel Dekker, New York, NY, pp 377–425Sugiyama N, Shimahara H, Andoh T, Takemoto M, Kamata T (1972) Molecular weights of Konjac Mannans of various sources. Agri Biol Chem 36(8):1381–1387Sworn G (2000) Gellan gums. In: Handbook of Hydrocolloids. Phillips GO, Williams PA (eds) CRC/Woodhead Publishing, Boca Raton, pp 117–35Takahashi R, Kusukabe I, Kusano S, Sakurai Y, Murakami K, Maekawa A, Suzuki T (1984) Structures of Glucomanno-oligosaccharides from the Hydrolytic Products of Konjac Glucomannan Produced by a β-Mannanase from Streptomyces sp. Agric Biol Chem 48, 2943–2950Takigami S (2000) Konjac Mannan. In: Handbook of Hydrocolloids. Phillips GO, Williams PA (eds) CRC/Woodhead Publishing, Boca Raton pp 413–424Tischer CA, Iacomini M, Wagner R, Gorin PAJ (2002) New structural features of the polysac- charide from gum ghatti (Anogeissus latifolia). Carbohydr Res 37:2205–2210Tsujisaka Y, Mitsuhashi M (1993) Pullulan. In: Whistler RL, BeMiller JN (eds) Industrial Gums. Polysaccharides and Their Derivatives, 3rd edn. Academic, San Diego, CA, pp 447–460Ueda S, Fujita K, Komatsu K, Nakashima Z (1963) Polysaccharide produced by the genus Pullularia. I. Production of polysaccharide by growing cells. Appl Microbiol 11:211–215Vargas M, Albors A, Chiralt A, Gonzalez-Martinez C (2006) Quality of cold-stored strawberries as affected by chitosan-oleic acid edible coatings. Postharvest Biol Technol 41:164–71Verbeken D, Dierckx S, Dewettinck K (2003) Exudate gums: occurence, production, and applica- tions, Appl Microbiol Biotechnol 63:10–21Wallenfels K, Bender H, Keilich G, Bechtler G (1961) On pullulan, the glucan of the slime coat of Pullularia pullulans. Angew Chem 73:245–246Wallenfels K, Keilich G, Bechtler G, Freudenberger D (1965) Investigations on pullulan. IV. Resolution of structural problems using physical, chemical and enzymatic methods. Biochem Z 341:433–450Weiss J, Takhistov P, McClements J (2006) Functional materials in food nanotechnology. J Food Sci 71(9):107–116Wielinga WC, (2000) Galactomannans. In: Handbook of Hydrocolloids, Phillips GO, Williams PA (eds) CRC/Woodhead Publishing, Boca Raton, pp 413–423Williams PA, Phillips GO (2000) Gum Arabic. In: Handbook of Hydrocolloids. Phillips GO, Williams PA (eds) CRC/Woodhead Publishing, Boca Raton, pp 155–168Yuen S (1974) Pullulan and its applications. Process Biochem 9:7–9Zhang D, Quantick PC (1998) Antifungal effects of chitosan coating on fresh strawberries and raspberries during storage. J Hort Sci Biotechnol 73:763–7
114 M.E. Kramerdemands on their performance. They have to possess strength and integrity to beremoved from backing material and then undergo whatever processing is necessaryto deliver the film to its intended use. One of the biggest challenges to freestandingfilms is to have individual layers remain separate and not adhere to each other or tocurl once product is cut into individual pieces or sheets. Usually, attention must bepaid to the packaging material to ensure that the water-soluble polymers used inthese products do not absorb moisture, which would result in the individual piecessticking together. Use of starch and starch derivatives for producing edible coatings has a longhistory (Kester and Fennema 1986). Generally, such coatings have the advantageof lower cost compared to other alternative high tensile strength materials. Use ofhigh amylose cornstarch improves the properties of the resulting films. Chemicalsubstitution and acid hydrolysis of amylose-containing starches improve clarity andflexibility of coatings made from them. Glycerin and polyhydric alcohols are effec-tive plasticizing agents, which improve film properties but do so at some expenseof barrier characteristics. Applications and methods used for preparation of ediblestarch films and coatings are described in this chapter.4.2 Starch Structure and PropertiesStarch is the main polysaccharide energy storage material in the plant kingdom. Itis a mixture of the predominantly linear a–(1→4) glucan or amylose (Fig. 4.1), andthe highly branched, high molecular weight glucan or amylopectin (Fig. 4.2).Amylopectin is a glucan with a–(1→4) glycosidic linkages containing a–(1→6)branch points. Of the two starch polymers, amylose is more closely associated with the abilityto form films and coatings due to its predominant linear nature. Starch is both abun-dant in nature and readily available as an inexpensive commercial product. A filmor coating can be made from any type of starch that contains amylose. Amylosederived from fractionated starch has also been used to make all-amylose films,Fig. 4.1 Structure of amylose
4 Structure and Function of Starch-Based Edible Films and Coatings 115Fig. 4.2 Structure of amylopectinresulting in several predictable properties that can be attributed to the amylose frac-tion of starch (Galliard 1987). All starches with some amylose will form films when cast under the right condi-tions. Young (1984) cites examples from the 1960s using amylose-containing starchand fractionated amylose and amylopectin to form films. The presence of water asa plasticizer is identified here. Water generally decreases the tensile strength of thefilm by weakening intermolecular forces. Amylose and amylopectin molecules are packaged into semi-crystalline aggre-gates and these aggregates are systematically packaged into starch granules. Inthese tightly packed starch granules, the starch molecules have little affinity forwater and are not functional (Blanshard 1987). Native starch granules observedmicroscopically under plane-polarized light exhibit the characteristic polarizationor “Maltese” cross, which is due to birefringence properties of the crystalline por-tion of the granule. If starch granules remained in their inert state as they are found in nature, therewould be little interest in starch for most applications. When heat is applied tonative starch in the presence of sufficient water, granules begin to open up, swelland hydrate, which initiates the process of “gelatinization” or loss of granular andmolecular order. The physical size of the granule swells to several times its originalsize, and native crystallinity is lost. Microscopic evaluation will demonstrate lossof the polarization cross. Gelatinization occurs over a range of temperatures, and is dependent uponthe type of starch and its modification. The most apparent change upon starchgelatinization is a dramatic increase in viscosity. Monitoring the viscositythrough heating and gelatinization steps is used to characterize differentstarches. Instruments used to generate pasting profiles include the Rapid ViscoAnalyser (RVA), manufactured by Newport (Fig. 4.3) and Brabender Viscoamy-lograph. Gelatinized starch has swollen starch granules with some of the amyloseleached into the surrounding inter-granular fluid. If the granule is heatedfurther, the granules grow larger and larger until eventually they lose theirintegrity and identity, with amylose and amylopectin released to the surroundingliquid.
116 M.E. KramerFig. 4.3 RVA graphs of selected modified starches4.3 Chemical ModificationIn commercial food processing, there are demands placed upon starch, which can-not be met with native starch forms. To compensate for the various ways that nativestarches fail to deliver optimal performance, starches are chemically modified toenhance their properties or to create starch products with unique properties for vari-ous applications. The Food and Drug Administration limits the types of reactionsand reagent levels that may be employed for the manufacture of food-grade modi-fied starches. The Code of Federal Regulations defines “modified food starch, orfood starch-modified” (21CFR172.892) specifically, and methods that deviate fromthose outlined may not be called food starch-modified (Anonymous 2007a). Thestarch manufacturer and food processor using these ingredients need not identifyspecific reactions or treatments used to produce modified food starches, providedthe detailed definition is met.4.3.1 Cross-Linked StarchesFor the majority of food processing applications, fully swollen, intact granules aredesired for maximum viscosity and optimum water stabilization. Fruits, vegetablesand other high water content foods have a tendency to leach water into the foodmatrix continuously in the first 3–4 days after processing and fully intact granules
4 Structure and Function of Starch-Based Edible Films and Coatings 117Fig. 4.4 Cross-linking using phosphorous oxychloridewill continue to absorb this freed water to maintain constant viscosity and texture.Many types of modified food starch products are chemically cross-linked usingphosphorous oxychloride, sodium trimetaphosphate or adipic anhydride to preventfragmentation of starch granules (Fig. 4.4). These chemical bonds reinforce thenative granule structure, which prevents early swelling and cookout, as well asunwelcome granule disruption. Specially modified starches designed for formation of films and coatings areusually not designed to maintain granule integrity. Full functionality of a coatingstarch is achieved only when the majority of starch granules are fully disrupted andamylose and amylopectin polymers are fully dispersed in the aqueous medium. Forthis reason, starches specially modified to possess useful coating attributes are nottypically cross-linked.4.3.2 Substituted StarchesIn addition to cross linking, starches are often substituted with various reagents tomodify then properties and functionality. Substitution reagents include succinicanhydride, acetic anhydride, and propylene oxide (Fig. 4.5). These chemical enti-ties covalently attach to carbohydrate polymers inside of the starch granule. There are several positive attributes contributed by substitution modifications. Thefirst is that introduced functional groups help to open up the granule, increasing its affin-ity for water. This results in lower starch gelatinization temperatures and better hydra-tion. Another advantage is that the resulting starch gel is much less firm and exhibitsbetter clarity. In native starches, the amylose portion of starch can re-associate withtime in a process referred to as retrogradation. As retrogradation proceeds, the gelgradually becomes more opaque as water is expelled out. Steric hindrance caused bysubstituted groups on the polymer chains prevents re-associations, so that retrograda-tion and weeping do not readily occur. This advantage also makes the gel more resistantto breakdown during successive freeze-thaw cycles, which generally cause unmodifiednative starch gels to lose water and thus, their functionality.
118 M.E. KramerFig. 4.5 Substitution reaction using propylene oxide It has been known since the 1960s that partial etherification with propyleneoxide will result in better starch-based films. Hydroxypropylated starches generallyproduce films, which are clearer and more flexible compared to native starch films.High amylose starches derivatized with propylene oxide were studied in the mid-1960s (Jokay et al. 1967).4.3.3 Oxidized StarchFood starches are oxidized to improve their adhesion properties in coating applica-tions such as batters. Sodium chlorite, calcium hypochlorite and sodium hypochlo-rite are all approved starch oxidizing reagents for use in batter applications. Deepfried food coatings such as tempura coatings, beer battered coatings and other coat-ing types for meats, fish and vegetables often contain oxidized starches. Frenchfries are frequently coated with a batter to improve their eating quality by retainingcrispness after frying or as a way of delivering seasoning to the surface. An idealbatter coating firmly adheres to the surface of the food to be coated throughout thefreezing and frying processes. When used, breadcrumbs need to be retained on thefood surface also. Moisture permeability can be a desirable property for coatings,because water vapor needs to be allowed to escape from food during cooking withoutblowing off pieces of the coating into the fryer.4.3.4 Acid-Hydrolyzed StarchesAnother type of chemical modification, which has found use in designing starchproducts specifically for films and coatings, is acid modification. Acid-treated or“thin boiling” starch is produced by treating granular starch with a mineral acid topartially depolymerize starch molecules to a desired end point (Fig. 4.6). Acid-modified
4 Structure and Function of Starch-Based Edible Films and Coatings 119Fig. 4.6 Chemical modification of starch – acid hydrolysisstarch is usually used in applications where there is a high level of solids present inaddition to maintaining a relatively low hot paste viscosity during processing, butwhere a firm or rigid setback is desired after processing and cool down. Examplesinclude imitation cheese, jelly candies, processed meats, and extruded snacks andcereals. Acid modification or thinning serve the purpose of partially debranchingthe amylopectin portion of starch located within granule amorphous regions, so thatbehavior of the treated starch becomes more amylose-like (due to an increase in thelinear component). Experience with dextrins and maltodextrins indicates thatshorter polymer length results in better film formation when compared to nativeforms of starch.4.3.5 Dextrins and MaltodextrinsDextrins are often used to make various types of coatings on everything from phar-maceutical products, to confections, to edible glues and sealants. The traditionalmethod of manufacture of dextrins is in a dry, heated environment where glucosepolymers partially depolymerize and then repolymerize in linkages different fromthe a–(1→4) and a–(1→6) glycosidic bonds found exclusively in native starches(Kennedy and Fischer 1984). Acid may also be employed and variables includestarch type, amount/type of acid, moisture content during heating, and time/tempera-ture of heating (Nisperos-Carriedo 1994). These dextrin products can be soluble incold water, and have fair film formation properties and good adhesive properties.Dextrins have found use in confectionery products as a coating and as an alternativeto gum acacia. In panned candies, a layer of gum acacia solution is often utilized asa barrier between a high fat candy component, such as chocolate or nut butter, anda sugar shell. An aqueous coating of dextrin is also applied to the outside of choco-late prior to coating with a solvent-based coating such as edible shellacs, oftenreferred to as confectioners’ glaze. The undercoating here prevents solvent flavorsfrom migrating from the coating into the chocolate thus spoiling the flavor. Tapioca-based and corn-based dextrins have been used successfully in these kinds of candy
120 M.E. Kramerapplications to partially or fully replace gum Acacia due to cost and availabilityconsiderations. Maltodextrins are also manufactured by partial depolymerization of starches. Incontrast to dextrins, maltodextrins are manufactured using a wet process that usu-ally begins with the complete disruption of the starch granule with the use of heat(Anonymous 1995). A combination of acid and enzymes is added to a native starchdispersion to hydrolyze starch polymers to a given end point measured by dextroseequivalent or DE. DE is a measure of the reducing power of a polymeric mixtureof glucose polymers, where dextrose is assigned the reducing power of 100. Starchpolymers have a single reducing end, and depolymerization brings about a drop inmolecular weight, which results in more reducing ends and an accompanying risein DE. Under the definition provided in 21CFR184.1444, maltodextrins are poly-mers of d-glucose linked primarily by a–(1→4) glycosidic bonds, possessing a DEof less than 20 (Anonymous 2007b). Maltodextrins are water-soluble at concentrations up to 70% (w/v), and havegood film forming properties. Being of intermediate molecular weight, they formweak coatings on their own with good oxygen barrier properties. Murray and Luft(1973) studied the use of maltodextrin as a functional coating on fruit slices andnutmeats to extend shelf life.4.4 High-Amylose CornstarchHigh-amylose starches are produced from genetic mutants of corn (maize) thathave higher than typical amylose to amylopectin ratios. Starches with amylosecontents of 50, 70 or even 90% are sometimes used to produce films. High-amylose starches generally have the disadvantage of being highly crystalline,requiring high temperatures to achieve full gelatinization. To cook out high- amy-lose starch granules to full dispersion requires cooking temperatures well above100°C, which can be only achieved at above atmospheric pressures or with directinjection of steam. High-amylose starches have found widespread use in applications where firmgels and some loss of water are desirable, such as jellied candies. These high-amylose starches are also used to make films and coatings, and were used in coatingsprepared for Apollo space flights. Films made from purified amylose isolated from conventional corn starch werealso evaluated (Young 1984). Lourdin et al. (1995) studied the effect of amylose toamylopectin ratio using a combination of native starches and starch fractions. Theyfound that tensile strength and elongation increased with increasing percentages ofamylose. There are more recent examples in the patent literature where the use ofhigh amylose starches have been used to extend the shelf life of deep fried foods(textural quality) after they have left the fryer (US patent 5976607). Battered vege-tables and French fries are often coated with a high-amylose starch batter so that
4 Structure and Function of Starch-Based Edible Films and Coatings 121they will remain crisp for additional minutes under a heat lamp. High-amyloseand hydroxypropylated modified food starches have been found to be effective forthese types of foods. Pagella et al. (2002) also found that high-amylose starchesproduced the most commercially acceptable freestanding films by criteria set forthin their study. Films made from high-amylose rice and pea starches were found tohave excellent oxygen barrier properties, better than those of protein-based alterna-tives (Mehyar and Han 2004).4.5 Additives4.5.1 PolyolsA number of additives that can be included in the formulation of a coating solutionwhich will alter the properties of the resulting coating layer or freestanding film toimprove performance. Generally, plasticizers are added to these polymers toimprove the overall flexibility and extensibility of the resulting film or coating. Inthe realm of edible films, polyhydric alcohols are the most common types of plas-ticizers for edible films, including propylene glycol, glycerin, sorbitol and otherpolyols. There are many publications where various types of polyols were studiedfor their effects on the resulting films (Arvanitoyannis et al. 1996, 1997; Psomiadouet al. 1996; Arvanitoyannis and Biliaderis 1998; Parra et al. 2004; Fama et al. 2005;Rodriguez et al. 2006). In most studies, starch-based films are plasticized mosteffectively with the use of glycerin, which has specific advantages of being rela-tively non-sweet, inexpensive, and having been granted GRAS (generally recog-nized as safe) status by the FDA. Strength, pliability and flexibility of a film or coating can be measured usingtensile testing techniques. A strip of pre-cast film of specific known dimensions, ineither rectangular or bar bell shape, is pulled apart under a known force usingTexture Analyzer or Instron-type testing instruments (ASTM D2370) AnonymousMethod #D2370. A strip of pre-cast film of specific known dimension is pulledapart at a carefully defined speed, while resistance is recorded over time. Peak forceneeded to break the film, as shown by a sudden drop in force, is recorded as ameasure of the overall film strength. The extent or distance that the film is stretchedprior to the failure point is the extensibility, which is often expressed as a percent-age of the length of the film piece tested. This percent extensibility is used as ameasure of flexibility, pliability and resiliency of the film or coating. In general,starch-based films are very strong when compared to those of other edible poly-mers, but usually score less favorably on the measurement of extensibility (Donhowand Fennema 1994; Chang et al. 2000). The strength of the film has also beendemonstrated to be dependent upon moisture content of the film, which is in turninfluenced by the relative humidity of the environment in which it is stored (Changet al. 2000; Bertruzzi et al. 2003).
122 M.E. Kramer Plasticizing polymers improves pliability and flexibility of the film or coating.Addition of glycerin or other plasticizing agents makes the resulting film morepliable. Further addition of plasticizing agents will result in rubbery, sticky films.Thus, it is necessary to optimize the amount of plasticizing agent used in a formu-lation to attain desired film properties. However, there are some applications, suchas vegetarian soft capsules, where a rubbery, extensible sheet is considereddesirable.4.5.2 SugarsSugars and other low molecular weight materials, when added to starch-basedfilms, should also act as effective plasticizers (Zhang and Han 2006a). Generallythis effect is true up to a point, but sugars generally make resulting films moreglass-like and brittle. Shamekh et al. (2002) obtained better results with films madefrom starch hydrolysates when low molecular weight sugars were removed. Insome coating applications (e.g. desserts), cracking as a result of brittleness does notconstitute a complete failure, and sugars can be incorporated up to the level that isnecessary to achieve desired sweetness. In more demanding applications where anoxygen barrier is desired, cracks are unacceptable, such as in tablet coatings forpharmaceutical products. Very little sugar can be tolerated in these starch-basededible films.4.5.3 MaltodextrinsMaltodextrins have a number of advantages as additives to edible films. They canslightly reduce the brittleness of starch films through a plasticization and humect-ancy effect due to their relatively lower molecular weight and slight hygroscopicproperties. The range of available DE for maltodextrins allows the coating devel-oper to dial in the desired property by choosing the appropriate DE to add to thecoating formulation. Obviously, in a tack coating to adhere spherical particulates toa food surface stickiness will be much more welcome than in an invisible coatingintended to extend shelf life of a high fat snack. The most important function that maltodextrin can serve is to increase thesolids of the coating solution to achieve faster drying. It is typical that 10–20%(w/v) solids of maltodextrin can be added to the solution before excessive vis-cosity, sweetness or undesirable flavors are observed. Although it is possible toraise solids levels to values much higher than 20% with addition of higher DEmaltodextrins or corn syrups, this strategy is often found to be counter produc-tive. Excessively high solids content for coating solutions is often found toprolong drying compared to those in the 20–40% range. This observation isprobably due to the increase in hygroscopicity of smaller molecular weight com-
4 Structure and Function of Starch-Based Edible Films and Coatings 123ponents and water binding capability of larger, starch-like fractions (Zhang andHan 2006b)4.5.4 DetackifiersA number of different products have been proposed as detackifiers for addition tofilm forming starch-based polymer solutions to decrease overall stickiness of theresulting surface. Polysorbates, lecithin and other surfactants have been used todecrease overall tackiness of starch-based films and coatings. One reason to reduce tackiness of films is to prevent multiple sheets offreestanding films or flat surfaces of coated materials from adhering to eachother. In addition to surfactant additives, small amounts of fine insoluble par-ticulates have been successfully used to decrease tackiness of a film or coatedsurface.4.5.5 HumectantsGlycerin is used as a plasticizer or humectant to maintain an adequate moisturelevel for a continuous film casting. Keeping the film hydrated assures adequateflexibility and resiliency. When starch-based edible films are subjected to relativehumidity environments below 20–25%, they can experience cracking. Use of glyc-erin and polyols can lower tolerances to 10–15% relative humidity. When a film ismade from highly soluble polysaccharides such as gum arabic, high relative humid-ity conditions will bring about dissolution of the film. One of the easiest families of functional ingredients to incorporate into free-standing films and coatings is color. FD&C colorants are commonly used at suchlow levels that they have a minimal effect on the integrity of the coating. Exceptionsto this rule are coatings with tight tolerances for performance, such as pharmaceuti-cal tablets, and those where an opacifier, like titanium dioxide, would need to beadded as an undercoat.4.5.6 LipidsAddition of lipids to a coating solution can improve barrier properties of the result-ing coating. This phenomenon has been demonstrated through the improvement ofwater vapor transmission and oxygen barrier properties of films and coatings(Garcia et al. 2000). Addition of high melting point waxes has been shown to beparticularly effective in improving moisture barrier properties of films (Han et al.2006). Addition of approximately 20% (based upon polymer weight) edible oil to
124 M.E. Kramera starch-based coating solution is generally found to extend shelf life of the coatinglayer in high-oil foods such as nutmeats.4.5.7 Emulsifiers and Wetting AgentsIt is sometimes beneficial to add a wetting agent or surfactant to the coating solu-tion to improve coating efficiency. When applying an aqueous solution to a fattysurface such as nuts, chocolate or compound coatings, it is usually advantageous toadd a little lecithin or other emulsifiers to the coating solution to lower surfacetension and allow the surface to be coated to wet. If the surface to which the coatingwill be applied is not sufficiently wetted by coating solution, the resulting coatinglayer will not tightly adhere to the food surface. Subsurface bubbles can ruin theappearance of the product. These bubbles will make a transparent coating opaqueor alter the hue of a colored coating.4.6 Methods of Application and ManufactureCoatings can be applied to food surfaces by just about any method. Starch solutionshave been applied using dipping, spraying, and ladling directly onto a tumblingmass of product. For meat products, a deluge machine has been used. This machinefunctions as a waterfall apparatus, and coats the product surface much the way thata chocolate enrober does. In each example, the liquid dispersion of polymer isapplied to the food surface to be coated, and water is allowed to evaporate off untilthe coating is deposited. The coating will be in equilibrium with the environmentof the package and also with the food itself. Coatings on low moisture foods willbe hard, non tacky and transparent. Coatings on higher moisture materials will bemore pliable and slightly tacky. High moisture foods such as meats will have asemi-solid paste like consistency.4.6.1 Free FilmsOne family of coatings that has received a lot of interest in the last 10 years is thatof freestanding films, which are intended to be consumed without any backingmaterial or center. Challenges of producing an acceptable breath-freshening film,for example, includes making the film with enough integrity that it can be cut,packaged and remain dispensable throughout product shelf life. These criteria mustbe accomplished without unacceptably extending the desired time of film dissolu-tion and flavor delivery on the tongue or roof of the mouth. Dissolution in the
4 Structure and Function of Starch-Based Edible Films and Coatings 125mouth is largely a function of the nature of polymers used and thickness of thepiece. Thicker pieces will have better strength, but might be unacceptable in themouth or have an undesirably long dissolution time. Freestanding films can be made in the laboratory on a variety of surfaces. Themethod most often used in our lab is to affix sheets of polyethylene food wrap ontothe bench top surface with adhesive tape. A thin film of starch dispersion is thenapplied using a Gardner draw down bar (Fig. 4.7) or bird applicator. After wateris allowed to evaporate, the film can then be peeled from the surface where it iscast and cut to whatever use is required. Surfaces for casting include plastic, glass,Plexiglas and various types of semi-flexible plastic sheets used for cutting boards.A textured surface or an especially flat, shiny surface can be imparted to the filmdepending upon the surface used. Backing material should be selected based onthe ease with which the film can be removed. Some materials, such as glass, canhave a tendency to hold onto the film without releasing it upon drying. Othermaterials, such as siliconized paper, might release too readily, which could resultin ripped sheets and small pieces as the film separates from the backing tooquickly and unevenly. Flexible materials have obvious advantages for removal ofedible film. Commercially, films are typically deposited, dried and removed on a continu-ous basis, usually on a rotating belt. The length of the belt, speed, temperatureand air velocity can all be altered to ensure good drying at the appropriate pointin the process. Belts made of silicone and stainless steel are often used for thedrying step.Fig. 4.7 Paul Gardner universal applicator (Paul N. Gardner Company, Inc., Pompano Beach, FL)
126 M.E. Kramer4.7 Methods for Measuring EffectivenessOne of the challenges of measuring any desirable property of a coating is that mosttesting protocols are designed for freestanding films. Much of the instrumentationand tests are based upon non-edible plastic packaging materials. A freestandingfilm is, by definition, not equivalent to a coating applied to a surface. Someresearchers have tried to control the difference between coatings and freestandingfilms by applying the test polymers to a neutral backing material, such as paper andmeasuring oxygen and water vapor transmission rates on the coated paper in com-parison to uncoated paper (Hurtado et al. 2001). The differences between a true coating and a freestanding film are particularlylarge when measuring fat barrier properties. Fat migration tests in which a givenquantity of oil is dropped upon a piece of pre-cast film to measure migration ratesto some collection surface, like a filter paper, are somewhat artificial. This is a verydifferent environment than the same peanut oil, for example, embedded in nut masswith an edible coating of gum acacia, dextrin or modified food starch used to pre-vent its migration over a period of months into a chocolate coating surrounding it. There is also the challenge of casting a film with defined dimensions. This istrue whether transmission rate or tensile strength is to be measured. Instrumentsand test procedures often require a particularly large piece of film. For inflexiblematerials, it can be difficult to produce an intact freestanding film of sufficient size.Instrumentation is usually designed with non-edible packaging in mind. Largersheets of film can often be cut to the width and length desired for testing, but thick-ness can be a problem. The common method of casting the film by pouring orspreading with draw down bars, film applicators, bird applicators, formed rods, orwire wrapped rods is often not acceptable for this purpose. Best results are usu-ally obtained when polymer solution is poured onto a perfectly flat surface withrestraining walls on four sides. This approach will minimize the variability in the Zdimension, but not eliminate it entirely.4.8 Coating Applications4.8.1 Economic ConsiderationsAs with any additive, the intended benefit has to justify the additional cost of itsuse. The cost of ingredients that make up an edible coating are often less importantthan the cost of equipment and time required to apply the coating and the cost ofdrying the coated product prior to packaging. Most equipment required for coatingprocesses is expensive. If in certain instances the cost of coating will add a sub-stantial cost to the final product, the overall benefit derived from coating theproduct must outweigh this additional cost. This way, consumer value of the coatedproduct is maintained.
4 Structure and Function of Starch-Based Edible Films and Coatings 1274.8.2 Coatings to Enhance AppearanceAn example of a coating used primarily for visual appeal, such as a shiny surface,is the application of shellac-based coatings to surfaces of chocolate-panned items.Chocolate-covered peanuts, malted milk balls and jellybeans commonly have ashine coat added to their surfaces (Fig. 4.8). In the case of chocolate items, shellacprovides the added benefit of preventing cocoa butter from staining packaging.A thin shellac layer also protects individual pieces from rubbing against each other,giving undesirable scuff marks to the chocolate. There are a number of challenges to replacing a solvent-based ingredient, suchas shellac, with an aqueous-based coating. It might be necessary to add a surfactantto the coating solution to allow the food surface to be coated while the coating isbeing deposited by evaporation. For coating sugar confectionery, it is a realchallenge to add an aqueous coating solution, containing perhaps 80% water, to asubstrate that is water-soluble. This obstacle can be overcome by either puttingdown a pre-coat of a water-insoluble material, such as wax, prior to application ofthe aqueous coating or by the use of aqueous coating techniques employed by thepharmaceutical industry such as dipping or spraying. Aqueous-dispersed, starch-based films are usually applied as a solution. The waterof the coating solution is then evaporated off to deposit the coating. Another disad-vantage that aqueous systems have over some solvent-based systems is that the coatingitself remains as water-soluble as the original starch used in the coating solution.Fig. 4.8 Malted milk balls (this figure is not referred to from in the text)
128 M.E. KramerStarch-based coatings do not undergo a cross-linking or curing step to make themmore water-insoluble. This can limit moisture barrier properties of the film, andrestrict use of the film in higher humidity environments. This limitation can alsobe considered a positive attribute in various applications where the coating is to bewashed off once it has performed its protective function, perhaps at some intermedi-ate step in a process. Perhaps the biggest challenge comes from the fact that water is less volatile thanethanol, which is used to disperse and deposit shellac and many protein-basedcoatings. The presence of water typically leads to longer drying times, which cancontribute to greater expense.4.8.3 Flavored CoatingsFlavored coatings can be divided up into basic categories. A coating might be of asimilar flavor as the item to be coated, thus, reinforcing the overall flavor impact.Coatings might also be flavored with a contrasting flavor for a novelty effect. If acoating is to be applied to extend shelf life, it might be necessary to flavor the coatingto diminish delay in the initial release of flavor when first placed in the mouth. In pharmaceutical tablets and nutritional supplements, it is often desirable toapply a coating to mask or disguise an unpleasant flavor. This goal is usuallyaccomplished by a combination of the masking properties of the polymer, a pleasantflavor to distract or with the addition of flavor masking agents.4.8.4 Oxygen BarriersStarch-based coatings usually compare very favorably to other coating alternativesin regard to oxygen barrier properties. By creating a barrier between atmosphericoxygen and the food, an extension of shelf life can be demonstrated (Phan et al.2005). One obvious type of food that might gain advantages from such a coatinglayer is nutmeats. Nutmeats have many characteristics that make them ideal candi-dates for coating. Because of their high oil content, oxidative rancidity is the limitingfactor in their shelf life. They also have a sufficiently high monetary value to justifywhatever costs might be associated with coating. Lastly, their need for individualpiece identity is enhanced with coating. There are some challenges in coating nuts.It is important that the coating step does not allow nuts to become bruised or crushed,such that they begin to express oils to their surfaces. Although nuts are usually coatedwith an aqueous solution that includes emulsifiers, once oil flows to the nut surface,coating pretty much becomes impossible. Walnuts and macadamia nuts have beenfound to be particularly problematic. Walnuts are very fragile and a small amount oftumbling can easily bruise the nuts. Macadamias are very hard, but also very high in fat.
4 Structure and Function of Starch-Based Edible Films and Coatings 129It is possible to coat either of these two nut varieties, provided care is taken to conductthe coating as gently and as quickly as possible. Nuts can also be a challenge foraqueous coatings, as it is very important that the water content of nuts remain verylow for both desired textural properties and overall shelf life. One area in which the use of starch-based edible films and coatings has enjoyedextensive practice is the process whereby volatile, oil soluble flavors and fragrancesare encapsulated into a glassy carbohydrate-based matrix. Fragrance and flavoroils are often highly susceptible to oxidation. Use of various gum, starch and malto-dextrin products to construct a carbohydrate-based capsule provides an effectivebarrier for greatly extended shelf life.4.8.5 Moisture BarriersWater-soluble polymers might not at first be thought of as a choice for impedingmoisture migration from a high moisture component of a food to that of a low moisturecontent. Starch-based coatings have been demonstrated to at least slow mois-ture migration (Hurtado et al. 2001; Chung and Lai 2005). Whether or not thereduction in moisture transfer is commercially significant is dependent upon the shelflife of the food and the gradient between the two components. Arvanitoyannis andBiliaderis (1998) found that addition of sodium caseinate to a starch-based filmlowered the water vapor transmission rate relative to that of a pure starch film, butdid so at the expense of the physical attributes of the film. In many chocolate confectionery applications, it is necessary to form an oilbarrier to prevent non-cocoa butter oils from entering the chocolate, causing thechocolate to lose its temper and to bloom. Oils with low melting points canmigrate to the surfaces of chocolates and re-crystallize, forming a greasy grayishwhite layer known as fat bloom (Minifie 1989). Coconut and nut oils can be keptisolated from chocolate in such products with the use of edible coatings. Anotheradvantage of coating high-fat confectionery products with a sealant coat on theouter surface is to avoid a scuffed appearance and to inhibit migration of mobilefat components to the product surface, leading to staining of the package material.Figure 4.8 shows coated malted milk balls to protect the product. Coatings can be formulated with antioxidant ingredients to improve the over-all protection provided by the film. Murray and Luft (1973) used SO2 in theirmaltodextrin coatings to further enhance color preservation of dried apple andapricot slices.4.8.6 Tack and Adhesive CoatingsOne relatively straightforward application for edible films is as a tack or adhesivecoating in which the wet solution is used as an edible glue to adhere one food
130 M.E. Kramercomponent to another. A very simple example might be an oil spray applied to asnack food, followed by coating with a seasoning blend. In this example, there isno drying step, and seasonings are weakly adhered to the snack food surface.Where it is necessary to improve adhesion or fix particulates, it is necessary touse a polymer-based adhesive coating material. In such instances, maltodextrinsare added to improve adhesion. Inclusion of a high DE maltodextrin within theformulation will increase adhesion and tackiness of the coating. This tackiness isaccompanied by an increase in pliability and hygroscopicity of the coating. An example of a tack coating is adherence of a powdered seasoning blend to aproduct surface. In this scenario, seasoning should be fixed fast to the surface of thesnack food to prevent rub off during distribution and/or to minimize the tendency ofseasoning to adhere to the consumer’s skin or to stain the fingers. For some snackand bakery applications, larger pieces, such as poppy, caraway or sesame seeds orgrains like wheat berries or oatmeal, might be adhered to product surfaces. Thesepieces can be held in place with an edible tack coating. There are other exampleswhere components need to be fixed to each other. Examples include granola clustersas well as granola bars. Ready-to-eat cereal flakes might be coated with pieces ofwhole grain, with or without additional flavorings applied to product surfaces. For applications in which large particulates need to be held fast onto a largerproduct piece (as in Fig. 4.9), best results are usually obtained with a three-stageapplication method. In a rotating drum or pan or on a belt, the larger piece is firstwetted with the film forming solution. Next, the smaller particulate is added, andproduct is mixed thoroughly. Lastly, an additional layer of tack coating is appliedon top as a seal coating. In these tack-type coating applications, it is usually onlynecessary to apply 0.2–0.5% of coating on a final dry weight gain basis toachieve desired results. This range is large, because both the density of the itemto be coated and the size of the piece (surface area) influence the amount of tackmaterial needed. Low moisture snack foods are not ideal substrates for use of a coating solutioncontaining up to 80% water. Extruded corn collets and wheat-based baked snackssuch as crackers are very prone to staling and deformation at higher moisturelevels. It is possible to apply starch-based coatings to these snack foods for shine,protection or to attach particulates. Good results can be achieved through applica-tion of a minimal amount of material to achieve the desired effect and quickdehydration of the coating before deleterious effects can begin to occur. Use of ahigh molecular weight coating material to assure adequate moisture control isalso important. For particularly sensitive materials, a side vented, perforatedwalled or aqueous film coating device might be necessary.4.8.7 Anti-Microbial CoatingsCoatings intended to delay or prevent growth of microorganisms have been pro-posed for many years (Fama et al. 2006). For many foods, deleterious, microbialgrowth is largely a surface phenomenon. Thus, limiting bacterial growth on the
4 Structure and Function of Starch-Based Edible Films and Coatings 131Fig. 4.9 Spices and particulates on breadsurface of food is anticipated to improve overall shelf life. Even tiny breaches inthe coating could be a large concern for these kinds of products. There is plenty ofinterest in these types of coatings in the industry, and there is evidence that they canbe very effective (Jagannath et al. 2006).4.8.8 Coatings to Alter or Enhance TextureIn sugar-shelled or hard-panned candies, a molded piece of chocolate, peanut butteror other confection is placed in a rotating candy pan and coated with multiple appli-cations of highly-concentrated sugar solution. The panning action ensures thatsolution is applied evenly and that a hard sugar shell results upon crystallization.Dextrins and starch-based coatings are sometimes included in final layers of coat-ings to produce speckled and mottled surface effects. In some cases, a starch-based
132 M.E. Kramerpolymer is added to more conventional sugar shelling to alter the bite or strength ofthe coating. Glassy polymers, such as high molecular weight maltodextrins andstarch hydrolysis products, have a more resilient and flexible texture, which makesthem less brittle in the mouth. Rough uneven coatings or less crystalline and brittlecoatings are typically considered to be faults, if they were not intentional. However,unusual flavors, colors, and textures are what drive novelty in confectioneryproducts. In some applications, it is advantageous to coat pieces to improve product flow,maintain superior piece identity or to prevent clumping and agglomeration of dif-ferent components during distribution and shelf life. Near transparent coatings thatprevent clumping in granola and trail mix coatings are one example of this type ofapplication.4.8.9 Flavor DeliveryA successful flavor delivery film has to possess the strength and stability of anyfreestanding film while delivering its load of flavor components. Flavor compoundsare often not water-miscible, which can present various challenges to water dispers-ible polymers such as starch. Oil-based flavors, such as citrus and other volatileoils, can be immobilized in the viscous film-forming liquid in droplets smallenough to prevent coalescence. Surfactants and emulsifying agents are only occa-sionally necessary for these applications. Emulsion breakdown and phase separa-tion are prevented through homogenization or high shear mixing to assuresuspension of small droplets and an adequately high solution viscosity to slow oildroplet mobility. Through these meane, coalescence and creaming are minimized.The temporary emulsion need only be stable for the time it takes for water to evapo-rate off, leaving behind the film with the oil droplets encased within the resultingglassy matrix. Many flavor ingredients such as cocoa are water insoluble, and have to be evenlydispersed throughout the polymer matrix, without being disruptive to the integrityof the film. As with delivery of any “active” component, the minimum level offlavor needed to deliver the desired impact must be balanced against whatevernegative contribution the insoluble component will have on strength and resiliencyof the film.4.8.10 Drug DeliveryDrug delivery through edible films has advantages over more conventional drugdelivery devices such as liquid, capsules, or tablets. Even without water, this typeof medication can be easily ingested. Edible film delivering medication can providean obvious advantage for people who have trouble swallowing, suffer from dysphagia
4 Structure and Function of Starch-Based Edible Films and Coatings 133or for patients who reject other easy to swallow medications. Small children andhousehold pets also fit into this category in which swallowing can be difficult.Topical application of films to a well-targeted area of the oral cavity is also animprovement over other delivery techniques. An example here would be a topicalanesthetic for pain relief.4.9 ConclusionThe concept of starch-based edible films is a technology that has been recognizedto have significant potential for providing a variety of solutions to the food industry.The real advantages of starch are its relatively low cost because it is abundant innature and it can be subjected to a number of modifications (chemical and genetic)to alter and improve its performance. In many successful applications of starch-based coatings, other polymers can be added to augment and improve performancecharacteristics. These could include gums to prevent loss of moisture, or maltodextrinsto change gloss and tack characteristics or cellulosic or protein-based ingredients toimprove their performance and functionality.ReferencesAnonymous (1995) MALTRIN® “maltodextrin and corn syrup solids for food formulations” Grain Processing CorporationAnonymous (2007a) 21Code of Federal Regulations 172.892Anonymous (2007b) 21Code of Federal Regulations 184.1444Anonymous Method #D2370 American Society of Testing MaterialsArvanitoyannis I, Billaderis CG (1998) Physical properties of polyol-plasticized edible films made from sodium caseinate and soluble starch blends. Food Chemistry 62(3): 333–342Arvanitoyannis I, Psomiadou E, Nakayama A (1996) Edible films made from sodium caseinate, starches, sugars or glycerol, Part 1. Carbohydrate Polymers 31: 179–192Arvanitoyannis I, Psomiadou E, Nakayama A, Aiba S, Yamamoto N (1997) Edible films made from gelatin, soluble starch and polyols, Part 3. Food Chemistry 60(4): 593–604Bertruzzi MA, Armada M, Gottifredi JC (2003) Thermodynamic analysis of water vapour sorp- tion of edible starch-based films. Food Science and Technology International 9(2): 115–121Blanshard JMV (1987) Starch granule structure and function: a physiochemical approach. In Galliard T (ed) Starch: Properties and Potential, 2nd Edn. Wiley, New York, NY, 16–54Chang YP, Cheah PB, Seow CC (2000) Plasticizing-antiplasticizing effects of water on physical properties of tapioca starch films in the glassy state. Journal of Food Science 65(3): 445–451Donhow IG, Fennema O, (1994) “Edible films and coatings: characteristic, formation, definitions, and testing methods. In Krochta J, Baldwin E, Nisperos-Carriedo M (eds) Edible Coatings and Films to Improve Food Quality, Technomic, Lancaster, 1–24Fama L, Rojas A, Goyanes S, Gerschenson L (2005) “Mechanical properties of tapioca-starch edible films containing sorbates.” Swiss Society of Food Science and Technology. Elsevier LWT 38: 631–639Fama L, Florese SK, Gerschenson L, Goyanes S (2006) Physical characterization of cassava starch biofilms with special reference to dynamic mechanical properties at low temperatures. Carbohydrate Polymers 66: 8–15
134 M.E. KramerGalliard T (1987) Starch availability and utilization. In Galliard T (ed) Starch: Properties and Potential, 2nd Edn. Wiley, New York, NY, 1–15Garcia MA, Martino MN, Zaritzky NE (2000) Lipid addition to improve barrier properties of edible starch-based films and coatings. Journal of Food Science 65(6): 941–947.Han JH, Seo GH, Park IM, Kim GN, Lee DS (2006) Physical and mechanical properties of pea starch edible films containing beeswax emulsions. Journal of Food Science 71(6): E290–E296Higgins C, Qian J and Williams K (1999) Water dispersible coating composition for fat-fried foods US Patent 5976607Hurtado ML, Estevez AM, Barbosa-Canovas G (2001) Physical characterization of a potato starch edible coating used in walnut storage. Proceeding of the 4th International Conference on Postharvest, Ben-Arie R, Philosoph-Hadas S, (eds) Acta Hort. 553, ISHS, 627–628Jagannath JH, Radhika M, Nanjappa C, Murati HS, Bawa AS (2006) Antimicrobial, mechanical, barrier and thermal properties of starch-casein based, neem (Melia azardirachta) extract con- taining film. Journal of Applied Polymer Science 101: 3948–3954Jokay L, Nelson GE, Powell EL (1967) Development of edible amylaceous coatings for foods. Food Technology 21: 1064–1066Kennedy HM, Fischer AC (1984) Starch and dextrins in prepared adhesives. In Whistler R, BeMiller JN, Paschall EF, (eds) Starch Chemistry and Technology, 2nd Edn. E. Academic, New York, NY, 593–610Kester JJ, Fennema OR (1986)Edible films and coatings a review. Food Technology 1986: 47–59Lourdin D, Dell Valle G, Colonna P (1995) Influence of amylose content on starch films and foams. Carbohydrate Polymers 27: 261–270Mehyar GF, Han JH (2004) Physical and mechanical properties of high amylose rice and pea starch films as affected by relative humidity and plasticizer. Journal of Food Science 69(9): E449–454Minifie B (1989) Chocolate, Cocoa and Confectionery, 3rd Edn. Van Nostrand Reinhold, New York, NY, p 109Murray DG, Luft LR (1973) Low-DE corn starch hydrolysates. Food Technology 27: 32–40Nisperos-Carriedo M. (1994) Edible coatings and films based on polysaccharides. In Krochta J, Baldwin E, Nisperos-Carriedo M, (eds) Edible Coatings and Films to Improve Food Quality, Technomic, Landcaster, 305–335Pagella C, Spigno G, DeFaveri DM (2002) Characterization of starch-based edible coatings. Trans IChemE 80(Part C): 193–198Parra DF, Tadini CC, Ponce PAB, Lugao AB (2004) Mechanical properties and water vapor trans- mission in some blends of cassava starch edible films. Carbohydrate Polymers 58: 475–481Phan TD, Debeaufort F, Luu D, Voilley A (2005) Functional properties of edible agar-based and starch-based films for food preservation. Journal of Agriculture Food Chemistry 53: 973–981Psomiadou E, Arvanitoyannis I, Yamamoto N (1996) Edible films made from natural resouces; microcrystalline cellulose (MCC), Methylcellulose (MC) and corn starch and polyols – Part 2. Carbohydrate Polymers 31: 193–204Rodriguez M, Oses J, Ziani K, Mate JI (2006) Combined effect of plasticizers and surfactants on physical properties of starch-based edible films. Food Research International 39: 840–846Shamekh S, Myllarinen P, Poutanen K, Forseell P (2002) Film formation properties of potato starch hydrolysates. Starch/Starke 54: 20–24Young A (1984) Fractionation of starch. In Whistler R, BeMiller J, Paschall E, (eds) Starch Chemistry and Technology, 2nd Edn. Academic, New York, NY, 249–284Zhang Y, Han JH (2006a) Mechanical and thermal characteristics of pea starch films plasticized with monosaccharides and polyols. Journal of Food Science 71(2): E109–E118Zhang Y, Han JH (2006b) Plasticization of pea starch films with monosaccharides and polyols. Journal of Food Science 71(6): E253–E261
136 F. Debeaufort and A. Voilley Bio-based polymers Extracted From biomass Synthesized from bio- Produced from microor- derived monomers ganisms Proteins Lipids Starch, cellulose Animal (waxes,gums and chitosan (casein, fat and gelatin) oils) Plant (zein, gluten) Polylactate and other Bacterial compounds polyesters (xanthan, pullulan)Fig. 5.1 Different types of biomaterialsFig. 5.2 Transfers that can be potentially controlled by edible barriersand Cuq 1998). Coatings are either applied to or formed directly on foods, whilefilms, on the other hand, are self-supporting structures that can be used to wrapfood products. They are located either on the food surface or as thin layers betweendifferent components of a food product. An example of the latter would be a filmplaced between the fruit and the dough in a pie to provide protection against trans-fer and mechanical stress (Fig. 5.2). Because they are both a packaging and a food component, edible films andcoatings have to fulfill the following specific requirements:– Good sensory attributes (neutral or favourable to the product to be coated)– High barrier and mechanical efficiencies
5 Lipid-Based Edible Films and Coatings 137– Biochemical, physicochemical, and microbial stability– Non-toxicity and safety– Simple technology– Non-polluting nature– Low raw material and processing cost5.2 Formulation of Edible Films and CoatingsBecause there are many different types of edible packaging, composition of ediblebarriers is very diverse. There are no specific regulations that deal with formulationand application of edible films and coatings. Since they are eaten with the food towhich they are applied, all food ingredients and additives allowed by CodexAlimentarius, US Food and Drug Administration, or European Union regulationscan be potentially used in their formulation. These regulations allow an almostinfinite choice of components for formulation of films and coatings. Choice ofwhich component to use, however, largely depends on the targeted product objec-tives and on technological and sensory constraints. The scientific and industrialpatent literature over the last 20 years reveals a broad range of substances cited asfilm and coating constituents. More recently, new film/coating formulations havebeen based on vegetable or fruit purees, including those of bananas, apples, andzucchini. Krochta and Demulder-Johnston (1997) have provided a fairly compre-hensive list of potential applications of film-forming substances. The most commonly used hydrophobic film-forming barrier materials include,in decreasing order of barrier efficiency:– Waxes– Lacs/lacquers– Fatty acids and alcohols– Acetylated glycerides– Cocoa-based compounds and their derivativesDecreasing efficiency can be explained by the chemical composition of the mole-cules, such as presence of polar components, hydrocarbon chain length, andnumber of unsaturation or acetylation. For components having a common chemicalnature, an increasing chain length modifies barrier properties because molecularpolarity decreases, and this does not favour water solubility of the film (McHughand Krochta 1994b, c).5.2.1 Lipid-Based Edible FilmsEdible barriers based on hydrophobic substances such as lipids were developedspecifically for limiting moisture migration within foods. These hydrophobic
138 F. Debeaufort and A. Voilleysubstances are effective barriers against moisture migration because of their apolarnature (Morillon et al. 2002). A list of hydrophobic substances used as componentsof edible films and coatings, based on research and patents published in thelast 15 years, is provided in Table 5.1. A very wide range of compounds could be used in formulation of edible packaging.The decision on what to use will depend mostly on the target application. Manystudies have investigated use of coatings on fresh fruits and vegetables to controldesiccation. Substances most often used for this application are waxes. In enology,wine bottle corks may be coated with beeswax and paraffin wax to prevent soakingof the cork and release of flavours from the cork to the wine. This coating methodoffers an alternative to use of plastic corks in wine bottles. Cocoa butter andcocoa-based films are widely used in confectionery and biscuit industries. Otherfilms are used in pizza and dough products to prevent moisture migration and incrispy and dry cereal-based products to prevent loss of flavour and water from fator aqueous stuffing and filling. Most food-grade lacs and varnishes are applied inthe pharmaceutical industry, as a protective layer for active substances. In the foodindustry, these are used to improve surface appearance (color, sheen, and gloss)and reduce surface stickiness. Few studies have investigated effects of applyinglacs and varnishes of natural origin to foods. Nevertheless, many food additivesuppliers have proposed using them as coating agents. Emulsifiers and surfaceactive agents are sometimes used as barriers to gases and/or moisture on fish ormeat products. They may also be added to a coating formulation to improve surfaceadherence between the coating and food article to be coated.Table 5.1 Hydrophobic substances used as film former or barrier compoundsOils, fats, shortening, margarine Animal and vegetable native oils and fats (peanut, coconut, palm, palm kernel oils, cocoa, milk butters, lard, tallow, etc.) Fractionated, concentrated and/or reconstituted oils and fats (fatty acids, mono-, di-, and triglycerides, cocoa butter substitutes, etc.) Hydrogenated and/or transesterified oils (margarine, shortenings, etc.)Waxes Natural vegetable and animal waxes: candelilla, carnauba, jojoba bees, whales Non-natural waxes: paraffins, mineral, microcrystalline, oxidized or non-oxidized polyethyleneNatural resins Asafoetida, Benjoin, Chicle, Guarana, Myrrhe, Olibanum (incense), Opoponax, Sandaraque, Styrax (Turkey) resinsEssential oils and liquorices Camphor, mint, and citrus fruit essential oils Liquorices and pure glycyrrhizinEmulsifiers and surface active agents Lecithins, mono- and diglycerides, mono- and diglyceride esters Fatty sucrose esters, fatty alcohols, fatty acids
5 Lipid-Based Edible Films and Coatings 1395.2.2 Composite Edible FilmsPure lipids can be combined with hydrocolloids, such as proteins, starches orcelluloses, and their derivatives, either by incorporating lipids into the hydrocolloidfilm-forming solution (emulsion technique) or by depositing lipid layers onto thesurface of the pre-formed hydrocolloid film to obtain a bilayer (Kamper and Fennema1985; Krochta and De Mulder Johnston 1997). Multi-component films havebeen extensively reviewed by Wu et al. (2002) and Debeaufort et al. (2002). Additionof non-lipid compounds or particles such as sugar crystals, fibres, and proteins as dis-persed components in fat materials permits formation of fat dispersions, such aschocolates (Fig. 5.3). These composite films take advantage of the functionalproperties of each component of the film to provide both barrier and mechanicalproperties. The resulting water barrier efficiency of bilayered films is often of thesame order of magnitude as that of pure lipid (Debeaufort et al. 2002), and is muchhigher than that of emulsion-based films (Debeaufort et al. 1993; Martin-Polo et al.1992a, b; McHugh and Krochta 1994a, b). However, the hydrocolloid layer ishydrophilic, and tends to absorb water when the film is in direct contact with a moistphase. Furthermore, additional processing steps for film making (casting and drying)make bilayer films difficult to use in high-speed commercial production. The most cited substances used to form composite films are cellulose ethers, butpectinate, chitosan, starch, alginates, and carrageenans have been used in othercomposite films (Karbowiak et al. 2006, 2007). These substances are often combinedwith stearic or palmitic acids, beeswax, acetylated monoglycerides, and lecithins(Wu et al. 2002).Fig. 5.3 Possible structures of lipid-based composite films
140 F. Debeaufort and A. Voilley5.2.3 Additives to Improve FunctionalityOther substances have often been added to film and coating formulations forimproving their functional characteristics, such as enhancing film-forming abilityof solutions, suspensions, or emulsions; promoting adherence of coating to thesupport; or controlling flow and spread properties of coating solutions, suspensions,and emulsions. Emulsifiers and texturizing agents have been used to stabilizedispersed systems; acid and alkaline substances have been used to improve proteinsolubilization; and tanning agents such as sulfites, aldehydes, and ascorbic acidhave been used to increase reticulation or grafting of biopolymers, such as proteins.Moreover, some antioxidants (e.g., ascorbic acid), antimicrobial agents, orenzymes (e.g., transglutaminase) can promote intra- or intermolecular bonds.Enzymes are also used to increase solubilization of biopolymers, whereas somesalts are used to induce polymer gelation (e.g., alginates or pectinates) (Guilbertand Cuq 1998).5.3 Film and Coating TechnologiesThere are many technologies that can be used to make edible films and coatings.The choice of a specific process depends on the nature of film or coating constitu-ents and on the intended shape of the barrier layer. Polysaccharides and proteinshave to be modified using processes such as polymerization, gelation, coagulation,and co-acervation. Lipids-based coatings are more often obtained from eithermelting and crystallization or solvent evaporation. Edible films can be obtained byextrusion, co-extrusion, spreading, casting, roll coating, drum coating, pan coating,or laminating techniques. Edible coatings, on the other hand, are mainly appliedusing spraying, drum coating, spray-fluidization, pan coating, or falling filmtechniques.5.3.1 Commercial Film-Making TechnologiesCOGIN® (carrageenans-based films), Chris-Kraft Polymer Inc. (hydroxypropyl-methylcellulose (HPMC)-based films), BioEnvelop® (cellulose derivative-based,starch-based, films), ENAK® (HPMC-, carrageenan-based films), and GREENSOL®(HPMC-based films) are firms that produce industrial films by spreading of afilm-forming solution followed by a roll-drying step. This technique is also called“casting” and is the most useful method for producing edible films and coatings atboth laboratory and pilot scales. On the lab scale, spreading thicknesses and dryingconditions (temperature and relative humidity) may be accurately controlled(Debeaufort et al. 2002).
5 Lipid-Based Edible Films and Coatings 141 Extrusion technologies are often used for industrial production of films, tubes,poaches, and casings. Such is the case with those produced by companies likeSOUSSANA® (gelatin-based tubes and collagen-based films); ENAK (alginate- andcarrageenan-based films); and GREENSOL-MONOSOL® (hydroxypropyl methyl-cellulose- and methylcellulose-based films).5.3.2 Coating TechnologiesCoating application consists of applying a liquid or a powder ingredient onto a baseproduct. Table 5.2 gives some examples of technology, products and principles. Surface properties play a key role in the success of coating application.Application of coatings generally requires a four-step process:1. Deposition of coating material (solution, suspension, emulsion or powder) on the surface of the product to be coated through spraying, brushing, spreading, or casting.2. Adhesion of coating material (solution, suspension, emulsion or powder) to the food surface.3. Coalescence (film-forming step) of the coating on the food surface.4. Stabilization of the continuous coating layer on its support or food product through co-acervation by drying, cooling, heating, or coagulation.Table 5.2 Coating processes and product applicationsTerm Industry Process PrincipleEnrobing Chocolate Enrobe Cover a confectionery centre with tempered chocolateEncapsu- Food Various Formulate and create by physical or chemical lation ingredient systems reactions a protective matrix or layer containing an active ingredient in view or preservation or controlled release.Panning Confectionery Pan Build successive layers (a few microns at a time) of sugar syrup or chocolate with alternative drying/cooling periodsSeed coating Seed Drum, fluid- Form a protective layer of a polymer film ized bed containing the active pesticides the seed requires in the storage and early stage of the germinationSeasoning Snack Drum Disperse a coarse or finely ground herbs and spices mix onto snacks, croutons, chips, etc.Breading Prepared meals Duster, Meat chunks, prepared cheese, vegetable pieces coater can be pre-dusted, coated with a batter, and covered with breading, a fine or coarse ingredient obtained from bread or a processed dough
142 F. Debeaufort and A. VoilleyTo achieve success in coating operations, specific parameters dealing with the base product to be coated, processing equipment, and the coating formulation have to be taken into account, as illustrated in Fig. 5.4. Choice of the coating system or apparatus depends mainly on size andshape of the product to be coated and on the desired thickness of the coating(Fig. 5.5).Fig. 5.4 Parameters to be controlled in a coating operationFig. 5.5 Coating techniques based on the size of the product to be coated
5 Lipid-Based Edible Films and Coatings 14188.8.131.52 EnrobingEnrobing involves application of a thick coating layer by dipping the product to becoated in solution batter or in molten lipid (e.g., a chocolate-based coating).Coating of fresh or frozen products with a batter and/or breading can enhance palat-ability, add flavor to an otherwise bland product and reduce moisture loss and oilabsorption during frying.184.108.40.206 Pan CoatingPan coating is used to apply either thin or thick layers onto hard, almost sphericalparticles in a batch process. For example, coating confectionery centres (peanuts andalmonds) with gum Arabic provides a uniform base layer for further coating and ahydrophilic/lipophilic surface, prevents moisture and fat migration and allows incor-poration of additional flavour.220.127.116.11 Drum CoatingDrum coating is often the best technique for applying either a thin or a thick layeronto hard or solid foods in a continuous process (e.g., nuts). Oiling and saltingof nuts enhances palatability, adds flavor, and delays lipid oxidation in peanuts.Adding a chocolate coating to cornflake cereals enhances palatability, adds flavorand delays moisture absorption (Fig. 5.6).18.104.22.168 Screw CoatingA screw coater allows application of a thin layer of coating onto a solid and firmfood material in a continuous process. For example, it is often used to deposit thincoatings on sticky particles, such as cheese shreds and pieces, to improve anti-cakingFig. 5.6 Drum coating of peanuts
144 F. Debeaufort and A. VoilleyFig. 5.7 A screw coater used in coating particles of cheeseproperties and prevent agglomeration of particles when product is stored in flexiblepackaging (Fig. 5.7).22.214.171.124 Fluidized-Bed CoatingFluidized-bed coating is a technique used to apply a very thin layer onto dryparticles of very low density and/or small size. Agglomeration of the powderpromoted by the fluidized-bed coating technique enhances dispersion and solu-bility of the coating material. Powder is fluidized with hot air and sprayed simul-taneously with a binder liquid. This process causes particle adhesion, agglomerationand drying of agglomerates. It is applicable to both batch and continuous opera-tions. The process of coating seeds with a pesticide slurry is often done by thistechnique. Seeds are treated by coating them with a polymer containing thedesired pesticide/fungicide combination needed for a successful germinationperiod. The process increases resistance of seeds to both mechanical breakageand biological attack.126.96.36.199 Spray CoatingThe spray-coating technique can be used alone or in combination with pan, drum,screw and fluidized-bed coaters. Spraying makes it possible to deposit either thinor thick layers of aqueous solution or suspensions and molten lipids or chocolate.It is the most commonly used technique for applying food coatings. A picture of aspray-coating apparatus and examples of products coated by this process are shownin Fig. 5.8. The spraying nozzle plays a critical role in the coating process. Spraying effi-ciency depends on the pressure, fluid viscosity, temperature and surface tension ofthe coating liquid, as well as nozzle shape or design. This in turn affects the flowrate, the size of the droplets, spraying distance and angle, and overlap rate.
5 Lipid-Based Edible Films and Coatings 145 Legend : 1) spraying nozzles 2) batch tank 3) level control 4) bypass for tankFig. 5.8 A spray coater and a coated chocolate cake5.4 Barrier Properties of Edible Packaging5.4.1 Control of Mass Transfers Within FoodsFood preservation helps food maintain its original properties/qualities up to thepoint of consumption. It is accomplished by protecting the food article againstconditions of its surrounding environment and controlling migration and masstransfer, including water loss. Indeed, product quality depends on the organoleptic,microbiological, nutritional and functional properties. These properties are subjectto change during storage and distribution, mainly due to moisture migration eitherfrom the food to the environment or between different parts within a compositeheterogeneous product.
146 F. Debeaufort and A. Voilley Many physical and/or chemical processes have been developed to improve foodstability and to prolong shelf-life. However, only food packaging makes it possibleto control mass transfer between a food material and its surrounding environment(Kadoya 1990). Although plastics can effectively protect a food product from itssurrounding environment, they often cannot be used to reduce mass transfer withina composite food. For instance, pizza crusts rapidly lose their crispiness because ofmoisture transfer from tomato paste. The dough of a tart, filled with apricots andlaid on custard cream, loses its crispy texture 8 h after cooking (Fig. 5.9). Even ifnutritional and microbiological quality of food products remains satisfactory, lossof key sensory properties represents significant product deterioration. In heterogeneous composite foods, moisture migration always occurs from thewet compartment to the dry one, either as liquid or as vapour, even when the wetcompartment contains solid water, as is the case with frozen products. For example,in an ice-cream cone, moisture transfer occurs as liquid (1) or vapour (2,3,4), asshown in Fig. 5.10 (Morillon et al. 2002). To prevent such transfers, a chocolate-based coating can be applied. Such a coatingmakes it possible to control migration of liquid water from the cryo-concentratedsucrose solution of the ice cream (1), as well as water vapour transfer within thecone (2 and 3) and from the external environment (4), because it guarantees an air-tight contact with the paper/aluminium material typically used as external packag-ing for such products. In all cases, no matter what the state of water, product temperature, or nature ofthe product, different regions within a food tend to balance their chemical poten-tial often expressed as water activity. Thus, the driving force that governs watertransfer is not the water content differential but the water activity or water chemi-cal potential differential. This phenomenon is well described and predicted byHenry’s and Fick’s laws.Fig. 5.9 Changes in water content in the dough of a pie filled with apricot and custard
5 Lipid-Based Edible Films and Coatings 147Fig. 5.10 Schematic representation of moisture transfers occurring in an ice-cream cone Moisture transfer within and throughout a food product depends on an extrinsicparameter, water activity differential; and on two intrinsic parameters, solubility coef-ficient (S), which represents product affinity for water (thermodynamics), anddiffusivity coefficient (D), which deals with water mobility (kinetics) in the system.Permeability is usually expressed as P = DS. On the other hand, moisture transferbetween two compartments with different hydration levels depends on both ther-modynamic and kinetic parameters. The primary means for reducing mass flowrests in controlling these two parameters. First, the product formulation should be changed in order to balance, as much aspossible, water activity of different compartments within a composite food. It is pos-sible to either increase or decrease water activity by decreasing the content of solutesand dry matter, or by adding water activity depressors (e.g., polyols), respectively.However, this remedy induces changes in the final product composition, which canoften be unfavourable to sensory quality. In general, it has been found that such trans-fers can be prevented by this means when maximum water activity differential is lessthan 0.1 and water activity of the food ranges between 0.3 and 0.75. Second, kinetics of migration can be modified by applying a barrier layer at theinterface between two compartments with differential moisture levels. These barri-ers are applied as thin layers, films, and coatings, which qualify as packagingmaterial when they provide selectivity against transfer (Debeaufort et al. 1998).Theoretically, these barriers can be applied to food independent of temperatureor moisture differentials between the different regions within a composite food. Infact, their efficiency is due to numerous factors (extrinsic or intrinsic), all of whichvary according to functional properties desired, the coating or film formulation,application process, and nature of the targeted food.
148 F. Debeaufort and A. Voilley5.4.2 Water Vapour Permeability of Edible FilmsTo protect products against moisture transfer, most efficient barriers are composedof hydrophobic substances. They are usually classified according to their watervapour permeability, as described in Fig. 5.11. Table 5.3 provides water vapour permeability values of some lipid-based ediblefilms as a function of composition and structure. Some lipids and food-gradehydrophobic substances have permeability values close to those of plastic films,such as low-density polyethylene or polyvinyl chloride. Permeability of lipid mate-rials having a high solid fat content is usually much lower than that of liquid lipids.However, most solid lipid-based films are brittle when used alone; so they often arecombined with hydrocolloids to form bilayer or emulsion films. Their structure andbarrier properties depend on the preparation technique, with the most commonpreparation techniques being the following:– Dipping the support in molten lipid to obtain a homogenous fat layer.– Casting and drying a film-forming emulsion in which fats are dispersed in a hydrocolloid aqueous solution to obtain an emulsified edible film.– Depositing a lipid layer previously molten or solubilized in an adequate solvent onto a hydrocolloid-based film, which is used as a mechanical support to obtain bilayer or multilayer films.Barrier efficiency of bilayer films is of the same order of magnitude as that of thepure lipid or plastic films, and is much lower than that of emulsion-based films.Permeability of the latter is often very close to that of protein- or polysaccharide-based edible films, as shown in Table 5.4. Water vapour permeability values canvary over a wide range, according to many parameters related to external condi-tions (such as temperature, relative humidity, and pressure) and composition andstructure of the film. Composition and structure of edible films affect the water transfer mechanism,and therefore their barrier performance, just as much as physicochemical proper-ties of the substance going through the barrier (e.g., concentration or moistureaffinity). Both edible films and coated or wrapped food products are exposed tovarious factors such as temperatures during processing, transport, and storage. So,knowledge of the behaviour of the barrier layer, as a function of physical and High Animal and plant waxes High melting point fats (T>35°C) Moisture Resins and natural lacs barrier Esterified mono- and di-glycerides efficiency Fatty alcohols Emulsifiers and surface active agents Fatty acids and low melting point fats (T< Low 20°C)Fig. 5.11 Classification of hydrophobic substances according water vapour permeability
5 Lipid-Based Edible Films and Coatings 149 Table 5.3 Water vapour permeability (WVP in 10−11 g m−1 s−1 Pa−1) of hydrophobic substances used in edible films Temperature RH gradient Composition (°C) (%) WVP Paraffin wax 25 0–100 0.02 Candelilla wax 25 0–100 0.02 Carnauba wax + shellac 30 0–92 0.18 Carnauba wax + glycerol monostearate 25 22–100 35 Carnauba wax + glycerol monostearate 25 22–65 1.36 Microcrystalline wax 25 0–100 0.03 Beeswax 25 0–100 0.06 Capric acid 23 12–56 0.38 Myristic acid 23 12–56 3.47 Palmitic acid 23 12–56 0.65 Stearic acid 23 12–56 0.22 Acetyl acyl glycerol 25 0–100 22 to 148 Shellac 30 0–84 0.36 to 0.77 Shellac 30 0–100 0.42 to 1.03 Gumlac dewaxed 25 22–100 2.37 Gumlac dewaxed 25 22–75 1.51 Triolein 25 22–84 12.1 Hydrogenated cotton oil 26.7 0–100 0.13 Hydrogenated palm oil 25 0–85 227 Hydrogenated peanut oil 25 0–100 390 Native peanut oil 25 22–44 13.8 Cocoa butter substitute 25 22–84 0.6 Non-tempered cocoa butter 26.7 0–75 23.5 Tempered cocoa butter 26.7 0–75 4.9 Tempered cocoa butter 26.7 0–100 26.8 Milk chocolate 26.7 22–75 1.12 Milk chocolate 26.7 0–100 89.2 Dark chocolate 20 0–81 0.24chemical parameters, is needed for improving the formulation of edible packaging.Many factors affect functional properties of edible films. These factors can becategorized into two groups (1) those concerning composition, and (2) those deal-ing with structure.5.4.3 Effect of Film Composition188.8.131.52 Chemical Nature and Concentration of IngredientsLipid-based edible films have a low affinity for water, which explains why theyhave low moisture permeability. However, each hydrophobic substance has its ownphysicochemical properties. Thus, edible films that are based on lipids exhibitvariable behaviours against moisture transfer. Polarity of lipid constituents hasto be considered, such as the distribution of electrostatic potential on molecules,
150 F. Debeaufort and A. VoilleyTable 5.4 Water vapour permeabilities (WVP in 10−11 g m−1 s−1 Pa−1) of composite edible films Temperature RH gradientComposition (°C) (%) WVPBilayer filmsMethylcellulose/paraffin wax 25 22–84 0.2–0.4Methylcellulose/paraffin oil 25 22–84 2.4Methylcellulose/beeswax 25 0–100 0.058Methylcellulose/carnauba wax 25 0–100 0.033Methylcellulose/candelilla wax 25 0–100 0.018Methylcellulose/triolein 25 22–84 7.6Methylcellulose/hydrogenated palm oil 25 22–84 4.9Hydroxypropylmethyl cellulose/stearic acid 27 0–97 0.12Carnauba wax + glycerol monostearate de 25 22–75 4.29 glycérol/dewaxed gum lacCarnauba wax + glycerol monostearate/dewaxed 25 22–65 0.69 gum lacEmulsion-based filmsMethylcellulose + PEG400 + behenic acid 23 12–56 7.7Methylcellulose + triolein 25 22–84 14.4Methylcellulose + hydrogenated palm oil 25 22–84 13.2Methylcellulose + PEG400 + myristic acid 23 12–56 3.5Carboxymethylcellulose + butter oil + pectine 25 22–84 15.1Hydroxypropyl cellulose + PEG400 + acetylated 21 0–85 8.2 monoglyceridesGluten + acegtylated monoglycerides 23 0–11 5.6–6.6Gluten + oleic acid 30 0–100 7.9Gluten + soy lecithin 30 0–100 10.5Gluten + paraffin wax 25 22–84 1.7Gluten + paraffin oil 25 22–84 5.1Gluten + trioleine 25 22–84 9.7Gluten + hydrogenated palm oil 25 22–84 7.4Sodium caseinate + acetylated monoglycerides 25 0–100 18.3–42.5Sodium caseinate + lauric acid 25 0–92 11Sodium Caseinate + beeswax 25 0–100 11.1–42.5Whey protein + palmitic acid 25 0–90 22.2Whey protein + stearilic alcohol 25 0–86 53.6Whey protein + beeswax 25 0–90 23.9–47.8which depends on the chemical group, aliphatic chain length, and presence ofunsaturation (Callegarin et al. 1997). Waxes are the most efficient substances for reducing moisture permeability,owing to their high hydrophobicity caused by their high content of long-chain fattyalcohols and alkanes. The most efficient substance is beeswax, followed by stearylalcohol, acetyl acyl glycerols, alkanes (hexatriacontane), triglycerides (e.g., tristearin),and fatty acids (e.g., stearic acid). This classification can be explained by molecularhydrophobicity, which defines the degree of interaction with water. Stearyl alcoholis a good barrier compared to triglycerides or fatty acids because its hydroxyl grouphas less affinity for water than carbonyl and carboxyl groups. Considering onlypolarity, alkanes would be predicted to be the best moisture barriers, though this was
5 Lipid-Based Edible Films and Coatings 151not observed to be the case for example hexatriacontane because of another contrib-uting factor, structure. For components having the same chemical nature, chain length influences mois-ture barrier properties. McHugh and Krochta (1994b, c) found that moisture barrierefficiency of fatty alcohols and fatty acids increases with the carbon atom number(from 14 to 18), because the relative proportion of the apolar part of the moleculeincreases, minimizing water solubility and moisture transfer. Many authors also haveshown that among carboxylic acids, stearic and palmitic acids present the lowestwater vapour permeabilities. Nevertheless, when the carbon chain contains more than18 atoms, films containing arachidonic or behenic acids have higher moisture per-meabilities. This observation is explained by the fact that very long chains induce aheterogeneous structure of the polymer network, decreasing moisture barrier properties(Koelsch and Labuza 1992). These results are shown in Fig. 5.12. Unsaturated fatty acids are less efficient in controlling moisture migration,because they are more polar and exhibit different crystallization tendencies thansaturated lipids. Indeed, films containing stearic or palmitic acids have been shownto better reduce the desiccation of oranges than coatings composed of oleic acid(Hagenmaier and Baker 1997). Conformation of unsaturated fatty acids is importantas well, because their chemical structures (e.g., molecular conformation) are different.Besides physical state, crystallization changes with the degree of unsaturation, andconsequently modifies film density and permeability. Concentration of hydrophobic substances is also a key factor in barrier effi-ciency. Water vapour permeability of films composed of stearic acid and HPMCdepends on fatty acid concentration, and strongly decreases at concentration valueshigher than 14–30% (Fig. 5.13). Moreover, the physical structure of all ingredientsis also responsible for barrier properties of composite, lipid-based edible films.Fig. 5.12 Influence of the chain length of fatty acids on water vapour permeability of emulsion-based edible films composed of methylcellulose and lipids
152 F. Debeaufort and A. VoilleyFig. 5.13 Influence of lipid content on water vapour transfer in emulsion-based films with differentfilm compositions (HPKO hydrogenated palm kernel oil)184.108.40.206 Effect of Physical State and Structure of IngredientsThe solid or liquid state of lipid compounds strongly influences the moisture barrierefficiency of a film. Permeability of a hydrogenated cottonseed-oil-based filmincreases 300 times when the liquid fraction of lipid varies from 0 to 40%. MartinPolo et al. (1992a) showed that permeability of paraffin wax increases by100 timeswhen the paraffin oil content increases from 75 to 100%. Several authors havedemonstrated that an increase in solid fat content, especially between 0 and 30%,improves barrier efficiency, as shown in Fig. 5.14. The solid structure of fats isdenser and limits diffusion of water. Moreover, solubility of water in solid lipids isalso reduced. However, for solid fat contents higher than a critical value, dependingon lipid nature, permeability can increase as a result of structural defects (e.g., poros-ity) within the film. This “porous structure” and heterogeneity observed for filmspossessing a high solid lipid content explain the noted decrease in barrier efficiencyof these films. Fat polymorphism (i.e., ability to crystallize in several forms) also affects moisturebarrier efficiency of lipid-based edible films, particularly for hydrogenated-oil- andcocoa-butter-based films. In the case of b and b¢ forms, crystals are stabilized byLondon forces, which occur between aliphatic chains to allow formation of densenetworks. On the contrary, these stabilizing forces do not exist in the a form, and leadto a hexagonal, non-stable structure. Kester and Fennema (1989a, c) studied the effect of polymorphism using a mixtureof fully hydrogenated soy and canola oils in relation to barrier performance.Resistance of these films to water vapour transfer at 25°C was 40,200; 30,600; and38,700 s m−1 for the a, b¢, and b forms, respectively. Higher flexibility of thehexagonal crystal structure provides plasticity to the film and prevents defectsfrom forming during crystallization. This in turn improves moisture permeability.
5 Lipid-Based Edible Films and Coatings 153Fig. 5.14 Influence of solid fat content (SFC) of lipid-based barrier layer (bilayers) on the watervapour transferCrystallization in the b form, when compared to crystallization in the b¢ form,increases mass transfer resistance of films. This effect is mainly explained by thegreater density of b crystals. Waxes serve as good barriers against moisture transfer, but their efficiencies cannotbe related to polymorphism or crystal size. Indeed, of the waxes, carnauba waxprovides the most heterogeneous, porous surface, whereas microcrystalline waxexhibits the smoothest surface. However, films composed of carnauba or microcrys-talline waxes have neither the best nor worst moisture barrier performance. Theirpermeabilities are probably more affected by their affinity for water. Kester and Fennema (1989b) studied the effect of ageing on moisture permeabil-ity of stearyl alcohol-based films in which size and shape of crystals were modifiedwithout changing polymorphism. Stearyl alcohol crystallizes in a orthorhombicform (b¢), and moisture transfer resistance of coatings stored at 48°C for 0, 14, and35 days increased from 11 to 50% during this time. The mechanism responsible forimprovement in barrier properties with time is not fully described and explained,but it seems that two parameters are important (1) the decrease in structural defectswhen recrystallization occurs at a low rate, and (2) the increase of solid fat contentas liquid lipid crystallizes. The chemical nature of film ingredients contributes to moisture barrier effi-ciency, because it partially affects affinity of the film for water. While physicalstructure of the lipids determines film structure, and thus moisture permeability,film structure is another parameter that needs to be considered.5.4.4 Influence of Film Structure on Barrier Properties220.127.116.11 Role of Preparation TechniqueEdible films containing lipids may be obtained using different techniques whichdetermine barrier structure. Several authors have studied the influence of film
154 F. Debeaufort and A. Voilleypreparation technique on barrier properties. Kamper and Fennema (1984) madeemulsion-based and bilayer films composed of hydroxypropylmethylcellulose andstearic and palmitic acids. Emulsion-based films exhibited a moisture permeability40 times lower than that of bilayer films (0.5 × 10−12 and between 19 and 28 × 10−12g m−1 s−1 Pa−1, respectively), even though the amount of lipid in emulsion-basedfilms was ten times lower than that of bilayer films. In contrast, Martin-Polo et al.(1992a) and Debeaufort et al. (1993) obtained opposite results for methylcellulose–paraffin wax films. For these films, water vapour permeability of the emulsifiedfilm was 40 times higher than that of bilayer films. These contradictory results arelikely explained by considering film preparation conditions. Though the initialemulsion prepared by Kamper and Fennema (1984) was homogeneous, a phaseseparation was observed during drying, which led to an apparent bilayer structurefor the emulsified film. Debeaufort et al. (1993), using scanning electron micros-copy, revealed the irregular, rough, and heterogeneous surface of emulsified filmsand, contrastingly, the smooth and homogeneous surface of bilayer films. Amore homogeneous distribution of the lipid layer at the film surface was found tobe more efficient for controlling water transfer. The most efficient moisture barriers are generally obtained when the film structurecontains a continuous lipid layer, obtained either from a bilayer technique or afterthe destabilization of the emulsion during drying for an emulsion-based film. Inchocolate, the continuous phase is composed of a lipid, as a result of conching andtempering. Dispersed hydrophilic particles (sucrose crystals, cocoa powder) do notsignificantly affect the water vapour permeability, except where there is high rela-tive humidity, for which film structure is modified. Because of their poor mechanical properties, lipids are often used in conjunctionwith a support, which can sometimes be considered as a model food to be coated.However, this support can strongly influence film properties by modifying the dis-tribution of hydrophobic substances. If the support is porous, the barrier is lessefficient because the surface to be protected is much greater and a rough surfacemakes application of a continuous and regular coating layer more difficult. Adhesion of a film to a food product is a physical phenomenon that can be con-trolled by the overlapping of rough surfaces; by wettability forces due to interfacialforces between materials, where at least one is liquid; by electrostatic forcesbetween charged polymers; or by chemical bonds when a reaction occurs. Barron(1977) showed that chocolate coating, whose adhesion to a biscuit is very good,tends to crack because the latter swells when moisture is absorbed. In this case, toostrong of an adhesion between the coating and support is not always an advantage.Interaction occurring between the support and coating has to be taken into accountbecause it can modify coating barrier properties, either due to a partial absorptionof the barrier layer by the support or due to a heterogeneous lipid distribution.Indeed, a barrier coating can be efficient only if it forms a homogeneous and con-tinuous layer on the entire surface of the food product to be protected. When cracksappear, all barrier properties are lost. Continuity and homogeneity of the barrieralso strongly depend on film thickness.
5 Lipid-Based Edible Films and Coatings 1518.104.22.168 Influence of the Film ThicknessFilm thickness can modify film properties, such as barrier performance. Accordingto the following equation, WVTR (water vapour transfer rate) corresponds to theamount of water vapour (∆m) transferred through a film area (A), during a definedtime (∆t), where permeability (WVTR) is normalized by thickness (x) and partialvapour pressure gradient (∆p): ∆m x WVTR = (g m −2 s −1 ) and P = WVTR (g m −1 s −1 Pa −1 ). A∆t ∆pAn increase in film’s permeability with thickness indicates water affinity, whichcould be due to the presence of hydrophilic compounds in the formulation. Itseems, then, that the influence of film thickness varies with the nature of both thelipid and other film components. Mass transfer resistance of lipid compounds against gas migration, such asoxygen, is mainly due to structure; the more dense (e.g., compact) the crystals andthe more homogeneously they are distributed and oriented, the more difficult thegas diffusion and the lower the permeability. In the case of water migration, barrierproperties are more complex. Affinity for water is often as important as the filmstructure itself. Thus, transfer of water molecules within films and coatings dependsboth on diffusivity (kinetic factor) and sorption (thermodynamic factor) phenomena,even in the case of hydrophobic substances.5.4.5 Effect of Properties of Penetrant MoleculesIn the case of dense materials as opposed to porous ones, properties of the pene-trant, such as its concentration, polarity, or physical state, affect not only its interac-tions with film components but also kinetic phenomenon of transfer. Size and shapeof the diffusing molecules influence the diffusivity, whereas polarity and its abilityto condense influence the sorption. Water is a polar compound having a small sizethat tends to favour both sorption and diffusivity in dense materials. This abilitymakes these materials more permeable to moisture than to non-condensable gases. Inthis chapter, only water transfer will be considered.22.214.171.124 Effect of Water Concentration GradientThe driving force for moisture transfer is the vapour pressure or the water activitydifference between the two sides of the film. The higher the gradient, the greaterthe transfer rate, if there is no interaction between water and the film. However,permeability remains constant, as observed with paraffin wax films, hydrogenatedcottonseed oil, or dark chocolate, as long as humidity on the high side of the gradient
156 F. Debeaufort and A. Voilleyis lower than 80%. Other behaviours were observed: particularly an increase inpermeability of paraffin oil coatings, cocoa liquor and butter, milk chocolate, andacetylstearyl glycerols. Water vapour permeability of milk chocolate increases from10.7 × 10−12 to 892 × 10−12 g m−1 s−1 Pa−1 when the humidity gradient variesfrom 22–75% to 0–100%. This phenomenon is attributed to moisture sorption byhydrophilic particles (milk powder, sucrose crystals, and cocoa powder) within thecoating, which leads to a loss of film integrity. It is well known that permeability of hydrophilic films depends both on the rela-tive humidity (RH) difference and on the absolute humidity values. For instance,for the same RH gradient, permeability increases with an increasing vapour pressurevalue. Tiemsra and Tiemsra (1974) established a direct relationship between watervapour transfer rate and humidity for films composed of peanut oil, peanut butter,or cocoa liquor. kaw1 ∆aw WVTR = . xIn this equation, WVTR is the water vapour transfer rate (g m−2 s−1), aw1 is thehigher water activity value of the gradient ∆aw, x is the film thickness (m), and k isan adjusted mass transfer coefficient (g m−1 s−1). This model would be more inter-esting if the k parameter could be correlated to a film’s physicochemical and/orstructural characteristics. In the case of hydrophilic films, the permeability increaseat high relative humidity levels is often due to swelling and plasticization of thepolymer network by moisture sorption. This creates a less dense structure in whichchain extremities are more mobile. In this scenario, water diffusivity and waterpermeation become easier. Even for hydrophobic substances, which theoretically have a low affinity formoisture, water affects the barrier efficiency of edible films and coatings when theycontain hydrophilic particles or polar groups, as in chocolate or cocoa-based coatings.Most published reports deal with transfer of water vapour. However, films and coatingsare often used for highly hydrated products in which water is in a liquid state, suchas gels. Water in contact with the barrier layer can also be in a solid state, as in thecase of frozen foods. Therefore, it is interesting to consider the effect of the physicalstate of water on its transfer.126.96.36.199 Effect of Physical State of Water on Barrier PerformancesFor edible films and coatings, a few authors consider the direct contact betweenthe barrier layer and the moist compartment. Morillon et al. (1998) studied theeffect of the physical state of water, liquid or vapour, on its migration throughlipid-based edible films and through hydrophilic and hydrophobic synthetic films.They reported that water permeability of lipid–sugar-based edible films is thesame for both water physical states as long as water activity is lower than 0.85(Fig. 5.15).
5 Lipid-Based Edible Films and Coatings 157Fig. 5.15 Effect of the state of water (liquid or vapour) on water transfer rate through cocoa-basededible barriers At higher water activities, transfer of liquid water through lipid-based ediblefilms and hydrophilic plastic films is much greater than transfer of vapour water.Two phenomena may occur (1) a partial solubilization of the sucrose of the film,and/or (2) a swelling of the matrix in hydrophilic films. When the penetrant is partly in a solid state, as water is in frozen foods, itstransfer through edible or plastic films has been scarcely studied. The discontinu-ity of solubility, diffusivity, or permeability of some molecules when the state ofthe diffusing molecule changes is commonly called the “Schroeder Paradox”(Vallieres et al. 2006), and is often observed for hydrophilic polymers over theirmelting temperature ranges. This phenomenon seems to be due to a modificationof energy required for deformation of molecules when they diffuse, and becomesvery weak above their melting points. Moreover, all molecules that diffuse in andthrough dense polymers are in a liquid state. So when there is no state change,such as melting or condensation, less energy is required for transfer. This phenom-enon could explain why a liquid penetrant in contact with the membrane oftenfavours moisture transfer. The influence of a penetrant’s physical state, and especially water transferthrough dense films and coatings, is a field that has been poorly considered to date,but is important to better understand the mechanism of moisture transfer in com-posite foods. Nevertheless, the physical state and structure of edible barriers alsostrongly depends on temperature.188.8.131.52 Influence of TemperatureFood products can be exposed to a wide range of temperature variations duringprocessing, and are often stored at sub-ambient temperatures. Temperature tremendously
158 F. Debeaufort and A. Voilleyaffects all thermodynamic and kinetic phenomena and, thus, moisture transfer.As long as there is no modification of the film or coating structure due to temperature,permeability, diffusivity, and solubility coefficients vary according to the Arrheniuslaw, as described by the following equation. P = P0 exp( − Ea,P / RT ), D = D0 exp( − Ea,D / RT ), S = S0 exp( −∆H S / RT ).In this equation, Ea,P and Ea,D are the apparent activation energies of the permeation anddiffusion phenomena (kJ mol−1); ∆HS is the enthalpy of sorption (kJ mol−1); P0, D0, andS0 are the reference values of permeability, diffusivity and solubility, respectively; Ris the ideal gas constant (8.31 kJ mol−1 K−1); and T is the temperature (K). From the definition of permeability, which is the product of solubility anddiffusivity coefficients, the relationship between energies is described by the fol-lowing equation. Ea,P = Ea,D + ∆H S .In this equation, ∆HS is always a negative value for water vapour, which means thatsolubility decreases as temperature increases, whereas Ea,D is positive and diffusiv-ity rises with temperature. According to the transfer, which is mainly driven eitherby kinetic or thermodynamic phenomena, permeability increases or decreases astemperature increases. For instance, water vapour permeability of polyethylenewaxes increases as temperature varies from 25 to 40°C; activation energy isbetween 5 and 15 kJ mol−1. This observation indicates that moisture transfer seemsto mainly depend on diffusion. Kester and Fennema (1989b) reported an increasein moisture transfer as temperature decreased, which can be explained by a greatermoisture sorption by the filter paper used as a mechanical support. Other authorshave not shown any effect of temperature on moisture transfer, because transfer ratevariations are directly related to the vapour pressure of water, as observed forhydrogenated cottonseed oil and cocoa butter over a temperature range of 3–26.7°C,or between 21 and 27°C for purified acetylstearyl glycerol. Over a wider range of temperatures, some authors have observed (1) a decreasein moisture permeability with temperature, and (2) an increase in permeability forlow temperatures. Indeed, this phenomenon was also observed for plastic packaging,edible films composed of fatty acid or fatty acid–beeswax mixtures and chocolate- orcocoa-based coatings (Fig. 5.16). This increase in moisture permeability observed by several authors can be dueto a constant or an increasing water vapour transfer rate, in spite of the temperaturedecrease. For lipid-based films, such as chocolate or cocoa butter, temperaturemodifies the solid fat content (SFC), and thus affects both structure and barrierperformance. Indeed, water vapour transfer rate of chocolate decreases between 26and 20°C, but remains constant from 20 to 10°C, which is explained by the fact
5 Lipid-Based Edible Films and Coatings 159Fig. 5.16 Effect of temperature on liquid and vapour water transfer rate (WTR) through cocoa-based filmsthat SFC increases from 80% at 26°C to 90% at 20°C. For both plastic and ediblepackaging materials, authors explain that this behaviour is due to phase transitions;the appearance of defects, such as holes or cracks caused by temperature dilatationor contraction; or by a greater moisture sorption at low temperatures. This particu-lar behaviour of permeability as temperature decreases was also reported byMorillon et al. (1999) for hydrophilic and hydrophobic films. However, theseauthors conclude that the driving force for moisture transfer is not vapour pressuredifference, but rather chemical potential. They further calculated a “corrected per-meability” that always decreases as temperature declines. Temperatures below 0°C allow better preservation of foods, particularly byinhibition of mold growth. But chemical and physicochemical reactions still occur,though they are significantly slowed down by sub-freezing temperatures. The effectof a temperature below 0°C on moisture transfer has been hardly studied in the fieldof edible barriers. Indeed, the few works published on moisture transfer at suchtemperatures only consider the amount of water amount gained or lost by the food.This approach does not take into account real barrier performance or permeationphenomena occurring within edible films.5.4.6 Prediction of the Shelf-Life of Coated ProductsInitially developed for prediction of shelf-life of products packaged in plasticflexible or semi-rigid packaging, several models have been adapted to coated foodsby considering edible films and coatings as conventional packaging. These models
160 F. Debeaufort and A. Voilleytake into account characteristics of the food product, surrounding medium, andbarrier layer (Labuza 1982; Cardoso and Labuza 1983; Hong et al. 1991). Forinstance, for water it is necessary to know– Film permeability, or water vapour transfer rate (WTR) of the coatings, as well as coating thickness.– Dry matter of the product to be coated, its initial and critical water contents, the sorption isotherm, and eventually its density and moisture diffusivity.– Water activity of the wet compartment and eventually its diffusivity.These methods consist of evaluating the amount of transferred water necessary toinduce product degradation, such as loss of crispness in a dry biscuit, and determin-ing the time necessary for that amount of water to go through the coating(Debeaufort et al. 2002). The simplest model uses the water transfer rate andcritical water content of the dry part of the product according to the followingequation. ( M C − M i )m ( M C − M i )m Time = = x. WTR A PA ∆pIn this equation, WTR is the water transfer rate (g m−2 s−1); A is the surface exposedto the transfer; x is the coating thickness (m); m is the dry matter of the product (g);Mi and Mc are the initial and critical water contents, respectively; and Dp is thewater vapour partial pressure differential across the barrier. However, this model assumes that the water activity differential between the twofaces of the coating remains constant over storage, which never occurs. The pro-gressive change in water activity in the dry compartment (e.g., a cereal-based bis-cuit) has to be taken into account from the sorption isotherm modelled as linearbetween the initial and critical water contents for predictions to be in accordancewith reality (Labuza and Contreras-Medellin 1981). Parameters used in this modelare given in Fig. 5.17, where Mi, Mc, and Me are the initial, critical, and equilibriumwater contents, respectively; awi, awc, awe are the water activities; and bs is the slopeof the linear-considered sorption isotherm between the initial and critical moisturecontent points. In an attempt to consider water activity variation in the dry compartment, Labuzaand Contreras-Medellin (1981) and Labuza (1982) suggested the following equation. M i − M e PAp 0 ln = time. Mc − Me xmbIn this equation, P is the coating permeability (g m−1 s−1 Pa−1), A is the exposedsurface (m2), p0 is the saturated vapour pressure at the experiment temperature, x isthe coating thickness (m), m is the dry matter of the product (g), and b is the slopeof the sorption isotherm of the dry compartment (gwater/gproduct). This model was usedby Biquet and Labuza (1988) for chocolate coatings applied between agar gel andmicrocrystalline cellulose. Morillon et al. (1998) also compared the estimatedshelf-life calculated from this latter model and experimental values determined from
5 Lipid-Based Edible Films and Coatings 161Fig. 5.17 Schematic representation of shelf-life prediction for a model composite food (stuffedbiscuit)sensorial experiments for a wafer coated with a cocoa-based coating. Figure 5.18provides the estimated (bars) and measured (triangles) shelf-life values for twodifferent coatings whose permeability is either 1 or 2.5 × 10−11 g m−1 s−1 Pa−1, andtwo wafers whose critical water activity varies from 0.35 to 0.45 before losingcrispiness. Shelf-life varied from 14 days to more than 18 months on the basis of coatingefficiency and wafer sensitivity to water. Very few results on real products have beenpublished, and one of the main difficulties is to know the coating permeability in realconditions of the application. More recently, Roca et al. (2006) and Bourlieu et al.(2007) have developed newer models that take into account moisture diffusivity ineach compartment (dry and wet and in the edible barriers), based on sorption kinetics,isotherm data, and water vapour permeability of the edible film.5.4.7 Oxygen and Carbon Dioxide Permeabilities of Edible Films and CoatingsBarrier properties of edible films and coatings against oxygen and carbon dioxideare given in Table 5.5. Gas barrier properties of hydrocolloid-based edible films arevery important for fresh fruit and vegetable applications. In dry conditions, perme-abilities of these edible films and coatings are very low, down to 3,000 times lowerthan those of plastic polymers. However, though oxygen permeability of plastic films(except EVOH or Nylon) remains constant irrespective of relative humidity, that ofedible films and coatings usually increases significantly in the presence of moisture.This behaviour is most often caused by plasticization of the biopolymer network by
162 F. Debeaufort and A. VoilleyFig. 5.18 Shelf-life of a wafer in ice cream, estimated from the Hong et al. (1991) model andsensory analyses (crispness) Table 5.5 Oxygen (PO2) and carbon dioxide (PCO2) permeabilities of edible films (10−15 g m−1 s−1 Pa−1) Film PO2 PCO2 T (°C) aw Methylcellulose 8.352 1315.60 30 0 Beeswax 7.680 – 25 0 Carnauba wax 1.296 – 25 0 Corn zein 0.560 9.50 38 0 Wheat gluten 0.016 0.31 25 0 Chitosan 0.009 – 25 0 Pectin 21.440 937.20 25 0.96 Wheat gluten 20.640 1,614.80 25 0.95 Starch 17.360 – 25 1 Chitosan 7.552 352.44 25 0.93water, which induces greater solubility and diffusivity of gases in the biopolymermatrix. Lipids are not as well suited as proteins or polysaccharides because of theirstrong affinity for oxygen. Moreover, some lipid compounds (mainly unsaturatedfatty acids) are oxygen sensitive, and can undergo rancidity, causing off-flavordevelopment.5.5 Mechanical PropertiesAs mentioned earlier, materials used to make edible or biopolymer film packaginginclude polysaccharides, proteins, and lipids, or combinations of these compoundsfor composite films. The goal is to combine advantages associated with differentcomponents to obtain optimal properties. Mainly, polysaccharides and proteins
5 Lipid-Based Edible Films and Coatings 163provide structural support, while lipids are used to create an effective water barrier.Moreover, several studies have shown the influence of the physical state and poly-morphism of lipids on functional properties of composite films. The way in whichlipid is added (dispersed in the hydrocolloid aqueous solution to obtain an emulsionin a single packaging layer or cast on an existing packaging to form a bilayer film)influences film mechanical properties. The food industry has focused on emulsifiedfilms, which require only one step in manufacture, as opposed to the two or moresteps required for bilayer and multilayer films. The nature of the emulsifier used forlipid dispersion controls film properties. Drying temperature and time have a largeimpact on film physical properties. Each of these experimental conditions associ-ated with film formulation and formation needs to be taken into account and studiedto evaluate impact of each parameter on film properties. Bravin et al. (2006) investigated the effect of different types of surfactants(glycerol monostearate (GMS), Tween 60 and 80) on tensile strength (TS) andpercentage of elongation at break (E) of an emulsified edible film composed ofcornstarch and methylcellulose (MC), containing cocoa butter or soybean oil aslipid compounds. Emulsified films were prepared by MC or starch solubilization inwater/alcohol or water, respectively, at temperatures higher than 75°C before beingmixed together. Lipid was then added before the mixture was spread onto glassplates using a thin layer chromatography spreader. Films were dried at 25°C, at arelative humidity of 40% for 15 h. All films were maintained for least 10 daysat 53% RH before mechanical properties were measured. Table 5.6 shows TSand E values of cocoa butter films in relation to lipid and emulsifier contents.Values showed substantial variation, depending on the film formulation used. Table 5.6 Tensile strength (TS) and elongation (E) of edible film as affected by cocoa butter/lipid content (L), emulsifier (EM) and emulsifier type (GMS, Tween 60 and 80) EM (%) TS (MPa) L (%) 10 20 GMS 10 11.9 9.1 30 10.9 8.5 Tween 60 10 9.9 8.6 30 8.3 6.7 Tween 80 10 20.6 8.6 30 18,2 10.7 E (%) L (%) 10 20 GMS 10 28.6 13.6 30 17.6 11.6 Tween 60 10 28.1 19.0 30 20.1 19.7 Tween 80 10 4.3 6.0 30 4.6 3.7
164 F. Debeaufort and A. VoilleyThe TS data are in the same range as those observed for LDPE films. Increasingthe total lipid level reduced TS, which correlated with development of a globalheterogeneous film structure after lipid was added (Fig. 5.19). Images of film sec-tions containing 20% butter revealed formation of a less oriented, less compactstructure, with evident internal cavities and discontinuities. Use of oil (liquid state)at a 10% addition level limited the adverse impact of lipid addition on film mechanicalproperties (Table 5.7). Phan et al. (2002a, b) investigated the effect of drying temperature on emulsifiedfilms made from arabinoxylans, hydrogenated palm kernel oil (HPKO), and twosucrose esters, SP 10 and SP 70 (emulsifiers that are soluble in oil and water,respectively). Film was prepared by solubilizing the polysaccharides in water at75°C before addition of glycerol at 15%. Lipid addition at a rate of 30% on a drybasis was carried out. The emulsifier mixture was dispersed prior to addition to thearabinoxylan film-forming solution. The solution was spread onto glass platesfor film drying. Temperatures of 30, 40, and 80°C were employed for drying.The values for the mechanical properties of the films as a function of the dryingtemperature are presented in Figs. 5.20 and 5.21. Tensile strength (S) and per-centage of elongation at break (E) for films containing lipid ranged from 0.8 to 3times lower than those without lipid addition. Despite the liquid fat choice, nopseudo-plasticizer effect or lubricant was observed, and both S and E decreased.Fig. 5.19 Scanning electron microscopy cross-section photomicrographs of 10% soybean oilfilms (a, b) and 20% cocoa butter films (c, d)
Table 5.7 Tensile strength (TS) and elongation (E) of edible film as affected by soybean oil/lipid content (L), emulsifier (EM) and emulsifier type (GMS, Tween 60 and 80) (Bravin et al. 2004) EM (%) TS (MPa) L (%) 10 20 GMS 10 11.3 10.4 30 11.1 9.2 Tween 60 10 26.2 19.9 30 14.8 12.9 Tween 80 10 22.8 15.7 30 24.4 19.6 E (%) L (%) 10 20 GMS 10 15.0 6.0 30 11.6 5.1 Tween 60 10 6.2 7.6 30 4.4 4.1 Tween 80 10 5.5 4.6 30 5.0 4.6 30 Strength at breaking (MPa) 40°C 80°C 25 20 15 10 5 0 AX + HPKO AX + HPKO + AX + HPKO + Homogeneous AX without emulsifier SP10 SP70Fig. 5.20 Strength (S) at breaking point for arabinoxylan-based edible films as a function ofdrying temperature (Phan et al. 2002b) (AX arabinoxylans, HPKO hydrogenated palm oil kernel,SP10 sucroester 10, SP70 sucroester 70) 12 Elongation at breaking (%) 40°C 80°C 10 8 6 4 2 0 AX + HPKO AX + HPKO + AX + HPKO + Homogeneous AX without emulsifier SP10 SP70Fig. 5.21 Elongation (E) at breaking point for arabinoxylan-based edible films as a function ofdrying temperature (Phan et al. 2002b) (AX arabinoxylans, HPKO hydrogenated palm oil kernel,SP10 sucroester 10, SP70 sucroester 70)
166 F. Debeaufort and A. Voilley Evaporation surface a b Evaporation surface Evaporation surface cFig. 5.22 Environmental scanning electron microscopy cross-section micrographs of arabinoxy-lan–HPKO–glycerol films dried at 80°C without emulsifier (a), containing 2.5% SP10 (b) orcontaining 2.5% SP70 (c)The nature of the emulsifier did not play any role in improvement of mechanicalresistance, but temperature greatly modified film physical performance. S decreasedwhile E increased as film drying temperature was increased from 40 to 80°C.At higher temperatures, the solvent evaporated more rapidly, and the films driedmore quickly. In addition, number of interactions between arabinoxylan chains wasreduced; the network was less organized and more stretchable, which tended toincrease E. Moreover, the increase in drying temperature promoted a bilayer-likefilm structure (Fig. 5.22), with superposition of the lipid phase over a homogeneousarabinoxylan film layer.5.6 Conclusions and Future TrendsAn extremely wide range of edible moisture barriers has been explored since the1950s. Their use has become popular. Combination of various types of film-formingagents (polysaccharides, proteins, lipids), in addition to process advancement infilm-forming methods, has greatly improved water vapour resistance of these bar-rier films. It is necessary to adopt an integrated approach in development of ediblebarriers to combine regulatory, nutritional, organoleptic and technical requirements
5 Lipid-Based Edible Films and Coatings 167(Bourlieu et al. 2007). Indeed, most published patents not only disclose barriercomposition but also the food product onto which it has to be applied and theappropriate technique for applying the barrier. This integrated approach should alsobe adopted in research to study determination of barrier efficiency for specificbarrier applications in a given food product. The field of ready-to-eat food products is still developing and provides a signifi-cant challenge in terms of mass transfer control. In particular, edible moisture barriersmay provide an interesting answer to consumer demand for composite productswith good nutritional value and stable organoleptic properties.ReferencesBarron LF (1977) The expansion of wafer and its relation to the cracking of chocolate and “bakers chocolate” coatings. J. Food Technol, 12:73–84Biquet B, Labuza TP (1988) Evaluation of the moisture permeability characteristics of chocolate films as an edible moisture barrier. J. Food Sci, 53:989–998Bourlieu C, Guillard V, Powell H, Valles-Pamies B, Guilbert S, Gontard N (2007) Modelling and control of moisture transfers in high, intermediate and low composite food. J. Food Chem, 106(4):1350–1358Bravin B, Peressini D, Sensidoni A (2006) Development and application of polysaccharide–lipid edible coating to extend shelf-life of dry bakery products. J. Food Eng, 76(3):280–290Callegarin F, Quezada Gallo JA, Debeaufort F, Voilley A (1997) Lipids and biopackaging. J. Am. Oil Chem. Soc, 74:1183–1192Cardoso G, Labuza TP (1983) Prediction of moisture gain and loss for packaged pasta subjected to a sine wave temperature/humidity environment. J. Food Technol, 18:587–606Debeaufort F, Martin-Polo M, Voilley A (1993) Polarity, homogeneity and structure affect water vapour permeability of model edible films. J. Food Sci, 58(2):426–434Debeaufort F, Quezada-Gallo JA, Voilley A (1998) Edible films and coatings: tomorrow’s packagings: a review. Crit. Rev. Food Sci, 38(4):299–313Debeaufort F, Voilley A, Guilbert S (2002) Les procédés de stabilisation des produits par des films “barrière” In Lorient D, Simatos D, Le Meste M (Eds.), “Propriétés de l’eau dans les ali- ments,” Tec & Doc, Lavoisier, Paris, pp. 549–600Guilbert S, Cuq B (1998) Les films et enrobages comestibles. In Multon JL et Bureau G (Eds.) L’emballage des denrées alimentaires de grande consommation, Tec & Doc, Lavoisier, Paris, pp. 472–530Hagenmaier RD, Baker RA (1997) Edible coatings from morpholine-free wax microemulsions. J. Agric. Food Chem, 45:349–352Hong YC, Koelsch CM, Labuza TP (1991) Using the L number to predict the efficacity of moisture barrier properties of edible coating materials. J. Food Proc. Preserv, 15:45–62Kadoya T. (1990) Food Packaging. Academic, New York, NYKamper SL, Fennema O (1984) Water vapour permeability of an edible, fatty acid, bilayer Film. J. Food Sci, 49:1482–1485Kamper SL, Fennema O (1985) Use of edible film to maintain water vapour gradients in food. J. Food Sci, 50:382–384Karbowiak T, Hervet H, Leger L, Champion D, Debeaufort F., Voilley A (2006), Effect of plasticiz- ers (water and glycerol) on the diffusion of a small molecule in iota carrageenan biopolymer films for edible coating application. Biomacromolecules, 7:2011–2019Karbowiak T, Debeaufort F, Champion D., Voilley A (2007) Influence of thermal process on structure and functional properties of edible films. Food Hydrocoll, 21(5–6):879–888
168 F. Debeaufort and A. VoilleyKester JJ, and Fennema O (1989a) The influence of polymorphic form on oxygen and water vapour transmission through lipid films. JAOCS, 66:1147–1153Kester JJ, Fennema O (1989b) Tempering influence on oxygen and water vapour transmission through a stearyl alcohol film. JAOCS, 66:1154–1157Kester JJ, Fennema O (1989c) Resistance of lipid films to water vapour transmission. JAOCS, 66:1139–1146Koelsch CM, Labuza TP (1992) Functional, physical and morphological properties of methyl cellulose and fatty acid-based edible barriers. Lebensm. Wiss. Technol, 25:404–411Krochta JM, DeMulder-Johnston C (1997) Edible and Biodegradable Polymer Films: Challenges and Opportunities. Food Technol, 51:61–74Labuza TP (1982) Moisture gain and loss in packaged foods. Food Technol, 36:92–97Labuza TP, Contreras-Medellin R (1981) Prediction of moisture protection requirements for foods. Cereal Food World, 26:335–343Martin-Polo MO, Mauguin C, Voilley A (1992a) Hydrophobic Films and Their Efficiency against Moisture Transfer. I. Influence of the film preparation technique. J. Agric. Food Chem, 40:407–412Martin-Polo M, Voilley A, Blond G, Colas B, Mesnier M, Floquet N (1992b) Hydrophobic films and their efficiency against moisture transfer. 2. Influence of the physical state. J. Agric. Food Chem, 40:413–418McHugh TH, and Krochta JM (1994a) Milk-protein-based edible films and coatings. Food Technol, 48(1):97–103McHugh TH, Krochta JM (1994b) Permeability properties of edible films. In: Krochta JM, Baldwin EA, Nisperos-Carriedo M. Edible Films and Coatings to Improve Food Quality. Technomic Publishing Company, Lancaster, USAMcHugh TH, Krochta JM (1994c) Water vapour permeability properties of edible whey protein– lipid emulsions films. JAOCS, 71:307–311Morillon V; Debeaufort F, Capelle M, Blond G, and Voilley A (1998) Effect of the water prop- erties on the moisture barrier efficiency of lipid-sugar based edible coatings. ISOPOW VII – Water Management in the Design and Distribution Of Quality Foods. May 30–June 4, Helsinki, FinlandMorillon V, Debeaufort F, Blond G.A., Voilley (1999) Temperature influence on the moisture transfer through synthetic films. J. Membr. Sci, 4377:1–9Morillon V, Debeaufort F, Blond G, Capelle M, Voilley A (2002) Factors affecting the moisture permeability of lipid-based edible films: a review. Crit. Rev. Food Sci. Nutr, 42(1):67–89Phan TD, Debeaufort F, Peroval C, Despre D, Courthaudon JL, Voilley A (2002a) Arabinoxylan- lipid-based edible films: 3 influence of drying temperature on emulsion stability and on film structure and functional properties. J. Agric. Food Chem, 50(8):2423–2428Phan TD, Peroval C, Debeaufort F, Despre D, Courthaudon JL, Voilley A (2002b) Arabinoxylan- lipid-based edible films: 2 influence of sucroester nature on the emulsion structure and film properties. J. Agric. Food Chem, 50(2):266–272Roca E, Guillard V, Guilbert S and Gontard N (2006) Moisture migration in a cereal composite food at high water activity: Effects of initial porosity and fat content. J. Cereal Sci, 43 (2):144–151Tiemsra PJ, Tiemsra JP (1974) Moisture transmission through peanut oil films. Peanut Sci, 1:47–50Vallieres C, Winkelmann D, Roizard D, Favre E, Scharfer P, Kind M (2006) On Schroeder’s paradox. J. Membr. Sci, 278(1–2):357–364Wu Y, Weller CL, Hamouz F, Cuppett SL and Schnepf M (2002) Development and application of multicomponent edible coatings and films: A review. Adv. Food Nutr. Res, 44:347–394
170 M.A. García et al.detection of structural and thermodynamic properties involving the crystalline-amor-phous structure. X-ray diffraction is probably the most important technique forobserving structural properties of crystalline solid materials, polymers andundoubtedly food materials (Gontard et al. 1993; Krochta and De Mulder-Johnson1997). Thermodynamic changes can be evaluated by several calorimetric techniquesand by thermomechanical analysis (Cherian et al. 1995; Roos 1995; Galietta et al.1998; García et al. 2000a; Sobral et al. 2001; Mali et al. 2002; Neto et al. 2005).Knowledge of thermodynamic state, molecular mobility and phase transitions areimportant, since they affect film barrier properties, which define performance of filmsunder conditions of common use and abuse. The objectives of this chapter are to describe: (a) properties of different starchand composite films and their relation to functionality, with special emphasis onfilm formulations based on starch, chitosan and methylcellulose; (b) commonmethods of characterizing composite films and coatings and (c) applications ofthese biomaterials.6.2 Formulation of Films and CoatingsHydrocolloids, proteins, and their derivatives represent the major components offilm formulations, and form the primary supporting matrix of films. Functional,organoleptic, nutritional and mechanical properties of an edible film can be modi-fied by addition of other ingredients in minor amounts. A main requirement for filmformulation components is that they be “generally recognized as safe” (GRAS)substances, and be used in accordance with good manufacturing practices. In general, protein films are poor moisture barriers due to the hydrophilic natureof most proteins, but are good barriers to gases such as oxygen and carbon dioxide(Cuq et al. 1998; McHugh and Krochta 1994a). Casein, collagen, zein, wheatgluten, whey proteins, gelatin and soy proteins have been extensively investigateddue to their availability and mechanical resistance as components of edible films(McHugh and Krochta 1994a; Were et al. 1999; Oh et al. 2004; Sohail et al.2006). Edible films and coatings discussed in this chapter are summarized inTable 6.1.Table 6.1 Film formulationsFilm matrix ComponentsStarch Gelatinized through thermal and alkaline treatment Starch source (% amylose content): corn starch native (25), amylomaize (65) and yam starch (30) Starch (2–4.5 g/100 g) Plasticizer: glycerol or sorbitol – 0–20 g/L)Starch and lipid Lipid: sunflower oil (0–8 g/L)Methylcellulose and chitosan (MC–CH) MC to CH ratio – 0:100, 25:75, 50:50, 75:25, 100:0Corn starch (thermal gelatinized) and CS (3.5–6 g/100 g) chitosan (CS–CH) Plasticizer glycerol, 0–50 g/100 g) CS to CH ratio – 0:100, 50:50 and 100:0
6 Characterization of Starch and Composite Edible Films and Coatings 171 Most commonly used polysaccharides are cellulose derivatives, chitosan, starch,alginate, carrageenan and pectin due to their good film-forming properties. Starchesare abundant in nature, commercially available, inexpensive and are totally biode-gradable. Thus, they are attractive raw materials for the development of completelydegradable products for specific market needs. Among the cellulose derivatives,methylcellulose (MC) has the best film-making properties, high solubility and effi-cient oxygen and lipid barrier properties (Park et al. 1993; Donhowe and Fennema1993a, b; Nisperos-Carriedo 1994). Chitin and its deacetylated product, chitosan, have received a lot of interest inagriculture, biomedicine, biotechnology and the food industry due to their uniqueproperties, biodegradability and bioactivity (Muzzarelli et al. 1988; Kumar 2000;Tharanathan and Kittur 2003). Based on its antifungal, mechanical and oxygen bar-rier properties (Chen et al. 1996; Caner et al. 1998), chitosan film is a promisingactive packaging film material (Vermeiren et al. 1999). Production of chitosan fromcrustacean shells, a byproduct of the seafood industry, is economically feasible(Kumar 2000). However it lacks universal approval for food applications. Composite biopolymer films can bring about improved mechanical and physicalproperties if components are structurally compatible. Thus, blending a starch ormethylcellulose with chitosan can produce films with interesting properties andnovel applications. Plasticizers are the other components of edible films. These are low molecularweight compounds that are added to soften the rigid structure of films. Plasticizersimprove mechanical, barrier and physical properties of biopolymer films (Banker1966). They must be compatible with film-forming polymers, and reduce inter-molecular forces and increase mobility of polymer chains (Donhowe andFennema 1993c, 1994). Hydrophilic compounds such as polyols (glycerol, sorbitol)and polyethylene glycol are commonly used as plasticizers in hydrophilic filmformulations (Gontard et al. 1993). Lipophilic compounds, such as vegetableoils, lecithin and, to a lesser extent, fatty acids, may also act as emulsifiers andplasticizers (Kester and Fennema 1986; Cuppet 1994; Donhowe and Fennema1994; Hernandez 1994). Food additives such as antioxidants, antimicrobial agents and nutrients, can beincorporated in film formulations to achieve specific functionalities. This conceptof “active films” is a very promising application as it creates new avenues fordesigning packaging materials. One of the most popular and oldest techniques to protect specific fruits andvegetables is application of natural wax and lipid coatings. Coatings are intendedto protect product against dehydration, attack by fungi, and abrasion duringprocessing and to improve product appearance (Hardenburg 1967; Paull and Chen1989; Drake and Nelson 1990; Drake et al. 1991; Baldwin 1994; Hagenmaier andBaker 1994; Baldwin et al. 1997). In some products, the oily appearance limits theiruse (Baker et al. 1994; Baldwin et al. 1997). Composite starch suspensions can be used as coatings or for preparation ofedible films. The most common method of food coating involves spraying orimmersion. Coating integrity is a critical factor that depends on, surface tension,adhesion to food substrate and flexibility of the coating. Unplasticized matrices are
172 M.A. García et al.often brittle and rigid once dried, due to strong interactions between polymer chainsthat favor crystal development. This brings formation of cracks or and peeling off,especially for irregularly shaped fruits. Addition of a plasticizer can remedy thisproblem, since it can improve coating flexibility by reducing interactions betweenpolymer chains. However the amount of plasticizer needs to be optimized since itsamount can negatively alter the barrier and mechanical properties of a coating. Garcíaet al. (1998a, b, 1999, 2000b, 2001) described how they optimized plasticizer incomposite coatings. For starch-based formulations, glycerol and sorbitol are commonplasticizers used with typical concentrations in coating solutions ranging between0 and 50 g/L. Maximum plasticizer concentration is limited by surface migration. Forexample, the maximum amount of glycerol suitable for these starch-based formulationswas 20 g/L, while higher concentrations resulted in plasticizer migration to thesurface, leading to a sticky coating (García et al. 1998a). For sorbitol, a concentrationgreater than 20 g/L can led to inconveniently long drying times. Sunflower oil was included in coating formulations at concentrations between 0and 8 g/L to enhance water barrier properties. Similar to plasticizers, lipid materialsalso may migrate to coating surface, depending on coating microstructure. Starch-based coatings containing less than 5 g/L sunflower oil did not exhibit oil migration(García et al. 2001). Wong et al. (1992) reported that similar lipid concentrationsdid not result in oil migration in chitosan-fatty acid films. However, a marked lipidmigration was reported for methylcellulose films (Greener and Fennema 1989;Vojdani and Torres 1989a, b, 1990). Lipid concentration has been optimized forbarrier properties by García et al. (2001). Apart from sunflower oil, a composite coating may also include active ingredientssuch as antimicrobial agents and antioxidants. Active components remain at thesurfaces of food products, where they are needed. The coating matrix limits diffusionof active components into the core of the food and thus, minimizes the amount ofadditive needed for the product (García et al. 2001). Another important application of coatings is to reduce oil uptake of productsduring deep fat frying. Excessive fat in the diet has been linked to coronary heartdisease. Thus, coatings applied to food before frying can help in reducing fatabsorption. Hydrocolloids, especially cellulose derivatives such as methylcellulose,can be used to minimize oil content of fried foods. The description of coating formulations used in published works (García et al.1998a, b, 1999, 2000b, 2001, 2002, 2004a,b) is shown in Table 6.2. Table 6.2 Coating formulations Coating matrix Components Starch Starch source (% amylose): corn starch native (25), amylomaize (65) Plasticizer – glycerol or sorbitol (0–20 g/L) Starch and lipid Lipid - sunflower oil (0–8 g/L) Starch and antimicrobial agent Active agents – potassium sorbate and citric acid Methylcellulose (MC) MC (0.5–1.5 g/100 g) Plasticizer – sorbitol (0–1 g/100 g)
6 Characterization of Starch and Composite Edible Films and Coatings 1736.3 Preparation and CharacterizationComposite films are prepared by using 2 or more hydrocolloids. This requires dis-solution of biopolymer molecules. Some polysaccharides, like cellulose deriva-tives, require solubilization at a higher temperature, while others require dissolutionin a pH-regulated medium (e.g., chitosan). Preparation of starch for the preparation of films requires gelatinization of nativestarch granules either by cold (e.g., alkaline treatment with NaOH) or thermaltreatments. The most common technique to gelatinize starch is through thermal treat-ment (Mali et al. 2002). However, alkaline dispersion can also be used to alter thesize distribution of starch polymers, that brings about a mild degree of starchhydrolysis or depolymerisation (García et al. 2000a; Romero-Bastida et al. 2005). In general, preparation of protein-based films requires dissolution of protein inan appropriate solvent, e.g., zein, which is a prolamin, requires dissolution in ethanol(Ghanbarzadeh et al. 2007). Other examples of alcohol-soluble proteins are wheatgluten and fish myofibrillar proteins. Hydration of protein facilitates its solubiliza-tion (Sobral et al. 2001). Cross-linking of proteins with lactic acid, tannic acid, ionized calcium or trans-glutaminase has been shown to increase resistance of films to water vapour and gas.In addition, preparation of films from aqueous emulsions of proteins and lipids or bylamination of a protein film with lipid can also decrease water vapour permeability(WVP). Lipids are frequently incorporated to reduce water vapour permeability, dueto their hydrophobic character. Addition of lipids to a hydrocolloids matrix can becarried out by overcasting, leading to bilayer films, or by emulsion techniques(Baldwin et al. 1997; Shellhammer and Krochta 1997). In the latter case, the sus-pension can be used to obtain either coatings or films. With solid lipids, such ascarnauba wax or saturated fats, the common procedure is to incorporate them viabilayer films, whereas the emulsion technique is preferred for liquid lipids, such asedible oils (Greener and Fennema 1989; Gontard et al. 1994; Hagenmaier andBaker 1994; Shellhammer and Krochta 1997). Emulsion preparation parametersare important factors for obtaining homogenous films and coatings, and will influ-ence performance. For example, in the case of starch-based films, a high stirringvelocity produced extensive foaming that could not be eliminated with a vacuumand thus produced low quality coating (García et al. 2001). Another importantfactor is the lipid to aqueous phase ratio. If the critical ratio is exceeded, migrationof lipid may occur. Plasticizers are often added once biopolymer solubilization has been achieved.Other functional additives (e.g., emulsifiers, antimicrobial or antioxidant agents)are incorporated into formulations after addition of the plasticizer. It must be stressedthat each individual additive may require a particular condition for proper andeffective incorporation. As described previously, composite suspensions can be used to obtain eithercoatings or films. In the case of coatings, surface tension and rheological behaviorof the suspension are important factors that will affect suspension spreadability
174 M.A. García et al.and coating adhesion. Plasticizer and lipid addition, in the case of a starch coatingsuspension, decrease surface tension (Table 6.3), providing better adhesion tofoodstuffs. The surface of vegetables already has low surface tension for naturalprotection. However, this natural advantage is a drawback for aqueous coatingapplications (Hershko and Nussinovitch 1998). Modifying the coating formula-tion to include plasticizers and/or lipids helps decrease surface tension to facilitateadhesion of coating to foodstuffs (Table 6.3). The similarity between liquid andsolid film in values of dispersive and polar components influences spreadabilityof the liquid (Hershko and Nussinovitch 1998). Ghanbarzadeh et al. (2007)reported that sugar addition increases surface tension of zein films, which wasattributed to an increase in polar forces and interactions within the film matrix. Understanding the rheological behavior of film or coating suspensions iscritical for process scale-up to ensure that processing requirements andmachinability issues can be properly addressed. Rheological properties ofcomposite starch suspensions exhibit pseudoplastic behavior (n < 1), while thePower law rheological model provided a satisfactory behavior fit enough toexperimental data (r2 > 0.96) (García et al. 2006). Plasticizer and lipid additionto corn and amylomaize starch suspensions decreased the flow behavior index andincreased the consistency index. Apparent viscosity of corn starch suspensionsdecreased with both plasticizer and lipid addition (Table 6.3). Measurement ofviscosity is important. Spraying requires a low viscosity, while immersion requiresa higher viscosity coating solution. In formulation of composite biopolymer films, it is important to characterizethe miscibility of biopolymers and interactions that may occur between them, sincethese attributes ultimately influence film microstructure. For example, chitosan-starch suspensions show pseudoplastic flow behavior similar to those obtainedwith chitosan suspensions (Fig. 6.1). The presence of chitosan in the suspensiondecreased peak viscosity of the suspension. When chitosan was blended withmethylcellulose, film solutions also showed pseudoplastic behavior (n < 1). Singlecomponent solutions of either MC or CH showed similar values for all rheologicalparameters; however, composite film solutions had higher apparent viscosities andTable 6.3 Characterization of composite film suspensions Surface tension Apparent viscosityFormulation (dyne/cm) hap at l = 692,48 s−1 (mPa s)Methylcellulose (MC) 87.00 ± 0.210 102.49 ± 0.83Chitosan (CH) 72.17 ± 0.710 112.73 ± 0.89CH:MC (75:25) 87.50 ± 0.690 140.68 ± 1.06CH:MC (50:50) 81.07 ± 0.320 134.57 ± 1.19CH:MC (25:75) 70.38 ± 0.470 127.11 ± 0.75Starch-based (w/o additive) 60.68 ± 0.120 12.85 ± 0.063Starch-based (w/ glycerol, G) 59.60 ± 0.764 11.95 ± 0.182Starch-based (w/G + sunflower oil, SO) 59.08 ± 0.679 11.31 ± 0.092Starch-based (w/sorbitol, S) 51.44 ± 0.082 12.59 ± 0.176Starch-based (w/S + SO) 54.02 ± 0.266 9.64 ± 0.182
6 Characterization of Starch and Composite Edible Films and Coatings 175 a 90 CH 75 CS+CH 60 CS+CH+G τ (Pa) 45 30 15 0 0 100 200 300 400 500 γ (sec−1) b 90 CS+G 75 CS 60 τ (Pa) 45 30 15 0 0 100 200 300 400 500 γ (sec−1)Fig. 6.1 Rheological behavior of film suspensions formulated with (a) chitosan (CH), cornstarch–chitosan (CS + CH) and corn starch–chitosan–glycerol (CS + G + CH); (b) corn starch(CS) and corn starch with glycerol (CS + G) (cornstarch at 5%)consistency indexes than those of single component solutions by themselves. Theseresults point to a likely synergistic effect between constituents of the film solution,suggesting a high compatibility and high degree of interaction between the twopolymer types. Besides, apparent viscosity of film solutions increased with CHconcentration (Table 6.3).6.4 Film PreparationFilms can be prepared by casting, extrusion or lamination, which are similar proc-esses used in the synthetic polymer industry (Stepto 1987). Casting is a common,small-scale production method used to obtain biodegradable films. In this technique,
176 M.A. García et al.a portion of the film suspension is poured onto acrylic plates, and then dried in aventilated oven (60°C) to a constant weight (García et al. 1999). This simple tech-nique produces films that can be easily removed from plates, and allows films ofvariable thickness to be obtained by varying the weight of film suspension appliedand the area of the plate onto which films are cast. Drying conditions (rate and temperature) determine film characteristics (e.g.,water content, crystallinity, etc.) that affect film microstructure and properties.Bader and Göritz (1994a, b, c) extensively studied the effect of drying on amylo-maize film microstructure, and developed a model relating X-ray diffractionpatterns, sorption isotherms and mechanical properties of films. They stressed thatdrying temperature lead to different X-ray diffraction pattern which are associatedwith different crystalline developments during storage. Thus, tailoring dryingconditions allows controlling of amorphous-crystalline structure, which is stronglyrelated to barrier and mechanical properties.6.4.1 Film and Coating CharacterizationThe main attributes involved in characterizing biodegradable films are: opticalproperties, water-solubility, water sorption/desorption, thickness, microstructure,crystallinity, biopolymer compatibility (composite films), thermal behavior, barrierproperties (vapour and gaseous permeabilities) and mechanical behavior.184.108.40.206 AppearanceThe visual properties of a film ultimately determine consumer acceptability ofthe packaged products. Both subjective and objective techniques are used to char-acterize optical properties of films, with surface color commonly measured by acolorimeter and opacity determined by spectrophotometry. Polysaccharide filmsare typically colorless, though those of CH may exhibit a slightly yellow appear-ance. However, the intensity of the yellowness was negligible in comparison to thatof whey protein-based films (Trezza and Krochta 2000a, b). Polysaccharide filmsare free of many of the problems associated with protein and lipid films, such asMaillard and oxidation reactions (Trezza and Krochta 2000a, b). Film opacity is a critical property to consider if the film is to be used at a foodsurface. It can be measured using the method proposed by Gontard et al. (1992),in which the film spectrum is recorded over the visible range. Opacity is estimatedas the area under the absorption curve (Au × nm). Transparent films are character-ized by low values for area under the absorption curve measurements. Table 6.4shows that CH films were the most transparent, and CS films the most opaque,increasing opacity with increasing starch concentration. Nevertheless, opacity valuesfor starch-based films were still lower than those reported for wheat gluten filmsobtained under different solubilization conditions (Gontard et al. 1992). Addition
6 Characterization of Starch and Composite Edible Films and Coatings 177Table 6.4 Optical properties of corn starch, chitosan and composite films Film color Film opacityFilm composition (Au × nm) Color differences (DE) Chromaticity b*Corn starch (CS) a 138.0 ± 0.8 0.83 ± 0.16 2.20 ± 0.25CS with glycerol 109.6 ± 0.9 0.60 ± 0.10 2.23 ± 0.08CS with chitosan 95.9 ± 1.05 1.74 ± 0.15 2.94 ± 0.15CS with glycerol and chitosan 88.7 ± 0.7 2.16 ± 0.19 3.68 ± 0.21Chitosan (CH) 18.9 ± 1.1 3.79 ± 0.50 5.04 ± 0.32a CS concentration: 5 g/100 g film suspension Table 6.5 Film solubility in water at 100°C of CH–MC films Film composition Film solubility in water (%) MC 98.4 ± 2.2 CH:MC (25:75) 40.7 ± 6.3 CH:MC (50:50) 27.7 ± 1.6 CH:MC (75:25) 14.0 ± 2.1 CH 9.3 ± 0.9of glycerol reduced starch film opacity, while blending corn starch with CH gener-ated films with reduced opacity, but increased yellowness.220.127.116.11 Water SolubilityWater solubility is an important factor in determining possible applications forcomposite biopolymer films. MC films are completely soluble in water, whileCH films have lower water-solubility values. Composite MC–CH films had inter-mediate water-solubility, which decreased with increasing chitosan concentration(Table 6.5). Thus, by adjusting CH concentration in the film formulation, water-solubility of the composite film can be changed to meet requirements of a specificapplication. A similar trend in water solubility was observed for CH-starch com-posite films.18.104.22.168 Water SorptionWater sorption isotherms are useful for determination of film stability undervarious conditions, as many film constituents, especially hydrocolloids, aresensitive to relative humidity and temperature. Though sorption isotherms canbe measured by several techniques, a simple procedure is described by Spiessand Wolf (1993). Sorption isotherms for yam starch films (with and without glycerol) and nativeyam starch were compared at 25°C (Fig. 6.2). All isotherms showed a similar
178 M.A. García et al. 80 70 Moisture content (% db) 60 50 40 30 20 10 0 0.11 0.43 0.58 0.65 0.75 0.90 0.97 Water activity (aw)Fig. 6.2 Water sorption isotherms of yam starch films and native yam starch at 25°C. (filleddiamond) yam starch (Film formulation: 4.0% yam starch (open square) without glycerol, (timessymbol) with 1.3% glycerol, and (filled square) with 2.0% glycerol)sigmoidal shape (type II isotherm). When samples were conditioned at wateractivity (aw) values greater than 0.43, the plasticized starch film showed higherequilibrium moisture contents than both the native yam starch powder and the non-plasticized starch film. The hygroscopic characteristics of glycerol-plasticizedstarch films contributed to an increase in hydrophilicity of the film. Controlled films showed higher equilibrium moisture content than native yamstarch at aw > 0.75. This result could be attributed to the fact that during film pro-duction, gelatinization led to a starch molecular reorganization that increased waterabsorption capacity of the unplasticized film compared to native starch. Unplasticizedfilms showed similar behavior to those reported by other researchers working withhigh-amylose corn starch (Bader and Göritz 1994b) and tapioca starch films(Chang et al. 2000).22.214.171.124 Thickness of FilmsFilm thickness can be measured with a digital film thickness gauge or by scanningelectron microscopy (SEM), the first method being simpler and faster. Correlationbetween film thickness measured by SEM and a digital film thickness gauge wasestablished for CH-starch films (García et al. 2006). These results are presented inTable 6.6 with a correlation coefficient of 0.9953.
6 Characterization of Starch and Composite Edible Films and Coatings 179 Table 6.6 Film thickness of corn starch, chitosan and composite films Film thickness (mm) Film composition Digital thickness gauge SEM Corn starch (CS) a 63.1 ± 1.7 69.2 ± 1.9 CS with glycerol (G) 44.4 ± 0.9 47.3 ± 1.9 CS with chitosan (CH) 51.5 ± 7.8 56.1 ± 11.3 CS with G and CH 52.2 ± 1.4 57.0 ± 2.1 CH 15.2 ± 1.8 13.9 ± 2.9 a CS concentration: 5 g/100 g film suspension Barrier and mechanical properties depend on film thickness. A wide range of filmthickness values has been reported for composite biopolymer films in the literature,indicating its dependence on both film composition and processing parameters.126.96.36.199 MicrostructureProperties of composite films and coatings depend on several factors such as: theratio of crystalline to amorphous zones, polymeric chain mobility, and specificinteractions between functional groups of polymers and the permeant substancewithin amorphous zones. Common techniques used to elucidate film structureinclude SEM, X-ray diffraction, differential scanning calorimetry (DSC), thermo-mechanical analysis (TMA), dynamic mechanical analysis (DMA) and Fouriertransform infrared spectroscopy (FTIR).188.8.131.52 Scanning Electron MicroscopySEM may be used to evaluate film homogeneity, layer structure, pores andcracks, surface smoothness and thickness. For example, cross sections of unplas-ticized corn starch film showed a multi-laminar structure, while those for filmscontaining a plasticizer showed a more compact structure, regardless of the plas-ticizer used (Fig. 6.3, Table 6.6). SEM images of plasticized films containing lipidexhibited smooth surfaces and a compact structure, indicative of a homogeneousdispersion of lipids within the film matrix. When corn starch was blended with chitosan, film surfaces appeared smooth(without pores or cracks) and homogeneous (no obvious phase separation), evenfor formulations that did not include a plasticizer (Fig. 6.4c, Table 6.6). Thecompact, homogeneous matrix of CS–CH films is an indicator of structural integ-rity and, consequently, good mechanical properties such as high resistance andelongation at break are expected. Similarly, in the case of MC–CH compositefilms, a compact structure with no pores or cracks was observed by SEM, eventhough film formulation did not include a plasticizer (Fig. 6.5). The composite
180 M.A. García et al.Fig. 6.3 SEM micrographs of the surface of corn starch-based films (a) without plasticizer, (b)with 20 g/L glycerol and (c) with 20 g/L sorbitol and 2 g/L sunflower oil (Magnification: 100 mmbetween marks)film showed multilayered structure (Fig. 6.5c), though both CH and MC are com-patible polymers that could limit chain mobility. When dealing with coatings, characterization of microstructure provides importantinsight into performance of the different formulations. Light microscopy is used forevaluation of coating adhesion, thickness and uniformity, while estimation of coatingintegrity is conducted by SEM. Improved visualization of starch-based coatings usinglight microscropy may be achieved via staining with iodine solution. Coating thicknessesvaried between 40 and 50 mm for all tested formulations (García et al. 1998a, b).184.108.40.206 Infrared SpectroscopyFourier transform infrared spectroscopy (FTIR) is a useful technique to supple-ment microstructural characterization of composite films, since it may be used toevaluate interactions between film components. Figure 6.6a shows the IR spectrafor films of MC, CH and a 50:50 CH–MC blend. The positions of peaks of thesingle component spectrum is similar to those described by different authors
6 Characterization of Starch and Composite Edible Films and Coatings 181Fig. 6.4 SEM micrographs of the cross-sections of (a) corn starch-based films (b) chitosan filmsand (c) a film obtained by blending corn starch and chitosan(Chen et al. 2003; Sionkowska et al. 2004; Wu et al. 2005; Zaccaron et al. 2005).Spectra of compo-site films show characteristic peaks of both polymers, andalso small shifts in the positions of the 1,500–1,700 cm−1 bands, which are relatedto amino and carbonyl groups. Figure 6.6b shows the effect of chitosan concen-tration in CH–MC blends with an increasing CH concentration, while spectra of
182 M.A. García et al.Fig. 6.5 SEM micrographs of the cross-section of (a) methylcellulose films, (b) chitosan films and(c) a film obtained by blending methylcellulose and chitosan (Magnification: 10 mm between marks)composite films approach that of the CH film. Further, composite films showed abroad band between 2,985 and 3,600 cm−1 corresponding to the N–H and –OHsuperposition of chitosan (Sionkowska et al. 2004), while MC film showed onlythe characteristic –OH stretching at 3,457 cm−1 (Zaccaron et al. 2005).
6 Characterization of Starch and Composite Edible Films and Coatings 183 a 120 100 MC 80 CH Transmitance (%) 50:50 60 40 20 0 0 500 1000 1500 2000 2500 3000 3500 4000 4500 Wavenumber (cm−1) b 120 100 25:75 50:50 80 75:25 Transmitance (%) 60 40 20 0 0 500 1000 1500 2000 2500 3000 3500 4000 4500 Wavenumber (cm−1)Fig. 6.6 FTIR characterization of: (a) MC, CH and 50:50 films and (b) composite films withdifferent CH:MC ratios According to Wanchoo and Sharma (2003), hydrogen bonding or other interac-tions between chemical groups of dissimilar polymers should theoretically cause ashift in the peak position of participating groups. In composite MC–CH films, thisbehavior is observed for –OH stretching, since this peak shifted from 3,463 cm−1in MC films toward 3,450 cm−1 in CH-MC composite mixtures with increasing
184 M.A. García et al.CH proportion. This observation could indicate that the –OH group movement iscompromised when another polymer is present. A shift was also observed in CHamino group (–NH2) band at 1,560 cm−1 as the amount of MC decreased in com-posite films. However, other characteristic peaks, including those at 1,411 cm−1(OH vibrations) and 2,904 cm−1 (C–H stretching) assigned by Pawlak and Mucha(2003) and Zaccaron et al. (2005) did not show a significant shift. These resultssuggest a mild interaction between CH and MC that might be attributed to theirsimilar chemical and linear structures.220.127.116.11 X-ray DiffractionX-ray diffraction patterns of edible films, either of single component or compositematerials, show an amorphous-crystalline structure characterized by sharp peaksassociated with the crystalline diffraction and an amorphous zone. The higher theamorphous zone, the lower the crystallinity. Amorphous regions within the sample canbe estimated by the area between the smooth curve drawn following the scatteringhump and the baseline joining the background within the low- and high-angle points.The crystalline fraction can be estimated by the relative area of the upper regionsabove the smooth curve (Snyder and Bish 1989; Köksel et al. 1983). In general,crystallinity of composite films is dependent on the following processing conditions:(1) biopolymer source and plasticizer, (2) completeness of biopolymer dissolution inwater, (3) conditions of film drying (rate and temperature), and (4) final moisturecontent of the samples (Van Soest et al. 1996; Van Soest and Vliegenthart 1997). Theshape and width of the diffraction profile are determined by both the mean crystal size(and distribution of crystal size within the specimen) and the particular imperfectionsof the crystalline lattice (Klug and Alexander 1974). X-ray diffraction can be used to track recrystallization of film polymers duringstorage. In the case of starch-based films, peak width decreased slightly and peakintensities increased, indicating a growth in crystallite size corresponding to aslow recrystallization process. X-ray diffraction patterns of composite films generallyrepresent a mixture of component features in which the characteristic peaks ofindividual components can be identified. For example, X-ray diffractograms ofcomposite MC–CH films are similar to those obtained for MC alone, althoughpeak intensity at 2θ = 8° (which is distinctive of MC films) decreased with anincreasing CH concentration, suggesting that CH interferes with MC ordering(Fig. 6.7). Similar results were reported for CH-gelatin films by Chen et al.(2003), who attributed the decreased crystallinity of the composites to reducedhydrogen bonding in CH molecules, leading to an amorphous structure for thepolyelectrolyte complex. Film preparation techniques also may lead to development of different matrixstructures. For films based on thermal gelatinization of starch, X-ray diffractionpatterns of yam starch films exhibited a B-type crystalline packing arrangement,characteristic of starch from tubers (Roos 1995). This pattern remained virtuallyunchanged over the course of storage. Starch and glycerol contents did not markedly
6 Characterization of Starch and Composite Edible Films and Coatings 185Fig. 6.7 X-ray diffractograms of methylcellulose (MC), chitosan (CH) and composite filmsFig. 6.8 X-ray diffractograms of amylomaize films stored at 20°C and 63.8%relative humidityfor 100 daysinfluence the X-ray pattern of these films (Mali et al. 2002). In contrast, when filmswere obtained from starch solubilized by alkaline treatment, X-ray diffraction pat-terns showed that starch films exhibited a crystalline structure of higher stability,namely an A-type starch pattern (Fig. 6.8). This shift in the crystalline pattern was
186 M.A. García et al.Fig. 6.9 X-ray diffractograms of amylomaize films plasticized with glycerol and sunflower oil,(a) at initial time and (b) stored at 20°C and 64% relative humidity for 60 daysalso observed for amylomaize films by Bader and Göritz (1994a, c) and was attrib-uted to film drying conditions. For drying temperatures up to 60°C, diffractogramsof films exhibited a B-type crystalline pattern, while those dried at 100°C exhibiteddiffractograms corresponding to A-type crystals. As film drying temperatureincreased over the range of 60–100°C, film diffractograms exhibited a continuoustransition from B- to A-type crystals. The crystallinity of starch films was primarilyrelated to the amylose content of the starch source, and depended on both dryingand storage conditions. High water content favors chain interactions and, thus,crystallization within starch films. In hydrocolloid films, as described for starch,water has an additional role, since it is incorporated in a structural active statethrough inter- and intramolecular hydrogen bondings (Even and Carr 1978). Starch films without plasticizer showed higher crystallinity (higher peaks) thanthose containing plasticizer, which resulted in a larger amorphous zone and lowerpeaks (Fig. 6.9). Films containing plasticizers also retained a stable diffractionpattern during initial stages of storage, while unplasticized starch films requiredmore time to reach a stable diffraction pattern (García et al. 2000a). Additionof sunflower oil did not strongly modify X-ray pattern of films during storage(Fig. 6.9b). Nevertheless, the presence of oil facilitated polymeric chain mobility,allowing rapid development of the most stable structure, and also reduced crystalgrowth by interfering with the polymeric chain arrangement.18.104.22.168 Differential Scanning Calorimetry of FilmsEvolution of the film matrix crystalline structure during storage can also be evalu-ated by DSC. As described in the results of X-ray diffraction, film preparation andstorage conditions impact the thermal properties of composite films. Films obtained
6 Characterization of Starch and Composite Edible Films and Coatings 187by starch thermal treatment, such as those formulated with yam starch, did notshow any peaks in DSC thermograms at the beginning of the storage time, indicat-ing that starch gelatinization during film production was complete. With storage(90 days at 20°C and 64% relative humidity), these films did not show any peaksin DSC thermograms (between 40° and 120°C), indicating stability of the matrix(Mali et al. 2002). However, starch films obtained by alkaline treatment showed an endothermictransition with a peak temperature around 50°C during storage (90 days). This peakbecame narrower and its melting temperature and the corresponding enthalpy (∆H)increased with increasing storage time (Fig. 6.10). This, DSC transition could be asso-ciated with several processes, such as the crystal growth of short chains (products ofhydrolysis) and recrystallization of amylose or other long lateral amylopectin chains. The presence of plasticizers in films limited crystal growth and recrystallizationsimilar to that previously described for X-ray analysis, leading to lower enthalpyvalues (∆H) and peak melting temperatures (Fig. 6.10). Sorbitol is a good plasticizerfor starch, since its molecular structure is similar to glucose units of starch chains,increasing the chance to interact with polymeric chains (García et al. 2000a).Additives may interfere with polymeric chain association due to steric hindrances,and in these cases film crystallinity will likely decrease.Fig. 6.10 DSC thermograms of amylomaize films stored at 20°C and 63.8% relative humidity
188 M.A. García et al.22.214.171.124 Glass Transition TemperatureThe glass transition temperature (Tg) is strongly dependent on both the film com-position and moisture content, and can denote stability of a film. As water contentof an amorphous material increases, Tg decreases. Thus, for a given storage tempera-ture, an amorphous matrix at low water content (in the glassy state) remains stableto molecular change, while the same matrix at higher moisture content, correspondingto the rubbery state, can undergo molecular reorganization. In the rubbery state,polymer chains possess sufficient mobility for crystal growth and perfection. Thus,knowledge of Tg is important, since it impacts mechanical and barrier properties ofa film under specific conditions of application and storage. Both DSC and TMA techniques are commonly used to estimate Tg, though Tgvalues obtained by DSC are slightly higher than those determined by TMA. Changand Randall (1992) stressed that the sensitivity of TMA is superior to that of DSCfor defining glass transition temperatures. Dynamic mechanical thermal analysis(DMTA) may also be used for determination of Tg. Table 6.7 provides some literature-reported Tg values for various film formulations. Plasticization decreases intermo-lecular forces between polymer chains and, consequently, reduces Tg (Guilbert andGontard 1995). For composite starch matrices, Tg values for films without plasti-cizer were higher than those of films containing glycerol (Table 6.7). In this regard,a similar trend was observed for films formulated with other polysaccharides(Debeaufort and Voilley 1997) and proteins of varied origin (Cherian et al. 1995;Galietta et al. 1998; Sobral et al. 2001).126.96.36.199 Barrier PropertiesBarrier properties ultimately determine the ability of films and coatings to improvestorage or shelf life of various food products. Common measurements includeTable 6.7 Glass transition temperature (Tg) of films with different compositions Glass transitionFilm formulation temperature, Tg (°C) Method (references)Yam starch 48.0 DSC (Mali et al. 2002)Yam starch 44.2 TMA (Mali et al. 2002)Yam starch 44.2 TMA (Mali et al. 2002)Yam starch plasticized with glycerol 12.2 DSC (Mali et al. 2002)Yam starch plasticized with glycerol 10.9 TMA (Mali et al. 2002)Gluten protein plasticized with glycerol 68.0 DMTA (Pommet et al. 2005)Gelatin plasticized with sorbitol 56.5 DSC (Sobral et al. 2001)Chitosan (depending on water content −23.0 to 67.0 DSC and DMTA (Neto and degree of acetylation) et al. 2005)Pectin 35.0 DSC (Iijimaa et al. 2000)DSC differential scanning calorimetry; TMA thermomechanical analysis; DMTA dynamicmechanical thermal analysis
6 Characterization of Starch and Composite Edible Films and Coatings 189water vapour and gas permeabilities, which are strongly related to film structure,since permeants generally, move through a film or coating via its amorphous zones.Film components, especially plasticizers, affect both barrier and mechanical prop-erties, because they modify film structure, chain mobility and diffusion coefficientsof permeants.Water Vapour PermeabilityDetermination of water vapour permeability (WVP) is strongly dependent on meas-urement conditions, such as temperature and the gradient of water vapour pressure.Coated biomaterials, such as fruits and vegetables, are characterized by irregularshapes and high water contents that make WVP measurements difficult. To overcomethis challenge, García et al. (1998a, b) used a biological model (coated slicedcarrots) that allowed surface area calculations to be accounted for WVP determina-tions of starch-based coatings (García et al. 1998a, b). WVP testing of films maybe conducted according to method E96 (ASTM 1996a) that includes some modifi-cations introduced by Gennadios et al. (1994). Since barrier thickness stronglyaffects water vapour transport through the film matrix, it is necessary to considerfilm thickness in WVP calculations. In addition, WVP determinations can beperformed using the PERMATRAN, a specific instrument developed by MOCONfor analysis of synthetic film materials. It is interesting to note that WVP results forcoatings (applied on fruits) and films have been shown to be similar, even thoughthe measuring techniques and driving forces for both systems are different. Thesefindings validate the use of films to characterize barrier properties of coatings(García et al. 1998b, 2000b, 2004c). Coatings without plasticizer often yield significantly higher WVP values thanthose with plasticizer (Table 6.8). This difference is attributed to the presence ofpores and cracks in unplasticized coatings, as observed by light microscopy andSEM (García et al. 1999). In the absence of cracks or pores, a plasticized film gener-ally would be expected to exhibit higher WVP than an unplasticized film (Banker1966). These results could be related to structural modifications to the starch net-work produced by the plasticizer and to the hydrophilic character of glycerol, whichfavors the absorption and desorption of water molecules to promote permeability.Gontard and coworkers (1993) working on wheat gluten films found similar resultson the effect of glycerol. Sorbitol generally resulted in lower WVP values comparedto glycerol in plasticized starch-based coatings (Table 6.8e). McHugh and Krochta(1994a, b, c) reported similar results for alginate and pectin films using the sameplasticizers at the same concentrations. Amylomaize films and coatings, which possessed higher amylose content,denser matrix structure and higher degree of crystallinity than those of standardcorn starch, also exhibited relatively lower WVP values (Figs. 6.8, 6.10). A similartrend has been observed by others (Noel et al. 1992; Miles et al. 1985a, b). How-ever, the effect of amylose content on the WVP of the starch film matrix wasminimized by incorporation of sunflower oil to the coating formulation (Table 6.8).
190 M.A. García et al. Table 6.8 Effect of formulation on water vapour permeability (WVP) of composite polysaccharide films Water vapour permeability Formulation (g m−1 s−1 Pa−1) × 1011 Methylcellulose (MC)a i 7.55 ± 0.60 Composite MC:CH (75:25)c 7.24 ± 0.35 Composite MC:CH (50:50)c 6.67 ± 0.74 Composite MC:CH (25:75)c 6.77 ± 0.92 Chitosan (CH)b 5.04 ± 0.81 Corn starch thermally gelatinized (CS)d 17.66 ± 2.97 CS + glycerol (G) 8.68 ± 0.20 Composite CH–CS (CH + CS)e 8.76 ± 0.87 Composite CH–CS (CH + CS + G)e 4.46 ± 0.37 Corn starchf (Without additives) 36.80 ± 22.40 Corn starchf (Glycerolg, G) 25.70 ± 10.40 Corn starchf (G + Sunflower oilh, SO) 19.20 ± 4.70 Corn starchf (Sorbitolg, S) 17.50 ± 1.40 Corn starchf (S + SO) 12.20 ± 1.10 Amylomaizef (Without additives) 26.20 ± 13.90 Amylomaizef (G) 21.40 ± 7.50 Amylomaizef (G + SO) 17.60 ± 3.70 Amylomaizef (S) 12.10 ± 1.50 Amylomaizef (S + SO) 9.70 ± 0.80 a C concentration = 1% b CH concentration = 1% c CH:MC (w/w) ratio d CS (corn starch) = 5% corn starch e CH–CS (w/w) f Corn starch or amylomaize concentration = 20 g/L g Glycerol or sorbitol concentration = 20 g/L h SO = sunflower oil (2 g/L) i value ± standard deviationAddition of sunflower oil significantly decreased WVP of starch-based films andcoatings. Baldwin and coworkers (1997) reviewed lipid effects on other non-starchcomposite films. As water vapour transfer generally occurs through the hydrophilicportion of a film, WVP is dependent on the hydrophilic-hydrophobic ratio offilm components (Hernandez 1994). In general, WVP increases as polarity anddegree of unsaturation/branching of the incorporated lipid increases, thoughwater absorption properties of polar components of the film must also be considered(Gontard et al. 1994). Yam starch film WVP is lower than those of many edible, biodegradable filmssuch as wheat gluten plasticized with glycerol and amylose and hydroxypropylmethylcellulose containing plasticizer and oil, (Gennadios et al. 1994). In general,starch films exhibit a lower order of magnitude of WVP compared both to proteinfilms and other polysaccharide-based films reported in literature (García et al.1999, 2001, 2004c; McHugh and Krochta 1994a, b, c; McHugh et al. 1994; Parraet al. 2004; Parris et al. 1995). In comparison to synthetic polymers, starch films
6 Characterization of Starch and Composite Edible Films and Coatings 191have WVP values similar to those of cellophane, but higher than low density poly-ethylene, the most common synthetic film. García et al. (2004b) studied the effect of composition on CH–MC compositebiopolymer films. Permeabilities of these composite biopolymer films did notdiffer significantly from those of single component films (Table 6.8). This result,together with X-ray analysis, provided evidence that matrices of composite filmswere very similar to those based on the single polymers. Table 6.8 also shows WVPvalues of composite films formulated with chitosan and corn starch. Addition ofglycerol decreased WVP of CS films as described previously. McHugh and Krochta(1994c) found similar results for alginate and pectin films. Blending CS with CHdecreased WVP of composite films. Plasticized composite CS–CH films haveWVP values that were similar to those of CH films, thus blending CH with CS is agood alternative to maintain barrier properties and reduce costs (García et al.2006). A summary of WVP values for several hydrophilic edible films and syntheticpolymer films is presented in Table 6.9. In comparison to other commercial biopol-ymers, chitosan films exhibit relatively low WVP. Composite films of CH, MC andTable 6.9 Comparison of WVP values of biodegradable and synthetic filmsFilm formulation WVP (g m−1 s−1 Pa−1) ReferencesCorn zein 5.35 × 10−10 Ghanbarzadeh et al. (2007)Corn zein plasticized with glycerol 8.90 × 10−10 Gennadios et al. (1994)Fish skin gelatin 2.59 × 10−10 Avena-Bustillos et al. (2006)Whey protein plasticized With sorbitol 7.17 × 10−10 McHugh et al. (1994)Wheat gluten plasticized With glycerol 7.00 × 10−10 Gennadios et al. (1994)Gelatin (obtained from pigskin) plasti- 1.6 × 10−10 Sobral et al. (2001) cized with sorbitolAmylose 3.8 × 10−10 Gennadios et al. (1994)Corn starch plasticized with glycerol 2.57 × 10−10 García et al. (2001)Corn starch plasticized with sorbitol 1.75 × 10−10 García et al. (2001)Amylomaize starch plasticized with 1.21 × 10−10 García et al. (2001) sorbitolHydroxypropylmethylcellulose with 1.90 × 10−10 Gennadios et al. (1994) plasticizer and oilAmylomaize starch with sorbitol and 9.7 × 10−11 García et al. (2001) sunflower oilMethylcellulose 8.70 × 10−11 Donhowe and Fennema (1993b)Methylcellulose 3% 8.4–12.1 × 10−11 Park et al. (1993)Chitosan 2% (unknown source) 3.66–4.80 × 10−11 Wong et al. (1992)Chitosan 3% 6.19–15.27 × 10−11 Caner et al. (1998)Cellophane 8.4 × 10−11 Shellhammer and Krochta (1997)PVDC 2.22 × 10−13 Shellhammer and Krochta (1997)LPDE-low density polyethylene 9.14 × 10−13 Smith (1986)HDPE-high density polyethylene 2.31 × 10−13 Smith (1986)
192 M.A. García et al.CS attain WVP values close to those of cellophane (Table 6.8), as might beexpected, due to similar chemical structures of these polymers (Shellhammer andKrochta 1997). However, WVP values of composite films are not comparable withthose of synthetic films, such as low density polyethylene (LDPE), (Smith 1986),the primary polymer used in the food packaging industry (Table 6.9).Gas PermeabilityMeasurement of film or coating permeability to CO2 and O2 is essential to under-standing quality and physiological aspects of coated fruit products during storage.In the case of coatings, gas permeability is commonly measured using isolatedfilms rather than coated products. This simplification is based on the finding thatWVP results for coatings and films are similar (García et al. 2000b). Different methods are used to determine gas permeability of films. Oxygenpermeability can be measured using commercial instruments, such as the OXTRANdeveloped by Mocon Company. In addition, CO2 and O2 permeabilities of films canbe assessed by using a specially designed cell (García et al. 2000a, b, 2001). Thisquasi-static method is based on measurement of gas diffusing through a film,which is quantified by a gas chromatograph. As was previously described for WVPdeterminations, calculated values for gaseous permeability must account for filmthickness. Film and coating integrity is a must for attainment of good gas barrierproperties. Starch films without plasticizers exhibit much higher CO2 and O2permeabilities and also higher standard deviation coefficients than the same formu-lations containing plasticizers (Table 6.10). This result was attributed to the presenceof pores within films without plasticizers, resulting in a lack of film integrity, asdetermined by SEM (García et al. 1999, 2000a). Starch films with sorbitol exhibit lower oxygen permeability values than thoseformulated with glycerol (Table 6.10). Sorbitol combined with an amylomaize filmmatrix provided the lowest gas permeability values for all materials testedTable 6.10 Effect of film formulation on gas permeability of starch-based films CO2 permeability (cm3 m−1 O2 permeability (cm3 m−1 s−1)Starch base Additives s−1) × 1010 LSD0.05 = 1.63 × 1010 LSD0.05 = 1.03Corn _ 292.1 ± 138.9 15.92 ± 2.99Corn Glycerol 56.9 ± 9.7 4.61 ± 0.51Corn Glycerol + SO 58.7 ± 5.8 3.83 ± 0.76Corn Sorbitol 41.9 ± 8.1 2.48 ± 0.32Corn Sorbitol + SO 47.2 ± 6.5 3.77 ± 0.03Amylomaize _ 280.5 ± 73.7 26.45 ± 2.48Amylomaize Glycerol 38.5 ± 12.8 3.21 ± 0.19Amylomaize Glycerol + SO 43.9 ± 9.0 2.36 ± 0.04Amylomaize Sorbitol 29.6 ± 4.6 2.28 ± 0.26Amylomaize Sorbitol + SO 34.3 ± 2.1 2.18 ± 0.04Glycerol and sorbitol concentration = 20 g/L; SO = sunﬂower oil (2 g/L)
6 Characterization of Starch and Composite Edible Films and Coatings 193(Table 6.10). McHugh and Krochta (1994a, b) found similar results working onmilk and whey protein films. Table 6.10 shows that O2 permeabilities for starch-based films were much lowerthan those of CO2, indicating variable permeability of these films to select gases.This effect can be attributed to a higher solubility of CO2 than O2 in the film matrix(Young 1984; McHugh and Krochta 1994a). Similar results were obtained byArvanitoyannis et al. (1994) while working with potato and rice starch films.Further, the addition of lipid, which is necessary to reduce water vapour permeabil-ity, maintained the selective gas permeability properties of the starch-based films(Table 6.10). Synthetic film materials, such as LDPE, show lower gas permeabilities (2.16 ×10−11 and 9.45×10−11 cm3 m−1 s−1 Pa−1 for O2 and CO2, respectively) than starch-based films. However, LDPE has a relatively low CO2 to O2 permeability ratio(»4), compared to an average ratio of 13 for starch-based films (Cuq et al. 1998;García et al. 1998a, b). Cuq et al. (1995) compared CO2 to O2 permeability ratiosof several synthetic and edible films, and reported that edible films show higherselectivities than synthetic films, with ratios for edible films ranging from 8 to 30.Development of composite edible films and coatings with selective gas permea-bilities could be very promising for controlling respiratory exchange and improvingconservation of fresh or minimally-processed vegetables (Cuq et al. 1998; Garcíaet al. 1998a, b). Table 6.11 shows that the CO2 permeability of starch-based films decreased withincreasing storage time (García et al. 2000a). Gas and vapour permeabilities offilms and coatings depend on several factors such as: (1) ratio of crystalline toamorphous zones, (2) polymeric chain mobility, and (3) specific interactionsbetween the functional groups of the polymers and gases within the amorphouszones. Gaseous permeability measurements of starch stored films correlate with theincrease in the crystallinity reported by DSC and X-ray diffraction (Fig. 6.8–6.10).According to Donhowe and Fennema (1993b), film permeability increases with adecreasing crystalline to amorphous zone ratio, since permeation occurs throughamorphous zones of the film. Table 6.11 Effect of plasticizer and starch type on CO2 permeabilities of starch-based films CO2 permeability [cm3/m sec Pa]a × 109 Starch base Plasticizer (20 g/L) Initial time Stored samplesb Corn _ 29.21 ± 13.89 8.90 ± 1.28 Glycerol 5.69 ± 0.97 2.76 ± 0.55 Sorbitol 4.19 ± 0.81 2.42 ± 0.46 Amylomaize _ 28.05 ± 7.37 7.71 ± 1.40 Glycerol 3.85 ± 1.28 2.28 ± 0.33 Sorbitol 2.96 ± 0.46 1.82 ± 0.15 a At stadard pressure and temperature conditions b Stored 20 days at 20°C and 63.8% relative humidity
194 M.A. García et al.188.8.131.52 Mechanical PropertiesMechanical properties of films and coatings are dependent on additive-matrix inter-actions, and are also strongly affected by physical, chemical and temperature condi-tions, which influence film stability and flexibility. Mechanical performance of a filmis usually characterized by deformation at break (extension at the moment of rupture,mm), percent elongation at break (deformation divided by initial probe length andmultiplying by 100%), tensile strength (force at rupture divided by film cross section,MPa) and elastic modulus (slope of force-deformation curve, N/mm) according to theASTM D882-91 method (1996b). These can be determined using a texturometeror an Instron machine. These parameters are related to the stretching ability of thefilm. It is well known that the environmental conditions during production, storageand usage of these materials affect their mechanical properties. Ageing phenomenaoccurring within the useful lifetime of films also cause great losses to mechanicalproperties, particularly with regards to film elongation. Plasticizers interfere with polymeric chain association facilitating their slippingand, thus, decreasing rigidity of the network, producing a less ordered film struc-ture. In the case of amylomaize films, high values of elastic modulus were obtained(Fig. 6.11). These results were attributed to their high amylose content. Accordingto García and coworkers (2001), the plasticizer-matrix interaction showed similartrends for both corn starch and amylomaize films, though plasticized corn starchfilms were more flexible than those of amylomaize. The combination of lipid andplasticizer addition increased film flexibility, and reduced the effect of starch typeon film mechanical properties. The stress–strain curves for composite films formulated with chitosan (CH) andcorn starch (CS) without plasticizer showed a pattern typical of brittle materials(Sarantopoulos et al. 2002; Mali et al. 2005a, b). This characteristic is more evident 16.00 12.00 Elastic Modulus (N/mm) 8.00 4.00 0.00 WA S G S + SO G + SOFig. 6.11 Tensile properties: elastic modulus of corn (open rectangle) and amylomaize (filleddot) films (WA = without additives; S = with sorbitol; G = with glycerol; S + SO = with sorbitoland sunflower oil and G + SO = with glycerol and sunflower oil)
6 Characterization of Starch and Composite Edible Films and Coatings 195in CH films than in CS films (Fig. 6.12). Blends of chitosan and corn starch did notshow significant differences in film deformation from single component films,although film stress of composite films decreased. These results would indicate thatinteractions between polymeric chains are weaker, reducing rigidity of the matrix,although both hydrocolloids are compatible (García et al. 2006). Plasticized films exhibit the stress-strain behavior of ductile polymers comparedwith unplasticized films (Fig. 6.12). Corn starch films plasticized with glycerol(CS + G) exhibited the most flexible behavior (García et al. 2006). Similar resultswere obtained by Laohakunjit and Noomhorm (2004) and Mali and coworkers(2005b) for cassava starch films plasticized with glycerol or sorbitol. For composite films (CS + CH + G), a lower plasticizing effect of glycerol wasobserved when compared with starch matrices (CS + G). Composite MC–CH filmsalso exhibited different behavior patterns under tensile tests. CH films showed highresistance at break, while MC was more flexible, exhibiting composite films withintermediate percent elongation values (Fig. 6.13) (Pinotti et al. 2007). Similarmechanical properties have been reported in the literature for MC films (Donhoweand Fennema 1993a, b, c; Park et al. 1993, 1994; Debeaufort and Voilley 1997). ForCH films, most literature reported values for tensile tests were higher than thoseobtained by Pinotti et al. (2007). These differences may be due to variations in CHcomposition and/or suppliers and film preparation (Chen and Lin 1994; Butler et al.1996; Caner et al. 1998). Caner et al. (1998) reported a wide range of elongationvalues (14–70%) for CH films, depending on the acid used for chitosan solubilization,plasticizer type, and storage time.Fig. 6.12 Mechanical properties of composite films formulated with 5% corn starch (CS),chitosan (CH), corn starch plasticized with glycerol (CS + G), corn starch and chitosan (CS + CH)and corn starch and chitosan plasticized with glycerol (CS + G + CH)
196 M.A. García et al. For CH–MC composite films, tensile strength and elastic modulus increasedwith an increasing CH concentration (Fig. 6.13b); accordingly, relative deformationdecreased (Fig. 6.13a). The blending of CH with MC enhanced film deformationand increased film flexibility, avoiding the need for plasticizer addition. Withregard to puncture tests, the elastic modulus showed the same trend as in tensiletests (Fig. 6.13b). However, all composite films have a similar values of deforma-tion at break, regardless of CH:MC ratio (Fig. 6.13a). Thus, CH may serve as apartial replacement of MC for generation of composite films with good punctureresistance and economic benefit, since MC is itself an expensive commodity. Table 6.12 compares mechanical properties determined for both biodegradableand synthetic films under identical test conditions. Tensile strength values forFig. 6.13 Mechanical properties of MC, CH and composite films with a different CH:MC ratios(Tensile and puncture tests: (a) elongation at break and (b) elastic modulus)
6 Characterization of Starch and Composite Edible Films and Coatings 197Table 6.12 Comparison of the mechanical properties of corn starch, chitosan and compositefilms with commercial synthetic films Mechanical propertiesFilm type Components Tensile strength (MPa) Elongation at break (%) CSa 47.4 ± 1.5 3.6 ± 0.5Biodegradable CS + G 7.1 ± 0.4 22.5 ± 4.2 CS + CH 24.7 ± 4.0 3.0 ± 0.2 CS + CH + G 28.7 ± 6.8 11.7 ± 4.0 CH 60.7 ± 5.8 3.3 ± 0.4Synthetic Cellophaneb 85.8 ± 8.9 14.4 ± 2.4 LDPEc 16.2 ± 4.0 68.7 ± 14.9 HDPEc 27.8 ± 3.2 150.0 ± 18.5a CS: corn starch at a concentration of 5%b Shellhammer and Krochta (1997)c Smith (1986)composite films were in the range of those for LDPE and HDPE, but were lowerthan that obtained for cellophane. However, synthetic polymers like LDPE andHDPE exhibited much greater values for elongation at break. Similar results werereported for synthetic films by Cunningham et al. (2000).6.5 Film and Coating ApplicationsVarious coating applications reported in literature have utilized vegetable, meat, sea-food and bread dough products among others (Olorunda and Aworth 1984; Drake et al.1987, 1991; Dhalla and Hanson 1988; Avena-Bustillos et al. 1993, 1994; Baldwinet al. 1997; García et al. 1998a, b). Since most coating applications are reported forfruits and vegetables, several specific examples will be highlighted here. The diversearray of fruits and vegetables offers many challenges to coating applications thatinclude adhesion of coating to slippery (e.g., tomatoes, mushrooms), irregular orrough (e.g., strawberries) surfaces. These will require addition of ingredients to for-mulations that will reduce coating solution surface tension to ensure coating uni-formity and absence of void holes. In the case of starch-based coatings, thosecontaining plasticizer have been shown to be homogeneous, and covered the wholesurface of strawberries, including the achenes (García et al. 1998a). On the otherhand, coatings without plasticizer were brittle and possessed undesirable cracks, asrevealed by iodine staining of the film surface (García et al. 1998a). Strategies to extend post-harvest quality of fruits and vegetables need toaddress several key challenges, like extending maturation and senescence peri-ods, minimizing dehydration and reducing the onset and rate of microbialgrowth. Edible films and coatings can offer simultaneous solutions to vegetables,such as Brussels sprouts, tomatoes, cucumbers, and red peppers (El Gaouthet al. 1991a, b; Viña et al. 2007), and for fruits like bananas (Banks 1984),
198 M.A. García et al.apples (Drake et al. 1987), and mangoes (Dhalla and Hanson 1988). Mali andGrossmann (2003) proposed the use of yam starch films as packaging for straw-berries contained within plastic trays, and compared performance of these filmswith that of PVC. Although the PVC film provided better weight and firmnessretention for strawberries, yam starch films could be considered a viable pack-aging alternative.6.5.1 Application of Coatings to Highly Perishable FruitsA good example is application of composite active coatings to extend storage life ofstrawberries, which are highly perishable fruits with only a short period of annualproduction and high susceptibility to fungal infection (El Gaouth et al. 1991a;García et al. 1998a, b, 2001). Cold gelatinization of starch was the chosen alterna-tive to comply with both requirements: (1) the dipping procedure selected for coat-ing application, and (2) the heat sensitive characteristics of strawberries. Formulationsof the tested starch-based coatings are shown in Table 184.108.40.206.2 Microbiological AnalysisSurface microbial growth is the main cause of spoilage for many food products.The microorganisms that grew on strawberries were mainly yeasts, molds andsugar-fermenting bacteria. Figure 6.14 demonstrates need of a composite coating todecrease microbial counts, as the unplasticized coating did not differ significantlyfrom the control in this regard. Coatings containing potassium sorbate, a well-known, effective antifungal agent, significantly decreased (P < 0.05) yeast and moldcounts on coated strawberries. Since the undissociated form of sorbic acid is theactive antimicrobial agent, citric acid was added to the coating formulation toincrease potassium sorbate effectivity. Fig. 6.14 shows that 0.2 g/L potassium sorbateused in conjunction with citric acid was the most effective formulation for decreasingmicrobial counts. Use of active coatings lowers the amount of preservative requiredto achieve the same antimicrobial efficacy as traditional techniques (Guilbert 1986;Guilbert et al. 1997; Vojdani and Torres 1989a, b). Storage life, defined as the time necessary to reach 106 CFU/g fruit, was 14days for uncoated fruit stored at 0°C. Coatings containing sorbitol extended storagelife to 21 days. At the maximum storage time evaluated (28 days), coating formu-lations containing both sorbitol and potassium sorbate still exhibited microbialcounts below the storage life limit of 106 CFU/g of fruit. While addition of potas-sium sorbate improved antimicrobial characteristics of the starch coatings, additionof both citric acid and potassium sorbate further enhanced antimicrobial effec-tiveness, yielding a composite coating with a storage life of more than 28 days(Fig. 6.14).
6 Characterization of Starch and Composite Edible Films and Coatings 199Fig. 6.14 Effect of coating formulation on growth of yeasts and molds (Log CFU/g fruit) instrawberries stored at 0°C and 84%RH (Control: uncoated fruits, (open diamond); composition ofcoating formulation: (open circle) amylomaize without plasticizer; (open square) amylomaize and20 g/L sorbitol; (open up triangle) amylomaize, 20 g/L sorbitol and 0.2 g/L potassium sorbate and(open down triangle) amylomaize, 20 g/L sorbitol, 0.2 g/L potassium sorbate and citric acid; barsindicate standard error)6.5.3 Quality Attributes of StrawberriesAll plasticized coatings effectively reduced strawberry weight loss during storage(Fig. 6.15). Significant differences (P < 0.05) were observed among the weight lossvalues for uncoated strawberries and those coated with common corn or high-amylose corn starch, with lowest weight loss values obtained with amylomaize.Weight losses of fruits coated with starch formulations without plasticizer weresimilar to those of controlled fruit, due to presence of pores and cracks. Coatingswith sorbitol led to significantly lower fruit weight losses than glycerol, regard-less of starch type. However, weight losses were unacceptable after 3 weeks ofstorage for coated fruits without lipid. Addition of sunflower oil was necessary toreduce weight loss and increase storage life, provided that microbial countscould be maintained below the established limit (106 CFU/g fruit) even at 28 daysof storage. The maximum weight loss reduction (63.2%) after 28 days of storagewas obtained for coating formulations that included sunflower oil (Fig. 6.15).Avena-Bustillos et al. (1997), working on apples and celery treated with caseinate
200 M.A. García et al.Fig. 6.15 Effect of coating formulation on weight loss of control and coated strawberries duringstorage at 0°C and 84%RH. (Control: uncoated fruits, (open circle); composition of coating for-mulation: (open square) amylomaize without plasticizer; (open up triangle) amylomaize with 20 g/Lsorbitol and (open diamond) amylomaize with 20 g/L sorbitol and 2 g/L sunflower oil)and acetylated monoglyceride coating, found a 75% increase in resistance to watervapour transfer and consequently, a decrease in weight loss of coated vegetablescompared to uncoated controls. Ultimately, changes in texture and appearance arethe most important factors that determine post-harvest storage life of fruits andvegetables. The rate and extent of firmness loss during ripening of soft fruits likestrawberries is also another factor of primary importance. According to Manning(1993), fruit softening is attributed to degradation of components of the cellwall, primarily pectic substances, due to activity of specific enzymes such aspolygalacturonase. For both control and coated fruits, breaking force decreased asa function of storage time. Coating formulations that minimized weight loss alsomaintained better firmness, since the firmness attribute is highly influenced bywater content. The effect of coatings on surface color modifications of strawberries was ana-lyzed, because this quality attribute may also determine consumer acceptability offruit. Glycerol or sorbitol significantly (P < 0.05) delayed development of surfacecolor, which resulted in a slight change in color lightness with time. Coating for-mulations containing glycerol gave better surface color results compared to thosewith sorbitol. Lipid addition did not significantly modify (P < 0.05) surface colorresults, regardless of the plasticizer used in formulations. Active starch-based coatings containing antimicrobial agents, plasticizer andlipid improved barrier properties to water vapour (Table 6.8), reduced microbialgrowth and showed selective gas permeability (Table 6.10), and thus, extendedstorage life of strawberries. The best coating formulation in our case contained
6 Characterization of Starch and Composite Edible Films and Coatings 201high-amylose starch, sorbitol, sunflower oil and potassium sorbate plus citric acidas antimicrobial agents.6.5.4 Physiological ModificationsPhysiological parameters, including titratable acidity, pH, anthocyanin level andsugar content, are good indicators of fruit maturation and senescence. Coatings maybe used to alter the natural physiological behavior, modifying organoleptic charac-teristics of fruits such as color, taste or flavor. In coated strawberries, these physiological parameters were slowed down, butdid reach commercially acceptable values (García et al. 1998b). These results indicatethat starch-based coatings retard metabolic reactions, and thus, senescence ofcoated fruits is delayed. The oxygen and carbon dioxide barriers lead to a reductionin respiration rate by limiting exposure to ambient oxygen, increasing internalcarbon dioxide, delaying ripening and senescence, and extending the storage life oftreated fruits (Baldwin 1994; Avena-Bustillos et al. 1993, 1994; Drake et al. 1991;García et al. 1998a, b). Another important parameter in fruits is the degree of maturity reached at thetime of application of the coating. For example, when composite starch-basedcoatings were applied on strawberries at 25, 50, 75 and 100% color maturity ripeningstages, 75% was selected as the optimum degree of maturity for prolonging storagelife. In this case, development of appropriate anthocyanin content, reducing andnon-reducing sugar levels and titratable acidity of strawberries were slowed downduring storage, reaching commercially acceptable values at the end of the storageperiod. The delay in development of physiological parameters observed in coatedfruits, regardless of the degree of maturity, was attributed to the differential gaseouspermeability of films and influence on respiratory activity.6.6 Coating Application on Fried FoodsAs mentioned previously, another novel application of coatings is to reduce oiluptake of products during deep-fat frying. Cellulose derivatives, such as methylcellulose (Table 6.2), can be used to decrease oil content of food products duringfrying. Hydrocolloids with thermal gelling or thickening properties, like proteinsand carbohydrates, have been investigated for this purpose. Williams and Mittal(1999a, b) found that methylcellulose (MC) films provided the best oil barrier prop-erties, and reduced fat uptake more than hydroxypropylcellulose and gellan gumfilms in pastry mix applications. Mallikarjunan et al. (1997) stressed that productscoated with cellulose derivatives form a protective layer at the surface of foodproducts during initial stages of frying, due to thermal gelation of the hydrocolloidat temperatures above 60°C. This protective layer limits transfer of moisture and
202 M.A. García et al.fat between the sample and the frying medium. MC formulations that includedsorbitol as plasticizer were applied to dough discs and potato strips to reduce oiluptake during deep fat frying (García et al. 2002, 2004a). Coating application didnot modify textural characteristics or sensory properties of the fried samples. MCcoating formulations were the most effective, reducing oil uptake between 35 and40% depending on the product. To obtain a coating with adequate adherence andintegrity, it is necessary to incorporate a plasticizer, sorbitol being the most effec-tive in the case of MC coatings. SEM micrographs showed good adhesion betweenthe coating and the dough, and no significant differences between coated anduncoated samples were detected by the sensory panel.6.7 Future TrendsThe use of coatings and packaging films by the food industry has become a topicof great interest, because of their potential for increasing shelf life of many foodproducts (Ahvenainen 2003; Coles et al. 2003; Giles and Bain 2001; Hernandezet al. 2000). By selecting the right materials and packaging technologies, it is possibleto maintain product quality and freshness of food products (Brown 1992; Stewartet al. 2002). Nowadays, a large part of materials used in packaging industries isproduced from fossil fuels, which are practically not degradable. Preservation ofnatural resources and recycling has led to a renewed interest in biomaterials andrenewable raw materials. A concerted effort to extend shelf life and to enhancefood quality, while reducing packaging waste, has encouraged exploration of newbio-based packaging materials, such as edible and biodegradable films from renew-able resources (Albertsson and Karlsson 1995; Trznadel 1995; Tharanathan andKittur 2003). However, like conventional packaging, bio-based packaging has tosupply a number of important functions with regards to food applications, includingcontainment and protection, maintenance of sensory quality and safety, and labe-ling (Robertson 1993). Polar biopolymers, such as polysaccharides and proteins, are being studied asprospective replacements for synthetic polymers in the film and plastic industries.Their potential benefits are both environmental and cost-related. Traditional tech-niques for processing thermoplastic synthetic polymers have been adapted tohydrophilic polymers like starch and gelatin. To date, use of biodegradable films for food packaging has been strongly limitedbecause of the poor barrier properties and weak mechanical properties shown bynatural polymers. For this reason, natural polymers are frequently blended withother synthetic polymers or, less frequently, chemically modified with the aim ofextending their applications (Guilbert et al. 1997; Petersen et al. 1999). Recentadvances in genetic engineering and composite science offer significant opportuni-ties for improving materials from renewable resources with enhanced support ofglobal sustainability, although use of materials obtained by genetic modification isstill controversial.
6 Characterization of Starch and Composite Edible Films and Coatings 203 For scientists, the real challenge lies in finding applications that wouldconsume sufficiently large quantities of these materials to reduce their cost,allowing biodegradable polymers to compete economically in the market. Starchand its derivates are promising raw materials, because they are renewable, widelyavailable and relatively low cost (Gonera and Cornillon 2002; Smits et al. 1998).As a packaging material, starch alone does not form films with appropriatemechanical properties, unless it is first plasticized or chemically modified.When starch is treated in an extruder by application of both thermal andmechanical energy, it can be converted to a thermoplastic material. In produc-tion of thermoplastic starches, plasticizers are expected to efficiently reduceintra-molecular hydrogen bonds and to provide stability to product properties.There are many opportunities for using starch as packaging materials (Kim andPometto 1994). As described previously, starch can be employed as packagingfor fruits, vegetables, snacks, or other dry products. For example, Novamont,an Italian company, commercializes EverCornTM, a starch-based material avail-able as films or bags. Similarly, Bioenvelope, a Japanese company commercial-izes Bio-PTM, another starch-based film. In these applications, however, efficientmechanical, oxygen and moisture protection is needed, as thermoplastic starchalone cannot meet all these requirements. Because of the hydrophilicity of thestarch, performance changes during and after processing, due to water contentchanges. To overcome this drawback, many different routes have been reported.Some biodegradable materials like Mater-BiTM, produced by Novamont, areavailable in the market, which is based on 60% starch and 40% alcohol. This ismainly commercialized in Europe and America. Today’s excellent performance of traditional plastics is an outcome of continuedR&D efforts of the last several years. However, existing biodegradable polymershave come to public view only recently. Prices of biodegradable biopolymers canbe realized through continued research and development efforts focused on opti-mizing composition and functionality to improve performance of edible films andcoatings.Acknowledgments The financial support provided by CONICET (Consejo Nacional deInvestigaciones Científicas y Técnicas), Agencia Nacional de Promoción Científica y Tecnológicaand Universidad Nacional de La Plata is gratefully acknowledged.ReferencesAhvenainen R (2003) Novel food packaging techniques. Boca Raton, FL: CRC Press LLCAlbertsson AC, Karlsson S (1995) Degradable polymers for the future. Acta Polymers, 46, 114–123Arvanitoyannis I, Kalichevsky M, Blanshard JMV, Psomiadou E (1994) Study of diffusion and permeation of gases in undrawn and uniaxially drawn films made from potato and rice starch conditioned at different relative humidities. Carbohydr. Polym. 24, 1–15ASTM (1996a) Standard test methods for water vapour transmission of material, E96 – 95. Annual book of ASTM. Philadelphia, PA: American Society for Testing and Materials
204 M.A. García et al.ASTM (1996b) Standard test methods for tensile properties of thin plastic sheeting, D882-91. Annual Book of ASTM. Philadelphia, PA: American Society for Testing and MaterialsAvena-Bustillos RJ, Cisneros-Zeballos LA, Krochta JM, Saltveit ME (1993) Optimization of edible coatings on minimally processed carrots using response surface methodology. Am. Soc. Agric. Eng. , 36 3, 801–805Avena-Bustillos RJ, Krochta JM, Saltveit ME, Rojas-Villegas RJ, Sauceda-Pérez JA (1994) Optimization of edible coating formulations on Zucchini to reduce water loss. J. Food Eng. 21, 197–214Avena-Bustillos RJ, Krochta JM, Saltveit ME (1997) Water vapour resistance of red delicious apples and celery sticks coated with edible caseinate-acetylated mono-glyceride films. J. Food Sci. 62, 2, 351–354Avena-Bustillos RJ, Olsen CW, Olson DA, Chiou B, Yee E, Bechtel PJ, McHugh TH (2006) Water vapour permeability of mammalian and fish gelatin films. J. Food Sci. 71, 4, 202–207Bader HG, Göritz D (1994a) Investigations on high amylose corn starch films. Part 1: wide angle X-ray scattering (WAXS). Starch/Stärke 46, 6, 229–232Bader HG, Göritz D (1994b) Investigations on high amylose corn starch films. Part 2: water vapour sorption. Starch/Stärke 46, 7, 249–252Bader HG, Göritz D (1994c) Investigations on high amylose corn starch films. Part 3: stress strain behaviour. Starch/Stärke 46, 11, 435–439Baker RA, Baldwin EA, Nisperos-Carriedo MO (1994) Edible coatings for processed foods. In: Krochta JM, Baldwin EA, Nisperos-Carriedo M (Eds.) Edible Coatings and Films to Improve Food Quality. Technomic Pub. Co., Lancaster, PA, pp. 89–104Baldwin EA (1994) Edible coatings for fruits and vegetables, past, present and future. In: Krochta JM, Baldwin EA, Nisperos-Carriedo MO (Eds.) Edible Coatings and Films to Improve Food Quality. Technomic Pub. Co., Lancaster, PA, pp. 25–64Baldwin EA, Nisperos-Carriedo MO, Hagenmaier RD, Baker RA (1997) Use of lipids in coatings for food products. Food Technol. 51, 6, 56–64Banker GS (1966) Film coating, theory and practice. J. Pharm. Sci. 55, 81Banks NH (1984) Some effects of TAL Pro-Long coatings on ripening bananas. J. Exp. Bot. 35, 127Brown WE (1992) Plastics in Food Packaging. Properties, Design, and Fabrication. New York, NY: Marcel DekkerButler B, Vergano R, Testin R, Bunn J, Wiles J (1996) Mechanical and barrier properties of edible chitosan films as affected by composition and storage. J. Food Sci. 61, 5, 953–961Caner C, Vergano P, Wiles J (1998) Chitosan film mechanical and permeation properties as affected by acid, plasticizer, and storage. J. Food Sci. 63, 6, 1049–1053Chang BS, Randall CS (1992) Use of subambient thermal analysis of optimize protein lyophilization. Cryobiology 29, 632–656Chang YP, Cheah PB, Seow CC (2000) Plasticizing – antiplasticizing effects of water on physical properties of tapioca starch films in the glassy state. J. Food Sci. 65, 3, 445–451Chen RH, Lin JH (1994) Relationships between the chain flexibilities of chitosan molecules and the physical properties of their casted films. Carbohydr. Polym. 24, 41–46Chen M, Yeh H, Chiang B (1996) Antimicrobial and physicochemical properties of methylcellulose and chitosan films containing a preservative. J. Food Process Preserv. 20, 379–390Chen M, Deng J, Yang F, Gong Y, Zhao N, Zhang X (2003) Study on physical properties and nerve cell affinity of composite films from chitosan and gelatin solutions. Biomaterials 24, 2871–2880Cherian G, Gennadios A, Weller C, Chinachoti P (1995) Thermomechanical behavior of gluten films; effect of sucrose, glycerin and sorbitol. Cereal Chem. 72, 1, 1–6Coles R, McDowell D, Kirwan MJ (2003) Food packaging technology. Oxford, UK: Blackwell Publishing LtdCunningham P, Ogale A, Dawson P, Acton J (2000) Tensile properties of soy protein isolate films produced by a thermal compaction technique. J. Food Sci. 65, 4, 668–671
6 Characterization of Starch and Composite Edible Films and Coatings 205Cuppet SL (1994) Edible coatings as carriers of food additives, fungicides and naturals antagonists. In: Krochta JM, Baldwin EA, Nisperos-Carriedo M (Eds.) Edible Coatings and Films to Improve Food Quality. Technomic Pub. Co., Lancaster, PA, pp. 121–137Cuq B, Gontard N, Guilbert S (1995) Edible films and coatings as active layers. In: Rooney ML (Ed.) Active Food Packaging. Chapman & Hall, UK, pp. 111–142Cuq B, Gontard N, Guilbert S (1998) Proteins as agricultural polymers for packaging production. Cereal Chem. 75, 1, 1–9Dhalla R, Hanson SW (1988) Effect of permeability coatings on the storage life of fruits. II. Pro-long treatments of mangoes (Mangifera indica L. cv. Julie). Int. J. Food Sci. Technol. 23, 107–112Debeaufort F, Voilley A (1997) Methylcellulose-based edible films and coatings: 2. Mechanical and thermal properties as a function of plasticizer content. J. Agric. Food Chem. 45, 685–689Donhowe IG, Fennema OR (1993a) Water vapour and oxygen permeability of wax films. J. Am. Oil Chem. Soc. 70 (9), 867–873Donhowe IG, Fennema O (1993b) The effects of solution composition and drying temperature on crystallinity, permeability and mechanical properties of methylcellulose films. J. Food Process Preserv. 17, 231–246Donhowe IG, Fennema O (1993c) The effects of plasticizers on crystallinity, permeability and mechanical properties of methylcellulose films. J. Food Process Preserv. 17, 247–258Donhowe IG, Fennema OR (1994) Edible films and coatings: characteristics, formation, defini- tions and testing methods. In: Krochta JM, Baldwin EA, Nisperos-Carriedo M (Eds.) Edible Coatings and Films to Improve Food Quality, Technomic Pub. Co., Lancaster, PA, pp. 1–21Drake SR, Fellman JK, Nelson JW (1987) Post-harvest use of sucrose polyesters for extending the shelf-life of stored Golden Delicious apples. J. Food Sci. 52, 5, 1283–1285Drake SR, Nelson JW (1990) Storage quality of waxed and nonwaxed “Delicious” and “Golden Delicious” apples. J. Food Qual. 13, 331–334Drake SR, Cavalieri R, Kupferman EM (1991) Quality attributes of “D’Anjou pears after different wax drying and refrigerated storage. J. Food Qual. 14, 455–465El Gaouth A, Arul J, Ponnampalam R, Boulet M (1991a) Chitosan coating effect on storability and quality of fresh strawberry. J. Food Sci. 56, 6, 1618–1620El Gaouth A, Arul J, Ponnampalam R, Boulet M (1991b) Use of chitosan coating to reduce water loss and maintain quality of cucumber and bell pepper fruits. J. Food Process Preserv. 15, 339–368Even WR, Carr SH (1978) Micromechanical fracture analysis of amylose. Polymer 19, 583–588Galietta G, Giola DD, Guilbert S, Cuq B (1998) Mechanical and thermomechanical properties of films based on whey protein as affect by plasticizer and crosslinking agents. J. Dairy Sci. 81, 3123–3130García MA, Martino MN, Zaritzky NE (1998a) Starch-based coatings: effect on refrigerated strawberry (Fragaria × Ananassa) quality. J. Sci. Food Agric. 76, 411–420García MA, Martino MN, Zaritzky NE (1998b) Plasticizer effect on starch-based coatings applied to strawberries (Fragaria × Ananassa). J. Agric. Food Chem. 46, 3758–3767García MA, Martino MN, Zaritzky NE (1999) Edible starch films and coatings characterization: sem, water vapour and gas permeabilities. J. Scanning Microsc. 21, 5, 348–353 García MA, Martino MN, Zaritzky NE (2000a) Microstructural characterization of plasticized starch-based films. Starch/ Stärke 52, 4, 118–124García MA, Martino MN, Zaritzky NE (2000b) Lipid addition to improve barrier properties of edible starch-based films and coatings. J. Food Sci. 65, 6, 941–947García MA , Martino MN, Zaritzky NE (2001) Composite starch-based coatings applied to straw- berries (Fragaria × ananassa). Nahrung/Food 45, 4, 267–272García MA, Ferrero C, Bértola N, Martino MN, Zaritzky NE (2002) Edible coatings from cellu- lose derivatives to reduce oil uptake in fried products. Innov. Food Sci. Emerg. Technol. 3–4, 391–397García MA, Ferrero C, Campana A, Bértola N, Martino M, Zaritzky N (2004a). Methylcellulose coatings reduce oil uptake in fried products. Food Sci. Technol. Int. 10, 5, 339–346
206 M.A. García et al.García MA, Martino MN, Zaritzky NE (2004b) Research advances in edible coatings and films from starch. In: Mohan RM (Ed.) Research Advances In Food Science. Global Research Network. Research Advances in Food Science 4, 107–128García MA, Pinotti A, Martino MN, Zaritzky NE (2004c) Characterization of composite hydro- colloid films. Carbohydr. Polym. 56, 3, 339–345García MA, Pinotti A, Zaritzky NE (2006) Physicochemical, water vapour barrier and mechanical properties of corn starch and chitosan composite films. Starch/Starke 58, 9, 453–463Gennadios A, Weller CL, Gooding CH (1994) Measurement errors in water vapour permeability of highly permeable, hydrophilic edible films. J. Food Eng. 21, 395–409Ghanbarzadeh B, Musavi M, Oromiehie AR, Rezayi K, Razmi E, Milani J (2007) Effect of plas- ticizing sugars on water vapour permeability, surface energy and microstructure properties of zein films. LWT 40, 1191–1197Giles GA, Bain DA (2001) Technology of Plastics Packaging for the Consumer Market. Boca Raton, FL: CRC Press LLCGonera A, Cornillon P (2002) Gelatinization of starch/gum/sugar system studied by using DSC, NMR and CSLM. Starch/Sta¨rke, 54, 508–516Gontard N, Guilbert S, Cuq B (1992) Edible wheat gluten films: influence of the main process variables on film properties using response surface methodology. J. Food Sci. 57, 1, 190–199Gontard N, Guilbert S, Cuq JL (1993) Water and glycerol as plasticizers affect mechanical and water vapour barrier properties of an edible wheat gluten film. J. Food Sci. 58, 1, 206–211Gontard N, Duchez C, Cuq JL, Guilbert S (1994) Edible composite films of wheat gluten and lipids: water vapour permeability and other physical properties. Int. J. Food Sci. Technol. 19: 39–50Greener IK, Fennema OR (1989) Evaluation of edible, bilayer films for use as moisture barriers for foods. J. Food Sci. 54, 1400–1406Guilbert S (1986) Technology and application of edible protective films. In: Mathlouthi M (Ed.) Food Packaging and Preservation. Theory and Practice. Elsevier Applied Science Publishing Co. London, UK, pp. 371–394Guilbert S, Gontard N (1995) Technology and applications of edible protective films. In: VII Biotechnology and Food Research – “New Shelf-Life Technologies and Safety Assessments”. Helsink, Finland, pp. 49–60Guilbert S, Cuq B, Gontard N (1997) Recent innovations in edible and/or biodegradable packag- ing materials. Food Addit. Contam. 14, 6, 741–751Hagenmaier RD, Baker RA (1994) Wax microemulsions and emulsions as citrus coatings. J. Agric. Food Chem. 42, 899–902.Hardenburg RE (1967) Wax and related coatings for horticultural products – a bibliography. Agric. Res. Serv. Bull. 965. Cornell University, Ithaca, NYHernandez E (1994) Edible coatings for lipids and resins. In: Krochta JM, Baldwin EA, Nisperos- Carriedo M (Eds.) Edible Coatings and Films to Improve Food Quality. Technomic Pub. Co., Lancaster, PA, pp. 279–304Hernandez R, Selke SEM, Cultler J (2000) Plastics Packaging: Properties, Processing, Applications, Regulations. Munich, Germany: Hanser Gardner PublicationsHershko V, Nussinovitch A (1998) Relationship between hydrocolloid coating and mushroom structure. J. Agric. Food Chem. 46, 8, 2988–2997Iijimaa M, Nakamura K, Hatakeyama T, Hatakeyamab H (2000) Phase transition of pectin with sorbed water. Carbohydr. Polym. 41, 101–106Kester JJ, Fennema OR (1986) Edible films and coatings: a review. Food Technol. 12, 47–59Kim M, Pometto III OR (1994) Food packaging potential of some novel degradable starchepoly- ethylene plastics. J. Food Prot., 57, 1007–1012Klug HP, Alexander LE (1974) Crystallite size and lattice strains from line broadening. In: X-ray Diffraction Procedures for Polycrystalline and Amorphous Materials. New York, USA: Wiley- Intersciences, pp. 618–708Köksel H, ahbaz F Özboy Ö (1983) Influence of wheat-drying temperatures on the birefringence and X-ray diffraction patterns of wet-harvested wheat starch. Cereal Chem. 70, 4, 481–483
6 Characterization of Starch and Composite Edible Films and Coatings 207Krochta JM, De Mulder-Johnson C (1997) Edible and biodegradable polymer films: challenges and opportunities. Food Technol. 51, 2, 61–77Kumar MNVR (2000) A review of chitin and chitosan applications. React Funct. Polym. 46, 1–27Laohakunjit N, Noomhorm A (2004) Effect of plasticizers on mechanical properties of rice starch film. Starch/Stärke 5, 8, 348–356Mali S, Grossmann MVE (2003) Effects of yam starch films on storability and quality of fresh strawberries (Fragaria ananassa). J. Agric. Food Chem. 51, 24, 7005–7011Mali S, Grossmann MV, García MA, Martino MN, Zaritzky NE (2002) Microstructural charac- terization of yam starch films. Carbohydr. Polym. 50, 4, 379–386Mali S, Grossmann MV, García MA, Martino M, Zaritzky N (2005a) Mechanical and thermal properties of yam starch films. Food Hydrocol. 19, 157–164Mali S, Sakanaka LS, Yamashita F, Grossmann MVE (2005b) Water sorption and mechanical properties of cassava starch films and their relation to plasticizing effect. Carbohydr. Polym. 60, 283–289Mallikarjunan P, Chinnan MS, Balasubramaniam VM, Phillips RD (1997) Edible coatings for deep-fat frying of starchy products. LWT 30, 709–714Manning K (1993) Soft fruits. In: Seymour GB, Taylor JE, Tucker GA (Eds.) Biochemistry of Fruit Ripenning. Chapman & Hall, London, pp. 347–373McHugh TH, Krochta JM (1994a) Milk-protein-based edible films and coatings. Food Technol. 48, 1, 97–103McHugh TH, Krochta JM (1994b) Sorbitol- vs glycerol- plasticized whey protein edible films: integrated oxygen permeability and tensile property evaluation. J. Agric. Food Chem. 42, 4, 841–845.McHugh TH, Krochta JM (1994c) Permeability properties of edible films. In: Krochta JM, Baldwin EA, Nisperos-Carriedo M (Eds.) Edible Coatings and Films to Improve Food Quality. Technomic Pub. Co., Lancaster, PA, pp 139–187McHugh TH, Aujard JF, Krochta JM (1994) Plasticized whey protein edible films: water vapour permeability properties. J. Food Sci. 59, 2, 416–419Miles MJ, Morris VJ, Ring SG (1985a) Gelation of amylose. Carbohydr. Res. 135, 257–269Miles MJ, Morris VJ, Orford PD, Ring SG (1985b) The roles of amylose and amylopectin in the gelation and retrogradation of starch. Carbohydr. Res. 135, 271–281Muzzarelli R, Baldassarre V, Conti F, Ferrara P, Biagini G, Gazzanelli G, Vasi V (1988) Biological activity of chitosan: ultrastructural study. Biomaterials 9, 3, 247–252Neto CGT, Giacomettib JA, Jobb AE, Ferreirab FC, Fonsecaa JLC, Pereiraa MR (2005) Thermal analysis of chitosan based networks. Carbohydr. Polym. 62, 97–103Nisperos-Carriedo MO (1994) Edible coatings and films based on polysaccharides. In: Krochta JM, Baldwin EA, Nisperos-Carriedo MO (Eds.) Edible Coatings and Films to Improve Food Quality. Technomic Pub. Co., Lancaster, PA, pp. 305–330Noel TR, Ring SG, Whittman MA (1992) The structure and gelatinization of starch [Review]. Food Sci. Technol. Today, 6, 159Oh JH, Wang B, Field PD, Aglan HA (2004) Characteristics of edible films made from dairy proteins and zein hydrolysate cross-linked with transglutaminase. Int. J. Food Sci. Technol. 39, 1–8Olorunda AO, Aworh OC (1984) Effects of Pro-long, a surface coating agent, on the shelf-life and quality attributes of plantain. J. Sci. Food Agric. 35, 573–578Park H, Weller C, Vergano P, Testin R (1993) Permeability and mechanical properties of cellulose- based edible films. J. Food Sci. 58, 6, 1361–1364, 1370Park HJ, Bunn JM, Weller CL, Vergano PJ, Testin RF (1994) Water vapour permeability and mechanical properties of grain protein-based films as affected by mixtures of polyethylene glycol and glycerin plasticizers. Trans ASAE 37, 4, 1281–1285Parra DF, Tadini CC, Ponce P, Lugão AB (2004) Mechanical properties and water vapour trans- mission in some blends of cassava starch edible films. Carbohydr. Polym. 58, 475–481Parris N, Coffin DR, Joubran RF, Pessen H (1995) Composition factors affecting the water vapour permeability and tensile properties of hydrophilic films. J. Agric. Food Chem. 43, 1432–1435
208 M.A. García et al.Paull RE, Chen NJ (1989) Waxing and plastic wraps influence water loss from papaya fruit during storage and ripening. J. Am. Soc. Hortic. Sci. 114, 937–942Pawlak A, Mucha M (2003) Thermogravimetric and FTIR studies of chitosan blends. Thermochimica Acta, 396, 153–166Petersen K, Nielsen PV, Bertelsen G, Lawther M, Olsen MB, Nilssonk NH (1999) Potential of biobased materials for food packaging. Trends Food Sci. Technol. 10, 52–68Pinotti A, García MA, Martino MN, Zaritzky NE (2007) Study on microstructure and physical properties of composite films based on chitosan and methylcellulose. Food Hydrocol. 21, 1, 66–72Pommet M, Redl A, Guilbert S, Morel MH (2005) Intrinsic influence of various plasticizers on functional properties and reactivity of wheat gluten thermoplastic materials. J. Cereal Sci. 42, 81–91Robertson GL (1993) Food Packaging. Principles and Practice. New York, NY: Marcel DekkerRomero-Bastida CA, Bello-Pérez LA, García MA, Martino MN, Solorza-Feria J, Zaritzky NE (2005) Mechanical and microstructural characterization of films prepared by thermal or cold gelatinization of non-conventional starches. Carbohydr. Polym. 60, 2, 235–244Roos YH (1995) Phase Transitions in Foods. Taylor, S.L. Academic Press San Diego, CA, USASarantopoulos C, de Oliveira M, Padula Coltro L, Vercelino Alves RM, Correa García E (2002) Embalagens Plásticas Flexíveis. Centro de Tecnología de Embalagem. Campinas, BrasilShellhammer TH, Krochta JM (1997) Whey protein emulsion film performance as affected by lipid type amount. J. Food Sci. 62, 2, 390–394Sionkowska A, Wisniewski J, Skopinska J, Kennedy CJ, Wess TJ (2004) Molecular interactions in collagen and chitosan blends. Biomaterials, 25, 795–801Smith SA (1986) Polyethylene, low density. In: Bakker M. (Ed.) The Wiley Encyclopedia of Packaging Technology. John Wiley & Sons, New York, pp. 514–523Smith JP, Hoshino J, Abe Y (1995) Interactive packaging involving sachet technology. In: Rooney ML (Ed.) Active Food Packaging. Blackie Academic and Professional, Glasgow, pp. 143–173Smits ALM, Ruhnau FC, Vliegenthart JFG (1998) Ageing of starch based systems as observed by FT-IR and solid state NMR spectroscopy. Starch/Starke, 50, 11–12, 478–483Snyder RL, Bish DL (1989) Quantitative analysis. In: Bish DL, Post JE (Eds.) Modern Powder Diffraction. Mineralogical Society of America, Washington, DC, pp. 101–144Sobral PJA, Menegalli FC, Hubinger MD, Roques MA (2001) Mechanical, water vapour barrier and thermal properties of gelatin based edible films. Food Hydrocol. 15, 423–432Sohail SS, Wang B, Biswas MAS, Oh JH (2006) Physical, morphological, and barrier properties of edible casein films with wax applications. J. Food Sci. 71, 4, 255–259Spiess WEL, Wolf WR (1993) The results of the COST 90 project on water activity. In: Jowitt R, Escher F, Hallstrom FB, Meffert MF, Spiess WEL, Vos G (Eds.) Physical Properties of Foods. Applied Science Publishers, London, pp. 65–91Stepto RFT, Tomka I (1987) Injection moulding of natural hydrophilic polymers in the presence of water. Chimia 41, 3, 76–81Stewart CM, Tompkin RB, Cole MB (2002) Food safety: new concepts for the new millennium. Innov. Food Sci. Emerg. Technol. 3, 105–112Tharanathan NR, Kittur SF (2003) Chitin-the undisputed biomolecule of great potential. Crit. Rev. Food Sci. 43, 61–83Trezza TA Krochta JM (2000a) The gloss of edible coatings as affected by surfactants, lipids, relative humidity and time. J. Food Sci. 65, 4, 658–662Trezza TA, Krochta JM (200b) Color stability of edible coatings during prolonged storage. J. Food Sci. 65, 7, 1166–1169Trznadel M (1995) Biodegradable polymer materials. Int. Polym. Sci. Technol. 22, 12, 58–65Van Soest JJG, Vliegenthart JFG (1997) Crystallinity in starch plastics: consequences for material properties. Trends Biotechnol. 15, 208–213Van Soest JJG, Hulleman SHD, de Wit D, Vliegenthart JFG (1996) Crystallinity in starch bioplastics. Ind. Crops Prod. 5, 11–22
6 Characterization of Starch and Composite Edible Films and Coatings 209Vermeiren L, Devlieghere F, van Beest M, de Kruijf N, Debevere J (1999) Developments in the active packaging of foods. Trends Food Sci. Technol. 10, 77–86Viña SZ, Mugridge A, García MA, Ferreyra RM, Martino MN, Chaves AR, Zaritzky NE (2007) Quality of refrigerated Brussels sprouts. Effect of plastic packaging film and edible starch coatings. Food Chem. 103, 701–709Vojdani F, Torres JA (1989a) Potassium sorbate permeability of methylcellulose and hydroxypro- pylmethylcellulose multi-layer films. J. Food Process. Preserv. 13, 417–430Vojdani F, Torres JA (1989b) Potassium sorbate permeability of polysaccharide films: chitosan, methylcellulose and hydroxypro-pylmethylcellulose. J. Food Process. Eng. 12, 33–48Vojdani F, Torres JA (1990) Potassium sorbate permeability of methylcellulose and hydroxypro- pylmethylcellulose coatings: effect of fatty acids. J. Food Sci. 55, 3, 841–846Wanchoo RK, Sharma PK (2003) Viscometric study on the compatibility of some water-soluble polymer-polymer mixtures. Eur. Polym. J. 39, 1481–1490Were L, Hettiarachachy NS, Coleman M (1999) Properties of cysteine-added soy protein-wheat gluten films. J. Food Sci. 64, 3, 514–518Williams R, Mittal GS (1999a) Water and fat transfer properties of polysaccharide films on fried pastry mix. LWT, 32, 440–445Williams R, Mittal GS (1999b) Low-fat fried foods with edible coatings: modeling and simula- tion. J. Food Sci. 64(2), 317–322Wong DWS, Gastineau FA, Gregorski KS, Tillin SJ, Pavlath AE (1992) Chitosan-lipids films: microstructure and surface energy. J. Agric. Food Chem. 40, 540–544Wu T, Zivanovic S, Draughon FA Conway WS, Sams CE (2005) Physicochemical properties and bioactivity of fungal chitin and chitosan. J. Agric. Food Chem. 53, 3888–3894Young AH (1984) Fractionation of Starch. In: Whistler RL, Be Miller JN, Paschall EF (Eds.) Starch, Chemistry and Technology, 2nd edn. Academic Press, Orlando, FL, USA, pp. 249–283Zaccaron C, Oliveira R, Guiotoku M, Pires A, Soldi V (2005). Blends of hydroxypropyl methyl- cellulose and poly(1-vinylpyrrolidone-co-vinyl acetate): miscibility and thermal stability. Polym. Degrad. Stab. 90, 1, 21–27
212 G.I. Olivas and G. Barbosa-Cánovaschanges in chemical and physical states due to synthetic and degradative biochemicalprocesses. Nutritional, flavor, textural, and pigmentation changes can all affect qualityof produce (Kays and Paull 2004). Maintaining quality of fruits and vegetables becomes even more difficult whenproduce has been minimally processed. Thus, fresh-cut or minimally-processedfruits and vegetables have become very important issues among food scientists andtechnologists in recent years. Initially, fresh cut produce was only offered to restaurantsor supplied to the food service industry, where commodities were then sold toconsumers within a short time; thus, there was no need to maintain quality of foodfor long periods. Now fresh cut fruits and vegetables have expanded to supermarketsin response to consumer demand. As with intact fresh produce, consumers likewise expect minimally processedfood commodities to be nutritious, attractive, and ready-to-eat, as well as to exhibithigh quality and long shelf life, with no differences in flavor and texture from theoriginal counterpart. These expectations are difficult to meet, since minimallyprocessed commodities undergo rapid deterioration, wherein increased respirationrate and ethylene production, and consumption of sugars, lipids and organic acidsaccelerate ripening process. These changes cause senescence and, thus loss oftexture and water, as well as undesirable changes in flavor and color (Kays 1991). Use of edible films and coatings has been studied as a good alternative for preser-vation of intact and fresh-cut fruits and vegetables, since such films can create semi-permeable barriers to gases and water vapor, maintaining quality of the product.Edible films and coatings have also been studied as potential carriers of additives tohelp preserve, or even improve quality of produce. Application of edible coatingsconsists of applying a thin layer of edible material to the food’s surface, while gen-eration of edible films involves casting a film of edible material to cover the com-modity. However, in studies on edible films and coatings, the two terms are generallyconsidered the same, and results are often reported interchangeably (Gordon 2005). Overall, the purpose of using edible films and coatings for fruits and vegetablesis to retard transfer of gas, vapor and volatiles, thus providing food with a modifiedatmosphere that decreases respiration and senescence, reduces aroma loss, retainsmoisture and delays color changes throughout storage.7.2 Postharvest PhysiologySince fruits and vegetables consist of living tissue, subsequent physiological andbiochemical changes which cause detrimental changes in quality and shelf life ofproduce are common after harvesting. Respiration, transpiration and ethyleneproduction are main factors contributing to deterioration of fruits and vegetables(DeEll et al. 2003). After harvest fresh, produce can also experience biotic andabiotic stresses, which can modify their characteristics prior to consumption. Extentto which quality and shelf life of produce is actually affected will also depend onfactors, such as cultivar, variety and stage of maturity.
7 Edible Flims and Coatings for Fruits and Vegetables 2137.2.1 Postharvest Physiology of Intact Fruits and Vegetables220.127.116.11 Ethylene ProductionEthylene is a hormone produced when vegetable or fruit undergoes stress. Ethylenetriggers ripening and senescence, and is partially responsible for changes in flavor,color and texture of fruits and vegetables (Kays and Paull 2004). On the other hand,removal of ethylene will slow ripening and senescence. Controlled atmosphere(CA) or modified atmosphere (MA) storage of produce can reduce ethyleneproduction/action, preserving quality of fruits and vegetables for longer periods.18.104.22.168 Water LossOne important factor, which is necessary to preserve quality of fruits and vegetables,is avoidance of water loss. Moisture is lost during transpiration when water is convertedfrom liquid to gas. Before harvest, the fruit or vegetable preserves the amount ofwater stored inside by replacing or taking back water lost (due to transpiration)through roots. When produce is harvested, it loses its source of water, so recuperationfrom water loss is not possible. When water is lost, turgor of produce decreases, asdoes firmness. Water stress also causes metabolic alterations changes in enzymeactivation causing accelerated senescence, reduced flavor and aroma, decline innutritional value, and increased susceptibility to chilling injury and pathogen invasion.Maximum acceptable water loss allowed before the commodity is consideredunmarketable varies; apples and oranges can tolerate 5% water loss, while celeryand cabbage can tolerate 10% (Kays and Paull 2004).22.214.171.124 RespirationEnzymatic reactions occur in fruits and vegetables during respiration where oxygenis consumed, carbon dioxide is produced, and heat and energy are released. Respirationis required to keep produce alive and to support any developmental changes.Respiration rate itself is influenced by temperature, humidity and gas composition.When oxygen composition is lowered, respiration decreases and hence, senescencedoes as well. However when oxygen concentration falls below threshold levelanaerobic respiration occurs, which in turn causes ethanol production, off-flavorformation and loss of harvested produce (Kays and Paull 2004).7.2.2 Postharvest Physiology of Minimally Processed Fruits and VegetablesProblems mentioned above increase with partial or total loss of skin in minimallyprocessed fruits and vegetables. Skin protects produce against water loss and pathogen
214 G.I. Olivas and G. Barbosa-Cánovasinvasion and provides partial barrier to gases. Slicing, chopping, and peeling, etc.,of fruits and vegetables can cause injury not only to cells immediately exposed bythe action, but also to unexposed cells deep within the tissue, increasing extent ofdamage (Saltveit 1997).126.96.36.199 Ethylene ProductionGenerally, there is noticeable increase in ethylene production when produce tissueis wounded, inducing deep physiological changes such as ripening in climactericfruits (Abeles et al. 1992). For example, in green tissues, ethylene triggers chloro-phyll degradation, whereas in carrots, high concentration of ethylene triggersincrease in phenolics and isocumarin, giving a bitter taste to the vegetable (Poenickeet al. 1977; Sarkar and Phan 1979). Rate of ethylene production experiencedin minimally-processed fruits and vegetables will depend on produce type andmaturity stage at which it is cut (Toivonen and DeEll 2002). For instance, infresh kiwifruit, tomatoes and strawberries, all three undergo increase in ethyleneproduction when cut (Watada et al. 1990), whereas pears do not (Gorny et al. 2000;Rosen and Kader 1989).188.8.131.52 Water LossCutting, slicing, and peeling, etc., of fruits and vegetables, will increase watertranspiration rate due to exposure of tissue following removal of natural epidermallayer, and will also increase surface area of exposure (Toivonen and DeEll 2002).Water loss through transpiration cannot be replaced and is problematic, since loss ofsmall amounts of water will severely impact produce quality. With water loss, turgorof produce drops, as well as turgidity and firmness. As mentioned, water stress alsocauses metabolic alterations, changes in enzyme activation, causing acceleratedrate of senescence, reduced flavor and aroma, decreased nutritional value, andincreased susceptibility to chilling injury and pathogen invasion (Sams 1999).184.108.40.206 RespirationWounding of fruits and vegetables also causes increase in respiration, therebyincreasing production of carbon dioxide and consumption of oxygen, further causingdecrease in stored reserves. This increase will also depend on commodity type,storage temperature and degree of wounding (Ahvenainen 1996). For instance, slic-ing a mature green tomato can increase respiration up to 40% at 8ºC, comparedwith intact fruit (Mencarelli et al. 1989). However minimally-processed apples donot show increased respiration (Lakakul et al. 1999). When minimally-processedproduce is packaged under modified atmosphere with very low oxygen concentration,anaerobic respiration will occur, with consequent formation of off-flavors, ethanol,
7 Edible Flims and Coatings for Fruits and Vegetables 215ketones and aldehydes. Increase in respiration depends on the commodity, as somefruits and vegetables do not show increase in these compounds (e.g., bananas), whileothers such as tomatoes do (Toivonen and DeEll 2002; Mencarelli et al. 1989).220.127.116.11 BrowningEnzymatic browning is one of the main problems encountered in maintaining qualityof fresh-cut fruits and vegetables. When a fruit or vegetable is cut, reaction occursthat is catalyzed by the enzyme polyphenol oxidase, wherein phenolic compoundsreact with atmosphere oxygen in the presence of copper, causing formation of darkcompounds (Ahvenainen 1996). Enzymatic browning is the main problem occurringin fruits such as apples, pears, bananas and peaches, as well as in vegetables suchas potatoes and lettuce (Sapers 1993).18.104.22.168 Microbial ContaminationWhen fruit or vegetable tissue is wounded, surface moisture and cytoplasmic remainsof ruptured cells with high concentrations of sugars and proteins will be present,which are ideal conditions for microbial growth (Saltveit 1997). This microbialgrowth could cause food borne illnesses and food spoilage (Nguyen and Carlin1994). Minimally-processed fruits and vegetables are susceptible to invasion bymicroorganisms, such as Pseudomonas spp., Erwinia herbicola, Flavobacterium,Xanthomona, Eterobacter Agglomerans, Leuconostoc mesenteroides, Lactobacillusspp., molds, and yeasts (Zagory 1999). It is important to be aware that a modifiedatmosphere can cause growth of and toxin production by C. Botulinum on fruitswith pH higher than 4.8, so provision should be made to coat tropical fruits inparticular to avoid C. Botulinum growth (Olivas and Barbosa-Cánovas 2005).7.3 History of Edible Films and Coatings for Fruits and VegetablesEdible films and coatings have been extensively studied for the last 20 years, andmuch has been published on their use for fresh and minimally-processed fruits andvegetables (Tables 7.1 and 7.2). Reviews found in literature on the topic of ediblecoatings for whole fruits and vegetables (Platenius 1939; Claypool 1940;Hardenburg 1967; Curtis 1988; Park and Chinnan 1990; Hagenmaier and Shaw1992; Banks et al. 1993; Baldwin 1994; Park 1999) and minimally-processed fruitsand vegetables (Wong et al. 1994; Baldwin et al. 1995a, b; Nisperos and Baldwin1996; Olivas and Barbosa-Cánovas 2005; Lin and Zhao 2007) have addressed theissue indicating different perspectives.
Table 7.1 Edible coatings on minimally processed fruits and vegetables 216 Coatings and Additives andFruits concentrations concentrations Variables evaluated Results ReferencesApple slices Apple puree–alginate CaCl2, N-acetylcysteine, C, EtOH, Et, F, ST, Coatings extended the shelf life Rojas-Graü et al. oregano oil, lemong MG of fresh-cut apple (2007) rass oil, vanillinApple Alginate or gellan Glycerol, CaCl2, B. lactis, WVP, WS, B. Gellan coatings avoided WL better than Tapia et al. (2007) and papaya sunflower oil lactis alginate coatings. Alginate- and cylinders gellan-based edible coatings carried successfully viable probiotics on papaya and apple cylindersApple slices CaCl2+ Alginate or Potassium sorbate, WL, C, F, MG, All coatings preserved F, and C. WL was Olivas et al. (Gala) alginate/acetylated alpha-monostearate TA, SS, FV delayed, mainly with (2007) monoglyceride– Alg-monoglyceride–linoleic acid linoleic acid coating. Higher amounts of Butanol, or alginate butter– hexanal, 1-hexanol, trans-2-hexenal on linoleic acid coated samples at end of storage.Mango slices Chitosan – ST, WL, C The coating retarded WL and drop Chien et al. in sensory quality, increasing (2007b) the SS content, TA and AA content and inhibiting MG.Shelled Pecans CMC PG, Sorbitol, lecithin, ST, R, C Imparted shine, F was not preserved, Baldwin and a-tocopherol, BHA, R was delayed. Wood (2006) BHT, citric acidApple slices WPC + Beeswax AA, cysteine Cys, WL, C, BI, ST WPC-AA and WPC-BW coatings reduced Pérez-Gago et al. or 4-hexylresorcinol B. WL was not (2006) prevented by coatings use.Apple slices WPI, WPC or HMPC Glycerol, stearic acid WL, BI WL was not avoided. WPI and WPC were Pérez-Gago et al. + Beeswax or more efficient at preserving C compared (2005a) carnauba with HMPC. G.I. Olivas and G. Barbosa-Cánovas
7Persimmon WPC–Beeswax or Glycerol WL, F, C, WPC–BW–Ascorbate coatings reduced B, Pérez-Gago et al. pieces WPC–Beeswax WL, and F loss in fresh-cut (2005a) + AA persimmonsApple slices WPI-beeswax Glycerol, stearic acid WL, C, ST Lower BI than uncoated apples. WL was Pérez-Gago et al. not reduced by use of coating (2003b)Pear wedges Methylcellulose (MC) AA, potassium sorbate, WL, F, MG, C, TA, Coating retarded B. WL was delayed on Olivas et al. (2003) and MC–stearic CaC12 SS, FV pears coated with MC–SA. Pear wedges acid (SA) coated with MC–SA formulation con- tained higher amounts of hexyl acetateBaby carrots Xanthan gum Calcium lactate calcium C, ST, Vitamin Calcium and vitamin E increased on coated Mei et al. (2002) gluconate, vitamin E E, b-carotene, carrots. Edible coatings improved C CalciumWPI whey protein isolate; F firmness; WL weight loss; TA titratable acidity; SS soluble solids; RR respiration rate; AA ascorbic acid; C color; MG microbialgrowth; IGC internal gas composition; FV flavor volatiles; DS decay symptoms; ST sensory test; EtOH ethanol; G gloss; Wh whitening; S sugars; Et ethylene;BI browning index; B browning; PG propylene glycol; BHA butylated hydroxyanisole; BHT butylated hydroxytoluene; R rancidity; WS water solubility Edible Flims and Coatings for Fruits and Vegetables 217
Table 7.2 Edible coatings on intact fruits and vegetables 218Fruits Coatings Additives Variables evaluated Results ReferencesMandarin Low molecular weight – WL, F, TA, AA, Fungal LMWC coating improved firmness, Chien et al. chitosan (LMWC) or decay titratable acidity, ascorbic acidity, (2007a) High molecular weight and water content. Mandarin coat chitosan (HMWC) ed with LMWC exhibited greater antifungal resistance than TBZStrawberry Starch Sorbitol C, F, WL, SS, MG C, Opaque coating Ribeiro et al. F, WL, SS, MG C, (2007) F, WL, SS, MG Carrageenan Glycerol + CaCl2 Preserved better firmness Tween 80 Chitosan Tween 80 + CaCl2 Delayed WL Delayed water lossCherry Aloe vera gel and – RR, WL, C, F, MG Delay in WL, F loss Martínez-Romero water 1:3 et al., (2006)Strawberry Chitosan Tween 80, oleic acid SSD, WVR, TA, pH, SS, Anthocyanin content decreased Vargas et al. (2006) anthocyanin, Fungal throughout storage in coated decay, RR, MP, ST samples. Coatings had no signifi cant effects on TA, pH and SS con- tent. Coated fruits had decrease in aroma and flavor, especially when the ratio oleic acid:chitosan was highStrawberry Calcium gluconate Fungal decay, WL, F, C, Coatings decreased surface damage Hernandez-Munoz or chitosan or chito pH, TA, SS and delayed fungal decay. Chito et al. (2006) san + Calcium gluco san coatings retained F and delayed nate changes in external CCherry LBG + Beeswax Polysorbate 80, F, C, WL, ST, EtOH C decay was not prevented by the Rojas-Argudo et al. or shellac glycerol, NH3 coating. WL and F loss was delayed 2005Strawberry Cactus–mucilage Glycerol F, C, ST Coating increased shelf life Del-Valle et al. of strawberry (2005) G.I. Olivas and G. Barbosa-Cánovas
7Guava Dextrans Glycerol FV, C Coatings showed poor water retention Quezada-Gallo et on fruits stored at room temperature. al. (2005) Best efficiency of dextrans was at 4°C, by increasing guava quality (size, color, aroma, water content)Grapes Aloe vera gel – WL, C, F, SS, TA, ST, RR, A. vera gel delayed postharvest quality Valverde et al. MG, Et losses, extending storability from (2005) 7 days at 1°C to 35 days. Coating reduced MGApricots MC + Stearic acid PEG, PEG + CA, WL, Vitamin C Coatings delayed WL of fresh Ayrancy and Tunc and PEG + AA apricots and green peppers. (2004) green Coatings containing AA or CA peppers lowered vitamin C lossCherry Sodium caseinate or milk Glycerol and Bees SS, TA, pH, WL Coatings reduced WL of the fruits. Certel et al. (2004) protein concentrate wax or stearic– Edible coatings had a beneficial palmitic acid blend effect on sensory quality of cherriesCherry Semperfresh™ 10 – F, WL, TA, SS, SC, Effective in reducing WL, Yaman and and 20 g/L AA, C and preserving F, AA, TA Bayo (2002) Edible Flims and Coatings for Fruits and Vegetables and C. Shelf life increased by 21% at 30°C and 26% at 0°Apple Shellac, candelilla, Shellac caused anaerobic respiration on Bai et al. (2003a) shellac–carnauba Braeburn and Granny Smith apples. This research recommends shellac for “Delicious,” carnauba–shellac for “Braeburn” and “Fuji” applesApple Zein Propylene glycol F, G, Wh, TA, FV, S, IGC, Good overall apple quality comparable Bai et al. (2003b) Et, ST to a commercial shellac coatingPlum HPMC + Beeswax or Stearic acid, glycerol WL, F, Et, EtOH WL of coated plums decreased as Pérez-Gago et al. shellac lipid content increased. F was not (2003a) affected by coating after short-term storage at 20°C. In prolonged stor- age, coatings significantly reduced F 219 loss and internal breakdown (continued)
Table7.2 (continued) 220Fruits Coatings Additives Variables evaluated Results ReferencesGrapes Chitosan NaOH to modify pH Inhibition of Botrytis They observed that inhibitory effect Romanazzi et al. to 5.6. cinerea originated from combination of | (2002) coating and antifungal effects and stimulation of defense responsesPear Carnauba wax – Decrease in pear friction discoloration Amarante et al. and internal O2 concentration (2001)Pear Carnauba wax – Modification of O2 instead of CO2 Amarante et al. was the means of delaying ripening (2001)Kiwifruit Soy protein + pullulan + Glycerol Peroxidase, pectin, TA, Coating retarded softening of kiwifruit Xu et al. (2001) stearic acid RR, EtMango Cellulose. Nature Seal® Preservative, acidu IGC, WL, FV, SS, TA, DS, Both coatings created modified atmos- Baldwin et al. 2020 hydroxypropyl- lant and emulsifier ST, F pheres, reduced decay, and impro (1999) cellulose Carnauba. Fatty acid soaps ved appearance. Polysaccharide coat- Tropical Fruit Coating ing delayed ripening and increased 213 (TFC) concentrations of flavor volatiles. Carnauba coating reduced WLF firmness; WL weight loss; TA titratable acidity; SS soluble solids; RR respiration rate; CA citric acid; AA ascorbic acid; C color; MG microbial growth; IGCinternal gas composition; FV flavor volatiles; DS decay symptoms; ST sensory test; EtOH ethanol; G gloss; Wh whitening; S sugars; Et ethylene; LGB Locustbean gum; SSD surface solid density; WVR water vapor resistance; MP mechanical properties; TBZ thiabendazole G.I. Olivas and G. Barbosa-Cánovas
7 Edible Flims and Coatings for Fruits and Vegetables 221 Application of edible coatings to preserve quality of fruits and vegetables is notnew. Hardenburg (1967) comments that their use dates back to the XII century,where oranges and lemons were coated with wax in China to preserve the fruitslonger. In the U.S., the first patent on use of edible coatings dates back to 1916,where a method preserving whole fruits with molten wax was patented by Hoffman(Hoffman 1916). In 1972, Bryan patented a method to preserve grapefruit halves withedible coating composed of low methoxyl pectin and locust bean gum dispersed ingrapefruit juice.7.4 Technical Development of Edible Films and CoatingsThe main purpose of employing edible films and coatings is to provide a semi-permeable barrier against gases and vapor; however, there are other purposes(e.g., to carry additives such as texture enhancers, antimicrobials, antioxidants, etc.;Table 7.3). In general, edible films and coatings represent an interesting option forintact and minimally-processed fruits and vegetables, since a barrier can be formedthat protects the produce and decreases rate of physiological postharvestdeterioration. Successful application of edible films or coatings as barriers for fruits andvegetables mainly depends on developing film or coating that can provide appro-priate internal gas composition for a specific fruit/vegetable (Park 1999). Somefactors/questions need to be addressed when developing a film or coating: (1) howproperties of coating solution will affect the product, (2) how coating will changewith time, (3) how coating will interact with the product that might lead to flavor/off-flavor generation, and (4) how storage conditions will affect coating. Otherconsiderations include importance of thickness, color, and flavor of coating, since theseparameters can change final quality of the coated product. Thus, to develop the appropriate film or coating, full understanding of the physio-logy of the fruit/vegetable being coated is needed, as well as a clear idea of the functionof the film or coating relative to the product. Different purposes of films and coatingsdeveloped for fruits and vegetables are more fully detailed in the next section. Table 7.3 List of additives incorporated into edible films and coatings for fruits and vegetables Additives Examples Antibrowning compounds Ascorbic acid Antimicrobial agents Potassium sorbate Texture enhancers Calcium chloride Nutrients Vitamin (E) Aroma precursors Linoleic acid Probiotics B. lactis Flavors and colorants Apple puree
222 G.I. Olivas and G. Barbosa-Cánovas7.4.1 Edible Films and Coatings for Preservation of Fruits and Vegetables22.214.171.124 Water LossEdible films/coatings decrease water vapor transmission rate by forming a barrier onthe fruit or vegetable surface. This barrier prevents texture decay, since water isessential for preservation of cell turgor (Garcia and Barret 2002). Metabolic altera-tions that can cause accelerated rate of senescence due to water loss can also beavoided with their use. Ability of films and coatings to function as barriers to watervapor relies on external conditions, which include (1) temperature and relativehumidity, (2) characteristics of commodity such as type of product, variety, maturityand water activity, and (3) characteristics of film such as composition, concentra-tion of solids, viscosity, chemical structure, polymer morphology, degree of cross-linking, solvents used in casting the film, and type of plasticizer used (Olivas andBarbosa-Cánovas 2005). In case of minimally-processed fruits, there is usuallyvery high water activity present at the surface, making it difficult to develop a coat-ing that delays water loss, since capacity of films to work as barriers to water vapordecreases as water activity increases in the commodity (or relative humidity of theenvironment) (Hagenmaier and Shaw 1990). However a number of coatings havebeen developed that can delay water loss in some minimally processed fruits andvegetables (Table 7.1).126.96.36.199 TextureWhen coating or film is applied to a commodity, a modified atmosphere is developed.Reduction of internal oxygen and increase of carbon dioxide in the commodity willin some cases delay softening (Kader 1986). Intact apples retained firmness whenstored under modified atmosphere (Knee 1980). Edible coatings can also preservetexture of fruits and vegetables by acting as a partial barrier to water and serving ascarriers of texture enhancers. Loss in texture has been delayed with application ofedible coating to whole avocados (Maftoonazad et al. 2007). Olivas et al. (2007);likewise preserved texture of cut-apples when coated with alginate films containingcalcium chloride.188.8.131.52 RespirationEdible films or coatings can reduce respiration and, hence increase shelf life of acommodity. In selection of a coating, several considerations should be addressed toavoid extremely low oxygen concentration inside the commodity. Low oxygenconcentration in the product could lead to anaerobic respiration, which can result
7 Edible Flims and Coatings for Fruits and Vegetables 223in deterioration of product due to production of off-flavors and accelerated senes-cence (Kays and Paull 2004). Some studies (Tables 7.1 and 7.2) show how ediblefilms/coatings have favorably delayed respiration, and in some cases caused anaer-obic respiration.184.108.40.206 EthyleneA well selected edible coating will produce a modified atmosphere inside the fruit,reducing levels of internal oxygen. If oxygen concentration inside the commoditydrops below 8%, there will be a decrease in ethylene production (Kader 1986), andthe commodity’s quality will be preserved longer.220.127.116.11 ColorOne of the most important attributes of fruits and vegetables is color (Kays 1999).For some minimally-processed fruits and vegetables, browning is a big problemthat can be controlled by use of films or coatings as carriers of anti-browningagents. The most common antioxidant used on fruits and vegetables is ascorbicacid; however other compounds have been successfully used such as cysteine,4-hexylresorcinol, citric acid and calcium chloride (Olivas et al. 2007; Pérez-Gagoet al. 2006). Baldwin et al. (1996) coated apple slices and potato cores with NatureSeal™ and found that ascorbic acid delayed browning more effectively whenapplied in edible coating than in aqueous solution. Depending on coating formula-tion, appearance of fruit can be affected positively or negatively by selectedcoating. For instance, candelilla wax gives a natural, noncoated appearance toapples, whereas shellac or carnauba coating (when in contact with water) will givewhitish color to apples (Bai et al. 2003a).18.104.22.168 FlavorPerhaps the most important attribute of fruits and vegetables is flavor. Consumersmay buy the commodity based on its appearance when first purchased, but if theflavor is not acceptable, they will avoid buying the product a second time. Flavorcan be preserved or modified with edible films or coatings by two different means:(1) as a barrier to aroma volatiles, and (2) as a carrier of flavors. Baldwin et al.(1999), for instance, found that a polysaccharide coating worked as a barrier toaroma volatiles on whole mango. Edible coatings can also modify internal atmos-phere of the commodity, causing low oxygen and high carbon dioxide concentra-tion.This is not beneficial to flavor, since it could lead to a decrease in productionof characteristic flavor compounds (Ke et al. 1994; Fellman et al. 2003). Some
224 G.I. Olivas and G. Barbosa-Cánovasworks have even suggested the possibility that edible coatings on cut fruits cansupply fruits with volatile precursors (Olivas et al. 2003, 2007). Pear wedgescoated with a methylcellulose–stearic acid formulation contained higher amountsof hexyl acetate throughout storage, probably due to synthesis in wounded tissuefrom the stearic acid contained in the coating (Olivas et al. 2003). Higher produc-tion of hexanol was observed in apples coated with alginate–linoleic acid.According to Paillard (1979), hexanol can be produced from fatty acids such aslinoleic acid.22.214.171.124 Microbial ContaminationIn case of minimally-processed fruits and vegetables, where natural protection(skin) has been eliminated, opportunity for microorganisms to invade and grow onthe surface of the fruit is present. Incorporating antimicrobial compounds intoedible films or coatings will preserve quality of fresh-cut fruits and vegetables.Since antimicrobials are needed just on the surface of the product, their applicationas part of a coating will help minimize antimicrobial usage (Vojdani and Torres1990). Retention of antimicrobial on coated produce surface will depend on coatingattributes (composition, hydrophilic characteristics and manufacturing procedure) andcommodity type (pH and water activity), as well as storage conditions (temperatureand duration) (Cagri et al. 2004). Antimicrobials most commonly used includepotassium sorbate, sodium benzoate, sorbic acid, benzoic acid and propionic acid;other natural antimicrobials such as lemongrass, oregano oil and vanillin have alsobeen used (Rojas-Graü et al. 2007).126.96.36.199 Nutritional QualityEdible films and coatings can affect nutritional quality of fruits and vegetables. Onone hand, they can be used as carriers of nutrients. On the other hand, they canproduce abiotic stress, which could modify metabolism of the commodity,affecting production of nutrients. Some works have determined effects of coat-ings on nutritional quality, and on phenolics and other phytochemicals. Viña et al.(2007) coated Brussels sprouts with starch and analyzed effect of coating onamount of ascorbic acid and total flavonoids retained in the vegetable after storage.Han et al. (2004) found higher amounts of vitamin E and calcium on strawberriescoated with chitosan, containing calcium and vitamin E in the formulation, due todiffusion of these nutrients into the fruit. Romanazi et al. (2002) observed anincrease in phenylalanine ammonia–lyase activity, a key enzyme for synthesis ofphenolic compounds, on grapes coated with chitosan. Edible coatings have alsobeen used as carriers of probiotics. Bacillus lactis was maintained for 10 dayson fresh-cut fruits under refrigeration, when applied on alginate- and gellan-based edible coatings (Tapia et al. 2007).
7 Edible Flims and Coatings for Fruits and Vegetables 2257.5 Properties of Edible Films and Coatings7.5.1 Edible Films and Coatings as Partial Barriers to Water Vapor and GasesEdible coating or film mainly works as a partial barrier to water vapor and gases bydecreasing transmission rate of a given partial pressure difference between internaland external atmospheres. This partial barrier is conducive to a modified internalatmosphere low in oxygen and high in carbon dioxide, suppresses respiration rateand reduces transpiration losses. Scientific literature provides vast amounts ofinformation on barrier properties of edible films; however, comparisons betweendifferent films are sometimes difficult or impossible due to use of different types ofequipment and dissimilar test conditions during measurements (Tuil et al. 2000).Choosing a proper coating is complex, because it depends on specific respirationand transpiration rates of the commodity and outside environmental conditions.When applying a coating to a fruit, whole or cut, permeability to gases is modifieddue to the barrier formed by coating. This could lead to anaerobic respiration. Respiration and ripening of fruits and vegetables involve gas exchange with theenvironment. Carbon dioxide, oxygen, water and other metabolic byproducts, suchas ethylene and other volatile compounds, are main substances exchanged duringstorage. Surface coatings modify gas exchange rate between environment and freshproduce, and thus control transpiration, respiration and other metabolic processesthat lead to loss of quality. The mechanics and main factors involved in mass transferprocesses through fruit skin and coated fruits follow. Fruits and vegetables exchange gases with their storage environment through aphenomenon known as gas diffusion. Gas diffusion is a passive transport phenomenonin which Gibbs free energy is minimized through mass transfer from a region withhigh concentration of a given chemical species to a region with lower concentrationof the same chemical species. During this spontaneous process, the interface betweenthe two mentioned regions (natural skin or an artificial coating) may present someopposition to the mass transfer process, affecting mass transfer rate. Unless theinterface in a system completely hinders mass transfer, diffusion carries on untilequilibrium is reached (i.e., when a concentration gradient ceases to exist). Inter-phases causing extremely high opposition to a specific compound are referred to as“impermeable”. Unidimensional steady state mass transfer, as the one witnessed infresh produce stored under specific conditions, may be mathematically described byFick’s first law of diffusion, which states that mass flux per unit area of a givenchemical species (J) is proportional to its concentration gradient (∂φ / ∂x). ∂φ J=D (7.1) ∂xMagnitude of the proportionality constant (D), known as diffusivity, theoreticallydepends on temperature (T ) , viscosity (h) of medium in which diffusion is takingplace, and on size of diffusing particles (r), according to the Stokes–Einstein relation,
226 G.I. Olivas and G. Barbosa-Cánovas k BT D= (7.2) 6ph rwhere kB is the Boltzmann constant (1.380 × 10−23J/K). In practice, howeverD values for specific situations may depart from this theoretical value due to structuralpeculiarities or chemical affinity effects, making empirical correction necessary. In order to have a mathematical expression to model and describe gas diffusion(normal to the surface) through biological membranes, Eq. (7.1) may be solved byseparating the variables and integrating from point x1, where concentration c1 of agiven chemical species is found to be point x2, and where concentration c2 of thesame chemical species exists, yielding: J=D (c1 − c2 ) (7.3) (x2 − x1 )Typically (x2–x1) represents thickness of the membrane, and since the chemicalspecies being diffused through the membrane is a gas, Eq. (7.3) may be substitutedby Eq. (7.4): r1 − r 2 J = DS (7.4) thicknesswhere gas concentrations and concentration gradient are expressed as a function ofthe partial pressure of diffusing gas on both sides of the membrane (r1 and r2),using Henry’s law: c = Sr (7.5)where concentration (c) of a gas is proportional to its partial pressure (r), dependingon a proportionality constant known as solubility (S). Diffusivity multiplied bysolubility of a specific gas through a specific membrane is known as permeabilitycoefficient P, changing Eq. (7.4) to its final form as: r 1 −r 2 (7.6) J=P thickness7.5.2 Edible Films and Coatings for Active PackagingBesides working as partial barriers to vapor and gases, edible films and coatingscan serve as carriers of ingredients to help preserve quality and improve nutritionalvalue of fruits and vegetables. When coating is used for more than providing a barrierto external conditions, it is called active coating (Rooney 1995). Antimicrobialagents, texture enhancers and anti-browning compounds can be added to preservequality of a commodity longer. Incorporation of some nutrients to the coatingcan increase nutritional value of the commodity. Aroma precursors can also beincorporated into a coating to increase flavor production (Olivas et al. 2003).
7 Edible Flims and Coatings for Fruits and Vegetables 2277.5.3 Factors Affecting the Properties of Films and CoatingsProperties of films (or coatings) are affected by characteristics of the film, commodity,and environment, such as coating solution composition, viscosity of coating solution,coating thickness, type of product, plant variety, fruit/vegetable maturity, previousfruit treatment, fruit surface coverage (how coating adheres to surface of fruit) andexternal atmosphere (Hagenmaier and Shaw 1992; Banks et al. 1993; Cisneros-Zevallos and Krochta 2002). A clear understanding of how these factors affectperformance of a film will aid in developing a proper coating for a specific product.Some of these factors are discussed next.188.8.131.52 Coating CompositionComposition of film or coating affects its permeability. Chemical structure, concen-tration, chemical nature, physical state, method of preparation, crystallinity, polarity,orientation, presence of additives and use of compound blends will all affectperformance of a film (Miller and Krochta 1997; Morillon et al. 2002). A coatingcontaining hydrophilic compounds is not a very good barrier to water vapor, whilehydrophobic substances perform well as barriers to moisture migration, since lipid-based edible coatings have low affinity for water due to their apolar nature (Morillonet al. 2002). Length of the hydrocarbon chain affects WVP (water vapor permeability)of lipid compounds. Higher the carbon number, lower the WVP, as the apolar partof the molecule generally increases with increasing number of carbons (McHughand Krochta 1994). However, if number of carbons is higher than 18, this behaviorreverses, presumably due to heterogeneous nature of coating produced (Koelschand Labuza 1992). Lipids with higher affinity to water when used in coatings willhave greater permeability to water vapor. Factors such as lipid concentration, physicalstate, degree of nonsaturation and chemical structure also affect WVP of lipid coatings.Morillon et al. addressed these important issues in a review published in 2002.7.5.3.2 Coating ThicknessCisneros-Zevallos and Krochta (2003b) published a work in which physical principlesof dip-plate coatings were applied to fruit coatings. They demonstrated that internalmodified atmosphere of a coated commodity depends on coating thickness, whileat the same time coating thickness depends on viscosity, concentration, density anddrainage time of coating solution. Debeaufort et al. (1993) found that water vaportransfer rate and permeability decreased when thickness of a triglyceride coatingincreased from 0 to 60 mm.184.108.40.206 Aging of FilmsIt is important to bear in mind that a coating will change over time along with itsproperties. Edible coatings, depending on their formulation, are subject to chemical
228 G.I. Olivas and G. Barbosa-Cánovasand physical changes that can cause degradation of polymer chains, migration oflow molecular weight additives, water absorption, etc. If there is migration of plas-ticizer, mechanical properties of film will be affected (Anker et al. 2001).220.127.116.11 Type of CommodityQuality of coated fruits can vary greatly, since each fruit, even those of the samevariety, is different in skin resistance, gas diffusion, fruit respiration rate, etc. Also,the effect of individual applications of coatings will vary between fruits, affectingcoating thickness and proportion of pores blocked by coating material (Banks et al.1993). Coatings developed for one variety of fruit may not be appropriate foranother. Bai et al. (2003a) studied coatings for apples and found that shellac is thebest coating for Delicious apples; however, this coating caused anaerobiosis onBraeburn and Granny Smith apples.18.104.22.168 Fruit Surface CoverageAccording to Banks et al. (1993), fruit coatings work as barriers to gases by blockingpores on the fruit’s surface. In addition, they found that coating of fruit cuticle canaffect water vapor diffusion.22.214.171.124 Storage ConditionsFilm permeability depends on relative humidity (RH) and gas composition of theenvironment, which can also affect properties of coating. In case of cut fruits, wateractivity of the coated fruit is also affected, as shown by Cisneros-Zevallos andKrochta (2002). When cut fruit was coated with a hydrophilic film, they found thatthe surrounding environment’s RH greatly affected barrier properties of the film.Temperature also affects properties of edible films or coatings. Kester and Fenema(1989) studied WVP of films at temperatures varying from 15 to 40°C, and observedthat WVP decreases when temperature decreases.7.6 Composition of Edible Films and CoatingsEdible films and coatings are composed of hydrocolloids, which consist of eitherpolysaccharides or proteins, or hydrophobic compounds (e.g., lipids or waxes).Edible films may also be composed of a mixture of hydrocolloids and hydrophobiccompounds (composite films or coatings). Figure 7.1 shows the most commoncompounds used in edible films and coatings.
7 Edible Flims and Coatings for Fruits and Vegetables 229 COATINGS CHS PROTEINS LIPIDS CELLULOSE VEGETAL WAX MC ZEIN BEESWAX HPC GLUTEN CARNAUBA HPMC SOY CANDELILLA CMC ANIMAL PARAFFIN GUMS WHEY SHELLAC ALGINATE CASEIN OIL GUAR MINERAL PECTIN VEGETAL STARCH FA ESTERS CHITOSANFig. 7.1 Main components of edible films and coatings for intact and minimally processed fruitsand vegetables (CHS carbohydrates; FA fatty acids; MC methylcellulose; HPMC hydroxypropyl-methylcellulose; HPC hydroxypropylcellulose, CMC carboxymethylcellulose)7.6.1 Carbohydrates126.96.36.199 ChitosanThe compound chitosan comes from marine invertebrates and is a derivate of chitin,which after cellulose, is the most abundant polysaccharide resource on earth(Tuil et al. 2000). Chitosan is a high-molecular-weight cationic polysaccharidecomposed of (1 → 4)-linked 2-acetamido-2-deoxy-b-D-glucopyranosyl and 2-amino-2-deoxy-b-D-glucopyranosyl units (Sebti et al. 2005), and produces transparentfilms. Chitosan is not water-soluble, so a coating solution comprised of weakorganic acid (acetic acid) must be used. Chitosan has been shown to be a natural foodpreservative, though the antimicrobial mechanism involved is not well elucidated.It is believed that positively charged chitosan molecules interact with negativelycharged microbial cell membranes, causing change in microbial cell permeabilitythat leads to leakage of cell constituents (No et al. 2007). Chitosan films or coatings can increase shelf life and preserve quality of fruitsand vegetables by decreasing respiration rates, inhibiting microbial developmentand delaying ripening. They have been used on fruits and vegetables withgood results, showing antimicrobial activity against Bacillus cereus,Brochothrix thermosphacta, Lactobacillus curvatus, Lactobacillus sakey, Listeriamonocytogenes, Pediococcus acidilactici, Photobacterium phosphoreum,Pseudomona fluorescens, Candida lambica, Cryptococcus humiculus, and Botrytiscinerea (Devlieghere et al. 2004; Romanazzi et al. 2002). Chitosan is consideredideal coating for fruits and vegetables, mainly because it can form a good film on thecommodity’s surface and can control microbial growth (Muzzarelli 1986; No et al. 2007).
230 G.I. Olivas and G. Barbosa-CánovasEven though the high hydrophilic character of chitosan films (Sebti et al. 2005) couldadversely affect their properties and use as coatings for fresh-cut fruits and vegetables,they have been used nevertheless on cut fruits such as peeled litchi (Dong et al. 2004)and fresh-cut Chinese water chestnuts (Pen and Jiang 2003) with good results. Chitosan coatings have also been used on grapes to control incidence of Botrytiscinerea. It was observed by Romanazzi et al. (2002) that besides having a directeffect against B. cinerea, chitosan caused an increase in phenylalanine ammonia–lyaseactivity (a key enzyme for synthesis of phenolic compounds, usually characterizedby antifungal activity). They concluded that the inhibitory effect of chitosan originatesfrom a combination of its antifungal properties and ability to stimulate defenseresponses in the host. Similar results were observed for strawberries where Botrytiscinerea and Rhyzopus stolonifer were inoculated and then coated with 1% chitosan;decay decreased and lower synthesis of anthocyanin was observed, compared tostrawberries treated with fungicide. El-Ghaouth et al. (1997) applied chitosan coatingson strawberry, bell pepper and cucumber, observing reduced lesion developmentdue to Botrytis cinerea and Rhizopus stolonifer, as well as delayed ripening. Othersfound (El-Ghaouth et al. 1992) that chitosan-coated tomatoes showed reduction inrespiration rate and ethylene production, were firmer with less decay, and had lessred pigmentation, compared to noncoated tomatoes. Litchi has also been coatedwith chitosan, where there was delay in reduction of anthocyanin content andincrease of PPO activity (Zhang and Quantick 1997; Jiang et al. 2005). Composite coatings containing chitosan are likewise a good option for fruits andvegetables. Chitosan coatings containing oleic acid had good water retentionproperties on coated strawberries (Vargas et al. 2006), while apples coated withN,O-carboxymethyl chitosan films and placed in cold storage could be maintainedin fresh condition for more than 6 months (Davies et al. 1989). Chitosan has been approved for use as a food additive in Japan and Korea. In theU.S., Generally Recognized as Safe (GRAS) notices were submitted (by a “notifier”)to the FDA in 2001 and 2005 to evaluate chitosan (from shrimp) and its suitabilityfor use; however (at notifier’s request) the FDA ceased evaluation of both notices(No et al. 2007; US FDA/CFSAN 2006).188.8.131.52 StarchStarch is an abundant, inexpensive polysaccharide obtained from cereals, legumes,and tubers, and is extensively utilized in the food industry. Starch is a polysaccharideconsisting of a–(1 → 4) d-glucopyranosyl units with d-glucopyranosyl chainslinked by a–(1 → 6) glycosidic bonds. It is composed of two macromolecules,amylose, essentially linear, and amylopectin, highly branched. Ratio of amylose andamylopectin varies with source. Regular or standard wheat, corn, and potato starchesgenerally contain lower amounts of amylose than those of most legumes (Hooverand Sosulsky 1991; BeMiller and Whistler 1996). Films formed with starch areoften very brittle and have poor mechanical properties (Peressini et al. 2003). Thesefilms are formed by drying of a gelatinized dispersion, as hydrogen bonds form
7 Edible Flims and Coatings for Fruits and Vegetables 231between hydroxyl groups (Lourdin et al. 1995). Since these interactions are weak,mechanical properties of starch-based films are of poor quality. To overcome thisproblem, it is necessary to blend starch with other compounds or chemically modifythe starch (Tuil et al. 2000). Proportion of amylose and amylopectin within starch will affect film-formingproperties. A higher proportion of amylose will improve mechanical properties of thefilm (Han et al. 2006), as the branch-on-branch structure of amylopectin interfereswith intermolecular association and disrupts film formation (Peressini et al. 2003).Rice and pea starch films (30 and 40% amylose, respectively, by weight) containingglycerol as plasticizer (starch:plasticizer ratio of 2:1) were found to have low oxygenpermeability and good elastic properties, with pea films showing highest elasticityand WVP (Mehyar and Han 2004). Han et al. (2006) reported higher oxygenpermeability and lower elongation (one order of magnitude) for pea starch films (~40%amylose) with glycerol as plasticizer (starch:plasticizer ratio 3:2). Nevertheless, thesestarch films still showed low oxygen permeability compared to other films, whileWVP of starch films was observed to be comparable to that of protein films. García et al. (1998) compared quality of strawberries coated with starch fromdifferent sources (corn starch – 25% amylose; potato starch – 23% amylose; high-amylose corn starch – 50% amylose; high-amylose corn starch – 65% amylose), andfound a significant effect of amylose on color, weight loss and firmness of coatedstrawberries. Strawberries coated with 50% and 65% high-amylose starches bestretained their quality attributes compared to other treatments. Since starch films are hydrophilic, their properties will change with fluctuationsin RH; for example, their barrier properties decrease with increasing RH. Starch istherefore not the best option when working with minimally-processed high-wateractivity commodities. Bai et al. (2002) coated apples with starch solutions andobserved high gloss at the beginning of storage. However, they observed a largedecrease in gloss during storage, though firmness, internal oxygen and carbon dioxideconcentrations of starch-coated apples had values similar to shellac-coated apples(a coating used commercially).184.108.40.206 CelluloseCellulose, the most abundant natural polymer on earth, is composed of linear segments(1 → 4)-linked b-D-glucopyranosyl units. Although very inexpensive, cellulose isdifficult to use as coating, because of its water-insolubility and highly associatedcrystalline structure. However, some cellulose derivatives produced commercially suchas carboxymethylcellulose (CMC), methylcellulose (MC), hydroxypropylcellulose(HPC), and hydroxypropylmethylcellulose (HPMC), can overcome limitationsassociated with native cellulose. Due to the cellulose linear structure, these deriva-tives tend to form good films, though film properties will depend on cellulosestructure and molecular weight (Park et al. 1993; Ayranci et al. 1997). Ayranci et al.(1997) found that WVP of HPMC films decreased with increasing molecularweight of HPMC. However, Park et al. (1993) observed the opposite result for MC
232 G.I. Olivas and G. Barbosa-Cánovasand HPC films, wherein WVP of these films increased with increasing molecularweight of HPC and MC. Comparison between MC, HPC, and CMC coatings,applied to shelled pecan nuts, showed CMC to be the best coating material for thisapplication (Baldwin and Wood 2006). CMC coating imparted sheen and delayedrancidity; however firmness was not preserved. WVP of HPMC and MC films wasalso observed to decrease with increasing polymer molecular weight (Ayranci et al.1997). Further, MC has been used to preserve green color and firmness of avocadosand lower their respiration rates during storage (Maftoonazad and Ramaswamy2005). Coating apricots and green peppers with a composite film of MC and stearicacid effectively reduced water loss; when coated with a film containing citric acid orascorbic acid, vitamin C loss was also reduced (Ayrancy and Tunc 2004). Carboxymethylcellulose has been widely used as coating for fruits. Some coatingformulations containing CMC are already on the market, such as Tal Pro-long™ andSemperfresh™. Tal Pro-long™ (or Pro-long) is composed of sucrose polyesters offatty acids and the sodium salt of CMC. Semperfresh™ is composed of sucroseesters of fatty acids, sodium salt of CMC, and mono- and diglycerides. These coatingshave been shown to retard ripening of fruits (Fig. 7.1). Quality of cherries coatedwith Semperfresh™ can be preserved for longer periods, reducing weight loss andpreserving firmness and skin color. Another cellulose product on the market, NatureSeal™, is composed of cellulose derivatives, but without sucrose fatty acid esters.A combination of Nature Seal™ and soy protein coatings carrying anti-browningagents and preservatives prolonged shelf life of cut apples by 1 week when storedat 4°C (Baldwin et al. 1996).220.127.116.11 AlginateAlginate, the sodium salt of alginic acid, is a block copolymer of b-d-mannuronicacid (M) and a-l-guluronic acid (G), and is isolated from brown seaweed (Sime 1990).Alginate forms strong, translucent, glossy films. Compared to CMC, gelatin, wheyprotein isolate, potato starch and sodium caseinate films, those of sodium alginate havelowest WVP, oxygen permeability and elongation percentage and highest tensilestrength (Wang et al. 2007). Sodium alginate films are soluble in water, acid, and alkali(Wang et al. 2007), making them a good choice for coating whole fruits and vegetables.These films are not as effective for coating minimally-processed fruits and vegetables,though incorporation of calcium cations to decrease solubility of polymers comprisingsuch films would make them a viable option (Olivas et al. 2007). Composition of alginate (M:G ratio) also affects WVP of films. Alginate–Ca2+films with higher concentrations of G have lower WVP than films with higherconcentrations of M due to greater ability of G to form intermolecular cross-linksvia calcium salt-bridges. Although properties of alginate films are influenced bysurrounding RH, alginate–Ca2+ films retain their strength, even at high RH values(Olivas and Barbosa-Cánovas 2008). Alginate–Ca2+ coatings have been used successfully to prolong shelf life of fresh-cut Gala apples without causing undesirable anaerobic respiration. These coatingsminimized weight loss and browning, and preserved firmness during storage.
7 Edible Flims and Coatings for Fruits and Vegetables 2337.6.2 ProteinsProteins can form edible films due to the ability of their side chains to form inter-molecular cross-links. Properties of these films depend on the nature of these linkages.In general, protein films are considered to have good gas barrier properties, thoughtheir water barrier properties are generally poor (Gennadios et al. 1994), sincethe latter depend on the RH of the environment and/or water activity of the food.Proteins generally used as coatings for fruits and vegetables are reviewed in para-graphs that follow.18.104.22.168 Zein CoatingsZein is a protein composed of prolamines found within corn endosperm, and issoluble in aqueous alcohol. Zein films have strong yellow color relative to HPMC,whey protein concentrate, shellac or whey protein isolate coatings (Trezza andKrochta 2000). Applied to tomatoes, zein coatings will delay color change, weightloss and softening without ethanol production (Park et al. 1994). Zein coatingscontaining vegetable oils, citric acid and antioxidants have been used to preventrancidity of nuts and inhibit moisture transfer from fruit pieces in dry mixes(Andres 1984). Park et al. (1996) found that apples coated with zein solutionsexperienced decrease in respiration rate, whereas zein-coated pears had an increasedrespiration rate, compared to uncoated controls. Nevertheless, zein coatings delayedweight loss in both apples and pears during storage. A zein coating formulation,containing 10% zein and 10% propylene glycol dissolved in aqueous alcohol,was developed for Gala apples by Bai et al. (2003b). This coating maintainedoverall fruit quality comparable to commercial shellac coating. Special attentionshould be taken when coating fruits and vegetables with zein solutions, since, zeincoatings can become white in color on contact with water, depending on thecoating’s concentration (Bai et al. 2003b).22.214.171.124 Gluten and Soy ProteinsGluten is the main storage protein in wheat and corn. Gluten films have good oxygenand carbon dioxide barrier properties, but exhibit relatively high WVP (Gennadios andWeller 1990). Mechanical treatment of gluten leads to disulfide bridge formationcreated by the amino acid, cysteine, which is relatively abundant in gluten. Wheatgluten has been used to preserve quality of fruits and vegetables. Peanuts werecoated with a composite coating of soy protein isolate and wheat gluten with theobjective of preventing fat deterioration. Soy protein also contains cysteine residuesthat can form disulphide bridges. Soy protein films are therefore similar to glutenfilms in mechanical properties. Baldwin et al. (1996) improved properties of NatureSeal™ coating on sliced apples and potatoes by adding soy protein, which reducedcoating permeability to oxygen and water vapor.
234 G.I. Olivas and G. Barbosa-Cánovas126.96.36.199 WheyMilk proteins contain 20% whey protein of which b-lactoglobulin is the main proteincomponent. Whey protein is water-soluble, but b-lactoglobulin denatures whenheated, exposing internal sulfur groups of cysteine, which then cross-link to forman insoluble film (McHugh and Krochta 1994). Whey protein has been studiedextensively as a coating for different foods, including intact and minimally-processedfruits and vegetables. Whey protein was shown to produce a translucent and flexiblefilm with excellent oxygen and aroma barrier properties at low RH (McHugh andKrochta 1994; Miller and Krochta 1997). Though some have found that wheyprotein films provide a poor moisture barrier, others have reported that incorpora-tion of lipids reduces WVP of whey protein films (McHugh and Krochta 1994;Shellhammer and Krochta 1997; Pérez-Gago and Krochta 2001). Another studyindicated that WPI (whey protein isolate) films are good gas barriers, but that theyare influenced by the RH of the environment, affecting resistance of coatingto oxygen and carbon dioxide permeation. As RH decreased, resistance of the coatingto gas transfer increased. At low RH, oxygen decreased and carbon dioxide increasedin coated fruits. At RH values ranging from 70 to 80%, anaerobic metabolism wasinduced due to low oxygen levels (Cisneros-Zevallos and Krochta 2003a). Whey protein-based coatings were more effective in reducing enzymatic brown-ing of Golden Delicious apple slices than HPMC-based coatings - probably due tothe antioxidant effect of amino acids, such as cysteine and/or higher oxygen barrierimparted by the protein. No differences in browning were found between WPI- andWPC- (whey protein concentrate) based films. Lipid inclusion also affected degree ofbrowning (measured with a colorimeter), but these differences were less evidentat the end of storage, as assessed by a sensory panel. Results suggest that additionof anti-browning agents to whey protein coatings, combined with proper storageconditions, could significantly extend shelf life of fresh-cut apples (Pérez-Gagoet al. 2005a).7.6.3 LipidsLipids can be included in formulation of edible coatings or films within a lipid-based film, as a single layer of lipids dispersed in a hydrocolloid network, or as asecondary layer (a lipid layer over a hydrocolloid layer). Coatings containing lipidsgenerally have good moisture barrier properties, since lipids have very low affinityfor water (Krochta 1997). The properties lipids confer to films and coatings willdepend on the characteristics of the lipid component, such as its physical state,degree of saturation and chain length of fatty acids. Saturated long-chain fatty acidsprovide coatings with best water vapor barrier properties (among fatty acids), asthey produce more densely packed structure and have less mobility than unsatu-rated short-chain fatty acids (Kamper and Fennema 1984). Lipids which are solidat the desired storage temperature will form coatings with better water vapor barrier
7 Edible Flims and Coatings for Fruits and Vegetables 235properties than lipids which are liquid under same conditions, mainly becausesolubility of water vapor in lipids is lower in films having more ordered molecularorganization (Kester and Fennema 1989).188.8.131.52 Carnuba and Shellac WaxCarnauba is a natural plant wax and is GRAS (generally recognized as safe). It isrelatively permeable to gases, and in microemulsion form, is quite shiny. The primaryproblems with carnauba wax are its loss of gloss during storage and its relativelyhigh gas permeability, which does not effectively delay ripening (Baldwin et al.1999). However, it is an excellent barrier to water vapor and can be combined withshellac to create a coating of moderate permeability to gases and low permeabilityto water vapor. Natural Shine™ 8000 (carnauba wax) is used to reduce oxygentransfer into and water vapor out of the fruit, while shellac is used to give a shinyappearance. Johnfresh™ is composed of both carnauba wax and shellac. Most Delicious apples marketed in the U.S. are coated with shellac or shellaccombined with carnauba wax (Bai et al. 2002). Shellac and carnauba wax are oftenused commercially as a coating for apples and citrus fruits to improve their appearanceby adding gloss, to prevent water loss leading to shriveling and loss of marketability,and to maintain quality through delayed ripening and senescence. Unfortunately,both materials are also associated with non-food uses; shellac also has problemswith low gas permeability, which can lead to delayed ripening in some fruits(Baldwin et al. 1999) and cause anaerobic conditions. The apple industry is especiallyconcerned that consumers may object to shellac, which does not currently haveGRAS status. Shellac has further problems with whitening, or “blushing” as it isreferred to in the industry, where water condenses on coated fruit surface afterremoval from cold storage. Nevertheless, shellac is recognized as one of the shiniestcoatings available, and was found to improve appearance of apples. In one study,subsequent sales of red and green apple cultivars, such as Delicious and GrannySmith, respectively, increased due to shellac coatings (Bai et al. 2003a).184.108.40.206 BeeswaxBeeswax can be used as a composite film. Han et al. (2006) added beeswax to peastarch films and found a decrease in WVP and an increase in oxygen permeability withbeeswax concentration higher than 30%. Beeswax-pea starch films were homoge-neous and translucent. Thickness of pea starch coating significantly increased withaddition of beeswax (Han et al. 2006). Beeswax has been used in composite coatingsin combination with WPI, WPC, and HMPC to preserve intact fruits such as plums(Pérez-Gago et al. 2003a) and minimally-processed fruits, such as apple slices andpersimmon pieces (Pérez-Gago et al. 2005a, b; Pérez-Gago et al. 2006). In mostcases, weight loss was not prevented with beeswax, with the exception of coatedplums and persimmon pieces (see Tables 7.1 and 7.2).
236 G.I. Olivas and G. Barbosa-Cánovas7.6.4 Other Films and CoatingsOther compounds have been used to form coatings for fruits and vegetables, suchas pullulan, gellan, aloe vera, cactus–mucilage and fruit puree. Aloe vera coatingshave been studied for their ability to preserve quality of cherries (Martínez-Romeroet al. 2006) and grapes (Valverde et al. 2005). Martínez-Romero et al. (2006) foundreduction in the microbial population of coated cherries, while control cherriesexperienced considerable increase in microbial population; aloe vera coatings alsopreserved texture and color, and decreased water loss in cherries. Valverde et al.(2005) extended storage life of grapes at 1°C from 7 to 35 days, with reduction inmicrobial load also observed for coated grapes. A cactus–mucilage film was studiedto preserve quality of strawberries (Del-Valle et al. 2005). Coatings containing a mixtureof fruit puree and hydrocolloid have likewise been used. Alginate–apple puree wasused as coating to preserve quality of apple slices (Rojas-Graü et al. 2007).7.6.5 Additives in Films and CoatingsAdditives in coatings and films have been used for different purposes. Thosealready discussed are shown in Table 7.3. Anti-browning compounds, antimicrobialagents, texture enhancers, nutrients, probiotics and flavors are examples of someadditives used in coatings. However, plasticizers are the main additives used infilms and coatings. Plasticizer is added to the formulation to improve mechanicalproperties of films and coatings. Without plasticizers, most films and coatings arebrittle, and it is difficult to form a homogenous coating. Plasticizer combines withthe main component of the film, moving the component’s chains apart, and thusreduces rigidity of the structure (Guilbert and Biquet 1996). Plasticizer also attractswater molecules around it, which reduces intermolecular interactions of the maincomponent (Ke and Sun 2001). Major plasticizers used have been polyols suchas glycerol, sorbitol and polyethylene glycol (Sothornvit and Krochta 2005), butlately, disaccharides such as sucrose and monosaccharides (e.g., fructose, glucose,and mannose) have been investigated (Zhang and Han 2006). Monosaccharideshave proved to be effective as plasticizers (Olivas and Barbosa-Cánovas 2008;Zhang and Han 2006), exhibiting films with lower WVP compared to thosecontaining polyols as plasticizers. Whey protein films that have been plasticizedwith sucrose have excellent oxygen barrier properties and display high gloss; however,sucrose tends to crystallize with time and lose its properties (Dangaran and Krochta2007). How plasticizers affect properties of films will depend on factors such astype of plasticizer (molecular size, total number of hydroxyl groups, configuration),its concentration and type of polymer. Plasticizers normally generate a homogenousmixture without phase-separation. However, some works attribute phase separationobserved between plasticizer and polymer to an excess of plasticizer or incompat-ibility between plasticizer and polymer (Aulton et al. 1981; Donhowe and Fennema1993; Ayranci et al. 1997; Jagchud and Chinnan 1999).
7 Edible Flims and Coatings for Fruits and Vegetables 2377.7 Challenges and Future TrendsNot much work has been done to identify the relationship between the internal atmos-phere caused by the coating and velocity of physiological ripening processes, suchas respiration, tissue softening, metabolic reactions, production of metabolites andsecondary compounds generated during storage. Most work in this area has dealtwith changes in quality due to application of coating. To preserve quality of fruits by means of decreasing oxygen in the internalatmosphere, special care should be taken not to minimize oxygen concentration toa point where anaerobic respiration may occur. Thus, for each fruit, it is necessaryto know the optimum oxygen concentration at which rate of consumption is mini-mized without promoting development of anaerobic respiration. Although extensive research has been done in the area of edible films and coat-ings for fresh and minimally-processed fruits and vegetables, most work has beenempirical in nature. Many factors should be studied to understand their effects oncoating performance for specific types of produce and properties such as:– Properties of coating solution: composition, concentration, viscosity and density– Properties of film: mechanical, gas and vapor barrier properties– Properties of coating: thickness, temperature, and atmospheric conditions– Properties of the produce (fresh or minimally-processed): respiration rate, water activity, composition, etcThus it is necessary to go beyond empirical studies to investigate how these factors/properties will affect the final product and how they can be controlled or modifiedto enhance quality. The study of edible coatings for fruits and vegetables deals with a wide range ofscientific fields including: chemistry, biochemistry, horticulture, food science andengineering. The final objective should be to develop edible films and coatings thatcan be marketed commercially. Thus, to place edible coatings on the market, futureresearch will need to concentrate on whole interdisciplinary works that providecomprehensive information that addresses all important issues relative to develop-ment of a specific coating for a specific product.Future research should include:– Characterization of physicochemical properties of coating solutions (composition, concentration, solubility, viscosity, density, surface tension, etc), including evaluation of how variation in chemical and physical conditions (e.g., pH, temperature, time, etc.) could affect these properties.– Characterization of films intended for use as coatings, under similar conditions as the commodity being treated. This includes gas and vapor permeability, mechan- ical and sensorial properties, thickness, solubility, digestibility, etc. Focus should be on understanding possible changes to properties of a film when chemical and physical conditions are modified, simulating likely events a commodity could face during actual handling and storage.– Study of metabolic reactions occurring within commodities and the extent to which they can be modified with coatings. This includes not only respiration,
238 G.I. Olivas and G. Barbosa-Cánovas but also metabolic reactions conducive to production of biochemicals that could be affected by modified atmosphere, or by the commodity itself while in contact and reacting with chemicals contained in a coating.– Study of internal gas composition of coated commodities and relationships between internal atmosphere and velocity of physiological ripening processes, such as respiration, metabolic reactions and production of secondary compounds during storage.– Study of impact of coatings on quality and shelf life of commodities, taking into account all possible conditions they could face during handling and storage.– Determination of optimal methods of applying coatings most conducive to obtaining high quality product at lowest possible cost.– Study of consumer acceptability of coatings.– Study of impact of edible coatings on final cost of commodities.Studies should focus on commercial viability of edible film and coating technologyfor fruits and vegetables. There is also a need to study effects of coatings on bio-chemicals and secondary metabolites.ReferencesAbeles FB, Morgan PW, Saltveit ME (1992) Ethylene in Plan Biology, 2nd edn. Academic Press, New YorkAhvenainen R (1996) New approaches in improving the shelf life of minimally processed fruit and vegetables. Trends in Food Science and Technology 7(6), 179–187Amarante C, Banks NH, Ganesh S (2001) Effects of coating concentration, ripening stage, water status and fruit temperature on pear susceptibility to friction discoloration. Postharvest Biology and Technology 21, 283–290Andres C (1984) Natural edible coating has excellent moisture and grease barrier properties. Food Processing 45(13), 48–49Anker M, Standing M, Hermansson AM (2001) Aging of whey protein films and the effect on mechanical and barrier properties. Journal of Agricultural and Food Chemistry 49, 989–995Aulton ME, Abdul-Razzak MH, Hogan JE (1981) The mechanical properties of hydroxypropyl- methylcellulose films derived from aqueous systems. Part 1. The influence of plasticizers. Drug Development and Industrial Pharmacy 7, 649–668Ayrancy E, Tunc S (2004) The effect of edible coatings on water and vitamin C loss of apricots (Armeniaca vulgaris Lam.) and green peppers (Capsicum annuum L.). Food Chemistry 87(3), 339–342Ayranci E, Buyuktas S, Cetin E (1997) The effect of molecular weight of constituents on properties of cellulose-based edible films. Lebensmittel-Wissenschaft und-Technologie 30, 101–104Bai J, Baldwin EA, Hagenmaier RD (2002) Alternatives to shellac coatings provide comparable gloss, internal gas modification, and quality for “Delicious” apple fruit. HortScience 37(3), 559–563Bai J, Hagenmaier RD, Baldwin EA (2003a) Coating selection for “Delicious” and other apples. Postharvest Biology and Technology 28, 381–390Bai J, Alleyne V, Hagenmaier RD, Mattheis JP, Baldwin EA (2003b) Formulation of zein coatings for apples (Malus domestica). Postharvest Biology and Technology 28, 259–268Baldwin EA (1994) Edible coatings for fresh fruits and vegetables: past, present, and future. In: Krochta JM, Baldwin EA, Nisperos-Carriedo MO (Eds.) Edible Coatings and Films to Improve Food Quality. Technomic, Lancaster, PA, pp. 25–64
7 Edible Flims and Coatings for Fruits and Vegetables 239Baldwin EA, Nisperos-Carriedo MO, Baker RA (1995a) Edible coatings for lightly processed fruits and vegetables. HortScience 30(1), 35–40Baldwin EA, Nisperos-Carriedo MO, Baker RA (1995b) Use of edible coatings to preserve quality of lightly (and slightly) processed products. Critical Reviews in Food Science and Nutrition 35(6), 509–524Baldwin EA, Nisperos MO, Chen X, Hagenmaier RD (1996) Improving storage life of cut apple and potato with edible coating. Postharvest Biology and Technology 9(2), 151–163Baldwin EA, Burns JK, Kazokas W, Brecht JK, Hagenmaier RD, Bender RJ, Pesis DE (1999) Effect of two edible coatings with different permeability characteristics on mango (Mangifera indica L.) ripening during storage. Postharvest Biology and Technology 17, 215–226Baldwin EA, Wood B (2006) Use of edible coating to preserve pecans at room temperature. HortScience 41(1), 188–192Banks N, Dadzie B, Cleland D (1993) Reducing gas exchange of fruits with surface coatings. Postharvest Biology and Technology 3, 269–284BeMiller JN, Whistler RL (1996) Carbohydrates. In: Fennema OR (Ed.) Food Chemistry, 3rd ed. Marcel Dekker, New York, pp. 157–223Cagri A, Ustunol Z, Ryser ET (2004) Antimicrobial edible films and coatings. Journal of Food Protection 67(4), 833–848Certel M, Uslu MK, Ozedemir F (2004) Effects of sodium caseinate- and milk protein concentrate- based edible coatings on the postharvest quality of Bing cherries. Journal of the Science of Food and Agriculture 84(10), 1229–1234Chien PJ, Sheub F, Ling HR (2007a) Coating citrus (Murcott tangor) fruit with low molecular weight chitosan increases postharvest quality and shelf life. Food Chemistry 100, 1160–1164Chien PJ, Sheu F, Yang FH (2007b) Effects of edible chitosan coating on quality and shelf life of sliced mango fruit. Journal of Food Engineering 78 (1), 225–229Cisneros-Zevallos L, Krochta JM (2002) Internal modified atmospheres of coated fresh fruits and vegetables: Understanding relative humidity effects. Journal of Food Science 67(6), 1990–1995Cisneros-Zevallos L, Krochta JM (2003a) Whey protein coatings for fresh fruits and relative humidity effects. Journal of Food Science 68(1), 176–181Cisneros-Zevallos L, Krochta JM (2003b) Dependence of coating thickness on viscosity of coating solution applied to fruits and vegetables by dipping method. Journal of Food Science 68(2), 503–510Claypool LL (1940) The waxing of deciduous fruits. American Society of Horticultural Science Proceedings 37, 443–447Curtis GJ (1988) Some experiments with edible coatings on the long-term storage of citrus fruits. Proceedings of the Sixth International Citrus Congress 3, 1514–1520Dangaran KL, Krochta JM (2007) Preventing the loss of tensile, barrier and appearance properties caused by plasticizer crystallization in whey protein films. International Journal of Food Science and Technology 42(9), 1094–1100Davies DH, Elson CM, Hayes ER (1989) N,O-carboxymethyl chitosan, a new water soluble chitin derivative. In: Skjåk-Bræk G, Anthonsen T, Sandford P (Eds.) Chitin and Chitosan: Sources, Chemistry, Biochemistry, Physical Properties and Applications. Elsevier, London, UK, pp. 467–72Debeaufort F, Martín-Polo M, Voilley A (1993) Polarity, homogeneity and structure affect water vapour permeability of model edible films. Journal of Food Science 58, 426–429, 434DeEll JR, Prange RK, Peppelenbos HW (2003) Postharvest physiology of fresh fruits and vegetables. In: Chakraverty A, Jujumdar AS, Raghava GSV, Ramaswamy HS (Eds.) Handbook of Postharvest Technology. Marcel Dekker, New York, pp. 455–484Del-Valle V, Hernandez-Munoz P, Guarda A, Galotto MJ (2005) Development of a cactus-mucilage edible coating (Opuntia ficus indica) and its application to extend strawberry (Fragaria ananassa) shelf-life. Food Chemistry 91(4), 751–756Devlieghere F, Vermeulen A, Debevere J (2004) Chitosan: antimicrobial activity, interactions with food components and applicability as a coating on fruit and vegetables. Food Microbiology 21, 703–714
240 G.I. Olivas and G. Barbosa-CánovasDong H, Cheng L, Tan J, Zheng K, Jiang Y (2004) Physicochemical properties and application of pullulan edible films and coatings in fruits preservation. Journal of Food Engineering 64, 355–358Donhowe IG, Fennema O (1993) The effects of plasticizers on crystallinity, permeability, and mechanical-properties of methylcellulose films. Journal of Food Processing and Preservation 17, 247–257El-Ghaouth A, Arul J, Grenier J, Asselin A (1992) Chitosan coating to extend the storage life of tomatoes. HortScience 27(9), 1016–1018El-Ghaouth A, Arul J, Wilson C Benhamou N (1997) Biochemical and cytochemical aspects of the interactions of chitosan and Botrytis cinerea in bell pepper fruit. Posthharvest Biology and Technology 12, 183–194Fellman JK, Rudell DR, Mattinson DS, Mattheis JP (2003) Relationship of harvest maturity to flavor regeneratin after CA storage of ‘Delicious’ apples. Postharvest Biology and Technology 27, 39–51Food and Agriculture Organization of the United Nations (2003) Increasing fruit and vegetable consumption becomes a global priority. Taken from: http://www.fao.org/english/newsroom/ focus/2003/fruitveg1.htm in 2007Ford ES, Mokdad AH (2001) Fruit and vegetable consumption and diabetes mellitus incidence among U.S. adults. Preventive Medicine 32, 33–39Garcia E, Barret DM (2002) Preservative treatments for fresh cut fruits and vegetables. In: Lamikanra O (Ed.) Fresh-Cut Fruits and Vegetables. CRC Press, Boca Raton, FL, pp. 267–304García MA, Martino MN, Zaritky NE (1998) Starch-based coatings: effect on refrigerated strawberry (Fragaria ananassa) quality. Journal of the Science of Food and Agriculture 76(3), 411–420Genkinger JM, Platz EA, Hoffman SC, Comstock GW, Helzlsouer KJ (2004) Fruit, vegetable, and antioxidant intake and all-cause, cancer, and cardiovascular disease mortality in a community- dwelling population in Washington County, Maryland. American Journal of Epidemiology 60, 1223–1233Gennadios A, Weller CL (1990) Edible films and coatings from wheat and corn proteins. Food Technology 44, 63–69Gennadios A, McHugh TH, Weller CL, Krochta JM (1994) Edible coatings and films based on proteins. In: Krochta JM, Baldwin EA, Nisperos-Carriedo MO (Eds.) Edible Coatings and Films to Improve Food Quality. CRC Press, Boca Raton, FL, pp. 201–278Gordon LR (2005) Edible and biobased food packaging materials. In: Food Packaging Principles and Practice. CRC Press, Boca Raton, FL, pp. 43–54Gorny R, Cifuentes RA, Hess-Pierce B, Kader AA (2000) Quality changes in fresh-cut pear slices as affected by cultivar, ripeness stage, fruit size, and storage regime. Journal of Food Science 65, 541–544Guilbert S, Biquet B (1996) Edible films and coatings. In: Bureau G, Multon JL (Eds.) Food Packaging Technology. VCH Publishers, New YorkHagenmaier RD, Shaw PE (1990) Moisture permeability of edible films made with fatty acid and (hydroxypropyl) methylcellulose. Journal of Agriculture and Food Chemistry 38, 1799–1803Hagenmaier RD, Shaw PE (1992) Gas-permeability of fruit coating waxes. Journal of the American Society for Horticultural Science 117(1), 105–109Han C, Zhao Y, Leonard SW, Traber MG (2004) Edible coatings to improve storability and enhance nutritional value of fresh and frozen strawberries Fragaria ananassa) and raspberries (Rubus ideaus). Postharvest Biology and Technology 33, 67–78Han JH, Seo GH, Park IM, Kim GN, Lee DS (2006) Physical and mechanical properties of pea starch edible films containing beeswax emulsions. Journal of Food Science 71(6), E290–E296Hardenburg RE (1967) Wax and related coatings for horticultural products. A bibliography. Agricultural Research Service Bulletin 51–15, USDA, Washington, DCHernandez-Munoz P, Almenar E, Ocio MJ, Gavara R (2006) Effect of calcium dips and chitosan coatings on postharvest life of strawberries (Fragaria × Ananassa). Postharvest Biology and Technology 39 (3), 247–253
7 Edible Flims and Coatings for Fruits and Vegetables 241Hoffman AF (1916) Preserving Fruit. US patent 19,160,104Hoover R, Sosulski FW (1991) Composition, structure, functionality and chemical modification of legume starches. Canadian Journal of Physiology and Pharmacology 69, 79–92Hung HC, Joshipura KJ, Jiang R (2004) Fruit and vegetable intake and risk of major chronic disease. Journal of National Cancer Institute 96, 1577–1584Jangchud, A. and Chinnan, M.S. (1999) Properties of peanut protein film: Sorption isotherm and plasticizer effect. Lebensmittel-Wissenschaft und-Technologie 32, 89–94.Jiang Y, Li J, Jiang W (2005) Effects of chitosan coating on shelf life of cold-stored litchi fruit at ambient temperature. Lebensmittel-Wissenschaft und-Technologie 38, 757–761Kader AA (1986) Biochemical and physiological basis for effects of controlled and modified atmospheres on fruits and vegetables. Food Technology 40(5), 99–104Kamper SL, Fennema O (1984) Water vapor permeability of an edible, fatty acid, bilayer film. Journal of Food Science 49(6): 1482–1485.Kays SJ (1991) Metabolic processes in harvested products. In: Postharvest. Physiology of Perishable Plant Products. Van Nostrand Reinhold, New York, pp. 75–142Kays SJ (1999) Preharvest factors affecting appearance. Postharvest Biology and Technology 15(3), 233–247Kays SJ, Paull RE (2004) Stress in harvested products. In: Postharvest Biology. Exon Press, Athens, GA, pp. 355–414Ke T, Sun X (2001) Thermal and mechanical properties of poly (lactic acid) and starch blends with various plasticizers. Transactions of the ASAE 44(4), 945–953Ke D, Yahia E, Mateos M, Kader A (1994) Ethanolic fementation of Barlett pears as influenced by ripening stage and atmospheric composition. Journal of the American Society for Horticultural Science. 32(6), 593–600Kester JJ, Fennema O (1989) An edible film of lipids and cellulose ethers: barrier properties to moisture vapor transmission and structural evaluation. Journal of Food Science 54, 1383–1389Knee M (1980) Physiological responses of apple fruits to oxygen concentrations. Annals of Applied Biology 96, 243–253Koelsch CM, Labuza TP (1992) Functional, physical and morphological properties of methyl cellulose and fatty acid-based edible barriers. Lebensmittel-Wissenschaft und-Technologie 25, 404–411Krochta JM (1997) Edible composite moisture-barrier films. In: Blakistone B (Ed.) 1996 Packaging Yearbook. National Food Processing Association, Washington, DC, pp. 38–54Lakakul R, Beaudry RM, Hernandez RJ (1999) Modeling respiration of apple slices n modified- atmosphere packages. Journal of Food Science 64, 105–110Lin D, Zhao Y (2007) Innovations in the development and application of edible coatings for fresh and minimally processed fruits and vegetables. Comprehensive Reviews in Food Science and Food Safety 6, 60–75Lourdin D, Valle GD, Colonna P (1995) Influence of amylose content on starch films and foams. Carbohydrate Polymers 27(4), 261–270Maftoonazad N, Ramaswamy HS (2005) Postharvest shelf life extension of avocados using methyl cellulose-based coatings. Lebensmittel-Wissenschaft und-Technologie 38, 617–624Maftoonazad N, Ramaswamy HS, Moalemiyan M, Kushalappa AC (2007) Effect of pectin-based edible emulsion coating on changes in quality of avocado exposed to Lasiodiplodia theobro- mae infection. Carbohydrate Polymers 68, 341–349Martínez-Romero D, Alburquerque N, Valverde JM, Guillén F, Castillo S, Valero D, Serrano M (2006) Postharvest sweet cherry quality and safety maintenance by Aloe vera treatment: a new edible coating. Postharvest Biology and Technology 39, 93–100McHugh TH, Krochta JM (1994) Milk-protein-based edible films and coatings. Food Technology 48(1), 97–103Mehyar GF, Han JH (2004) Physical and mechanical properties of high-amylose rice and pea starch films as affected by relative humidity and plasticizer. Journal of Food Science 69(9), E449–E454
242 G.I. Olivas and G. Barbosa-CánovasMei Y, Zhao Y, Yang J, Furr HC (2002) Using edible coating to enhance nutritional and sensory qualities of baby carrots. Journal of Food Science 67, 1964–1968Mencarelli F, Saltveit ME, Massantini R (1989) Lightly processed foods: ripening of tomato slices. Acta Horticulturae 244, 193–200Miller S, Krochta JM (1997) Oxygen and aroma barrier properties of edible films: a review. Trends in Food Science Technology 8, 228–37Morillon V, Debeaufort F, Blond G, Cappelle M, Voilley A (2002) Factors affecting the moisture permeability of lipid-based edible films: a review. Critical Reviews in Food Science and Nutrition 42(1), 67–89Muzzarelli RAA (1986) Filmogenic properties of chitin/chitosan. In: Muzzarelli RAA, Jeuniaux C, Gooday GW (Eds.) Chitin in Nature and Technology. New York, Plenum Press, pp. 389–396Nguyen C, Carlin F (1994) The microbiology of minimally processed fresh fruits and vegetables. Critical Reviews in Food Science and Nutrition 34(4), 371–401Nisperos MO, Baldwin EA (1996) Edible coatings for whole and minimally processed fruits and vegetables. Food Australia 48(1), 27–31No HK, Meyers SP, Prinyawiwatkul W, Xu Z (2007) Applications of chitosan for improvement of quality and shelf life of Foods: a Review. Journal of Food Science 72(5), R87–R100Olivas GI, Barbosa-Cánovas GV (2005) Edible coatings for fresh cut fruits. Critical Reviews in Food Science and Nutrition 45, 657–670Olivas GI, Barbosa-Cánovas GV (2008) Alginate-calcium films: water vapor permeability and mechanical properties as affected by plasticizer and relative humidity. LWT-Food Science and Technology 41, 359–366Olivas GI, Rodriguez JJ, Barbosa-Cánovas GV (2003) Edible coatings composed of methylcel- lulose stearic acid, and additives to preserve quality of pear wedges. Journal of Food Processing and Preservation 27, 299–320Olivas GI, Mattinson DS, Barbosa-Cánovas GV (2007) Alginate coatings for preservation of mini- mally processed “Gala” apples. Postharvest Biology and Technology 45, 89–96Paillard NMM (1979) Biosynthese des produits volatils de la pomme: formation des alcools et des esters a partir des acides gras. Phytochemistry 18, 1165–1171.Park HJ, Chinnan MS (1990) Properties of edible coatings for fruits and vegetables. American Society of Agricultural Engineers. Paper no. 90–6510. p. 19Park HJ, Weller CL, Vergano PJ, Testin RF (1993) Permeability and mechanical properties of cellulose based edible films. Journal of Food Science 58, 1361–1364, 1370Park HJ, Chinnan MS, Shewfelt RL (1994) Edible coating effects on storage life and quality of tomatoes. Journal of Food Science 59(3), 568–570Park HJ, Rhim JW, Lee HY (1996) Edible coating effects on respiration rate and storage life of Fuji apples and Shingo pears. Foods and Biotechnology 5(1), 59–63Park HJ (1999) Development of advanced edible coatings for fruits. Trends in Food Science and Technology 10, 254–260Pen LT, Jiang YM (2003) Effects of chitosan coating on shelf life and quality of fresh-cut Chinese water chestnut. Lebensmitte–Wissenschaft und Technologie 36, 359–364Peressini D, Bravin B, Lapasin R, Rizzotti C, Sensidoni A (2003) Starch-methylcellulose based edible films: rheological properties of film-forming dispersions. Journal of Food Engineering 59, 25–32Pérez-Gago MB, Krochta JM (2001) Lipid particle size effect on water vapor permeability and mechanical properties of whey protein/beeswax emulsion films. Journal of Agricultural and Food Chemistry 49, 996–1002Pérez-Gago MB, Rojas C, Del Río MA (2003a) Effect of hydroxypropyl methylcellulose–lipid edible composite coatings on plum (cv. Autumn giant) quality during storage. Journal of Food Science 68(3), 879–883Pérez-Gago MB, Serra M, Alonso M, Mateos M, Del Río MA (2003b) Effect of solid content and lipid content of whey protein isolate-beeswax edible coatings on color change of fresh-cut apples. Journal of Food Science 68(7), 2186–2191
7 Edible Flims and Coatings for Fruits and Vegetables 243Pérez-Gago MB, Serra M, Alonso M, Mateos M, Del Río MA (2005a) Effect of whey protein- and hydroxypropyl methylcellulose-based edible composite coatings on color change of fresh-cut apples. Postharvest Biology and Technology 36, 77–85Pérez-Gago MB, Del Río MA, Serra M (2005b) Effect of whey protein-beeswax edible composite coating on color change of fresh-cut persimmons cv. “Rojo Brillante.” Acta Horticulturae 682 (3), 1917–1923Pérez-Gago MB, Serra M, Del Río MA (2006) Color change of fresh-cut apples coated with whey protein concentrate-based edible coatings. Postharvest Biology and Technology 39, 84–92Platenius, H (1939) Wax Emulsions for Vegetables. Cornell University Agricultural Experimental Station Bulletin No.723. p 43Poenicke EF, Kays SJ, Smittle DA, Williamson RE (1977) Ethylene in relation to postharvest quality deterioration in processing cucumbers. Journal of the American Society for Horticultural Science 102, 303–306Quezada-Gallo J, Gramin A, Pattyn C, Diaz Amaro M, Debeaufort F, Voilley A (2005) Biopolymers used as edible coating to limit water transfer, colour degradation and aroma compound 2-pentanone lost in Mexican fruits. Acta Horticulturae 682(3), 1709–1716Ribeiro C, Vicente AA, Teixeira JA, Miranda C (2007) Optimization of edible coating composition to retard strawberry fruit senescence. Postharvest Biology and Technology 44, 63–70Rojas-Argudo C, Pérez-Gago MB, Del Río MA (2005) Postharvest quality of coated cherries cv. “Burlat” as affected by coating composition and solids content. Food Science and Technology International 11(6), 417–424Rojas-Graü M, Raybaudi-Massilia RM, Soliva-Fortuny RC, Avena-Bustillos RJ, McHugh TH, Martín-Belloso O (2007) Apple puree-alginate edible coating as carrier of antimicrobial agents to prolong shelf-life of fresh-cut apples. Postharvest Biology and Technology 45, 254–264Romanazzi G, Nigro F, Ippolito A, Di Venere D, Salerno M (2002) Effects of pre- and postharvest chitosan treatments to control storage grey mold of table grapes. Journal of Food Science 67(5), 1862–1867Rooney ML (1995) Overview of active food packaging. In: Rooney ML (Ed.) Active Food Packaging. Blackie Academic and Professional, Glasgow, pp. 1–37Rosen JC, Kader AA (1989) Postharvest physiology and quality maintenance of slices pear and strawberry fruits. Journal of Food Science 54, 656–659Saltveit ME (1997) Physical and physiological changes in minimally processed fruits and vegetables. In: Tomas-Barberan FA, Robins RJ (Eds.) Phytochemistry of Fruit and Vegetables. Clarendon Press, Oxford, New York, pp. 205–220Sams CE (1999) Preharvest factors affecting postharvest texture. Postharvest Biology and Technology 15(3), 249–254Sapers GM (1993) Browning of foods: control by sulfites, antioxidants, and other means. Food Technology 47(10), 75–84Sarkar SK, Phan CT (1979) Naturally-occurring and ethylene-induced compounds in the carrot root. Journal of Food Protection 42, 526–534Sebti I, Martial-Gros A, Carnet-Pantiez A, Grelier S, Coma V (2005) Chitosan polymer as bioactive coating and film against Aspergillus niger contamination. Journal of Food Science 70(2), M100–M104Sime WJ (1990) Alginates. In: P. Harris (Ed.), Food Gels, Elsevier Applied Science, London pp. 53–58.Sothornvit R, Krochta JM (2005) Plasticizers in edible films and coatings. In: Han JH (Ed.) Innovations in Food Packaging. Elsevier Academic Press, London, pp. 403–433Tapia M, Rojas-Graü M, Rodríguez F, Ramírez J, Carmona A, Martin-Belloso O (2007) Alginate- and gellan-based edible films for probiotic coatings on fresh-cut fruits. Journal of Food Science 72(4), E190–E196Toivonen PMA, DeEll JR (2002) Physiology of fresh-cut fruits and vegetables. In: Olusola Lamikanra (Ed.) Fresh-cut fruits and vegetables. CRC Press, Boca Raton, FL, pp. 91–123Trezza TA, Krochta JM (2000) Color stability of edible coatings during prolonged storage. Journal of Food Science 65(7), 1166–1169
244 G.I. Olivas and G. Barbosa-CánovasTuil R, Fowler P, Lawther M, Weber CJ (2000) Properties of biobased packaging materials. In: Weber CJ (Ed.) Biobased Packaging Materials for the Food Industry: Status and Perspectives. The Royal Veterinary and Agricultural University, Denmark, pp. 13–45United States Department of Agriculture, USDA (2001–2002) Agriculture Fact BookUS FDA/CFSAN (2006) Inventory of GRAS notices: summary of all GRAS notices. Available from: http://www.cfsah.fda.gov/~rdb/opa-gras.html. Accessed July 2007Valverde JM, Valero D, Martinez-Romero D, Guillen F, Castillo S, Serrano M (2005) Novel edible coating based on Aloe vera gel to maintain table grape quality and safety. Journal of Agricultural and Food Chemistry 53(20), 7807–7813Vargas M, Albors A, Chiralt A, González-Martínez C (2006) Quality of cold-stored strawberries as affected by chitosan-oleic acid edible coatings. PostHarvest Biology and Technology 41 (2), 164–171Viña S, Mugridge A, García MA, Ferreyra RM, Martino MN, Chaves AR, Zaritzky NE (2007) Effects of polyvinylchloride films and edible starch coatings on quality aspects of refrigerated Brussels sprouts. Food Chemistry 103(3), 701–709Vojdani F, Torres JA (1990) Potassium sorbate permeability of methylcellulose and hydroxypropyl methylcellulose coatings – effect of fatty-acids. Journal of Food Science 55(3), 841–846Wang LZ, Liu L, Holmes J, Kerry JF, Kerry JP (2007) Assessment of film-forming potential and properties of protein and polysaccharide-based biopolymer films. International Journal of Food Science and Technology 42(9), 1128–1138Watada AE, Abe K, Yamauchi N (1990) Physiological activities of partially processed fruits and vegetables. Food Technology 20, 116, 118, 120–122Wong DWS, Camirand WM, Pavlath AE (1994) Development of edible coatings for minimally processed fruits and vegetables. In: Krochta JM, Baldwin EA, Nisperos-Carriedo MO (Eds.) Edible Coatings and Films to Improve Food Quality. Technomic, Lancaster, PA, pp. 65–88World Health Organisation. (2002) The world health report: reducing risks, promoting healthy life. Geneva: World Health OrganisationXu S, Chen X, Sun D (2001) Preservation of kiwifruit coated with an edible film at ambient temperature. Journal of Food Engineering 50(4), 211–216Yaman Ö, Bayoindirli L (2002) Effects of an edible coating and cold storage on shelf-life and quality of cherries. Lebensmittel-Wissenschaft und-Technologie 35, 146–150Zagory D (1999) Effects of post-processing handling and packaging on microbial populations. PostHarvest Biology and Technology 15: 313–321Zhang D, Quantick PC (1997) Effects of chitosan coating on enzymatic browning and decay during postharvest storage of litchi (Litchichinensis Sonn.) fruit. Postharvest Biology and Technology 12, 195–202Zhang Y, Han JH (2006) Mechanical and thermal characteristics of pea starch films plasticized with monosaccharides and polyols. Journal of Food Science 71(2), 109–E118
246 Z. Ustunol Common covalent cross-linking agents such as gluteraldehyde, calcium chloride,tannic acid, and lactic acid are used to improve water resistance, cohesiveness,rigidity, mechanical strength and barrier properties of edible films and coatings(Guilbert 1986; Marquie et al. 1995; Ustunol and Mert 2004). Exposure to UV lightincreases cohesiveness of protein films and coatings by promoting cross-linking(Brault et al. 1997). Alternatively, enzymatic cross-linking treatments with trans-glutaminases or peroxidases can be used to stabilize films. Renewed interest in edible films and coatings in recent years has been due toconcerns about the environment and a need to reduce the amount of disposablepackaging, as well as consumer demand for higher quality food products andextended shelf life. Edible films and coatings are not intended to replace nonediblesynthetic packaging materials or to be their biodegradable counterpart. Edible filmsare secondary packaging materials; they may offer protection to a food productafter the primary packaging has been opened. They also provide food processorswith a number of new unique opportunities for product processing, handling anddevelopment. Edible films and coatings can provide protection to a food product by serving asbarriers to moisture migration, and preventing diffusion of gases important in fooddeterioration, such as O2 or CO2. They can also enhance quality and appearance ofa food product by preventing flavor and aroma migration and by providing structuralintegrity. Edible films and coatings can also serve as carriers for antimicrobials,antioxidants, nutrients, color, herbs and spices, and provide for localized or delayedactivity if needed. Currently, edible films and coatings are used in a variety of foodapplications. Collagen films and sausage casings are probably the most successfulcommercial application of edible films in meat products. This chapter reviewsapplication of edible films and coatings for meat and poultry products.8.2 Historical BackgroundEdible films and protective coatings have been used for centuries to prevent qualityloss such as shrinkage, oxidative off-flavors, microbial contamination, and discol-oration in meat and poultry products. Yuba, the first freestanding edible film, wasdeveloped in Japan from soymilk during the fifteenth century, and was used forfood preservation purposes. In sixteenth century England, cut meats were coated infats to reduce moisture loss and, thus, shrinkage in a process called “larding”(Kester and Fennema 1986). Since then, a number of lipid coating formulationshave been used to enhance quality of meat and meat products. Letney (1958) pro-posed coating meat with melted fat and letting it solidify to form a film to extendstorage life of meat products during refrigerated storage and maintain “bloom”(a term used in the industry to signify the conversion from the purple state to the redstate in the presence of oxygen). Carnauba wax, beeswax, and candelilla have beenused to coat frozen meat to increase its shelf life (Daniels 1973). Use of acylatedacylglycerol containing chlortetracycline (Ayers 1959), mixtures of mono-, di- and
8 Edible Films and Coatings for Meat and Poultry 247triacylglycerols in alcohol (Anderson 1960, 1961a, b), and acetylated mono- anddiacylglycerol coatings have been suggested to reduce off-flavors and moistureloss, as well to maintain color and prevent freezer-burn in meat products.Applications of paraffinic acid mono-, di- and triacylglycerol with or withoutcarboxylic acid have also been reported to improve meat quality and storage life(Schneide 1972). Other researchers have reported application of acetylated monoa-cylglycerol in vacuum-packed meats (Griffin et al. 1987; Leu et al. 1987). Emulsioncoatings containing lipids have also been demonstrated to be useful in enhancingmeat quality (Zabik and Dawson 1963; Bauer et al. 1968; Bauer and Neuser 1969;Kroger and Igoe 1971; Hernandez 1994; Baldwin et al. 1997). Films and coatingsmade from lipids alone, however, lack structural integrity and are brittle. Hirasa(1991) reported that highly saturated acetylated monoacyglycerol coatings tend toflake and crack during cold storage and have bitter aftertaste (Morgan 1971). Also,unsaturated acylglycerols are susceptible to oxidation. More recently, lipids havebeen incorporated in formation of composite protein or polysaccharide films toimprove moisture barrier characteristics and provide flexibility to these films(Baldwin et al. 1995). Various edible polysaccharide films and coatings such as starch and its deriva-tives, alginates, carrageenans, cellulose ethers and pectin also have been used toimprove quality of meat and poultry products (Kester and Fennema 1986).Polysaccharide films are nongreasy and have visual appeal, which make themdesirable for application as wraps in meat products (Labell 1991). They are goodbarriers to gases; however, because of their hydrophilic nature, they are poor barriersto moisture. Alginate coatings require a gelling agent, such as calcium chloride,which may impart bitterness (Earle 1968; Lazarus et al. 1976; Williams et al. 1978).Earle (1968) reported extending shelf life of meat products by coating them withan aqueous solution of algin and dextrose, followed by application of calcium solu-tion. Carboxymethylcellulose (CMC) has been reported to improve adhesion ofbreading after baking when used in commercial breading mix (Suderman et al.1981). Other derivatives of cellulose, methylcellulose (MC) or hydroxypropylmethylcellulose (HPMC) form reversible thermal gels, and have been used to pro-duce glazed sauces for poultry and seafood. This treatment minimizes runoff duringcooking, thereby reducing moisture loss (Baker et al. 1994). Protein films and coatings have also been investigated throughout history toenhance quality of meat and poultry products. In the nineteenth century, use ofgelatin films to preserve meat was proposed by Harvard and Harmony (1869) andMorris and Parker (1896). Patents as early as 1869 disclose gelatin-based films(Gennadios et al. 1997). Additional patents have been granted for acidic, aqueoussolutions of gelatin and a metaphosphate polymer (Keil et al. 1960), and aqueoussolutions of metal gelatinates (Keil 1961) as coatings on processed meats such assausages, Canadian bacon, and boned hams to inhibit mold growth and lipid oxida-tion, and reduce handling damage. Incorporation of polyhydric alcohols (i.e., pro-pylene glycol, ethylene glycol, glycerol, or sorbitol) into gelatin-film-formingsolutions produce quick-setting, flexible films that exhibit good barrier properties(Whitman and Rosenthal 1971). Gelatin films have been applied to poultry products
248 Z. Ustunolto prevent microbial growth and moisture loss and retard oil absorption during frying.Gelatin films also have been used as carriers of antioxidants for poultry products(Klose et al. 1952; Childs 1957; Gennadios et al. 1997). Villegas et al. (1999)reported on improved oxidative stability and color retention in frozen meat piecesused as pizza topping when they were gelatin-coated. However, gelatin films lack the strength of those from collagen. Today, reconsti-tuted or regenerated collagen films and sausage casings are probably the mostsuccessful commercial applications of edible films in the meat industry. Collagenfilms are used as wraps in hams and netted roast (Gennadios et al. 1997). Sausagecasings are used in sausage production to hold meat batter together until it is heat-setto obtain the desired shape, form, and size (Wang 1986). Natural casings have been the traditional sausage casings used throughout his-tory. The collagen casing came about as a more sanitary and uniform alternativeto gut casings. Compared to natural casings, they also have improved strength andflexibility and, therefore, better machinability. Collagen casings provide for moreuniform products and better control of net product weight at high processingspeeds. In addition, because of rapid uptake of smoke and smoke color by colla-gen, the smoking cycle may be shortened, thereby reducing product shrinkage dueto smoking. Historical development of the collagen casing has been reviewed byHood (1987). The coating of meat with gelatin obtained from partially hydrolyzedcollagen is believed to be the origin of modern casing technology. However, a lackof collagen-like fibrillar structure within gelatin films has limited commercialdevelopment of gelatin-based casings, owing to their inelasticity and brittleness(Hood 1987). The work of German scientist Oscar Becker during the 1920s and 1930s onsynthetic collagen casings is believed to have led to manufacture of regeneratedcollagen casings, particularly those based on the dry extrusion principle (Becker1936, 1938, 1939). Historically, industrial manufacture of collagen casings isdivided into two distinct processes. Collagen casings have been produced fromcorium (the flesh side) of cattle hides using a “dry” process (“dry spinning technology”)originally developed in Europe during the 1930s or the “wet” process (“wet spinningtechnology”) developed in the 1960s in the United States. The dry process involves alkaline treatment of hide coriums followed by acidi-fication to pH 3. Acid-swollen coriums are then shredded to preserve maximumfiber structure of collagen, and are mixed to produce a dough high in solids (>12%solids). Plasticizers and cross-linking agents are added, and dough is pumped andextruded to form tubular casings followed by drying, conditioning, neutralizing,and/or providing for additional cross-linking. This process produces a tough casing,which was not acceptable to American sausage makers and therefore was notadopted by US casing manufacturers. In contrast, the wet process starts with acid-or alkaline-dehairing of cattle hides. The hide corium is decalcified, ground andmixed with acid to produce a swollen slurry of 4–5% solids using high shearhomogenization. Cellulose and carboxymethylcellulose may be added to improvemechanical properties of the casing. The slurry is then homogenized and extruded,after which it passes through a coagulation bath of brine and shaped into a tubular
8 Edible Films and Coatings for Meat and Poultry 249casing. Casings are washed free of salts, and treated with plasticizing and cross-link-ing agents to provide for improved flexibility and strength, respectively. They arethen shirred (or collapsed like an accordion) to fit over various-sized sausage stuffinghorns, dried to 13–18% moisture, sealed in plastic bags and packaged (Hood 1987).Their shelf life depends upon maintaining favorable temperature and relativehumidity conditions during storage. Proper alignment of the collagen fibers is important in obtaining desirable prop-erties for collagen casings. Orientation of the fibers in the direction of extrusion isundesirable because the casing can be readily split or torn lengthwise. Extrusionshould realign collagen fibers as they exit the orifice of the extruder to produce awoven, crosshatched, fibrous collagen casing structure. The design of the extruderrotating disc and its action has a critical role in arrangement of collagen fibers,influencing strength and flexibility of the final collagen casings. The wet extrusionprocess typically produces shorter collagen fibers and provides for faster processingand larger production volumes. Dry extrusion technology produces thicker, longercollagen fibers and more expensive casings (Hood 1987). A number of patents have been issued on improvements to collagen casings.Burke (1976) described a process for preparing collagen casings from limed bovinehide collagen that was soaked in an edible acid at pH < 5.5. Hides were then neu-tralized and washed, ground and formed into collagen slurry, and processed intocollagen casings. Wilson and Burke (1977) reported that water and a mixture ofpartial fatty acid esters of glycerin and sorbitol could be used to coat the inside ofunshirred collagen casings to improve the shirring process. Ziolko (1977, 1979)produced tubular collagen casing by extruding two gel “ropes” from collagen, witheach individual rope consisting of several smaller ropes. The casing extruder wasequipped with inner and outer orifices and extruded the ropes, orienting fibers inthe direction of extrusion. Directing them outward in a radial and helical directionformed the first tubular layer; the second tubular layer was formed by directinginward in a radial and helical direction opposite from the first layer that was con-centric to the first. The two layers were then united by a hardening step. It is important that a sausage casing be able to stretch and shrink to withstandcontraction and expansion of meat batter during various steps of processing(Schmidt 1986). Collagen casings must be strong enough to withstand the rigorsof high-speed filling and linking, as well as to withstand high temperature andhumidity conditions encountered during sausage manufacturing. Collagen fibercontent, drying conditions, and extent of cross-linking influence the strength ofcollagen casings. Cross-linking agents, such as gluteraldehyde, provide forstronger and more coherent films of collagen fibrils that possess improved longi-tudinal and transverse strength, regardless of whether the casing is re-wetted ordry (Rose 1968). Glyceraldehyde (which lacks toxicity associated with other alde-hydes used for cross-linking) also promotes cross-linking of fibrils and increasesfilm strength and temperature resistance (Gennadios et al. 1994).Carboxymethylcellulose and salt treatments prevent disintegration of collagencasings during high-temperature cooking or frying (McKnight 1964a, b). UV irra-diation of 180–420 nm increased collagen casing strength (Miller and Marder 1998).
250 Z. UstunolTsuzuki and Lieberman (1972) reported that enzymatic treatments employed inmanufacture resulted in collagen casings with a more uniform diameter, greaterthickness, and increased tenderness. Addition of protease from Aspergillus niger var.macroporous to collagen batter partially solubilized collagen prior to the extrusionstep. Similarly, Miller (1983) reported that the wet process could be improved byincorporating proteases such as papain, bromolain, ficin, fungal protease, trypsin,chymotrypsin, or pepsin into the collagen batter prior to extrusion. Boni (1988)reported that mechanical properties of collagen casings at low temperatures wereimproved by incorporating an alkyl diol into the collagen batter to reduce intermo-lecular hydrogen bonding and increase molecular spacing. More recently, coatingof sausage batter with a thin layer of collagen material has been accomplished byco-extruding sausage batter and collagen (Deacon and Kindleysides 1973; Hood1987; Smits 1985; Waldman 1985; Kobussen et al. 1999). In addition to collagen, other proteins such as casein, whey proteins, soy protein,wheat gluten, corn zein and egg albumin have also been investigated in the produc-tion of edible films and coatings for meat applications (Ben and Kurth 1995). Suchfilms are good barriers to gases such as oxygen and carbon dioxide, and adhere wellto hydrophilic surfaces. But being hydrophilic in nature, these coatings are typicallypoor barriers to moisture, limiting their application in meat products (Gennadiosand Weller 1990; Baldwin et al. 1995). Also, there has been some concern regardingtheir potential allergenicity, especially in the use of milk, egg, peanut, soybean andrice proteins in films and coatings.8.3 Technical Developments8.3.1 Protein-Based Films and CoatingsCo-extrusion technology is an alternative to the conventional method of stuffingsausage batter into a preformed collagen casing for manufacture of sausage(Deacon and Kindleysides 1973). Smits (1985) further refined the process. Thisprocess involves simultaneous co-extrusion of collagen and sausage emulsion tocreate a thin layer of collagen coating at the meat batter surface. The end of theextruder barrel is equipped with a nozzle through which sausage batter flows out.A thin layer of collagen suspension is extruded directly onto the surface of thesausage as it is pumped through the extruder. Counter-rotating concentric cones areemployed to orient the collagen fibers in a woven structure. MC is incorporated toprovide additional strength to the casing and reduce its disintegration during cooking(Hood 1987). The collagen-coated sausage is then immersed in a brine bath tofurther set the collagen casing. Smoking and drying of sausages in subsequent stepsallow further interactions between the collagen fibers and meat proteins. Co-extrusionproduces a casing that is more tender than preformed or reconstituted collagencasings (Waldman 1985). Smits (1985) has described a continuous co-extrusion
8 Edible Films and Coatings for Meat and Poultry 251process that is capable of large production volumes. Over the years, various modi-fications to the co-extrusion process have been reported. Kobussen et al. (1999)developed a modified extrusion attachment for sausage stuffing machines. Thisattachment consists of three passageways, where meat emulsion is extruded fromtwo passageways and is coated with a thin layer of extruded collagen pumpedthrough the third passageway. The collagen coating is set with liquid smoke and adehydrating agent (i.e., alkali or salt solution) to produce a casing that is strongenough that it can be twisted to produce sausage links. The “hybrid technology” for manufacture of collagen casings was described byOsburn (2002). This technology combines fundamentals of dry and wet processingtechnologies described previously for collagen-casing manufacture. In the hybridprocess, collagen slurry (no more than 5% collagen) is prepared similar to wetprocessing (dehairing of cattle hides by acid or alkaline, decalcification, grindingand mixing with acid to produce swollen slurry, high shear homogenization). Thetubular collagen casing is extruded, and inflated with an ammonia–air mixture toprevent the collapse of the casing. In the next steps, the casing tube is flattened,washed and plasticized in sequence in a manner similar to the wet extrusion process.Then, the casings are re-inflated, dried, and shirred. The hybrid process producescollagen casings with improved tensile strength and smaller diameter. They areusually straight and suitable for manufacture of small sausage casings. But thisprocess is limited in the manufacturing of larger diameter and longer sausage casingsand where curved casings may be needed. Collagen is also used for production of sheet films (cut to the dimensions requiredby the customer) and in rolls (continuous film reeled on a cylindrical core; typicalfilm length: 50 m or 100 m; typical film widths between 380 and 620 mm), whichare used as wraps for netted meats, such as hams or roasts, to prevent the elastic netfrom sticking to the meat product (Gennadios et al. 1997). In the course of the cook-ing and smoking process, the collagen film becomes an integral component of themeat, allowing the elastic net to be easily removed from finished product withoutdoing harm to the meat surface, providing for an attractive appearance. Collagenfilms are also reported to reduce shrink loss and increase juiciness in these nettedproducts. Farouk et al. (1990) studied Coffi®, an edible collagen film (BreechteenCo.) widely used in specialty smoked meats and roasted meat products, which areheat-processed in elastic stretch netting or coarse stockinette. They observed signifi-cant reduction in exudation of meat products, including beef round steaks, uponwrapping in Coffi® compared to unwrapped controls. However, wraps had no signifi-cant effect on color or lipid oxidation of the meats. Over the years, the growing US processed-meat industry has relied heavily onimported collagen to meet the needs of production. Since the late 1990s, the safetyof imported collagen has become a concern owing to the link between bovinespongiform encephalopathy (BSE or “mad cow” disease) and Creutzfeldt–Jacobdisease, a highly fatal disease in humans. On May 20, 2003, the USDA placed animport restriction on ruminant material coming from Canada because of possiblerisk of BSE. Whey protein-based films and casings have been proposed as alterna-tives to collagen films and sausage casings (Kim and Ustunol 2001a–c; Simelane and
252 Z. UstunolUstunol 2005; Amin and Ustunol 2007). Kim and Ustunol (2001a) developed wheyprotein/lipid emulsion edible films that were heat-sealable, and could be formedinto tubular casing. They reported increased hydrogen and covalent bonding(involving C–O–H and N–C) as the main forces responsible for the sealed jointformation of the films. These films were further modified through heat-curing tomake them more closely resemble collagen films that would be amenable to hot dogmanufacture (Amin and Ustunol 2007). Heat-cured films were further tested undervarious combinations of time, temperature and relative humidity typically encoun-tered in meat processing. Manufacture of whey protein-based sausage casings isviable because of the high film degradation temperatures (>130°C) and heat seal-ability of these whey-based films. Furthermore, the ability of these films to with-stand temperature/time/relative humidity conditions that would be typicallyencountered during sausage manufacturing has confirmed their suitability (Simelaneand Ustunol 2005). The same research group subsequently developed heat-sealable whey protein–basedcasings containing sorbic acid, p-aminobenzoic acid, or sorbic acid–p-aminobenzoicacid (1:1) for use in hot dog manufacture, and compared these casings to commercialcollagen and natural casings (Cagri et al. 2002, 2003). Antimicrobial properties of thesecasings are further discussed in Sect. 8.3.5. Limited information exists on use cereal and oilseed proteins (i.e., soy pro-tein, wheat gluten, corn zein) as edible films in meat and poultry applications.Corn zein and corn zein–tocopherol coatings were reported to reduce lipid oxi-dation in precooked pork chops, but did not retard shrinkage (Hargens-Madsenet al. 1995). Herald et al. (1996) reported that addition of an antioxidant, emulsifierand plasticizer to corn zein films reduced rancidity in cooked turkey breastslices; however, they also reported production of off-flavors. Kunte (1996)reported that a 7S soy protein fraction-based coating was not effective in pre-venting warmed-over flavor (WOF) formation in pre-cooked chicken breast,compared to phosphates. Soy protein and wheat gluten coatings were shown tobe as effective as polyvinyl chloride films in reducing moisture loss on coatedprecooked beef patties during 3 days of refrigerated storage (Wu et al. 2000).Furthermore, both soy protein and wheat gluten coatings reduced lipid oxida-tion, as indicated by decreased thiobarbituric acid and hexanal values, for coatedmeat samples relative to those that were not coated. Rhim et al. (2000) reportedthat wheat gluten and soy protein coatings were as effective as polyvinyl chloridefilms in reducing moisture loss. Wheat gluten coatings were also effective inreducing lipid oxidation.8.3.2 Lipid Films and CoatingsLipids suitable for use in edible films and coatings include waxes (i.e, candelilla,carnauba, beeswax), acylglycerol (vegetable or animal origin), as well as fatty acidsand derivates (Kester and Fennema 1986). Lipids, because of their hydrophobicity
8 Edible Films and Coatings for Meat and Poultry 253and tightly packed crystalline structure, are good barriers to moisture and gasmigration. Their effectiveness, however, is dependent on lipid type, chemical struc-ture, chemical arrangement, polarity/hydrophobicity and physical state (solid orliquid), and on its interactions with other components (i.e., proteins and polysac-charides). Lipid films and coatings lack structural integrity, and do not adhere wellto hydrophilic surfaces (Ben and Kurth 1995). Lipids are also used with proteinsand polysaccharides in production of composite films and coatings to improvemoisture barrier characteristics and provide flexibility (Baldwin et al. 1995). Theycan also serve as “release agents” or lubricants to prevent coated foods from stick-ing together or from sticking to other surfaces such as packaging material (Baldwinet al. 1995). “Larding” is a process of coating meats with fat to extend shelf life, and waspracticed in sixteenth century England. Fats are still used today to coat a variety offoods, including fresh and frozen meat and poultry (Hernandez 1994). McGarth(1955) reported that a coating of wax eliminated downgrading of fresh meats dueto discoloration. The wax provided a transparent, attractive coating that alsoafforded ease in handling product at the supermarket by minimizing mechanicaldamage. Since then, carnauba wax, beeswax, and candelilla, have been used suc-cessfully to coat frozen meat pieces to reduce dehydration during frozen storage(Daniels 1973). Letney (1958) used molten fats as coatings by allowing them tosolidify over fresh meat surfaces to form a film/coating to lengthen storage life atrefrigerated temperatures, lessen surface hydration and maintain “bloom.” Ayers(1959) reported that an acetylated acylglycerol coating with incorporated chlortet-racycline was effective in reducing off-flavors and retaining moisture; however, itproduced an unappealing meat color. Three patents for lipid-based coatings wereissued to Anderson (1960, 1961a, b). Coating solutions, containing 40% mono-,di- and tri-acylglycerol in alcohol, were heated to 50°C, and sprayed directly on themeat surface or applied to meat products in the molten state by dipping. Althoughinitial studies with fresh lamb were not successful, application of coatings to otherfresh meats prior to freezing improved color and texture. Schneide (1972) coatedbeef, veal, pork steaks and fish fillets with different compositions of mono-, di- andtriacylglycerols of paraffinic and/or carboxylic acids to improve keeping quality ofmeat and maintain its desirable sensory properties. Stemmler and Stemmler (1976)described coating formulations containing cellulose proprionate and acetylatedmonoacyglycerol (obtained from lard) used to prolong freshness, color, aroma,tenderness and microbiological stability of fresh beef and pork cuts. Heine et al.(1979) reported that an acetylated mixture of fatty acid mono-, di-, and triacylglyc-erols applied to fresh beef and pork pieces helped retain desirable color and reducedmoisture loss during 14 days of refrigerated storage. A product called Myvacet®(Eastman Chemical Products, Inc., Kingsport, TN), a distilled acetylated monoa-cylglycerol, has been marketed as a protective coating for frozen poultry. It isapplied as a dip or spray prior to the freezing of meat; the coating is then left onproduct during cooking (Hernandez 1994). Griffin et al. (1987) and Leu et al.(1987) coated vacuum-packaged strips of loins and top rounds with an acetylatedmonoacylglycerol coating. They observed no differences in microbial counts, color,
254 Z. Ustunolor odor of vacuum-packaged steaks or roasts after 4 and 7 weeks of refrigeratedstorage, respectively. Acetostearin films have also been reported to provide oxida-tive stability when used on meat surfaces, whereas acetoolein films were less resist-ant to oxidation (Feuge 1955; Baldwin 1994). Water-in-oil emulsions from animal fats or vegetable oils have been used asprotective coatings and as flavor carriers for meat and poultry products (Baueret al. 1968; Hernandez 1994; Baldwin et al. 1997). Emulsion coatings were effec-tive in protecting frozen chicken pieces and pork chops from dehydration. Increasedmeat yield, decreased moisture loss and flavor, and improved tenderness wereobserved when these meats were coated (Zabik and Dawson 1963; Kroger and Igoe1971; Baldwin et al. 1997). Addition of MC to water-in-oil emulsion coatingsprovided for more stable coatings at lower temperatures and prevented excessivemoisture loss during cooking for pork, beef, chicken, comminuted meat, sausages,fish and seafood (Bauer and Neuser 1969).8.3.3 Polysaccharide Films and CoatingsStarch, alginate, dextrins, pectin, chitosan and carrageenans are used in polysac-charide films and coatings. Water-soluble polysaccharides are long-chain polymersthat are typically used in foods for thickening and/or gelling abilities (Glicksman1983; Whistler and Daniel 1990; Nisperos-Carriedo 1994). Polysaccharide films aregood barriers to gases, and possess resistance to fats and oils; however, theirhydrophilic nature makes them poor water vapor barriers (Ben and Kurth 1995).They have been used to extend shelf life of meat and poultry products by retardingdehydration, oxidative rancidity and surface browning. The ability of some polysac-charides (e.g., methylcellulose) to form thermally induced gelatinous coatings hasalso made them desirable for reducing oil absorption during frying (Nisperos-Carriedo 1994). Starch, being one of the largest component biomasses produced on earth, is abun-dant and readily available for use in edible films and coatings. Starch is availablefrom different botanical sources, including wheat, corn, rice, potato, cassava, yam,and barley, among others; corn represents the major commercial source (Riaz 1999).There are also several genetic mutant varieties of corn created to alter starch contentand the ratio of amylose to amylopectin, the two main polymers of starch. Starch-based films are similar to plastic films in their properties; they are odorless, tastelessand colorless. They are nontoxic, biologically absorbable and semipermeable tocarbon dioxide and are good barriers to oxygen (Nisperos-Carriedo 1994). Ediflex®,an extruded hydroxypropylated high-amylose starch film, was developed and usedas a wrap for frozen meats and poultry in the late 1960s (Anonymous 1967; Krogerand Igoe 1971; Morgan 1971; Sacharow 1972). Ediflex® was flexible, a good oxy-gen barrier, oil-resistant and heat-sealable, and therefore was effective in protectingmeat products during frozen storage. The coating also dissolved during thawing andcooking (Kroger and Igoe 1971; Morgan 1971; Sacharow 1972).
8 Edible Films and Coatings for Meat and Poultry 255 Alginates are derived from brown seaweed and, in the presence of divalentcations, produce films that are particularly useful for applications that enhancequality of meat and poultry products (Kester and Fennema 1986; Nisperos-Carriedo 1994). Calcium is the most common and effective divalent cation ingelling alginates, though magnesium, manganese, aluminum, ferrous, or ferricions are also used (Kester and Fennema 1986). At levels of 5 M or greater, calciumchloride may provide a bitter taste to foods, so other calcium salts may be substi-tuted or lower levels used (Baker et al. 1994). Alginate film strength may furtherbe improved in the presence of modified starches, oligosaccharides or simplesugars (Gennadios et al. 1997). Allen et al. (1963) coated beefsteaks, pork chops and chicken drumsticks inalginate or cornstarch by dipping them first in coating solution and then in calciumchloride solution. Coatings were effective in reducing moisture loss and, therefore,shrinkage during 1 week of refrigerated storage. They also provided improvedjuiciness, texture, color and odor within the meats. However, calcium chloride con-tributed a bitter taste. Calcium gluconate, nitrate, or proprionate provides moreacceptable flavor; however, due to their weak ionizing properties, the coatings arenot as strong as those formed with calcium chloride (Allen et al. 1963; Hartal1966). Lazarus et al. (1976) reported that alginate coatings gelled by calcium chlo-ride reduced weight loss of lamb carcasses during refrigerated storage. Althoughthe alginate coatings were not as effective as plastic films in preventing weight loss,bacterial counts were significantly reduced in the alginate-coated carcasses. Inother studies, alginate coatings were not reported to affect cooking loss, flavor,odor, or overall acceptability of coated beef (Mountney and Winter 1961), pork(Nisperos-Carriedo 1994) and poultry products (Williams et al. 1978). Alginatecoatings also did not decrease weight loss, off-odor and drip of beef cuts comparedto noncoated controls (Williams et al. 1978). The coated meats were acceptable inflavor, tenderness, appearance and cooking loss. However, after 4.5 months ofrefrigerated storage, drying of the coating was noted. As consumer demand for more convenient foods has increased, considerableresearch effort has been focused on improving quality of precooked meat products.Precooked meat products are susceptible to lipid oxidation, which results in a ran-cid or warmed-over flavor (WOF) during refrigerated storage (Tims and Watts1958; St. Angelo et al. 1987; Love 1988). Moisture loss is also a critical factoraffecting quality and shelf life of precooked meats. Among the many techniquesused, edible films and coatings have also been studied as a means for controllingquality of precooked meats. Wanstedt et al. (1981) observed that alginate-coatedprecooked, frozen and stored pork patties had reduced oxidative off-flavors (thus,WOF), better sensory properties and greater desirability than the uncoated controls.Coatings of starch–alginate, starch–alginate–tocopherol and starch–alginate–rosemaryhave been reported to reduce WOF in precooked, refrigerated pork chops and beefpatties (Hargens-Madsen et al. 1995; Ma-Edmonds et al. 1995; Handley et al.1996). Starch–alginate–stearic acid composite films were effective in controllinglipid oxidation, WOF and moisture loss in precooked ground beef patties (Wu et al.2001). Tocopherol-treated films were more effective than the non-tocopherol controls;
256 Z. Ustunolhowever, none of the films was as effective as polyester vacuum bags in retardingmoisture loss and lipid oxidation. Cellulose and its derivatives also produce edible films and coatings that arewater-soluble, tough, flexible and resistant to fats and oils (Krumel and Lindsay1976; Baldwin et al. 1995). However, their application to meat and poultry productshas been limited. Ayers (1959) reported that application of methylcellulose (MC)–lipid coatings prevented desiccation and extended shelf life of beefsteaks. Thesecoatings were transparent and peeled easily. MC and HPMC coatings on meats andpoultry are used during deep fat frying to reduce oil uptake and moisture loss(Balasubramaniam et al. 1997; Meyers 1990), and extend shelf life of the frying oil(Balasubramaniam et al. 1997; Holownia et al. 2000). They can also help main-tain integrity of the breading or batter during frying. Specifically, CMC has beenshown to improve breading adhesion (Suderman et al. 1981). Carrageenan is a complex mixture of polysaccharides extracted from redseaweed (Nisperos-Carriedo 1994). Carrageenan-based coatings have been reportedto extend shelf life of poultry (Pearce and Lavers 1949; Meyers et al. 1959).Carrageenan and agar (another seaweed-derived polysaccharide) coatings containingantibiotics were shown to extend shelf life of coated poultry (Meyers et al. 1959)and beef (Ayers 1959), though coatings did not reduce moisture loss. More recently,incorporation of nisin (a bacteriocin) into agar coatings together with food-gradechelators (EDTA, citric acid, or polyoxyethylene sorbitan monolaureate) effec-tively reduced levels of Salmonella typhimurium on poultry products (Natrajan andSheldon 1995). Limited reports are available on application of chitosan and pectin films andcoatings to meat and poultry products. Stubbs and Cornforth (1980) showed thatcalcium pectinate gel coatings significantly reduced shrinkage and bacterial growthfor beef patties.8.3.4 Composite FilmsA single-component film generally has either good barrier or good mechanicalproperties, but typically not both. Thus, multiple components are often combinedto form composite films with desired properties. Polysaccharides and proteins,owing to their intermolecular interactions, form films and coatings that have goodstructural integrity and mechanical properties; but they are generally not effectivebarriers to moisture because of their hydrophilic nature. Lipids, on the contrary, aregood barriers to moisture as a result of their hydrophobic character, though theirfilms lack structural integrity, are brittle, and do not adhere well to hydrophilicsurfaces. In formation of composite films and coatings, two or more components arecombined to improve mechanical properties, gas exchange, adherence to surfacesand/or moisture barrier properties (Baldwin et al. 1995). They may be applied asemulsions or bi-layers. Plasticizers, such as glycerol, polyethylene glycol, or sorbi-tol, may be added to modify film mechanical properties and provide increased
8 Edible Films and Coatings for Meat and Poultry 257flexibility (Ben and Kurth 1995). Cross-linking of proteins with enzymes (e.g.,transglutaminase) or polysaccharides with polyvalent ions (e.g., calcium cations)may be employed during the film-forming process, and various additives to improvespecific film attributes may also be incorporated. Ben and Kurth (1995) reportedthat clarity of caseinate–lipid composite films could be improved by addition ofthree enzymes to cross-link sodium caseinate molecules. Resulting films hadimproved appearance, and meat was juicier because of reduced drip loss. Packagingwaste and handling was also reduced owing to the elimination of an absorbent pad(Ben and Kurth 1995).8.3.5 Antimicrobial Films and CoatingsEdible films and coatings can serve as carriers for a wide range of food additives,including antimicrobials, which can reduce microbial growth at meat and poultrysurfaces to improve product safety and extend product shelf life. The primaryadvantage of antimicrobial edible films and coatings is that inhibitory agents inthese films can be specifically targeted to postprocessing contaminants on the foodsurface, with diffusion rates of antimicrobials into the food product being partiallycontrolled by properties of the antimicrobial agent itself, as well as the propertiesof the film. As consumer demand for convenience continues to increase, demand for ready-to-eat (RTE) foods will also continue to grow. Quality, safety and shelf life of RTE foodsis often dictated by the type and numbers of pathogenic and spoilage bacteria presenton the food surface. Approximately two-thirds of all microbiologically related class Irecalls in the United States result from postprocessing contamination during subse-quent handling and packaging, as opposed to processing itself. Most of these recallsare prompted by contamination with Listeria monocytogenes, for which the UnitedStates has maintained a policy of zero tolerance since 1985. From January 1998 toFebruary 2003, over 130 Listeria-related class I recalls involving more than 80 mil-lion pounds of cooked RTE meats have been issued (CDC 2000). More than 35 mil-lion pounds of hot dogs and luncheon meats were voluntarily recalled in 1998 by oneMichigan manufacturer in response to an outbreak that resulted in 101 cases of liste-riosis (including 21 fatalities) spread across 22 states. Two years later, another liste-riosis outbreak involving 29 cases and ten states (including seven fatalities) promptedrecall of approximately 14.5 million pounds of turkey and chicken delicatessen meat;again, the product became contaminated with L. monocytogenes after processing(USDA-FSIS 2001). More recently, the largest product recall ever issued, 27.4 mil-lion pounds of fresh and frozen RTE turkey and chicken products, was linked toanother major outbreak of listeriosis emanating from a manufacturer in Pennsylvania.Each year, approximately 2,300 cases of foodborne listeriosis are reported in theUnited States at an estimated cost of $2.33 billion (~$1 million per case), makingL. monocytogenes the second costliest foodborne pathogen after Salmonella (2.38billion) (USDA-FSIS 2001).
258 Z. Ustunol Product slicing and packaging operations are points at which both pathogenicand spoilage organisms can be introduced to cooked RTE foods. In commercialmanufacturing facilities, slicing of RTE meat products can easily increase micro-bial population 100-fold or greater (Cagri et al. 2004). Heightened consumerdemand for enhanced keeping quality and freshness of RTE foods has given rise tothe concept of active packaging – a type of packaging that alters conditions sur-rounding the food to maintain product quality and freshness, improve sensoryproperties, or enhance product safety and shelf life. A specific function of activepackaging includes restriction of antimicrobial activity through controlled diffusionof one or more antimicrobial agents from packaging material into the product.Antimicrobial edible films and coatings can potentially serve as active food packagingmaterials by altering permeability of a product to water vapor and oxygen, as wellas by minimizing growth of surface contaminants during refrigerated storage, pro-viding an alternative to postprocess pasteurization for inactivation of surfacecontaminants. Some of the more commonly used preservatives and antimicrobials in ediblefilms and coatings include benzoates, proprionates, sorbates, parabens, acidifyingagents (e.g., acetic and lactic acids), curing agents (e.g., sodium chloride andsodium nitrite) bacteriocins, and natural preservatives (e.g., natural oils, lysozyme,liquid smoke) (Cagri et al. 2004). Antifungal compounds, organic acids, potassiumsorbate, or the bacteriocin, nisin, were reported to be more effective in reducinglevels of foodborne microorganisms when immobilized or incorporated into ediblegels (i.e. starch, carrageenan, waxes, cellulose ethers, or alginate) and applied tomeat surfaces than when these agents were used alone (Cutter and Sumner 2002). Incorporation of antibiotic and antifungal compounds into carrageenan filmswas reported by Meyers et al. (1959), who showed a two log reduction in bacterialcounts at the surfaces of coated poultry products. Hotchkiss (1995) reported incor-porating antimycotics into wax and cellulose-based coatings. Siragusa and Dickson(1993) reported that organic acids were more effective in reducing L. mono-cytogenes, S. typhimurium and E. coli O157:H7 levels on beef carcasses whenthey were immobilized in calcium alginate gels (and applied), compared to when theywere applied alone. Baron (1993) verified that potassium sorbate and lactic acidincorporated into an edible cornstarch film inhibited growth of S. typhimurium andE. coli O157:H7 on surfaces of poultry. Incorporation of the bacteriocin, nisin, intocalcium alginate gels was investigated by Cutter and Siragusa (1996, 1997). Theyshowed greater reductions in bacterial populations and greater retention of nisinactivity on both lean and adipose beef surfaces when nisin was immobilized in analginate gel matrix, compared to controls that were treated with only nisin. Natrajanand Sheldon (2000) reported that incorporation of nisin and chelators into protein-and polysaccharide-based films inhibited growth of Salmonella on poultry skin.Control of L. monocytogenes at the surface of refrigerated RTE chicken wasachieved with edible zein film coatings containing nisin and/or calcium propionate(Janes et al. 2002). McCormick et al. (2005) reported that wheat gluten filmscontaining nisin were effective in reducing populations of L. monocytogenes, butwere not effective against S. typhimurium. Inhibition of L. monocytogenes was
8 Edible Films and Coatings for Meat and Poultry 259demonstrated on turkey frankfurters coated with soy protein films containing nisincombined with grape seed and green tea extracts (Theivendran et al. 2006). Millerand Cutter (2000) incorporated nisin into collagen-based films to provide protec-tion against pathogenic and spoilage organisms. A sausage casing containing sorb-ate and glycol was commercially marketed by Union Carbide (Labuza and Breene1989). Incorporation of essential oils has also been investigated in production of anti-microbial edible films and coatings. Although antimicrobial properties of essentialoils have been recognized for centuries, there has been renewed interest in their usebecause of consumer demand for natural ingredients and additives. Essential oilsare responsible for odor, aroma and flavor of spices and herbs. These compoundsare added to edible films to modify flavor, aroma and odor, as well as to impartantioxidant and antimicrobial properties. Films containing these ethanol-solublecompounds show activity against both Gram-positive and Gram-negative bacteria.Essential oils of angelica, anise, carrot, cardamom, cinnamon, cloves, coriander,dill weed, fennel, fenugreek, garlic, nutmeg, oregano, parsley, rosemary, sage andthymol are inhibitory to various spoilage and/or pathogenic bacteria, as well asmolds. Oussalah et al. (2004) produced milk protein-based edible films containingoregano, pimiento and oregano-pimiento mixtures. The oregano-containing filmsprovided the greatest antimicrobial activity against E. coli O157:H7 and Pseudomonasspp. on beef muscle slices, whereas pimiento-containing films were least effectiveagainst these two bacteria. More recently, Zivanovic et al. (2005) reported thatchitosan films enriched with essential oils (anise, basil, coriander and oregano) hadstrong antimicrobial effects on L. monocytogenes when applied to inoculated bolo-gna samples. Other antimicrobial films based on whey protein isolate (WPI) containing sorbicacid or p-aminobenzoic acid were developed by Cagri et al. (2001). Both filmsreportedly inhibited L. monocytogenes, E. coli O157:H7 and typhimurium DT104on a nonselective plating medium. Subsequently, these films were tested with beefbologna and summer sausage slices that were surface-inoculated with these samepathogens at levels of 106 CFU/g (Cagri et al. 2002). WPI films containing sorbic orp-aminobenzoic acid decreased L. monocytogenes, E. coli O157:H7 and S. typh-imurium DT 104 populations by 3.4–4.1, 3.1–3.6 and 3.1–4.1 log, respectively, onbologna and sausage slices after 21 days of aerobic storage at refrigerated tempera-ture. Growth of mesophilic aerobic bacteria, lactic acid bacteria, mold, and yeaston meat slices was also inhibited by the same antimicrobial WPI films, comparedto those coated with antimicrobial-free control films. The same research group subsequently developed heat-sealable WPI casingscontaining sorbic acid, p-aminobenzoic acid, or sorbic acid–p-aminobenzoic acid(1:1 ratio) for hot dog manufacture (Cagri et al. 2003). WPI casings containingp-aminobenzoic acid inhibited L. monocytogenes on hot dogs for 42 days of refrig-erated storage; however, films containing sorbic acid or sorbic acid–p-aminobenzoicacid were less effective. Sensory (texture, flavor, juiciness, overall acceptability),chemical (thiobarbituric acid; pH; moisture, fat, and protein contents), physical(purge, color) and mechanical (shear force) characteristics of hot dogs processed
260 Z. Ustunolwithin WPI casings containing p-aminobenzoic acid were comparable to thoseprepared with collagen and natural casings. Thus, WPI casings containingp-aminobenzoic acid may eventually provide a viable alternative to postprocesspasteurization of hot dogs for minimization of Listeria risk. Incorporation of other antimicrobials into edible films and coatings such as liq-uid smoke, sodium chloride and nitrites, has not been extensively studied. Liquidsmoke, which contributes antimicrobial, antioxidant, color and flavor attributes, isalso a potentially attractive film additive. Liquid smoke has been studied in conjunc-tion with edible collagen casings, where liquid smoke is introduced into theacid-swollen collagen mass before extrusion as a casing or film (Miller 1975).Because liquid smoke is generally very acidic (pH 2.5 or less), it is compatible withthe gel system, and can replace a portion of acid normally added to induce swellingof collagen. Sodium chloride (common salt) has been recognized as a food pre-servative since ancient times, and can be used alone or in combination with otherpreservation techniques, such as pasteurization or fermentation. Most bacterialfoodborne pathogens are susceptible to elevated concentrations of salt, particularlyin the presence other preservatives. Incorporation of salt into protein-based films(e.g., whey protein) as an antimicrobial agent is of limited use, since physical propertiesof protein films are altered with increasing ionic strength. At high ionic strength,proteins aggregate to form turbid, opaque gels with high water-holding capacity(Smith and Culbertson 2000). Nitrite has not yet been studied as an edible filmadditive, although it appears to be suitable for production of antimicrobial ediblefilms. Application of films containing nitrite to RTE meat products may not onlyhelp prevent growth of L. monocytogenes and spoilage bacteria that can contaminatesuch products after processing, but might also improve meat surface color. Release of antimicrobial agents from an edible film and controlling the condi-tions for release are very important considerations for effectiveness of antimicrobialfilms and coatings. Release of antimicrobial substances from edible films isdependent on many factors, including electrostatic interactions between the antimi-crobial agent and polymer chains, ionic osmosis and structural changes induced bythe presence of the antimicrobial and environmental conditions. Diffusion of anti-microbials through the edible film is also influenced by film (type, manufacturingprocedures), food (pH, water activity), hydrophilic characteristics and storageconditions (temperature, relative humidity, duration).8.3.6 Incorporation of Other AdditivesMany potential benefits of edible films as carriers of other additives (e.g., flavors,antioxidants, coloring agents, vitamins, probiotics and nutraceuticals) justify con-tinued research in the field of active packaging. However, only antioxidants havebeen investigated extensively. Although oxygen-barrier properties of edible filmsand coatings may reduce need for oxidative stabilization, antioxidants have beenused in edible coatings to provide further protection to meat and poultry products.
8 Edible Films and Coatings for Meat and Poultry 261Incorporation of antioxidants such as gallic or ascorbic acids into carrageenancoatings to extend shelf life of poultry products has been reported as early as 1948(Stoloff et al. 1948; Allingham 1949). Antioxidants were incorporated into a mix-ture of lard and tallow coating containing lactic acid–fatty acid triacylglycerol,which was used to coat freeze-dried and fresh meats, including beef steaks, porkchops and beef cubes (Sleeth and Furgal 1965). Thiobarbituric acid levels weresignificantly reduced in meats to which antioxidant-containing coatings wereapplied, compared to those of non-coated controls (Sleeth and Furgal 1965). Porkchops treated with alginate–starch coatings containing tocopherol were reported tobe juicier and less susceptible to lipid oxidation, compared to the untreated con-trols. However, they still developed off-flavors (Hargens-Madsen et al. 1995).Herald et al. (1996) reported that turkey breasts wrapped in corn zein films contain-ing butylated hydroxyanisole (BHA) had a lower hexanal content than samplespackaged in polyvinylidene chloride (PVDC). Essential oils from oregano, sage rosemary, thyme and pimiento are reported topossess antioxidant properties comparable to or greater than BHA or butylatedhydroxytoluene (BHT) (Wu et al. 1982; Shelef 1983; Howard et al. 2000; Bendiniet al. 2002). Oussalah et al. (2004) have reported on antioxidant properties of milkprotein-based edible films containing oregano, pimiento and oregano-pimiento mix.Pimiento-containing films provided the highest antioxidant activity on beef muscleslices; oregano-based films were also able to inhibit lipid oxidation in beef musclesamples. Armitage et al. (2002) evaluated egg albumen coatings with natural anti-oxidants, fenugreek, rosemary and vitamin E, for antioxidant activities in diced rawand diced cooked poultry breast meat. In both raw and cooked experiments, coatingswith no added antioxidant showed greatest inhibition of lipid oxidation as monitoredby thiobarbituric acid reactive substances (TBARS). Although some edible films have received consumer acceptance, further researchis needed to develop cost-effective production and application methods for continu-ous extrusion and application of films and coatings as flat sheets or casings.8.4 Film-forming Techniques and ApplicationSeveral different techniques, including solvent removal, thermal gelation andsolidification of melt, have been developed for forming edible films and coatings.Solvent removal has been used to produce hydrocolloid edible films. In this processa continuous structure is formed and stabilized by chemical and physical interac-tions between polymer molecules. Macromolecules in film-forming solution aredissolved in a solvent, such as water, ethanol or acetic acid, which contains otherfunctional additives (plasticizers, cross-linking agents, solutes). Film-forming solu-tion is then cast in a thin layer, dried and peeled from the surface. Freestandingfilms are formed by a casting technique in which film-forming solutions are pouredonto a smooth, flat, level surface, and allowed to dry, usually within a defined sur-face (Donhowe and Fennema 1994).
262 Z. Ustunol In preparing some types of protein films (e.g., whey protein, casein, soy protein,wheat gluten), solution is heated to promote protein gelation and coagulation,which involves denaturation, gelation, or precipitation, followed by rapid cooling.Intramolecular and intermolecular disulfide bonds in the native protein complex arecleaved and reduced to sulfhydryl groups during protein denaturation (Okamoto1978). When film-forming solution is cast, disulfide bonds re-form to link polypep-tide chains together to produce the film structure, which is further stabilized byhydrogen and hydrophobic bonding. Melting followed by solidification is a means for producing lipid-based films.Casting molten wax on dried methylcellulose films followed by solubilization of themethylcellulose can also be used to form wax films (Donhowe and Fennema 1993). Edible films and coatings may be applied to meat and poultry products by foaming,dipping, spraying, casting, brushing, individual wrapping, or rolling (Donhowe andFennema 1994; Grant and Burns 1994). Foam application is used for emulsioncoatings, where a foaming agent is added to the coating or foam is created bycompressed air; meat may be coated with protective foam as it moves over rollers.Flaps or brushes may also be used to distribute coating over the product (Grant andBurns 1994). Irregular surfaces of food products present particular challenges touniform application of coatings. Thus, several applications may be needed to obtaina uniform coating on a food surface. Emulsions may work in case of multiple appli-cations where the coating will need to set (or solidify). This is done typically afterdipping product that is being coated, letting the coating drain and set prior to appli-cation of the next coating layer (Donhowe and Fennema 1994). Spraying is mostsuitable where thinner films are needed, or when a coating is applied to only oneside of a product. Spraying is also used when dual applications are used to promotecross-linking (e.g., with alginate–Ca2+ coatings) (Donhowe and Fennema 1994).Early procedures for coating meat and poultry products involved spraying materialsonto rollers or brushes, and allowing meat to be coated by the tumbling action ofthe product (Grant and Burns 1994). Brushing and/or rolling the coating directlyonto meat surfaces may also be used to apply edible coatings. Edible films andcoatings applied to food products will need to set or solidify at the food surface.This requirement can be accomplished at ambient temperatures or with the use ofheat. Shorter drying times tend to provide for more uniformly distributed coatings(Grant and Burns 1994). Other than on collagen films and casings, only limited information is availableon continuous extrusion of freestanding films for meat applications.8.5 Regulatory AspectsThe process of determining acceptability of most ingredients used in edible filmsand coatings is similar to that used for food formulations (Heckman and Heller1986). If the edible film or coating is made from materials that have been generallyrecognized as safe (GRAS) and its use in the film or coating is in accordance with
8 Edible Films and Coatings for Meat and Poultry 263good manufacturing practices, it will be considered GRAS. If materials are notGRAS, but safety of the film or coating can be demonstrated, the manufacturer mayfile a GRAS Affirmation Petition with FDA or proceed without FDA concurrenceon the basis of self-determination. The manufacturer may not need to establish thatmaterials used are GRAS if the film or coating materials have received a pre-1958FDA clearance or “prior sanction”. If materials used in films and coatings are notGRAS or have not received prior sanction, then a food additive petition to the FDAmust be filed (Krochta and De Mulder-Johnston 1997). With the exception of chitosan, polysaccharides including cellulose and itsapproved derivatives (CMC, MC, HPMC), starches and their approved derivatives,and seaweed extracts (agar, alginates, carrageenan), are either approved food addi-tives or GRAS substances. Regulations regarding their specific use are described inthe Code of Federal Regulations (CFR) Title 21 (Nisperos-Carriedo 1994). Manyof the lipid compounds used are classified either as GRAS or food additives (FDA1991). Beeswax, carnauba wax, candelilla wax, carnauba wax, mono-, di-, and tria-cylglycerols, glyceryl monooleate, glyceryl monostearate and steric acid are GRASsubstances. Acetylated monoacylglycerol is classified as a multipurpose additive;fatty acids are approved as lubricants and defoamers (CFR Title 21; Baldwin et al.1997). Proteins that are most commonly used for edible films and coatings, such ascorn zein, wheat gluten, soy protein and milk proteins, have GRAS status. However,some concerns have been raised due to allergenicity or intolerance some consumershave to wheat proteins or lactose. Since edible films and coatings become part ofthe food to be consumed, all materials used in these products must be appropriatelydeclared on the label. Regulations regarding incorporation of antimicrobials, anti-oxidants, essential oils, color and other additives are the same as those that will beapplicable to food formulations.8.6 ConclusionsEdible films and coatings provide numerous opportunities to meat processors aswell as to consumers. Alternatives to collagen casings are feasible. Incorporation ofantimicrobials, antioxidants, flavors and colors provide for additional opportuni-ties. Once thermoplastic processing of other proteins and materials are refined,large-scale production of these films will be viable. Development and applicationof these materials should improve quality and safety of meat products.ReferencesAllen L, Nelson AI, Steinberg MP, McGill JN (1963) Edible corn carbohydrate food coatings. II. Evaluation of fresh meat products. Food Technol. 17, 1442–1446Allingham WJ May 17, 1949. U.S. patent 2,470,281
264 Z. UstunolAmin S, Ustunol Z (2007) Solubility and mechanical properties of heat cured whey protein-based edible films compared to collagen collagen and natural casings. Int. J. Dairy Tech. 60(2), 149–153Anderson TR August 9, 1960. U.S. patent 2,948,623Anderson TR June 20, 1961a. U.S. patent 2,989,401Anderson TR June 20, 1961b. U.S. patent 2,989,402Armitage DB, Hetiarachchy NS, Monsoor MA (2002) Natural antioxidants as a component of an egg albumin film in the reduction of lipid oxidation in Cooked and uncooked poultry. J. Food Sci. 67, 631–638Anonymous (1967) Edible packaging offers pluses for frozen meat, poultry. Quick Frozen Foods 29, 165–167, 213–214Ayers JC (1959) Use of coating materials or film impregnated with chlortetracy-cline to enhance color and shelf life of fresh beef. Food Technol. 13, 512–515Baker RA, Baldwin EA, Nisperos-Carriedo MO (1994) Edible coatings and films for processed foods. In: JM Krochta, EA Baldwin, MO Nisperos-Carriedo (eds.) Edible Coatings and Films to Improve Food Quality. Technomic Publishing, Lancaster, PA, pp 89–104Balasubramaniam VM, Chinnan MS, Mallikarjunan P, Phillips RD (1997) The effect of edible film oil uptake and moisture retention of a deep-fat Fried poultry product. J. Food Process Eng. 20, 17–20Baldwin EA (1994) Edible coatings for fresh fruits and vegetables: past, present and future. In: JM Krochta, EA Baldwin, MO Nisperos-Carriedo (eds) Edible Coatings and Films to Improve Food Quality. Technomic Publishing, Lancaster, PA, pp 25–64Baldwin EA, Nisperos NO, Baker RA (1995) Use of edible coatings to pre-Serve quality of lightly (and slightly) processed products. Crit. Rev. Food Sci. Nutr. 35, 509–524Baldwin EA, Nisperos NO, Hagenmaier RD, Baker RA (1997) Use of lipids in coatings for food products. Food Technol. 51(6), 56–62, 64Baron JK (1993) Inhibition of Salmonella typhimurium and Escherichia coli O157:H7 by an antimicrobial containing edible film. MS Thesis, University of Nebraska, LincolnBauer CD, Neuser GL December 9, 1969. U.S. patent 3,483,004Bauer CD, Neuser, GL, Pinkalla HA October 15, 1968. U.S. patent 3,406,081Becker OW October 6, 1936. U.S. patent 2,056,595Becker OW April 26, 1938. U.S. patent 2,115,607Becker OW June 13, 1939. U.S. patent 2,161,908Ben A, Kurth LB (1995) Edible film and coatings for meat cuts and primal. Meat’95. The Australian Meat Industry Research Conference. CSIRO, September 10–12 1995Bendini A, Gallina TG, Lercker G (2002) Antioxidant activity of oregano (Origanum vulgare L.) leaves. Ital. J. Food Sci. 14, 17–24Boni KA December 27, 1988. U.S. patent 4,794,006Brault D, D’Aprano G, Lacroix M (1997) Formation of free-standing steri-Lized edible films from irradiated caseinates. J. Agric. Food Chem. 45, 2964–2969Burke NI January 13. 1976. U.S. patent 3,932,677Cagri A, Ustunol Z, Ryser E (2001) Antimicrobial, mechanical and moisture barrier properties of low pH whye protein-based edible films containing p-aminobenzoic acid and sorbic acids. J. Food Sci. 66, 865–871Cagri A, Ustunol Z, Ryser E (2002) Inhibition of three pathogens on bologna and summer sausage slices using antimicrobial edible films. J. Food Sci. 67, 2317–2324Cagri A, Ustunol Z, Osburn WN, Ryser E (2003) Inhibition of Listeria monocytogenes on hot dogs using antimicrobial whey protein based edible casings. J. Food Sci. 68, 291–299Cagri A, Ustunol Z, Ryser E (2004) Antimicrobial edible films and coatings: A review. J. Food Prot. 67, 833–848Centers for Disease Control and Prevention (2000) Multi-state outbreak of listeriosis. Morb. Mortal. Wkly. Rep. 49, 1129–1130Cherian G, Gennadios A, Weller C, Chinachoti P (1995) Thermo-mechanical behavior of wheat gluten films: effect of sucrose, glycerin, and sorbitol. Cereal Chem. 72, 1–6Childs WH October 29, 1957. U.S. patent 2,811,453
8 Edible Films and Coatings for Meat and Poultry 265Cuq B, Gontard N, Cuq JL, Guilbert S (1997) Selected functional properties of fish myofibrillar protein-based films as effected by hydrophilic plasticizers. J. Agric. Food Chem. 45, 622–626Cutter CN, Siragusa GR (1996) Reduction of Bronchotrix thermosphacta on beef surfaces following immobilization of nisin in calcium alginate gels. Lett. Appl. Microbiol. 23, 9–12Cutter CN, Siragusa GR (1997) Growth of Bronchotrix thermosphacta in ground beef following treatments with nisin and calcium alginate gels. Food Microbiol. 14, 425–430Cutter CN, Sumner SS (2002) Application of edible coatings in muscle foods. In: Protein-Based Films and Coatings. A Gennedios (ed). CRC, Boca Raton, FLDaniels R (1973) Edible Coatings and Soluble Packaging. Park Ridge, NJ, Noyes DataCorpDeacon MJ, Kindleysides L (1973) U.S. patent 3,767,821. In Sausage casing technology, Food Technology, Review No. 14. Karmas E (ed) Park Ridge NJ: Noyes Data Corp. p. 88–89Donhowe IG, Fennema O (1993) Water vapor and oxygen permeability of Wax films. J. Am. Oil Chem. Soc. 70, 867–873Donhowe IG, Fennema O (1994) Edible films and coatings: Characteristics, formation, definitions and testing methods. In: Edible Coatings and Films to Improve Food Quality. JM Krochta, EA Baldwin, MO Nisperos-Carriedo (eds). Technomic Publishing, Lancaster, PA, pp 1–24Earle RD July 30, 1968. US patent 3,395,024Farouk MM, Price JF, Salih AM (1990) Effect of an edible collagen film overwrap on edudation and lipid oxidation in beef round steaks. J. Food Sci. 55:1510–1515Feuge RO (1955) Acetoglycerides – new fat products of potential value for the Food industry. Food Technol. 9, 314–318Galietta G, Di-Gioia L, Guilbert S, Cuq B (1998) Mechanical and ther-momechanical properties of films based on whey proteins as affected by plasti-izer and crosslinking agents. J. Dairy Sci. 81:3123–3130Gennadios A, Hanna MA, Kurth LB (1997) Application of edible coatings on meats, poultry and seafoods: A review. Lebensm. Wiss. Technol. 30, 337–350Gennadios A, McHugh T, Weller CL, Krochta JM (1994) Edible coatings and films based on proteins. In: Edible Coatings and Films to Improve Food Quality p. 201–277. JM Krochta, EA Baldwin. MO Nisperos-Carriedo (eds). Technomic Publishing, Lancaster, PAGennadios A, Weller CL (1990) Edible films and coatings from wheat and corn proteins. Food Technol. 44, 63–69Glicksman M (1983) Food Hydrocolloids. Vol. III. CRC, Boca Raton, FLGontard NG, Guilbert S, Cuq JL (1993) Water and glycerol as plasticizers affect mechanical and water vapor barrier properties of an edible wheat gluten film. J. Food Sci. Technol. 58, 201–211Grant LA, Burns J (1994) Application of coatings. In: Edible Coatings and Films to Improve Food Quality. JM Krochta, EA Baldwin, MO Nisperos-Carriedo (eds) Technomic Publishing, Lancaster, PA, pp 189–200Griffin DB, Keeton JT, Savell JW, Leu R, Vanderzant C, Cross HR (1987) Physical and sensory characteristics of vacuum packaged beef steaks and roasts treated with an edible acetylated monoglyceride. J. Food Prot. 50, 550–553Guilbert S (1986) Technology and application of edible protective films. In: Packaging and Preservation – Theory and Practice. M Mathlouthi (ed). Applied Science, Elsevier, New York, NY, p 371Handley D, Ma-Edmonds M, Hamouz F, Cuppett S, Madigo R, Schnepf M (1996) Controlling oxidation and warmed over flavor in precooked pork chops with rosemary oleoresin and edible film. In: Natural antioxidants chemistry, health effects and applications. Shahidi F. (ed). AOCS Champaign, IL, pp 311–318Hargens-Madsen M, Schnepf M, Hamouz F, Weller C, Roy S (1995) Use of edible films and tocopherol in the control of warmed over flavor. J. Am. Diet. Assoc. 95, A-41Hartal D (1966) The development and evaluation of carbohydrate-alginate food coatings. MS Thesis, University of Illinois, UrbanaHeine C, Wust R, Kamp B January 39, 1979. US patent 4,137,334Heckman JH, Heller IR (1986) Food, drug and cosmetic packaging regulations. In: The Wiley Encyclopedia of Packaging Technology ed. M Bakker. Wiley, New York, NY, pp 351–359
266 Z. UstunolHerald TJ, Hachmeister KA, Huang S, Bowers JR (1996) Corn zein pack-ageing materials for cooked turkey. J. Food Sci. 61:415–417,421Harvard C, Harmony MX June 1869. U.S. patent 90,944Hernandez E (1994) Edible coatings from lipids and resins. In: Edible Coatings and Films to Improve Food Quality. JM Krochta, EA Baldwin, MO Nisperos-Carriedo (eds). Technomic Publishing, Lancaster, PA, pp 279–303Hirasa K (1991) Moisture loss and lipid oxidation in frozen fish-effect of a casein-acetylated monoglyceride edible coating. M.S. Thesis, University of California, DavisHood LL (1987) Collagen in sausage casings. In: Advances in Meat Research Vol. 4. AM Pearson, TR Dutson and AJ Bailey (eds) New York, NY: Van Nos